185 31 9MB
English Pages 463 Year 2006
ELECTRONIC STRUCTURE, CORRELATION EFECTS AND PHYSICAL PROPERTIES OF d AND fMETALS AND THEIR COMPOUNDS
i
ii
ELECTRONIC STRUCTURE, CORRELATION EFECTS AND PHYSICAL PROPERTIES OF d AND fMETALS AND THEIR COMPOUNDS
V.Yu.Irkhin and Yu.P.Irkhin
CAMBRIDGE INTERNATIONAL SCIENCE PUBLISHING iii
Published by Cambridge International Science Publishing Ltd 7 Meadow Walk, Great Abington, Cambridge CB21 6AZ, UK http://www.cisppublishing.com
Published March 2007
© Cambridge International Science Publishing © V.Yu.Irkhin and Yu.P.Irkhin
Conditions of sale All rights reserved. No part of this publication may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopy, recording, or any information storage and retrieval system, without permission in writing from the publisher
British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library
ISBN 13: 9781904602552 Cover design Terry Callanan Printed and bound in the UK by Lightning Source (UK) Ltd
iv
PREFACE There exist several reasons to pick out the physics of transition group metals as a separate branch of solid state physics. The first one is the variety of properties of transition metals (TM) and their compounds, which are not only much more complicated, but have some important peculiarities in comparison with simple metals. In particular, ferromagnetic ordering takes place practically in TM and their compounds only. The second reason is the importance of investigating TM both from theoretical and practical point of view. TM yield an example of a strongly interacting manyelectron system, which does not enable one to introduce in a simple way an effective oneelectron potential. Thus we deal with the full manyparticle quantum problem which requires application of the all modern theoretical physics methods. The term ‘transition metals’ has two meanings. In the narrow sense of the word, TM are elements with partly occupied 3d, 4d and 5dshells, which form large periods in the Mendeleev periodic table. Sometimes this term is applied to all the elements with partly filled inner electron shells (transitiongroup elements), including 4f (rare earths, RE) and 5f (actinides). As a rule, we shall use the notion ‘transition metals’ in the narrow sense, but all the classes of transitiongroup elements will be discussed in the book. We have 24 TM, 13 RE and 8 actinides, so that about one half of elements belong to TM in the broad sense (at the same time, there exist only 25 simple metals). Among TM we find most practically important metals which exhibit maximum strength, melting temperature etc. The most wellknown example is Fe: up to now we live in the iron age. More and more applications find rare earths. For example, the intermetallic compound SmCo 5 yields a basis for best permanent magnets. Actinidies are widely used in nuclear energetics. A rather large number of books is available which treat metal physics. They are devoted mainly to simple metals and contain usually some separate paragraphs concerning TM. True, detailed monograps [15–17] discuss properties of rareearth metals and their compounds. At the same time, similar books on dmetals seem to be absent. This is probably explained by that systematization of corresponding large material, which may be found in original and review papers on particular topics, is a more difficult problem. However, in our opinion, it is useful v
to collect most important results on TM physics and discuss some general regularities. Let us list some distinctive physical properties of TM and their compounds: (i) large binding energies (high strength and melting temperature) (ii) large electronic specific heat (heavy electron masses) (iii) strong magnetism: large paramagnetic susceptibility and sometimes ferro or antiferromagnetic ordering (iv) superconductivity, often with high T C (v) anomalous transport properties (in particular, extraordinary halvanomagnetic effects). The book is devoted to consideration of these nontrivial physical properties, especial attention being paid to connection with the electronic structure. (The latter term includes both the properties of partially filled d and fshells and the anomalies of band structure.) We do not pretend to consider all the variety of TM compounds and alloys, but try to illustrate some interesting physical phenomena, which are not pronounced for elemental metals, by some bright examples. The book contains, where possible, a simple physical discussion of a number of problems. At the same time, we use widely in last three Chapters such methods of theoretical physics as the second quantization, atomic representation, Green's function approach. These methods permit to apply microscopic manyelectron models which describe systems with strong interelectron correlations. Besides traditional questions of the solid state physics, we treat some modern topics, e.g. magnetism of highly correlated and lowdimensional electron systems, anomalous properties of exotic rare earth and actinide systems (Kondo lattices, heavyfermion compounds), formation of unusual quantum states with nontrivial excitation spectrum etc. More difficult mathematical aspects of these topics are considered in Appendices A–P. Inclusion of numerous rather long Appendices makes the ‘topological’ structure of the book somewhat nontrivial and nontraditional. However, such a structure reflects manysided connections which exist between various branches of TM physics. At present the TM theory is far from completeness, and a number of important problems are still not resolved. Therefore the treatment of some TM properties may seem to be not so clear and logical as that of corresponding issues of general solid state physics in classical textbooks and monographs [1–14]. However, we believe that description of the modern complicated situation in the TM physics is justified since this may excite the interest in the unsolved questions and stimulate further researches. vi
The plan of the book is as follows. In the introductory Chapter 1 we treat atomic aspects of TM physics which, unlike the case of simple metals, are rather important since d and especially fstates retain in a large measure atomic features. Detailed mathematical consideration of some related questions is given in Appendices A–C. In particular, we review applications of the Racah's angular momentum formalism and Hubbard's manyelectron operator representation in the solid state theory, which are seldom discussed in the literature on the metal theory. Chapter 2 considers the electronic structure of TM from the ‘band’ side. We review briefly methods of band structure calculations, including the density functional approach, with especial attention to TM peculiarities. Besides that, we discuss some simple model approaches to the band spectrum and related experimental (especially spectral) data. We consider also theoretical and experimental results concerning the Fermi surfaces. In Chapter 3 we discuss thermodynamical properties of TM: cohesive energy and related properties, stability of crystal structures, and specific heat, electronic contributions being treated in details. Chapter 4 deals with magnetic properties. Here we discuss various theoretical models describing highly correlated d and felectrons. These models permit allround consideration of the complicated metallic magnetism problem which includes the atomic (‘localized’) and band (‘itinerant’) aspects of delectron behaviour. A large number of Appendices, related to this Chapter (D–K), demonstrate concrete practical applications of the manyelectron models, mainly within the simple method of doubletime retarded Green's functions. Chapter 5 is devoted to transport phenomena in TM which demonstrate a number of peculiarities in comparison with simple metals, e.g., occurrence of spontaneous (anomalous) effects. Quantitative treatment of these effects is performed with the use of densitymatrix approach in the operator form (Appendix M). Finally, in Chapter 6 we treat some questions of the anomalous fcompound theory. In particular, we discuss various mechanisms for occurence of ‘heavy’ electron mass and the problem of competition between the Kondo effect and magnetic interactions. We consider also model descriptions of the electronic structure in twodimensional highlycorrelated systems including copperoxide highTc superconductors. We intended to consider in the book all main properties of TM and corresponding theoretical concepts. However, the choice and volume of the material in different Chapters are determined to some extent by scientific interests of the authors. In particular, we pay a great attention to the theory of magnetism and transport phenomena, vii
but discuss in less details lattice properties, and almost do not touch superconductivity (the latter topic develops now extensively and is widely discussed in modern review and monograph literature). We list once more some examples of nontraditional questions which are treated in the book: the influence of density of states singularities on electron properties; manyelectron description of strong itinerant magnetism; the problem of quenching and unquenching of orbital magnetic magnetic momenta in solids and their significance for magnetic anisotropy; microscopic theory of anomalous transport phenomena in ferromagnets. The book is partly based on the lection course of the transition metal physics, which was read for a number of years at the Ural State University. Except for numerical estimations, we use often in formulas the system of units with e = k B = = 1. We hope that the book may be of interest for researchers working in solid state physics and for beginners, both for theorists and experimentators. Some parts of the material may be used in lecture courses for students. The authors are grateful to A.Zarubin, A. Ignatenko, P. Igoshev, A.Nasibullin and A.Katanin for their help in preparing the electronic version of the book.
viii
CONTENTS
PREFACE ............................................................................................v 1 INTRODUCTION ...........................................................................1 1.1 Partly filled atomic shells and electron localization in transition metals 1.2 Atomic and band approaches in the transition element theory 1.3 Crystal field and orbital momenta in solids
1 7 12
2 BAND THEORY ........................................................................... 20 2.1 Orthogonalized plane wave method and pseudopotential 2.2 Augmented plane wave (APW) and KorringaKohnRostoker (KKR) methods 2.3 The HartreeFockSlater and density functional approaches to the problem of electron correlations 2.4 Discussion of band calculation results 2.5 Experimental investigations of band structure: spectral data 2.6 Band calculations of rare earths and actinides 2.7 Fermi surface 2.7.1 Methods of Fermi surface investigation and de Haasvan Alphen effect 2.7.2 Experimental and theoretical results on the Fermi surfaces
23 27 31 39 54 67 72 72 76
3 THERMODYNAMIC PROPERTIES .........................................86 3.1 Cohesive energy and related properties 3.2 Crystal structure 3.3 Specific heat 3.3.1 Lattice specific heat 3.3.2 Electronic specific heat 3.3.3 Specific heat of magnetic metals
86 100 109 109 113 120
4 MAGNETIC PROPERTIES .....................................................124 4.1 Exchange interactions and the Heisenberg model for localized spins 4.2 Magnetic susceptibility of paramagnetic transition metals 4.3 Itinerant electron ferromagnetism and the Stoner theory 4.4 Spinfluctuation theories 4.5 Electronic structure and properties of halfmetallic ferromagnets 4.6 Magnetism of highlycorrelated dsystems 4.7 Magnetism of rare earths and actinides 4.8 Magnetic anisotropy 4.8.1 Quenching of orbital momenta by periodic lattice
ix
125 129 136 145 151 161 167 173
potential and magnetic anisotropy of dmetals 4.8.2 Magnetic anisotropy of rare earths
176 179
5 TRANSPORT PROPERTIES .....................................................183 5.1 General classification of transport phenomena 5.2 Calculation of transport coefficients 5.3 Resistivity 5.3.1 Electronelectron scattering 5.3.2 Mott sd scattering mechanism 5.3.3 Resistivity of magnetic metals 5.3.4 Resistivity of transition metal alloys 5.3.5 Twocurrent model of ferromagnetic metals 5.4 Thermoelectric power 5.5 The Hall effect 5.6 Magnetoresistivity 5.7 Anomalous transport effects in ferromagnetic metals 5.7.1 The extraordinary Hall effect 5.7.2 Magnetoresistivity in the presence of spontaneous magnetization 5.7.3 Magnetooptical effects 5.7.4 Thermomagnetic effects
184 188 190 196 200 202 207 208 213 218 227 231 231 242 245 248
6 THE KONDO EFFECT AND PROPERTIES OF ANOMALOUS d AND fCOMPOUNDS 6.1 6.2 6.3 6.4 6.5 6.6
The onecentre Kondo effect The Kondo temperature for dimpurities Spin dynamics and electronic properties of Kondo lattices Ground state of the Kondo lattices Intermediate valence systems Magnetic ordering in Kondo lattices and heavyfermion compounds 6.7 Current carriers in a twodimensional antiferromagnet 6.8 Spinliquid state in systems with spin and charge degrees of freedom
A B C D E F G
254 258 262 267 270 279 289 295
Manyelectron creation operators for atomic configurations and Hubbard operators ................................................................... 301 Angular momentum operators and double irreducible tensor operators .............................................................................. 308 Hamiltonian of a crystal with manyelectron atoms ................... 314 Interatomic electrostatic interaction and derivation of the Heisenberg Hamiltonian ................................................................ 321 Spin waves in Heisenberg magnets and the Green's function method ............................................................................... 329 Hubbard operator approach in the Heisenberg model ............. 336 Electronmagnon interaction in magnetic metals ....................... 341
x
G.1 Ferromagnets 342 G.2 Antiferromagnets 353 H The Hubbard model with strong correlations ............................. 363 I Narrowband sd exchange model and tJ model ....................... 370 J Electron states and spin waves in the narrowband Hubbard ferromagnet ..................................................................... 374 K sf exchange model and indirect exchange interaction in rare earths ........................................................................................ 379 L Spinorbital interaction ................................................................... 383 M The density matrix technique for derivation of transport equations and the theory of the anomalous Hall effect ............. 388 M.1 Impurity scattering 392 M.2 Scattering by phonons 395 M.3 Scattering by spin inhomogeneities 398 N Degenerate Anderson model ........................................................ 405 O Meanfield approximation for the ground state of magnetic Kondo lattices .................................................................................. 412 P Schwinger and DysonMaleev representations in the theory of twodimensional Heisenberg antiferromagnets ........ 417 CONCLUSIONS ..................................................................................... 424 REFERENCES ........................................................................................ 427 INDEX ...................................................................................................... 447
xi
xii
Introduction
Chapter 1 INTRODUCTION 1.1 PARTIALLY FILLED ATOMIC SHELLS AND ELECTRON LOCALIZATION IN TRANSITION METALS The ‘hydrogenlike’ scheme of energy levels depending on oneelectron principal and orbital quantum numbers n and l corresponds to consecutive filling of atomic shells with increasing n and l. (The ‘accidental’ degeneracy of the levels with different l for a given n in the purely Coulomb potential 1/r, which is connected with a dynamical symmetry, is lifted for manyelectron atoms where the potential rdependence is modified.) However, in the periodic table this sequence is violated several times. This results in the formation of large periods of transition elements with partially filled d( f )shells and peculiar physical properties. To first time, such a situation occurs in the fourth period where filling of 4sstates starts in potassium, the 3dshell remaining empty. This tendency holds also in calcium (configuration of valence electrons is 4s2), and filling of 3dshell starts only for the next element, i.e.scandium (configuration 3d4s). This element opens the 3d transition group (iron group). The filling of the 3dshell goes in a not quite regular way (Table 1.1). So, chromium has the atomic configuration 3d14s 2 (instead of 3d4s 2 ), and copper 3d 10 4s (instead of 3d 9 4s 2 ). One can see that a tendency to formation of configurations d 0 , d 5 and d 10 exists. The stability of these configurations is apparently connected with that they correspond to zero summary orbital momentum of all the delectrons, i.e. to a spherically symmetric electron density. It should be noted that in some cases copper demonstrates a considerable contribution of d 9 s configuration, which is connected with an appreciable s−d hybridization. Therefore, we shall discuss Cu side by side with transition metals. A situation, similar to 3d metals, takes place for 4d, 5d, 4f and 5f transition metals groups (Tables 1.1, 1.2). Thus, the filling of dand fshells is delayed, and, after it begins, the electrons from the 1
Chapter 1 Table 1.1. Atomic configurations and ground terms for the free atoms and M 2+ ions, and third ionization potentials (eV) in dseries. 3d
Sc
Ti
V
Cr
Mn
Fe
Co
Ni
Cu
4d 5d
Y La
Zr Nb
Nb Ta
Mo W
Tc Re
Ru Os
Rh Ir
Pd Pt
Ag Au
3d
d1s2
d2s2
d3s2
d 5s
d5s2
d6s2
d7s2
d8s2
d10s
4d 5d 3d 4d 5d M2+ 3d, 4d, 5d
d1s2 d1s2 2 D3/2 2 D3/2 2 D3/2 d1 2 D3/2
d2s2 d2s2 3 F2 2 F2 3 F2 d2 3 F2
d 4s d3s2 4 F3/2 6 D1/2 4 F3/2 d3 4 F3/2
d 5s d 4s 7 S3 7 S3 5 D0 d4 5 D0
d5s2 d5s2 6 S5/2 6 D9/2 6 S5/2 d5 6 S5/2
d 7s d6s2 5 D4 5 F5 5 D4 d6 5 D4
d 8s d7s2 4 F9/2 4 F9/2 4 F9/2 d7 4 F9/2
d10 d 9s 3 F4 1 S0 4 D3 d8 3 F4
d10s d10s 2 S1/2 2 S1/2 2 S1/2 d9 2 D5/2
3d
24.75
27.47
29.31
30.95
33.69
30.64
33.49
35.16
36.83
4d 5d
20.51 19.18
22.98 28.1
25.04 22.3
27.13 24.1
31.9 26
28.46 25
31.05 27
32.92 28.5
34.82 30.5
Table 1.2. Atomic configurations and ground terms for free atoms and R 3+ ions of rare earths and actinides. Rare earths and heavy actinides (starting from Am) are characterized by the most stable valence of 3+. Beside that, the 4+ state is possible for Ce, Tb and Pr, and the 2+ state for Nd, Sm, Eu, Tm and Yb. Light actinides exhibit a large variety of valence states. La f 0d D23/2
R R3+
f0 S0 Gd 1
9
D2 f7 8 S7/2
R3+
Ac
R3+
Pr f3 I49/2
Nd f4 I54
Pm f5 H65/2
2
f1 F5/2 Tb
3
f2 H4 Dy
4
f3 I9/2 Ho
f4 I4 Er
f 8d
f 10
H17/2 f8 7 F6
5
f 7d
R
R
Ce f 1d H34
Th
o 1
0 2
f0
f1
fd f d 2 D3/2 3F2 1
S0
2
F5/2
8
4
I8 f9 6 H15/2
Pa
U
Np
5
f 12
I15/2 f 10 5 I8
3
5 0
6 0
f2
f3
f4
f d f d f d f d 4 K11/2 2L6 6H5/2 7F0 3
H4
4
I9/2
5
I4
6
f5 H5/2 Tm
7
f 13
Cm
7 1
7 1
Cf
8 1
f d f 10d0 8 H17/2 5J8
f d 9 D2
f5
f6
f7
f8
H5/2
7
S7/2
7
2
S0 f 13 2 F7/2
Bk
f d 8 S7/2
8
f 14 1
F7/2 f 12 3 H6
Am
F0
f6 F0 Yb
2
H6 f 11 4 I15/2
Pu
3 1
Eu f7 S87/2
6
f 11
2 1
Sm f6 F70
F6
f9 6
H15/2
Introduction 4s, 4p shells with higher energies do not pass into ‘free’ d( f )states. These phenomena are connected with inapplicability of the simple oneelectron picture, which is based on the hydrogen atom theory, for manyelectron atoms. Consider the radial atomic potential V l(r), ‘felt’ by electrons. This is an effective potential which is obtained after averaging twoparticle interaction among electrons and including the rotational motion energy (centrifugal potential):
Z (r ) l (l + 1) , + (1.1) r r2 where Z(r) is an effective nuclear charge, which depends on the electron coordinate r (measured in Bohr radia). For the hydrogen atom we have Z(r)=1 and V l (r) has the usual form with a minimum at r 0=l(l+1) (Fig.1.1). This picture holds in hydrogenlike atoms where the condition Z(r) = const is satisfied to high accuracy. However, in more complicated situations the dependence Z(r) becomes important because of nonuniform screening of nuclear potential. It is this dependence that may lead to an anomalous form of the function V l(r) for a large centrifugal term (i.e. sufficiently large values of l). In particular, for Vl (r ) = −
r1 < r < r2 , A/ r , Z (r ) = (1.2) const , r < r1 , r > r2 , V l(r) may have two minima separated by a potential barrier. Concrete calculations demonstrate that V(r) may even become positive in an interval [r 1 ,r 2 ]. The results for Ba and La are shown in Fig.1.2. In fact, the interval [r 1 ,r 2 ] corresponds to the position of orbits of 5s and 5pelectrons which screen strongly the nucleus. In other words, strong repulsion between 4f and s, pelectrons occurs in the
Fig.1.1. The effective potential for a hydrogenlike atom. 3
Chapter 1
Radius, units of a o Fig.1.2. The effective potential V eff and radial wavefunctions P 4f (r) for BaI (broken lines) and LaI (solid lines) [18].
region of localization of the latter. In the presence of two minima, the electron density may be concentrated in any one, depending on the form of Z(r). The energy of the corresponding states is, generally speaking, considerably different, as one can see from Fig.1.2. At passing from Ba to La, the lanthanide collapse of 4fstates, i.e. a sharp decrease of the 4fshell radius takes place. Further, for cerium 4fstates become more energetically favourable than 5s, 5p and 6s ones, the maximum of 4felectron density passes to the first minimum and filling of 4flevels starts. Thus the main reason of irregular filling of atomic levels are interelectron interaction and appreciable value of the orbital energy at l≠0. These effect become important from l=2 and are strongly pronounced for rare earths (l=3). In Fig.1.3 the data on energy levels of external electrons and their density distribution are shown for the gadolinium atom. Now we treat the question about true capacity of d( f )states which remain in transition elements, from the point of view of the simple oneelectron theory, partially unfilled (despite filling of higher shells). According to the latter theory, each shell with the orbital quantum number l may contain 2(2l+1) electrons, their energies being equal because of spherical symmetry. However, this is is not true when interelectron correlations are taken into account. This may be performed in the manyconfiguration approximation [20] where a Hartree– 4
Introduction a
b
Fig.1.3. (a) energy levels (eV) of external atomic electrons in the Gd atom [19] (b) radial distribution of the Hartree–Fock charge density for 4f, 5s, 5p and 6selectrons of the Gd 3+ ion [16].
Focktype potential, which depends on electron configuration, is introduced. We present a simple illustration of this effect. Write down the energy of n electrons in a lshell (the principal quantum number is dropped for brevity)
1 Eln = nε l + n(n − 1)Ql , (1.3) 2 where εl is the sum of the kinetic energy and additive part of the potential energy, Q l is the interelectron repulsion for the shell. The energies of the configurations l n+1 and l nl ′ (e.g., d( f ) n+1 and d( f ) ns) read 1 Eln +1 = (n + 1)ε l + n(n + 1)Ql , 2
(1.4) 1 E = nε l + ε ' + n(n − 1)Ql + nQ ' , l ll 2 with Q ll ′ being the repulsion between l and l ′ electrons. One can see that the configuration l has the higher energy provided that n l
Ql − Q ' > (ε ' − ε l )/n. ll
l
(1.5)
In transition elements, the intrashell repulsion is much stronger than the intershell one, Q sd(f) Q d(f) , and the difference ε s − ε d(f) is not too large. Therefore the maximum possible filling of the d( f )−shell is not energetically favourable. The atomic picture of 4felectrons which are well localized holds 5
Chapter 1 in metals. A possible exception is given by cerium, which opens the 4fseries, so that the felectron lies apparently near the centrifugal potential barrier. The γ−α transition in the metallic Ce is assumed now to be connected with the tunneling of the felectron through the barrier and its appreciable delocalization (see 6.5). A similar situation occurs in Sm, Nd and Pr under high pressure of order of 1Mbar [21]. Besides that, in some rare earth compounds felectrons become partially delocalized because of hybridization mixing with conduction electrons. The description of dstates in solids is rather difficult. Unlike 4felectrons, they demonstrate both ‘localized’ and itinerant features. Such a behaviour is determined by the corresponding atomic potential, which differs essentially from that for s, pelectrons. The presence of a potential barrier results in an appreciable localization of dstates and decrease of overlap between dfunctions at different lattice sites. However, the density of delectrons still lies partially outside the potential barrier. As a result, their kinetic energy turns out to be considerable, and the corresponding bandwidth values are comparable with those for s, pelectrons. The second factor, which determines the delectron spectrum, is the Coulomb repulsion between them. This depends strongly on the number of delectrons inside the barrier. Therefore the effective oneelectron energies and wavefunctions should be rather sensitive to the manyelectron configuration d n±1s 1⫿1, and the degeneracy is lifted:
ε d = ε d (d n ),
ε d (d n ) < EF < ε d (d n +1 ) ε d (d n ) + Q
(1.6)
(the Fermi energy E F determines the band filling). In Appendix C we discuss these effects in more detail by using manyelectron Hamiltonian and angular momentum theory. Owing to increase of the dshell radius, the localization degree of delectrons decreases when we move in the periodic Table both from right to left and from up to below. Thus 3delectrons are considerably more localized than 4d and especially 5delectrons. This explains the fact that magnetic ordering, which is connected with existence of pronounced local moments, occurs for 3dmetals only. A similar difference in the localization degree takes place between 4felectrons in rare earths and 5felectrons in actinides. In light actinides (from Th to Pu) 5felectrons form wide energy bands and may be considered as itinerant, and in actinides with higher atomic numbers they are localized. However, the delocalization in Am, Cm, Bc and
6
Introduction Cf may occur under pressure [22, 23].
1.2 ATOMIC AND BAND APPROACHES IN THE TRANSITION ELEMENT THEORY Most important peculiarity of transition metals from the theoretical point of view is an important role of electron correlations. There exist a number of approaches to the problem of treating manyelectron (ME) systems with strong correlations. The first one was the selfconsistent field (Hartree–Fock) approximation at solving the Schroedinger equation for ME atoms, which yielded satisfactory quantitative results. The Hartree–Fock method allows to take into account ME atomic terms, but its full version requires the solution of a complicated system of integrodifferential nonlinear equations [20], so that its direct generalization on solids (systems of large number of atoms) is hardly possible. Main successes of the solid state theory were connected with firstprinciple oneelectron band structure calculations. Modern versions of this approach, which are based on the spindensity functional method (2.3), enable one to obtain a precise description of ground state characteristics [24]. At the same time, the band theory is wittingly insufficient for strongly localized fstates, and also at treating some physical phenomena, e.g. magnetism (especially at finite temperatures) and metalinsulator (MottHubbard) transition [25]. Such oversimplified versions of the HartreeFock method, as the Stoner meanfield theory of itinerant magnetism, turned out to be not too successful. Later, some shortcomings of the Stoner theory were improved by semiphenomenological spinfluctuation theories [26], which, however, do not take into account in most cases correlation effects in the ground state. To treat electron correlations, various perturbation approaches in the electronelectron interaction (e.g., diagram techniques) were used. Besides that, the Fermiliquid theory was proposed to describe systems with strong electron interactions [27]. However, this theory is violated in the cases where the correlations result in a reconstruction of the ground state, e.g. for systems with a Mott–Hubbard gap [25]. Another approach to the problem of electron correlations was proposed by Hubbard [28–31] who considered the simplest microscopic model including the strong onsite Coulomb repulsion. Starting from the atomic limit, Hubbard carried out a decoupling of Green’s functions and obtained an interpolation solution, describing both atomic and band limits for sstates [28] and the simplest model of degenerate band [29]. In the subsequent paper [30] this solution was improved
7
Chapter 1 to describe the metalinsulator transition. In the paper [31] Hubbard proposed a general formalism of ME Xoperators (atomic representation) which enables one to take into account intraatomic interactions in the zerothorder approximation. This formalism for real atomic configurations is considered in Appendix A. It is clear from the physical point of view that interelectron correlations are most important for the electrons of the same atomic shell (the equivalent electrons). The modern form of the theory of atomic spectra is based on the Racah formalism for angular momenta (see, e.g., [20]). In some cases, calculations may be considerably simplified by using the irreducible tensor operator technique in the second quantization representation [32] (related questions are considered in Appendix B). This powerful mathematical technique introduces the representation of manyelectron quantum numbers Γ={SL µ M} instead of oneelectron ones, γ ={lm σ }, S = ∑si ,
L = ∑1i
i
i
(1.7)
being the total angular spin and orbital momenta and µ and M their projections. Then numerous possible combinations of γsets for a partially occupied shell are replaced by the sets of Γ. The total number of ME state is the same, but the energy degeneracy is lifted, so that in most physical problems one can retain only the lowest ME term. According to Hund’s rules, this term corresponds to maximum L and S. Within this approach, the problem of electrostatic interaction in the system is reduced to calculating a few Slater integrals F (p) (Appendix C). These integrals may be calculated with the use of atomic wavefunctions [33] or determined from experimental data on energies of atomic terms (see [34]). Information on the energy of the Hund atomic terms may be obtained from the values of atomic ionization potentials. Table 1.1 presents the values of third ionization potentials (of M 2+ ions) in drows, which characterize the binding of delectrons (first and second ionization potentials correspond as a rule to moving away of selectrons from the d ns 2 configuration). One can see that with increasing atomic number the binding in the drows increases. Such a dependence explains the corresponding increase of delectron localization in solids, which is discussed in previous Section. In solids the values of the Slater integrals become modified. In the recent paper [35] the lowering ∆F (p) /F (0) , which is due to the change in correlation effects (in particular, in interconfiguration interaction) in a crystal, was calculated. At p=2, the values of this 8
Introduction quantity of 0.22 and 0.16 were obtained for Ti 2+ (d 2 ) and Ni 2+ (d 8 ) ions, respectively. Besides the band approach, the ME approach with inclusion of the atomic spectroscopy mathematical technique should be very useful for the development of quantitative theory of solids. Such an approach is applicable in the case of strong electron localization and especially effective for equivalent electron shells of d and fions with a complicated term structure. It is important for the solid state theory that the second quantization representation (unlike the standard atomic theory) enables one to consider processes with changing electron number in a shell or an atom (Appendix C). An account of band energy dependence on manyelectron quantum numbers corresponds to the degenerate Hubbard model (Appendices C,H). The localization degree of 4felectrons is sufficient to justify using the atomic picture. On the other hand, for d and 5felectrons the crystal field effects result in at least partial quenching of orbital momenta and destruction of atomic terms. However, atomic structure is important for local effects (e.g., in the case of dmetal impurities). Atomic description may be useful also at considering some physical phenomena in periodic crystals (e.g., strong magnetism with pronounced local magnetic moments, formation of an insulating state in dcompounds). An interesting manyelectron term effect for a pure metal is the 6eV satellite in the XPS spectrum of nickel which may be attributed to the multiplet structure of the d8configuration (see also 2.6). Another example is provided by Auger spectra for dstates which exhibit clearly the term structure. This is due to large localization of delectrons in the presence of highly correlated twohole atomic states which occur after the core hole decay. The Coulomb interaction of dholes U in Cu is so large that the twohole final state is split off from the onehole band states. Therefore one can distinguish in the Cu spectrum (Fig.1.4) all the terms of the d 8 configuration. A somewhat less pronounced multiplet structure of the dconfiguration is observed in the Auger spectrum of metallic nickel. The value of U in Ni is of order of the onehole bandwidth and the twohole states mix strongly with band states (the initial state is a mixture of d 9 and d 10 configurations). Figure 1.5 shows an interpretation of the L 3 VV spectrum in terms of the multiplet structure corresponding to the main peak 1 G with
4 (2) 1 (4) F + F . (1.8) 49 441 The comparison of XPS and L3VV spectra for nickel and its compounds U (1 G ) = F (0) +
9
Count, 10 3
Chapter 1
Kinetic energy, eV Fig.1.4. Experimental L 2,3 M 45 M 45 Auger spectra from copper and zinc. Atomic multiplet structures are shown as lines under spectra [36].
[37] permitted to estimate the value of U and determine its dependence on crystal surrounding. Experimental energies of the XPS satellite correlate with the energy of the L 3 VV peak in all the cases. A fit of the Slater integral yields
F (0) = 1.7, (in eV) which leads to
F (2) = 9.6,
10
F (4) = 6.4,
Introduction
F0 = 1.7 eV
Normalised intensity
Exp.
F0 = 2.7 eV
E, eV Fig.1.5. Effect of multiplets on the L 3 VV Auger spectra of nickel. Lower panel: XPS VB after subtraction of satellite N(E) and its selffold D 0 (E). Middle and top panels: experimental spectrum and calculated contributions from individual d 8 terms with different values of Slater integrals [37].
U (1 S ) = 6.3,
U (1 G ) = 2.5,
U (3 P) = 7.85,
U (3 F ) 0.
U (1 D) = 1.6,
A considerable decrease in the value of F in comparison with atomic one demonstrates strong screening of the Coulomb interaction by 11
Chapter 1 Table 1.3. Probabilities of Auger transitions in Cu (10 −4 a.u.) [38].
Term Multiplicity L3M45M45 L2M45M45
1
1
S
3
G
1 1.15 0.58
9 2.88 21.43
P
9 1.39 0.69
1
D
5 7.40 3.69
3
F
21 16.18 8.10
conduction electrons. The overlap of the atomic 3 F state with bandlike states may influence appreciably electronic properties of nickel. Besides the energy characteristics, the transition probabilities in spectral measurements are also of interest for investigating the ME term structure features in the solid state. The probabilities of the Auger processes L 2,3 M45 M 45 for the d 8 multiplet of Cu were calculated in [38] with the use of modified wavefunctions of continuum Auger electrons (using the plane waves yielded a drastic disagreement with experimental data). The results are presented in Table 1.3. One can see that the probabilities are not proportional to term multiplicities, which indicates a considerable change of atomic states in the metal. The values of Slater integrals with account of Coulomb interaction screening by extraatomic electrons in twohole states, which were obtained in [38], are
F (2) = 10.0,
F (4) = 5.6.
They are appreciably suppressed in comparison with the atomic values
F (2) = 11.65,
F (4) = 7.18.
1.3 CRYSTAL FIELD AND ORBITAL MOMENTA IN SOLIDS As discussed above, electrostatic interactions in free transitionelement atoms result in occurrence of partially filled d(f)shells, their states being characterized by manyelectron quantum numbers. Now we consider the role of extra interactions which are present in crystals containing such atoms. In particular, we discuss the problem of role of orbital magnetic momenta in solids. The orbital momentum L is one of principal atomic characteristics. This quantum number determines the ground state of the atom according 12
Introduction to the second Hund’s rule and the general picture of excited terms. Existence of orbital magnetic momenta (OMM) in ME atomic configurations should result in a number of important effects in solids. In particular, one might expect the occurrence of the orbital magnetism with large magnetic momenta and strong anisotropy. Such a situation does take place in rareearth systems [16, 39] where magnetism is determined by the total angular momentum J = L + S. Orbital momenta play also an important role in actinides because of strong spinorbital coupling. In most dmetals and their compounds, the contribution of OMM to physical properties is considerably smaller (e.g., for Ni the investigation of L absorption edge [40] yielded l=0.05 µ B ). This is explained by the fact that the delectrons are influenced by the crystal field (CF) considerably stronger than welllocalized 4felectrons. The ME levels of dions are split by CF, so that OMM become quenched: 〈L〉=0 in not too strong magnetic fields. However, other interactions in the crystal unquench them partially, and (even small) OMM that arise are important for the anisotropy of physical properties due to coupling to the lattice. In particular, strong anisotropy of paramagnetic susceptibility owing to the orbital contribution takes place in a number of hexagonal transition metals (see a detailed discussion in Sect.4.2). In the problem of quenching of orbital momenta, three basic interactions should be taken into account: the Coulomb interaction V Q, the spinorbit coupling V so and the CF potential V cf. There occur three cases. For a weak crystal field where Vcf Vso VQ ,
(1.9)
we have the coupling scheme
∑s i
i
= S,
∑l
i
= L,
i
L + S = J.
(1.10)
Then OMM are unquenched (the whole quantum number set is {SLJM}). The coupling between L and S is rigid, and CF orients the total momentum J in some crystallographic directions, which results in a large magnetic anisotropy. The weak field approximation is valid for rareearth ions where 4fshells are strongly screened from V cf by s, p, d shells, and the value of V so is appreciable due to the large nuclear charge Z. For the intermediate crystal field
13
Chapter 1 Vso Vcf VQ ,
(1.11)
L and S still persist, but the momentum J is not formed because of CF splitting. Then OMM are oriented in easy crystal directions and spin momenta are coupled to them by a weak spinorbit coupling. At inclusion of an external magnetic field H in a hard direction, the deviation of spin momentum from the easy direction will be proportional to the ratio µ B H/V cf . The orbital contribution to magnetization will be negligible because of smallness of the ratio µBLH/Vcf in any realistic fields. The intermediatefield situation apparently takes place for dimpurities in some salts [41] and for some nonmetallic dcompounds. This case is compatible with orbital ordering, which exists in a number of dsystems [42]. Finally, for the strong crystal field Vso VQ Vcf
(1.12)
the Russel–Saunders coupling between delectrons is totally destroyed. Then their energy levels are to be considered as oneelectron ones which are split by CF. The Coulomb interaction should be now treated as a perturbation for the states with a new symmetry, and orbital momenta are transformed into quasimomenta which are determined by the corresponding irreducible representations of the point group. The strong field situation is usually assumed to take place for transition metals and their alloys. However, the estimation V cf ∼V Q seems to be more realistic in such systems. This leads to difficulties at developing a consistent quantitative theory. The CF theory is well developed for paramagnetic ions in nonmetallic crystals where a general qualitative analysis of the dshell structure can be made on the basis of the local point group, corresponding to a given site. General expansion of the CF potential in spherical functions has the form
Vcf = ∑Aλµ 〈r λ 〉Yλµ (θ , φ ). λµ
(1.13)
For a lshell, it is sufficient to retain in (1.13) the terms with λ≤ 2l only; λ is even in the presence of inversion symmetry. The crystal potential can be also expanded in cubic harmonics V λµ . For λ=2
V20 = 3z 2 − r 2 ,
V22 = x 2 − y 2 ,
14
Introduction
V21 = xz,
V2−1 = yz,
V2−2 = xy.
(1.14)
In many cases, it is convenient to use the method of Stevens equivalent momentum operators which have the same matrix elements as spherical functions. For example,
1 V22 = α J 〈 r 2 〉[( J + )2 + ( J − )2 ], 2
V20 = α J 〈 r 2 〉[3( J z )2 − J ( J + 1)],
1 V21 = V22 = α J 〈r 2 〉( J x J z + J z J x ), 2 where α J (and similar factors β J , γ J for λ=4.6) are the Stevens proportionality coefficients which depend on the configuration l n [16, 41, 43]. The Stevens operator representation holds beyond the multiplet with a given J (or L) only. Of course, the operator (1.5), unlike (1.7), has also matrix elements between different terms. The method of equivalent operators in problems with changing J or L is more complicated (see [41]). Consider concrete examples of d n configurations in the crystal field. Since various situations may take place for delectrons in CF, constructing interpolation schemes is useful [43]. The picture of the twohole spectrum for the Ni 2+ ion (configuration 8 d ) is shown in Fig.1.6. We use Bethe’s notations 2S+1Γ i for irreducible representations of the cubic group: Γ 1 (A 1g ) and Γ 3 (E g ) are onedimensional, Γ4(T1g) is twodimensional, Γ4 (T1g) and Γ 5(T2g) are threedimensional. An arbitrary position of oneelectron levels is chosen; an analogue of the Hund rule takes place for the effective orbital momentum in CF [41]. One can see that the initial orbital momentum L=3 is quenched in intermediate crystal field provided that the lowest state is the orbital singlet 3 Γ 2 . For threedimensional ‘Hund’ representations 3Γ4 and 3Γ5, quenching is absent. In the strong CF, electron orbital momenta are quenched provided that the lowest oneelectron state is e g (which corresponds to metallic nickel). We see that, a regrouping of e g and t 2g states takes place at increasing Coulomb interaction, which may result in a new ground state with unquenched OMM. The ion Fe 2+ (configuration d 6 ) possesses the lowest term 5 D in the intermediate CF and the configuration (e g ) 4 (t 2g ) 2 in the strong field (the case of the configuration (t2g) 6 is trivial). The corresponding interpolation scheme is shown in Fig.1.7. We see that in the intermediate CF quenching takes place only provided that the level 3 Γ 3 is lower. 15
Chapter 1
Fig.1.6. Interpolation scheme of levels for Ni 2+(d 8 ) ion in the crystal field. The numbers in brackets stand for degeneracy of a state.
Fig.1.7. Fragment of level scheme for Fe 2+(d 6 ) ion. Position of levels in the ground state corresponds to unquenched orbital momenta for both strong and intermediate CF. Unlike Fig.1.6, interpolation is not shown, since not all corresponding levels are included.
In the strong CF, the state 3 Γ 5 , corresponding to threedimensional t 2g representation, has an unquenched orbital quasimomentum. The examples considered demonstrate that, generally speaking, in the case of a high lattice symmetry a local CF results in only partial degeneracy lift which cannot provide total quenching of OMM. Even in the case where such a quenching does take place, OMM may be partially unquenched by the Coulomb interaction which has offdiagonal matrix elements between different point group irreducible representations, both for intermediate and strong CF cases, e.g., the matrix elements of the type 〈e g Qt 2g 〉 unquench OMM in the state e g . On the other hand, in the case of intermediate CF, offdiagonal matrix elements of the crystal field itself may mix different terms and unquench OMM of the ground state term. 16
Introduction Thus the local CF potential does not explain almost total quenching of OMM in transition metals and their alloys. The quenching mechanism owing to the periodic lattice potential will be considered in Sect.4.8.1. This potential results in an appreciable kinetic energy of delectrons. The formation of rather wide energy dbands leads also to destruction of localized spin momenta and suppression of magnetism in most dmetals. a
b 2presonant photoemission
Intensity, arb. units
Photon energy, eV
c
Final state Satellite
Fig.1.8. Resonance photoemission experiment on CuO (a) spectra with the photon energies sweeping to the point of the 2p resonance (b), the resonance intensity (c) and the number of spectra on the extended scale [47].
17
Chapter 1
A U ∆ T
= = = =
3.0 7.5 7.0 1.6
A = 3.9 eV U = 8.5 eV ∆ = 8.8 eV T = 2.2 eV
eV eV eV eV
Intensity, arb. units
Photoemission intensity, arb. units
The role of OMM effects in highlycorrelated dcompounds is debatable. Often the description of the electronic structure of Mott insulators (e.g, transition metal oxides and sulphides) is performed within the density functional approach, which does not take into account ME term structure [44, 45]. At the same time, there exist attempts of interpretation of their optical properties within a picture including spectroscopic terms with account of CF splitting [46, 13]. Detailed investigations of optical and Xray spectra (Sect.2.5), which contain information on selection rules in L, seem to be useful for solving these problems. It should be noted that the orbital contributions may be different for the configurations s(p)d n–1 and d n which are mixed by the crystal field. The resonance photoemission spectrum of CuO is shown in Fig.1.8. The resonance intensity allows the identification of the various atomic multiplets of the d 8 final state. Figures 1.9 and 1.10 [45] show a comparison of the XPS valence band spectra of MnO and NiO with the results of cluster calculations. The parameters of cluster calculations are shown in diagrams. One can see from Fig.1.10 the strong hybridization between the d 7 and d 8 L −1 final state.
Exp. XPS
Exp. XPS
Binding energy Fig.1.9. XPSvalence band spectrum of MnO and analysis of the spectra by cluster calculations of two groups [48,49].
18
Introduction Α = 6.60 eV ∆ = 6.2 eV T = 2.2 eV
1487 eV
h ν = 1486.6 eV
Intensity
∆ = 4.0 eV U = 7.5 eV T = 2.2 eV
U( 4 T 1) = 6.7 eV U( 2E) = 10 eV
Binding energy, eV Fig.1.10. Comparison of experimental XPS valence band spectra of NiO with the results of cluster calculations [50, 51].
19
Chapter 2
Chapter 2 BAND THEORY Band theory is now a large and rather independent branch of solid state physics, which uses the whole variety of modern computational methods. The corresponding problems are discussed in detail in a number of monographs and reviews [12, 13, 52–57]. Nevertheless, we include this material in the book with two main purposes (i) to consider in a simple form main band calculation methods bearing in mind their physical basis (ii) to concretize the advantages and drawbacks of various methods as applied to transition metals. Further we discuss the results of band calculations for TM and compare them with experimental data. Band theory deals with description of electron spectrum in a regular lattice with a periodic crystal potential, V (r ) = V (r + R ) = ∑υ (r − R ), R
where υ (r) is the potential of an ion, R are the lattice sites. According to the Bloch theorem, oneelectron states in a periodic potential may be chosen in the form
ψ nk (r ) = unk (r)eikr ,
(2.1) (r) and form a set
They are classified by the quasimomentum u nk of energy bands with the index n. At considering the band spectrum, two opposite approaches are possible. The first one starts from the picture of isolated atoms and uses the crystal potential of neighbour atoms as a perturbation, the intraatomic potential being taken into account in the zerothorder approximation. The simplest method of band calculations is the tightbinding method which uses oneelectron atomic wave functions φ γ (r). The corresponding wavefunctions of a crystal are written as
φγ k (r ) = ∑φγ (r − R )eikR . R
(2.2)
The band spectrum in this approximation contains a set of bands originating from atomic levels. In the case of the sband for the simple 20
Band theory cubic lattice in the nearestneighbour approximation we have Ek = ε s + 2 β (cos k x + cos k y + cos k z ),
(2.3)
β = ∫φ * (r )v (r )φ (r + a) dr.
(2.4)
where
is the transfer integral. The width of the energy bands is determined by the overlap of atomic wavefunctions at neighbour lattice sites and decreases rapidly for inner shells. As a rule, the bands, which originate from different levels, overlap considerably. Taking into account offdiagonal matrix elements and combining the atomic functions with γ ≠ γ ' we come to the method of linear combination of atomic orbitals (LCAO). This method was widely used in early band calculations. A version of this method was developed by Slater and Coster [58]. An important drawback of the LCAO method is nonorthogonality of atomic functions at different lattice sites (see Apendix C) and absence of delocalized states with positive energies in the basis. Thus it is difficult to describe weakly localized electron states in metals within this method. The opposite limiting case corresponds to the picture of nearly free electrons with a large kinetic energy, so that the whole periodic crystal potential may be considered as a perturbation which results in formation of gaps (forbidden bands) in the energy spectrum. Contrary to the tightbinding approximation, the strength of crystal potential determines the widths of gaps rather than of electron bands. Free electrons have the wavefunctions and the energy spectrum 2 k 2 . (2.5) 2m The matrix elements of the periodic lattice potential are given by
ψ k (r ) = eikr ≡  k 〉,
Ek =
〈k  V  k' 〉 = ∑Vgδ g
,
k − k' g
,
(2.6)
where g are reciprocal lattice vectors which are defined by gR = 2π n, n = 0, ± 1, … (2.7) For most values of k, corrections to the spectrum may be calculated to second order of perturbation theory ∆ Ek = ∑ g
 Vg 2 Ek − Ek −g
.
(2.8)
However, the denominators of the terms in (2.8) with E k = E k−g , i.e.
21
Chapter 2 (2.9) 2(kg) = g 2 , vanish and we have to calculate the spectrum with the use of the Brillouin–Wigner perturbation theory which yields E − Ek Vg
Vg* = 0, E − Ek − g
(2.10)
or 1/2
E=
1 1 ( Ek + Ek − g ) ± ( Ek − Ek − g ) 2 +  Vg 2 . 2 4
(2.11)
Thus we obtain the splitting of the spectrum with formation of the energy gap ∆ Eg = 2  Vg  .
(2.12)
The equation (2.9) just determines the boundaries of the Brillouin zone where the gaps occur. The nearlyfree electron approximation is applicable provided that the crystal potential is small in comparison with the bandwidth W. Since the matrix elements of crystal potential are of order of a few eV, this condition may be satisfied for external s and pelectrons with W ~ 10 eV. On the other hand, delectrons form more narrow bands and disturb considerably the conduction band because of s–d hybridization. Thus this approximation describes satisfactorily the conduction electron states in simple (in particular, alcaline) metals only. In most cases both above pictures are insufficient to obtain a quantitative description of the electron spectrum. Especially difficult is this problem for delectrons in transition metals, which are characterized by an intermediate degree of localization. It should be noted that the shortcomings of the simplest band calculation methods occur because of the approximate solution of the problem in any real calculations. Using an infinite full set either of localized or extended wavefunctions would in principle provide an exact result (of course, in the oneelectron approximation only). However, the use of a physically reasonable basis enables one to obtain much better results for a finite set. Evidently, the true wavefunctions should have an atomic character in the region near the lattice site and are close to plane waves in the outer space. Therefore modern methods of band calculations (e.g., the methods of augmented and orthogonalized plane waves), which are discussed briefly in the next sections, use combinations of atomic functions and plane waves. 22
Band theory The second difficulty of the band theory is connected with the problem of electron correlations, which are large for transition metals. The Coulomb interaction among electrons, which has a twoparticle nature and prevents reducing the manyelectron problem to the oneelectron one. In principle, the possibility of such a reducing is provided by the Hohenberg–Kohn theorem [59]. This theorem guarantees the existence of an unique density functional which yields the exact ground state energy. However, explicit constructing of this functional is a very complicated problem. In the situation, where correlations are not too strong, the Coulomb interaction may be taken into account by introducing a selfconsistent potential which depends on electron density. These questions are treated in Sect.2.3. The correlation effects are especially important for narrow d and fbands. The strong intrasite Coulomb repulsion may lead to splitting of oneelectron bands into manyelectron subbands, and the usual band description (even in the tightbinding approach) is inapplicable. In particular, in the case of one conduction electron per atom the Mott–Hubbard transition takes place with increasing interatomic distances, so that electrons become localized at lattice sites. In such a situation, we have to construct the correlation Hubbard subbands with the use of the atomic statistics and manyelectron quantum numbers (Appendices C, H). Development of firstprinciple band calculation methods in the manyelectron representation is an exciting problem. Such calculations might be based on a modification of the eigenfunctions of a spherically symmetric potential, which are used, e.g., in APW and OPW methods, by expressing them in terms of manyelectron functions of the atomic problem. In particular, the dependence of oneelectron radial functions on manyelectron quantum numbers S, L occurs in the full Hartree–Fock approximation (see Sect.2.3). Picking out the functions, which correspond to lowest (Hund) atomic terms should modify considerably the results of band calculations.
2.1 ORTHOGONALIZED PLANE WAVE METHOD AND PSEUDOPOTENTIAL The main shortcoming of the nearlyfree electron method is a poor description of strong oscillations of electron wavefunctions near atomic cores in terms of not too large a set of plane waves. This shortcoming is removed in the orthogonalized plane wave method (OPW) where the wavefunctions are chosen to be orthogonal with respect to core states:
23
Chapter 2
χ k (r ) = eikr + ∑bcφ kc (r ). c
(2.13)
where φ ck (r) are the tightbinding Bloch functions originating from the core levels. The condition
∫χ
k
(r )φ ck (r ) dr ≡ 〈 χ  c〉 = 0
(2.14)
yields bc = − ∫φ kc (r )e − ikr dr ≡ −〈k  c〉.
(2.15)
The orthogonalized plane wave (2.13) oscillates rapidly near atomic nucleus and is close to the plane wave between the atoms. The trial wavefunction of the crystal is chosen as a superposition of OPW:
ψ k = ∑αk −g χ k −g
(2.16)
g
(g are reciprocal lattice vectors). The coefficients α are determined from the Schrödinger equation. The matrix elements of the crystal potential for OPW (unlike those for plane waves) turn out to be small, so that it is sufficient to take in the expansion (2.16) not too many terms. It should be noted that the OPW basis is overfilled so that the increasing the number of functions in the set does not necessarily increase the accuracy of calculations. Further development of the OPW method led to the idea of introducing a weak pseudopotential which permits (unlike the real crystal potential) the use of perturbation theory. To this end one introduces the pseudowavefunction
ψ k = ∑αk −g ei (k −g )r = ψ k + ∑〈c  ψ 〉φ kc , g
c
(2.17)
which coincides with the true wavefunction outside the core region but does not exhibit oscillations, which are due to strong core level potential, within it. Substituting (2.17) into the usual Schroedinger equation H ψ = E ψ we get Hψ k + ∑ ( E − Ec )〈c  ψ 〉φ kc = Eψ k , c
(2.18)
which may be represented in the form of a new Schrödinger equation
2 ∆ + W ψ k = Eψ k . − (2.19) 2m where the nonlocal energydependent pseudopotential operator W is defined by
W = V (r ) + V R ; 24
(2.20)
Band theory V Rψ k (r ) = ∑ ( E − Ec )〈c  ψ 〉φkc . c
(2.21)
For E > E c , the matrix elements of the potential V R
∫ψ
* k
(r )V Rψ k (r ) dr = ∑( E − Ec )  〈c  ψ 〉 2 c
(2.22)
are positive. At the same time, the matrix elements of the true periodic potential V are negative and large in the absolute value in the core region. Thus the diagonal matrix elements of W turn out to be positive and small because of partial cancelation of two terms in (2.20). In particular, the pseudopotential does not result, unlike the real crystal potential, in formation of bound states, corresponding to core levels. Therefore the pseudopotential method describes conduction electron states only. Generally speaking, the pseudopotential approach is not simpler than the original OPW method since it requires introducing a nonlocal potential function which is not defined in a unique way. Therefore one uses frequently empirical or model local pseudopotentials which are fitted to experimental data, rather than firstprinciple ones. Perturbation theory with the use of such potentials enables one to describe the whole variety of properties of simple metals [55]. The standard form of the pseudopotential theory is inapplicable both in noble and transition metals because delectrons are much stronger localized than s, pelectrons. To describe delectron states one introduces into (2.17) the contribution from functions [9]  ψ 〉 = ψ 〉 − ∑ 〈c  ψ 〉  c〉 + ∑ad  d 〉,
(2.23) ∼ where, as well as for simple metals, the pseudowavefunction ψ is a linear combination of plane waves. One has to take into account the difference between potentials of free ion and of ion in a crystal, c
d
δ v(r ) = υ ion (r ) − υ (r). Define the operator V h by
V h  d 〉 = δ v  d 〉−  d 〉〈d  δ v  d 〉.
(2.24)
Then we obtain ad = −〈 d  ψ 〉 +
〈d  V h  ψ 〉 , Ed − E
and the Schrödinger equation for the pseudowavefunction takes the form
25
Chapter 2
2 V h  d 〉〈 d  V h  ψ 〉 W − ∆ + 〉 +  ψ = E  ψ 〉, ∑d (2.25) E − Ed 2m where the pseudopotential operator of the transition metal is given by W  ψ 〉 = V  ψ 〉 +
∑ ( E − E )  i〉〈i  ψ 〉 + ∑( d 〉〈d  V i
i =c,d
h
 ψ 〉 + V h  d 〉〈d  ψ 〉). (2.26)
d
The most important peculiarity of Eq.(2.25) is the presence of the terms, which have a resonance denominator E−E d. The physical origin of this is as follows. As discussed in Sect.1.1, the atomic potential for delectrons may have a centrifugal barrier where υ (r) is positive. Therefore there exist bound dlevels merged in the continuous spectrum. The strong scattering of continuous spectrum electron by localized levels takes place with the phase shift of π /2. Such a situation may be also described by the s–d hybridization model. The corresponding energy spectrum is strongly distorted and should be calculated by exact diagonalization which yields 1/2
1,2 k
E
2 1 2 k 2 1 2 k 2 + Ed ± − Ed +  Vkh 2 . = 2 2m 4 2m
(2.27)
Far above the resonance the hybridization potential may be considered, as well as the usual pseudopotential, within the framework of perturbation theory. This permits a satisfactory description within the modified pseudopotential approach [60] of noble metals where the dresonance, although crossing conduction band, lies well below E F . In transition metals the resonance lies near the Fermi energy and perturbation theory is inapplicable. Thus one has to pick out the singularity, corresponding to the resonance. A method of completely orthogonalized plane waves [61], application of which to transition metals is discussed in [57, 62], gives in principle a possibility to eliminate this difficulty. However, this method is rather complicated and goes far beyond the original concept of the OPW method. Generally, such approaches require in a sense exact diagonalization of a matrix and lose in fact the main advantage of the pseudopotential idea – applicability of perturbation theory. More recent applications of the pseudopotential method for band calculations of transition metals are considered in [63, 64]. There exist a number of model pseudopotential forms, in particular including explicitly the dresonance. However, they do not provide as a rule sufficiently satisfactory description of TM. Recently a model
26
Band theory pseudopotential was successfully applied to explain properties of iridium [65]. The reasons of the good fit to experimental data for this particular dmetal are not quite clear.
2.2 AUGMENTED PLANE WAVE (APW) AND KORRINGA–KOHN–ROSTOKER (KKR) METHODS The idea of other modern band calculation methods is to describe electron states in different space regions in a proper way using different bases. To this end, one builds around each site an atomic sphere with the volume which is somewhat smaller than that of the lattice cell, so that spheres centered at different sites do not overlap. The crystal potential at each site is taken in the socalled muffintin (MT) form
v(r ), r < rMT , vMT (r ) = (2.28) vc , r > rMT . Inside the sphere the potential is supposed to be spherically symmetric, and the corresponding wavefunctions for a given energy may be expanded in spherical harmonics
φ (r ) = ∑Clm Rl (r , E )Ylm (rˆ ), r < rMT lm
(2.29)
(R l are the solutions of the corresponding radial Schrödinger equation) which permits to simplify greatly the calculations due to using the angular momentum technique. Since beyond the spheres the MT potential is constant, the basis wavefunctions φ (r) may be chosen in the form of plane waves. Using the expansion (C.28) we may join continuously the solutions at the∧ sphere boundaries and determine the coefficients C lm = C lm (k)
jl (krMT ) * ˆ Ylm (k ). Rl (rMT , E )
Clm = i l (2l + 1)
(2.30)
Then the function (2.29) is called the augmented plane wave (APW). The wavefunction of the crystal are searched as a linear combination of APW’s with the same energy:
ψ k (r ) = ∑α k −gφk −g (r ). g
(2.31)
Substituting (2.31) into the Schrödinger equation one obtains the system of linear equations. Poles of its determinant yield the dispersion law E(k) which contains the crystal potential in a compli
27
Chapter 2 cated way. To obtain accurate results, it is sufficient to restrict oneself by not too large number of terms in (2.31). Practically, one uses up to 100 APW’s, and for a larger set the solution is as a rule stabilized. The application of the APW method to dbands requires an account of a larger number of APW’s in comparison with, s,pbands. However, such band calculations were performed for all the transition dmetals [53, 54]. For 4d and 5dmetals, relativistic effects (in particular, spinorbital interaction) are important. The corresponding version of the APW method (the RAPW method) was developed by Loucks [66]. The Green’s function method, developed by Korringa, Kohn and Rostoker (KKR), uses, as well as APW method, the expansion in spherical functions inside the MT spheres (2.28). At the same time, the wavefunctions outside them are constructed not from plane waves, but also from spherical waves which are scattered from other sites. Formally, this is achieved by using the integral form of the Schrödinger equation ( κ = E 1/2 ) 1 exp (iκ  r − r ′ ) V (r′)ψ (r ′) dr ′. 4π ∫  r − r′  Using the Bloch theorem condition
ψ (r ) = −
(2.32)
ψ k (r + R ) = ψ k (r )eikR , one reduces (2.32) to the form
1 Gk (r − r ′, E )v(r′)ψ k (r ′) dr′, 4π ∫ where the integration goes over one lattice cell and
ψ k (r ) = −
Gk (r , E ) = ∑ R
exp(iκ  r − R ) ikR e . r − R 
(2.33)
(2.34)
is the lattice Green’s function. The functional describing the system and corresponding to (2.33) has the form
1 ψ k* (r )v(r )Gk (r − r′, E )v(r ′)ψ k (r′) dr dr ′. 4π ∫∫ Substituting (2.29) into (2.35) yields [52] Λ = ∫  ψ k (r ) 2 dr + Λ=
∑ (A
lm , ll 'm'
+ κδ δ ll '
lm , l 'm'
mm '
cot ηl )Clm C ' ' . lm
(2.35)
(2.36)
Here η l is the ldependent phase shift owing to the MTpotential,
28
Band theory cot ηl =
κ rMT nl′ (κ rMT ) − Dl ( E )nl (κ rMT ) , κ rMT jl′ (κ rMT ) − Dl ( E ) jl (κ rMT )
(2.37)
where j i and n l are the spherical Bessel and Neumann functions, (2.38) Dl ( E ) = rMT Rl′ (rMT , E )/Rl ( rMT , E ). are the logarithmic derivatives of the radial wave function. The energy spectrum is determined by zeros of the determinant of the matrix Λ. The structural constants A are given by ˆ )C l ′m′′′ ′′ Alm ,l ′m′ = 4πκ ∑eikR ∑[nl ′′ (κ R ) − ij '' (κ R )]Y ''* '' (R lm ,l ,m R≠0
l
l'' m′′
l m
(2.39)
~
(the quantities C are defined in (C.9)). These constants do not depend on crystal potential and may be calculated once for all for a given lattice. The advantage of the KKR method in comparison with the APW one is the decoupling of structural and atomic factors. For the same lattice potentials, the KKR and APW methods yield usually close results. The intimate relation of these methods is discussed in [52]. The main difficulty of the KKR method is the energy dependence of the structural constants. However, this dependence may be eliminated if we use so called atomic sphere approximation (ASA) where the volume of the sphere in the MT potential (2.28) is put to be equal to the lattice cell volume, rMT = s, so that the volume of the intersphere region vanishes. Then one puts for simplicity the kinetic energy beyond the atomic spheres, E− υ c to be zero, and the ASA–KKR equations take a very simple form [56]
det  Slm,l ′m′ (k ) − Pl ( E )δ ll ′δ mm′  = 0, where the potential function is given by Pl ( E ) = 2(2l + 1)
Dl ( E ) + l + 1 , Dl ( E ) − l
(2.40)
(2.41)
and the structural constants are energy independent, Slm,l ′m′ (k ) = (4π )1/2 (−1)m′+1 (−i )λ ×
(2l ′ + 1)(2l + 1) × (2λ + 1)
(λ + µ )!(λ − µ )! ∑eikRYλµ* (Rˆ )( s/R)λ +1 , (l ′ + m′)!(l ′ − m′)!(l + m)!(l − m)! R ≠ 0
(2.42)
where
λ = l + l' ,
µ = m − m' .
The wavefunctions corresponding to the MTpotential with zero kinetic 29
Chapter 2 energy E− υ c may be chosen in the form
φlm (r, E ) = i l Ylm (rˆ )φl (r , E ),
(2.43)
r < s, 1, l − l −1 φl (r , E ) = Rl (r , E ) Dl + l + 1 r l − Dl r + , r > s. 2l + 1 s 2l + 1 s
where the coefficients are determined from the condition of joining the tail continuously and smoothly at the boundary of the MTsphere. It is convenient to subtract the term which describes the diverging spherical wave. Then we obtain the socalled MTorbitals
φl (r , E ) Dl + l + 1 r l − , r < s, 2l + 1 s φl ( s , E ) χ l ( r , E ) = φl ( r , E ) − l −1 l − Dl r r > s. 2l + 1 s ,
(2.44)
Condition of cancelation of tails of the MT orbitals, which originate from other sites, leads again to the KKR equations. A modification of LCAO method which uses instead of atomic functions the MTorbitals is called the LCMTO method, the linear combinations of MTorbitals being constructed similar to (2.1). Substituting these trial functions into the Schrödinger equation we obtain the LCMTO equations [67]. In the general APW, KKR and LCMTO methods the matrix elements are functions of energy. Therefore, at calculating eigenvalues one has to compute the determinants in each point of kspace for a large number values of E (of order of 100) which costs much time. To simplify the calculation procedure Andersen [67] proposed to expand the radial wavefunctions at some energy value to linear terms in E. Then the Hamiltonian and overlap matrices do not depend on energy. The error owing to the linearization does not as a rule exceed that owing to the inaccuracy in the crystal potential (in particular, owing to the MTapproximation). The accuracy may be increased by account of higherorder terms in the expansion. The linear methods (LMTO and LAPW) permitted to perform band calculations of a large number of transition metal compounds with complicated crystal structures [57]. Using the MTorbital basis gives a possibility to carry out band calculations beyond MTapproximation for the potential itself. Such an approach (the fullpotential LMTO method) enables one to 30
Band theory improve considerably the accuracy of calculations. Very good results are achieved also within the framework of the fullpotential LAPW method [68].
2.3 THE HARTREEFOCKSLATER AND DENSITY FUNCTIONAL APPROACHES TO THE PROBLEM OF ELECTRON CORRELATIONS The above consideration of the electron spectrum was performed within the oneelectron approximation. Main purpose of the calculation methods discussed was joining of atomiclike solutions near the lattice sites with wavefunctions in the outer space where the crystal potential V(r) differs strongly from atomic one. The Coulomb interaction among conduction electrons was assumed to be included in V(r). Such an inclusion should be performed in a selfconsistent way. In the simplest approximation, this may be achieved by introducing into the Schrödinger equation the averaged Coulomb potential,
2 ∆ + V (r ) + VC (r ) ψ i (r ); 2m
ε iψ i (r ) = − VC (r ) = −e ∫
ρ (r ′)  r − r′ 
ρ (r ) = −e∑'  ψ i (r ) 2 ,
d r ′,
(2.45)
(2.46)
i
where the sum goes over occupied electron states and integration includes summation over spin coordinate. The Hartree equations (2.45) do not include the exchange interaction which results from antisymmetry of electron wavefunctions. Substituting the antisymmetrized product of oneelectron wavefunctions (Slater determinant) (A.2) in the Schrödinger equation for the manyelectron system with the Hamiltonian (C.1) and minimizing the average energy E = 〈Ψ  H  Ψ〉 / 〈Ψ  Ψ〉, we obtain the Hartree–Fock equations 2 ∆ + V (r ) + VC (r ) ψ i (r ) − 2m
ε iψ i (r ) = −
ψ j (r ′)ψ i (r ′) δ σ i σ j dr ′, − e ∑'ψ j (r ) ∫  r − r′  j *
2
(2.47)
where ε i are the Lagrange multipliers. The exchange term (last term in the lefthand side of (2.47)) has a nonlocal form, i.e. is not reduced to multiplication of the wavefunction ψ i by a potential function. It
31
Chapter 2 should be noted that the terms, describing the electron selfinteraction (i = j) are mutually cancelled in the Coulomb and exchange contributions to (2.47). Due to orthogonality of spin wave functions, the exchange interaction occurs between electron with parallel spins only. Parameters of the Hartree–Fock equation depend, generally speaking, not only on oneelectron quantum numbers, but on the whole set of manyelectron quantum numbers in a given state. For example, in the manyelectron atom, the coefficients at the Slater parameters (except for F 0) in the multipole expansion of the Coulomb interaction (C.19) depend explicitly on the manyelectron SLterm. This results in the dependence of the radial wavefuctions on the quantum numbers S,L. The corresponding expression for the parameters ψ i may be represented as [20] 2 ε l = E (l n SL) − ∑ ( GSSL′L′ ) E (l n −1S ′L′' ). S ′L ′
(2.48)
~
where E is the energy of the ‘frozen’ ion with the same radial functions as the nelectron atom, G are the fractional parentage coefficients. ~ Evidently, E exceeds the energy of the true ion, which is calculated from the Hartree–Fock equation. In systems with large number of ~ electrons N the differences E–E may be neglected since they give corrections of order of 1/N only [9]. The quantity (2.48) differs from the energy, measured in spectral experiments
ε l ( SL, S ′L′' ) = E (l n SL) − ∑E (l n −1S ′L′), S ′L'
(2.49)
which corresponds to a concrete transition SL→S'L' (experiments with not too high resolution yield the Lorentz broadening which differs from (2.48)). In the band theory the dependence on ME quantum numbers is usually neglected. Then the parameters ε i have the meaning of oneelectron energies, – ε i being equal to the ionization energy of the corresponding state in the crystal (the Koopmans theorem [9]). Obviously, the Koopmans theorem is inapplicable for partially filled shells in transition metals where the energy of a level depends essentially on filling of other states (see Sect.1.1). The selfconsistent field method, which considers oneelectron levels only, does not take into account such correlation effects. Nevertheless, simple averaged exchangecorrelation potentials, expressed in terms of electron density, are widely used to calculate electron structure of partially filled dbands in transition metals. When applied to free atoms, this approach yields atomic levels with a noninteger filling. Although not quite physically correct, such 32
Band theory a picture permits a satisfactory description of atomic and molecular spectra [69]. To calculate the energy of optical transitions, one takes the selfconsistent potential calculated in the socalled transition state which corresponds to the level filling of 1/2. The solution of the Schrödinger equation with a nonlocal potential resulting from the exchange interaction is a very complicated problem. The case of free electron may be considered analytically. Performing the integration for plane waves we obtain from (2.46)
2 k 2 + Vx (k ) ψ k (r ) 2m
ε kψ k (r ) =
(2.50)
with the local exchange potential 1/3
3 Vx (k ) = −8 ρ F (k/kF ), 8π where ρ = N/V is the electron density,
(2.51)
1 1 − z2 1 + z ln . + (2.52) 2 4z 1− z The logarithmic singularity in F(z), and, consequently, in the electron spectrum results in a nonphysical behaviour of the density of states near the Fermi level, N(E → E F ) → 0. This singularity is due to the longrange character of the Coulomb interaction and should be in fact removed by correlation effects which result in screening. Thus the Hartree–Fock approximation turns out to be insufficient to describe the free electron gas because of the strong kdependence. To avoid this difficulty Slater [69] proposed to use the potential which describes the motion of an electron in an averaged exchange field. The exchange potential for a given state may be represented in the form F ( z) =
ψ i* (r )ψ *j (r ′)ψ j (r )ψ i (r ′) Vxi (r ) = −e ∑ σ σ ∫ [ψ i* (r )ψ i (r )] dr ′. (2.53) i j  r − r′  j The expression (2.53) may be interpreted as the potential of a charge with a value of e which is removed from the hole surrounding the ith electron. We may write for the averaged potential 2
Vx (r ) = −e
2
'δ
∫∑ δ σ σ '
ij
i j
ψ i* (r )ψ *j (r ′)ψ j (r )ψ i (r′)  r − r′ 
33
dr ′
∑ψ '
i
* i
(r )ψ i (r ). (2.54)
Chapter 2 Averaging the freeelectron gas potential (2.51) over k we obtain 1
F = ∫F ( z) z 2 dz 0
1
∫z 0
2
3 dz = ; 4
(2.55)
1/3
3 Vx = −6 ρ . (2.56) 8π Starting from the expression (2.56), Slater introduced the local exchangecorrelation potential with the same dependence on electron density 1/3
3 VxS (r ) = −6 ρ (r ) . (2.57) 8π An alternative approach to the problem of constructing exchangecorrelation potential [70] uses the calculation of the total energy. Carrying out the integration of oneelectron energy for the electron gas one obtains 2k 2 1 E = 2∑ + Vx ( k ) = 2 k < kF 2 m =
e2 2 aB
3 0.916 3 2.21 2 − Ry, 2 5 ( k F aB ) − 2π k F aB = rs a B ( rs aB )
(2.58)
where Ry = e 2 /2a B = 13.6 eV, 1/3
3 rs = (2.59) 4πρ is the radius of the sphere with the volume which corresponds to one electron for a given uniform density ρ . When measured in the units of Bohr radius a B , r s is of order of the ratio of potential energy of an electron to its mean kinetic energy. The second summand in (2.58), which comes from the exchange interaction, is comparable with the first one for realistic metallic values r s = 2−6. In the highdensity limit the problem of the electron gas may be treated more rigorously by expanding ε in r s [12]: 2.21 r r 0.916 − + 0.622ln s − 0.096 + O s Ry. (2.60) E= 2 rs /aB aB aB (rs /aB ) The corrections in (2.60) describe correlation effects beyond the HartreeFock approximation. Taking into account the exchange energy of the uniform gas per particle and neglecting correlations we obtain the Gaspar–Kohn– 34
Band theory Sham exchange potential [70] 1/3
3 VGKS (r ) = −4 ρ (r ) . (2.61) 8π This potential differs from the Slater approximation (2.57) by a factor of 2/3. This fact is due to that the operations of varying the total energy and of statistical averaging do not commute. The expression (2.60) may be also obtained from the potential (2.51) by putting k = k F (F = 1/2). A more general exchangecorrelation potential (x α potential) may be written as
(2.62) Vxα (r ) = VxS (r ). The optimization of the parameter α < 1 enables one to take into account effects of electron correlations. The potential (2.61) was successfully applied for calculations of electron structure of large number of solids [69,57]. However, the reasons of this success were not clear until the density functional method was developed. The results of xαcalculations for pure metals turn out to be not too sensitive to the choose of α . Earlier calculations with α = 1 yielded results, which agreed satisfactory with experimental data and are close to those for optimal α . This is apparently due to that the error in the total energy for α = 1 is partially compensated by increasing the depth of the potential well. However, the correct choose of α is important for metallic and insulating compounds. For transition metals the atomic densities are usually taken for d n−1 s configuration in the 3d and 4dseries and for the d n − 2 s 2 configuration in the 5dseries, the optimal values of α lying in the interval 0.65÷0.8. An important step in the theory of electron correlations in solids was made by Hohenberg and Kohn [59] who proved the general theorem, according to which the ground state energy is an unique functional of electron density. Kohn and Sham [70] represented this density functional (DF) in the form
E[ ρ (r)] = ∫ρ (r)Vext (r)dr + +
1 ρ (r) ρ (r′) + T [ ρ (r)] + Exc [ ρ (r)] d r dr′. ∫∫ 2  r − r′ 
(2.63)
where V ext is the external potential of lattice ions, T is the kinetic energy of noninteracting electrons with the density ρ , the functional ε xc corresponds to exchange and correlation contributions. The DF approach may be generalized to consider spinpolarized systems. 35
Chapter 2 Representing the electron density in the form (2.46) and varying (2.63) with respect to ψ i we obtain
2 ∆ + Vext (r ) + VC (r ) + Vxc (r ) ψ i (r ), 2m
ε iψ i (r ) = −
(2.64)
where the Lagrange multipliers ψ i correspond to the quasiparticle energies, the exchangecorrelation potential V xc is defined by varying ε xc with respect to density, (2.65) Vxc (r ) = δ Exc [ ρ (r )]/δρ (r ). Thus the manyelectron problem is reduced to the oneparticle one with the local exchangecorrelation potential. However, it should be stressed that the DF approach guarantees the correct value of the ground state energy only and describes exactly the distribution of charge and spin densities and related physical quantitities. Here belong elastic characteristics and exchange parameters, which are expressed in terms of corresponding energy differences, saturation magnetic moment etc. On the other hand, the Kohn–Sham quasiparticles do not coincide with true electrons, so that the wavefunctions ψ i do not have a direct physical meaning. Therefore the possibility of calculation of the whole excitation spectrum is, generally speaking, not justified. Especially doubtful is the description of the states far from E F and of finite temperature behaviour. Nevertheless, the DF method is widely used to consider various physical properties. The true functional (2.63) is of course unknown, and one has to use some approximations. The formally exact expression for ε xc may be represented in the form of the Coulomb interaction of an electron with the exchange–correlation hole which surrounds it:
ρ (r, r′ − r) 1 ρ (r) xc dr dr′. (2.66) ∫∫ 2  r − r′  The corresponding electron density may be obtained by integration over the coupling constant λ [71,72] Exc [ ρ (r)] =
1
ρ xc (r, r ′ − r ) = ρ (r ′) ∫[ g (r, r ′, λ ) − 1]d λ ,
(2.67)
0
where g is the pair correlation function. Since the hole contains one electron, the charge density should satisfy the sum rule
∫ρ
xc
(r, r′ − r ) dr′ = −e.
(2.68)
The functional ε xc depends in fact on the spherically averaged charge density, which follows from the isotropic nature of the Coulomb
36
Band theory interaction [72]. Indeed, the variable substitution in (2.66) allows to perform integration over angles of the vector r − r':
Exc =
ρ (r , R) 1 ρ (r) R 2 xc dr dR, ∫∫ 2 R
ρ xc (r , R ) = ∫ρ xc (r, R ) d Ω.
(2.69)
Thus approximate expressions for ε xc can give exact results even if the detailed description of ρ xc (in particular, of its nonspherical part) is inaccurate. Further we have to concretize the form of the correlation function. In the local density approximation (LDA), which is used as a rule in band calculations, ρ xc is taken in the same form, as for uniform electron density with the replacement ρ → ρ(r) and the corresponding correlation function g 0 : 1
ρ xc (r , r′ − r ) = ρ (r ) ∫[ g 0 ( r − r ′ , λ , ρ (r )) − 1]d λ .
(2.70)
0
Substituting (2.70) into (2.69) we obtain the LDA functional, which has the local form Exc [ ρ ] = ∫ρ (r )ε xc ( ρ ) dr,
(2.71)
where ε xc is the exchange and correlation energy per electron for the interacting uniform electron gas. This quantity was calculated numerically to a high accuracy and various interpolation analytical formulae are available. Therefore the LDF approach enables one to construct various local exchangecorrelation potentials. The simplest exchange potential is given by the x α expression (2.61). This expression may be generalized as (2.72) Vxc (r ) = β ( rs /aB )VGKS (r ). Thus the xα method becomes justified in the density functional theory, the parameter α being dependent of electron density. The value of α changes from 2/3 to 0.85 as r s increases from zero (highdensity limit) to values which are typical for metals in interatomic region (r s /a B = 4). An example of an interpolation approximation is the Hedin–Lundqvist potential [73] which corresponds to (2.73) β HL ( z ) = 1 + 0.0316 z ln(1 + 24.3/z ). The functional of local spin density (LSD) approximation which is applied to consider magnetic transition metals reads Exc [ ρ↑ , ρ↓ ] = ∫ρ (r )ε xc ( ρ↑ (r ), ρ↓ (r )) dr.
37
(2.74)
Chapter 2 The simplest LSDA von Barth–Hedin potential [74] has in the first order in spin polarization m(r) = n ↑ (r) − n ↓ (r) the form
m(r ) 1 Vxcσ (r ) = σδ (n) VGKS (r ), 3 n(r )
(2.75)
where n(r) = n ↑ (r) + n ↓ (r) and the parameter δ takes into account correlation effects. In the highdensity limit δ = 1, and δ = 0.55 for r s = 4. The LD approximation oversimplifies greatly the general DF approach which is based on the Hohenberg–Kohn theorem. In particular, LDA does not take into account correctly the dependence of ρ xc (r, r') on ρ (r) in the whole space (compare (2.67) with (2.70)). However, it provides good results in the case of a slow varying density ρ (r). Besides that, this approximation works well in the highdensity limit since it includes correctly the kinetic energy of the noninteracting system. In the original papers [70], attempts were made to take into account nonuniform corrections to LDA by expanding ρ xc with respect to grad ρ (r). However, such an expansion yields small contributions only and does not hold in the case of strongly nonuniform electron systems (e.g., for 4felectrons in rare earths and narrow dbands), and is therefore, strictly speaking, not justified for TM. Other modifications of LDA are discussed in the review [72]. The problem of account of multiplet structure in the density functional approach is treated in [75,76]. One of drawbacks of LDA is the inexact (unlike the full HartreeFock approximation) cancelation of the unphysical interaction of an electron with itself. In this connection, the socalled selfinteraction correction (SIC) approach [72] was developed. The SIC functional within the LSDA reads ESIC = ELSD [ ρ↑ (r ), ρ↓ (r )] − ∑δ Eiσ . iσ
(2.76)
The subtracted SI correction for the orbital i σ has the form
1 ρiσ (r) ρiσ (r′) dr dr′ + Exc [ ρiσ ,0], (2.77) 2 ∫∫  r − r′  where the first term is the selfinteraction energy, and the second term is the LSD approximation to the exchangecorrelation energy of a fully spinpolarized system with the density ρiσ(r). The functional (2.76) is exact for a system with one electron. The SI corrections are negligible for planewavelike states due to smallness of ρ i σ (r).
δ Eiσ =
38
Band theory However, they may be important for description of strongly localized states. The SIC approach was successfully applied to model systems with Hubbard correlations and to transitionmetal oxides [72, 77, 100].
2.4 DISCUSSION OF BAND CALCULATION RESULTS
Density of states, at –1 ·Ry –1
Band structure calculations yield the whole picture of electron spectrum of a given substance. The corresponding dependences E(k) and densities of states may be found in [24, 78]. The calculations of [24] are performed for cubic symmetry only. Besides that, the 5dmetals are omitted since they require relativistic methods. In the handbook [78], real crystal structure for all the transition metals was taken into account. The Slater–Coster parametrization of the band spectrum was applied, the basis containing t 2g and e g states being used even for metals with the hexagonal structure. Bibliography on earlier band structure calculations is given in Sect.2.7 (see Table 2.6). Some examples of densities of states for transition metals are shown in Figs.2.1–2.7. The real accuracy of the detailed and complicated information on the electron spectrum turns out often to be in fact insufficient. Therefore it is instructive to consider some general characteristics of band spectra (classification and widths of energy bands, position of the Fermi level, the value of the density of states N(E F)) within simple model concepts.
Energy, Ry Fig. 2.1. Total density of states for titanium [159]. 39
Chapter 2 Energy, eV
Density of states, Ry –1
Density of states, eV –1
Total density of states
Energy, Ry Fig. 2.2. Total and partial densities of states for zirconium [78].
The KKR method gives a possibility to separate the structural and dynamical aspects of the band structure. Using the atomic sphere approximation, which is discussed in Sect.2.2, enables one to obtain socalled canonical bands which depend on the crystal structure only. These bands are obtained by neglecting offdiagonal structural constants with l ≠ l' in the KKR equations (2.40), considering the potential functions P l(E) as independent variables and diagonalizing the matrix S lm,l'm'(k) for each value of l. Then for the set n, l we get 2l+1 nonhybridized energy bands E ni (k) defined by (2.78) Sli (k ) = Pl ( E ), i = 1, 2, … , 2l + 1. The canonical bands S l(k) for the bcc, fcc and hcp lattices are shown in Figs.2.8–2.10, and the corresponding densities of states in Fig.2.11. Because of the infinite range of stype MTorbitals, a pure canonical 40
Band theory Energy, eV
Density of states, eV –1
Total density of states
Energy, Ry
Density of states, eV –1
Integral density of states
Fig. 2.3. Total and partial densities of states for hafnium [78].
Energy in relation to Fermi energy, eV Fig.2.4. Total and partial densities of states for vanadium [78]. 41
Chapter 2 Energy, eV
Density of states, eV –1
Density of states, Ry –1
Total density of states
Energy, Ry Fig. 2.5. Total and partial densities of states for chromium [78].
sband diverges at the centre of the Brillouin zone,
Ss (k ) → −6(ks ) −2 + const. Therefore one has to use in Figs.2.8–2.10 the freeelectronlike scale [1−(2/ π ) 2S s] −1 . The width of a canonical band is estimated from the second moment: W = (12S 2 )1/2 , l
Sl2 =
l
1 2l +1 ∑∑Sli2 (k ) = 2l + 1 i =1 k = 2l + 2 (2l + 1)
(4l − 1)!! ∑ (s/R)2(2l +1) l!(2l )! R ≠ 0
(2.79)
and depends only on the number of atoms in coordination spheres. For the bcc, fcc and ideal hcp lattices one has respectively W = 18.8, 18.7, 18.6; p
42
Band theory Energy, eV
Density of states, Ry –1
Density of states, eV –1
Total density of states
Energy, Ry Fig. 2.6. Total and partial densities of states for rhodium [78].
Wd = 23.8, 23.5, 23.5. The canonical bands may provide a basis for further analysis of the band structure. They reflect an important experimental fact: resemblance of band structures of crystals with the same lattice. Real energy bands for various elements are obtained from the canonical bands by specifying the functions P l (E). The hybridization of bands with different l does not influence strongly the spectrum provided that the bands do not cross each other. However, for crossing s,p,dbands in transition metals the hybridization may lead to qualitative changes. Consider the problem of the shape of energy bands, in particular the origin of peaks in the density of states N(E). As follows from the formula N ( E ) = ∫δ ( E − Ek ) dk = ∫
dS ,  grad k Ek 
(2.80)
a peak of N(E) corresponds to a nearly flat region (e.g., extremum) 43
Chapter 2 Energy, eV
Density of states, eV –1
Density of states, Ry –1
Total density of states
Energy, Ry Fig. 2.7. Total and partial densities of states for platinum [78].
of the surface E(k) with a constant energy in the kspace. Such peculiarities of the spectrum occur in the onedimensional case where dE/dk = 0 at the boundaries of the Brillouin zones. As a result, DOS has divergences of the form (2.81) N ( E ) = E − Eb −1/2 . According to the Van Hove theorem, in the general situation, DOS singularities (divergence of N(E) or N'(E)) occur at some points E c by topological reasons. In the twodimensional case, these singularities are logarithmic. The N(E) pictures demonstrating the Van Hove singularities were obtained for simple cubic, fcc and bcc lattices for an sband in the nearestneighbour approximation [79] (Figs.2.12, 2.13). The divergence of DOS at the band centre in the bcc lattice and the logarithmic singularity in the fcc lattice at the band bottom are removed when one includes nextnearest neighbours (Fig.2.14). Thus in the threedimensional case the usual Van Hove singularities
44
Band theory
Fig. 2.8. The nonhybridized canonical bands for the fcc lattice [56].
have as a rule the onesided squareroot form
δ N ( E ) = E − Ec 1/2 θ (±( E − Ec ))
(2.82) and are too weak for explaining sharp DOS peaks. However, the peaks may form at merging of Van Hove singularities along some lines in the kspace. As demonstrated in [81], this leads to twosided logarithmic singularities (2.83) δ N ( E ) = − ln  E − Ec  . As follows from analysis of calculations [24,78], the merging along the P–N line in the bcc lattice results in formation of the ‘giant’ Van Hove singularities (2.83) in Li, V, Cr, Fe, Ba [81]. A similar situation takes place for fcc Ca and Sr. Some peaks in the canonical DOS’s may be identified with the Van Hove singularities. Despite a general similarity, the DOS, obtained in realistic band calculations, contain a more number of peaks than canonical DOS’s. The additional peaks in calculated DOS pictures, which take into account offdiagonal matrix elements (hybridization) between s,p,dbands, may be connected with splitting of a peak at the band intersection. 45
Chapter 2
Fig. 2.9. The nonhybridized canonical bands for the bcc lattice [56].
A comparison of canonical bands with real band calculations which take into account hybridization is performed in the review [56]. The effect of hybridization turns out to depend strongly on the mutual position of the bands. As an example, Fig.2.15 shows the density of dstates for Nb. The effect of p–d hybridization is weak since p and dband are well separated. The s–d hybridization effect is more appreciable since s and dbands overlap (as well as in other transition metals). However, the sband is influenced stronger than the degenerate dband with a large electron capacity. Another typical example is provided by molybdenum where the splitting of some peaks occurs due to s–d hybridization (Fig.2.16) [82]. Now we discuss the position and width of energy bands. These characteristics of band structure may be investigated either by direct using results of numerical calculations or by parametrization within simple models which neglect unimportant details. The latter approach permits to obtain a more clear physical picture and to treat the problem analytically. The simplest model of transition metals is the Friedel model [83] which considers their electron system as containing free selectrons 46
Band theory
Fig. 2.10. The nonhybridized canonical bands for the ideal hcp lattice [56].
and the narrow dband with the constant density of states of 10/W d . The lowering of electron energy at formation of the dband from the level is given by the expression
δ Eband
nd nd 2 = 5Wd − + . 10 10
(2.84)
A model description of band spectrum was proposed by Harrison [13]. Using the set of one sfunction and five dfunctions in the form 47
Chapter 2
Density of states
BCC
FCC
HCP
Structural constant Fig. 2.11. Densities of states (per spin) for the nonhybridized canonical bands shown in Figs.2.8–2.10.
Fig. 2.12. The density of states for the sband in the bcc lattice in the nearestneighbour approximation [79]. 48
Band theory
Fig. 2.13. The density of states for the sband in the fcc lattice in the nearestneighbour approximation [79].
γ = 3
γ = 0.82
Fig. 2.14. The density of states for sband in the fcc lattice with the ratio of next nearest and nearestneighbour transfer integrals γ = t 2 /t 1 = 0.8 and 3 [80].
of MT orbitals (2.44) he reduced the potential matix elements to two parameters – the width of dband W d and its position with respect to the sband bottom E d . As follows from (2.44), the Rdependence of the intersite matrix 49
Chapter 2
FCC
Density of states, at –1 Ry –1
BCC
Energy, Ry Fig. 2.15. s, p and dprojected densities of states for fcc palladium and bcc niobium [56].
elements of the potential has the form
V' =C
ll ' m
ll m
= ( rMT R)l +l' +1 ,
(2.85)
where l, l' are the orbital quantum numbers and m = σ , π , δ are determined by the angle between the direction of the orbital and the vector which connects the atoms. In particular, Vssσ ∼ R −1 ,
Vspσ ∼ R −2 ,
V ppσ ,π ∼ R −3 ,
Vddm ∼ R −5
(2.86)
(Note that in the freeelectron approximation all the matrix elements are proportional to R −2 which results in a divergence after volume integration). In an explicit form one may write down 2 rd3 . (2.87) mR 5 where the dstate radius r d is a characteristics of the element, η are dimensionless constants which are tabulated in [13] (see also consideration of felements in paper [84]). The values of rd are obtained Vddm = ηddm
50
Density of states, Ry –1
Band theory
Energy, Ry Fig. 2.16. Density of states of molybdenum for the lowest six bands [82].
from comparison with the firstprinciple band calculations. The quantities Wd are obtained in terms of the matrix elements with the use of standard formulas. For example, for the bcc lattice with the account of the nearest and nextnearest interactions,
8 32 Wd = − Vdd(1)σ + Vdd(1)π − 3Vdd(2)σ + 4Vdd(2)π . 3 9 The values of E d and W d in the drows, together with the results of band calculations [78] and experimental data [85], are presented in the Table 2.1. One can see that E d and W d increase from Sc to V and decrease from V to Cu. In the pseudopotential theory, one can derive also the relation between the effective masses of s and delectrons [13] −1
ms m = 1 + 2.91 . (2.88) md md A number of theoretical models were proposed to describe the electronic structure of ferromagnetic 3dmetals Fe, Co and Ni [85–88]. These models are based on the idea of separating of localized and itinerant dstates with different symmetry (e.g., of t 2g and e g states). Now we consider some general regularities in the results of band calculations. These results agree qualitatively with abovediscussed simple model notions. In agreement with the idea of canonical bands, 51
Chapter 2 Table 2.1. Calculated characteristics of band structure for dmetals: the number of delectrons n d , position of the Fermi level E d (eV) and density of states N(E F ) (eV −1 at −1 ) [78], the model parameters [13]: average energy E d (relative to the sband bottom, eV) and the bandwidth W d (eV); experimental data on W d from PES and IPES [40] are presented for 3dmetals only. 3d 4d 5d
Sc Y La 1.76
Ti Zr Hb 2.90
V Nb Ta 3.98
Cr Mo W 4.96
Mn Tc Re
Co Rh Ir
Ni Pd Pt
4.6↑
4.8↑
4.82↑
3.06↓ 7.99 7.65
4.15↓ 8.96 8.74
10.01 9.89 7.90 6.30 7.32
5.98
nd
EF
Fe Ru Os
Cu Ag Au 9.91
1.68 2–
2.96 2.69
4.10 3.78
5.07 4.73
6.23 5.73
2.34↓ 7.24 6.70
5.82 5.39 2–
8.03 7.42 7.87
9.26 9.06 9.31
10.6 10.6 11.3
10.3 10 . 3 10.9
10.2 10.1 11.6
9.53 8.61 10.4
8.71 7.06 8.68
0.85↑
0.14↑
0.15↑
0.66↓ 1.32 0.90
1.54↓ 2.31 1.67
0.06 0.18
1.76
0.54
1.61
0.65
2.72
0.15
1.69 2–
0.53 0.41
1.20 1.04
0.52 0.36
0.91 0.70
0.24↓ 0.81 0.65
Ed
7.05 6.75 2–
7.76 7.17 9.12
8.13 7.29 9.50
8.01 7.12 9.45
7.91 6.67 8.99
7.64 6.02 8.38
7.36 5.08 7.35
6.91 4.52 6.51
5.90 2.49 5.18
Wd
5.13 6.59 2–
6.08 8.37 9.56
6.77 9.72 11.2
6.56 9.98 11.4
5.60 9.42 11.0
4.82 8.44 10.3
4.35 6.89 8.71
3.78 5.40 7.00
2.80 3.63 5.28
Weexp (3d)
6.2
6.6
6.8
6.5
8.5
8.5
6.9
5.4
2.9
N(EF)
the DOS pictures for elements of one column in the periodic table demonstrate a similarity. This is illustrated by comparison of DOS for hcp metals Ti, Zr and Hf (Figs.2.1–2.3). A similar situation takes place for Sc and Y (hcp), V, Nb and Ta (bcc), Cr, Mo and W (bcc). In Tc and Re (hcp) the heights of the DOS peaks (especially of the lower ones) differ appreciably. The same difference occurs between Ru and Os (hcp), Rh and Ir (fcc), Pd and Pt (fcc). The canonical band idea works also for elements of different columns with the same lattice, the position of the Fermi level being changed roughly according the rigid band model. This may be illustrated by comparison DOS of V and Cr (bcc), Rh and Pt (fcc). The values of partial DOS of s,p,dtype, which are given in 52
Band theory Table 2.2. Partial s, p, d densities of states at the Fermi level and the number of delectrons in 3dmetals [78].
s p t2g eg ng
Sc
Ti
V
Cr
Mn
Fe↑
Fe↓
C o↑
C o↓
N i↑
N i↓
0.34 6.06 13.70 10.12 1.76
0.07 0.80 4.61 2.69 2.9
0.43 2.46 18.0 3.95 3.98
0.08 0.72 6.52 2.31 4.96
0 . 19 0.31 17.9 19.1 5.98
0.22 0.14 10.5 1. 0 7 4.6
0.02 0.04 2.80 0.41 2.34
0.36 0.23 0.65 1.22 4.8
0.06 0.44 5.54 3.48 3.06
0.28 0.24 1. 2 5 0.74 4.82
0.16 0.09 13.07 7.94 4.15
Table 2.2, demonstrate that dstates in transition metals are dominating ones. They make up about 70–90% of the total DOS at the Fermi level. One can see also from Table 2.2 that large and small values of N d (E F ) alternate when passing to a neighbour element. This rule holds even irrespective of the crystal structure and demonstrates an important role of atomic configurations. The regularity is to some extent violated in the end of dperiods. This may be explained by ferromagnetism of Fe, Co, and Ni and violation of regularity in dshell filling. It should be also noted that the numbers of delectrons per ion in metals exceed by about unity the atomic values [78]. To end this section, we discuss the problem of accuracy of band calculations. This problem is connected with a number of approximations: choose of initial atomic configuration, the density functional approach for states which are far from E F, the local approximation, the form of crystal potential (including exchange–correlation contribution), the calculation method used, an account of relativistic effects etc. The role of these approximations may be clarified by comparing results of various calculations. Such a comparison is performed in numerous Table 2.3. Experimental (angleresolved photoemission) and calculated energy on the Γ∆L axis in palladium (in eV relative to the Fermi level) [90]. k point, band number Γ2 , 3 , 4 Γ2 , 3 , Γ5,6
Exper. [90]
– 2.556+ 0.15 2– 2.46+ 0.2
Γ4
2– 1.156+ 0.1 2– 0.46+ 0.2
Γ5
2– 0.16+ 0.1
Γ7
+7.76+ 0.3
Γ7
+18.46+ 0.5
Γ8
+21.76+ 0.5
RAPW [91] 2– 2.79 2– 2.98 2– 1.17 2– 0.14 1+ 0.05 1+7.30 1+ 17.71 1+ 21.65
53
RAPW [92]
HFS [93]
2 – 2.49 2– 2.62 2–
2– 2.59 2– 2.70 2– 2.70
2– 2– 2–
2– 0.06 2– 0.06
2– 2–
Pseudopot. [94] 2– 2.56 2– 2.66 2– 2.66
2– 2–
2– 0.09 2– 0.09 2– 2–
2–
2–
Chapter 2 b
a
Fig. 2.17. Energy bands of vanadium, calculated for two possible choices of the crystal potential [83].
review papers and monographs (see e.g. [57]). For example, influence of initial atomic configuration is illustrated by band calculations of vanadium (Fig.2.17). The width of the sband differs by two times for the configurations 3d 34s 2 and 3d 44s 1. The Table 2.3 shows results of band energy calculations at some Brillouin zone points in Pd by different methods [91–94] and corresponding experimental results [92]. We may conclude that the accuracy of energy determination makes up about 0.1−0.3eV. The disagreement with experimental data may be about 0.5eV. At comparing the calculated band spectrum with angleresolved emission and de Haas–van Alphen effect data, one has often to shift it by such values. In temperature units, the corresponding uncertainty is of the order of 103 K which makes difficult precise calculations of thermodynamic properties within the band approach.
2.5 EXPERIMENTAL INVESTIGATIONS OF BAND STRUCTURE: SPECTRAL DATA A number of quantities, which are obtained in band calculations (e.g., the position of energy bands and the shape of the Fermi surface, the electronic structure near the Fermi level) may be analyzed and 54
Band theory compared with results of experimental investigations. There exist a large number of spectral methods for investigating electron structure. They may be divided in emission and absorption spectroscopy methods. The first ones enable one to obtain data on the filled part of the band (below E F), and the second on the empty part (above EF). Both the optical and Xray regions may be investigated. Let us list main spectral methods and corresponding notations [40]: • • • • • • • • • • • • •
PES – XPS – UPS – IPES – AES – BIS – EELS – MXD – MXS – SEC – XAS – XANES – EXAFS –
Photoelectron (Photoemission) Spectroscopy Xray Photoelectron Spectroscopy Ultraviolet Photoelectron Spectroscopy Inverse Photoemission Spectroscopy Auger Electron Spectroscopy Bremsstrahlung Isochromat Spectroscopy Electron Energy Loss Spectroscopy Magnetic Xray Dichroism Magnetic Xray Scattering Secondary Electron Spectroscopy Xray Absorption Spectroscopy Xray Absorption Near Edge Spectroscopy Extended Xray Absorption Fine Structure
When the spectroscopies are performed angleresolved and spinpolarized, acronyms AR and SP are added. An advantage of the Xray spectroscopy is the simple separation electron states with different angular moments. By virtue of the selection rule, ∆l = ±1, Kspectra (transitions from 1sstates of inner core levels of an atom) contain information on pstates of higher bands, and Lspectra (transitions from 2pstates) on s and dstates. Due to large difference in the energies of K and Lshells, these spectra are well separated. This simplifies the comparison with band calculations which also yield separately s,p,dcontributions. The optical part of the spectrum corresponds to transitions between external overlapping energy bands or inside them. Therefore the qualitative analysis of the optical spectra is much more complicated. We do not discuss in detail these spectra of transition metals where the interpretation is especially difficult (see [95]). On the other hand, the resolution of Xray spectra in the energy measurement is smaller than for optical spectra because of the large intrinsic width of internal levels (of order of 1eV, see the handbook [96]). The situation is somewhat better only for soft Xray spectra
55
Chapter 2 (e.g., for the Nspectra the width of the internal 4flevel makes up about 0.15eV). Besides that, there exist the contribution to level width which is due to finite lifetime of electrons and holes. This contribution increases with increasing distance from the Fermi energy: (2.89) Γk ∼ ( Ek − EF ) 2 . Provided that the density of states in a band contains a symmetric maximum which does not overlap with contributions of other bands, its position may be determined with a satisfactory accuracy (about 0.1 eV). However, such a determination is prevented in the presence of overlapping bands. Usually comparison of Xray data with calculated spectra is performed by smoothing out the band structure with account of the level width. Occupied states are investigated in PES and ultraviolet PS methods. The former yields, in particular, information on K, L, M, N and Ospectra of 3d, 4d and 5dmetals. Very promising is the angle resolved photoemission method which yields information on not only the density of state, but also the spectrum E(k). Methods of Xray spectroscopy for empty states include XAS, XANES, BIS, IPS. The relation between
a
b
c
E, eV Fig. 2.18. Xray emission spectra of vanadium [57] (a) Kband (b) L III band (c) M III band; 1 are the experimental data, 2 and 3 are the results of calculations with different perturbation operators.
56
Band theory
E, eV Fig. 2.19. Xray emission spectra of Y and Zr; solid line shows experimental data, and broken line the results of calculations [57].
the IPES and BIS methods is roughly the same as between the ultraviolet PS and Xray PS ones. Large widths of internal levels in K, L and M PESspectra prevent as a rule do resolve the density of state structure in the conduction band. The comparison on K, L and Mspectra of vanadium with results of theoretical calculations are shown in Fig.2.18. One can see that the complicated DOS structure [78] becomes smeared. At the same time, total width of the spectrum coincides roughly with the calculated bandwidth after account of the level broadening. So, the width is 8 eV for the Kspectrum and 6 eV for the L spectrum, the calculated bandwidth being equal to 4 eV. The second typical example is the spectrum of zirconium (Fig.2.19). Here the L III spectrum (4d–2p transitions) has the width of 3.4 eV, and the M V spectrum (3d–4d transitions) the width of 2.9 eV. Highenergy maximum corresponds to the M IV spectrum, and lowenergy maximum at 6−7 eV has probably a satellite origin. Although the width of the internal 4plevel is considerably smaller than that of the 2plevel, the experimental broadening is approximately the same for the L III and N III spectra. Possibly, this is due to larger contributions from the s–4p transitions to the N III spectrum. For next elements of 3d and 4dseries, the widths of internal 57
Chapter 2
Fig. 2.20. Experimental Xray emission bands of 5dmetals [57].
levels for K, L, M spectra increase so that their quality becomes worse. The situation is more favorable for the 5d series where the spectra N VI,VII (5d–4f) and O II,III (5d–5p, 5s–5p) with a small internal level width occur. Because of the closeness of 4f and 5d levels, four lines lie in the interval of the order of 10 eV. Nevertheless, because of small widths of f and 5p levels, these lines are clearly resolved in the beginning of the 5d series, emission bands being rather contrast and intensive. In the end of the series, the intensity of lines decreases and their structure becomes unclear. For the N VI,VII bands an opposite tendency takes place (Fig.2.20). An important role in the spectra of 5dmetals belongs to the spinorbital interaction. According to the selection rules, the transitions into internal doublets f 5/2 , f 7/2 go from d 3/2 and d 5/2 levels of the conduction band. Analysis of experimental data demonstrates that the distributions of d 3/2 and d 5/2 states in the conduction band are different. Fig.2.21 shows the N VI,VII spectra of iridium and platinum with resolution of N VI (i.e. d 3/2 ) and N VII (d 5/2 ) states. The main maximum b 2 is connected with states of both types. The highenergy maximum b 3 is due to d 3/2states, and the lowenergy one b 1 to the 58
Band theory
N VIItheor
N VIItheor
N VItheor
N VItheor
N VI,Vtheor
N VI,VIItheor
N VI,VIIexp
N VI,VIIexp
E, eV
Fig. 2.21. N VI,VII emission spectra of Ir (a) and Pt (b). Lower curves are experimental data [57].
d 5/2 states. Thus, the d 5/2 states dominate at the dband bottom and the d 3/2 states near the Fermi level. It is interesting that the spectra of Ir and Pt are satisfactory explained by atomic calculations which indicates a considerable localization of 5delectrons in these metals. A more complicated situation occurs for the N VI,VIIspectra in the middle of the 5dseries (Ta, W, Re, Os), see [57]. The experimental width of the O III spectrum turns out to be larger than the calculated one. This is connected with extra interactions and manyelectron effects (e.g., the influence of the vacancy in the O III shell). The ARP method takes into account not only energy, but also quasimomentum of an electron in the conduction band. Consequently, it enables one to determine experimentally the dispersion law E(k) for various branches, which gives a possibility to calculate the density of states to high accuracy. This method was applied to investigate Cu [97], Ag [98], Au, Pt [99], Pd [90], Ir [57]. The results for the spectrum of Cu in the 〈211〉 direction [97] agree well with the free electron model. Himpsel and Eastmann [90] measured E(k) for Pd in the 〈111〉 direction to accuracy of 0.1− 0.2 eV, the accuracy in determining k being about 5% of k max (Table 2.3). One can see that agreement is not too good. A similar situation takes place as for Pt and Au [99]. Although investigating the occupied part of the conduction band is more important for the electron properties of a metal, data for 59
Chapter 2 Table 2.4. Positions of density of states peaks, and widths of empty and occupied part of the band W ± for 3d and 4d metals (in eV) [101].
3d 4d Eexp
peak
theor Epeak
W2– Wtheor theor W1
W +theor theor
W1
xp W +eexp
W1 2
– W +theor theor + –W theor 1
2 W exp
Sc Ti Y Zr 1.8, 3.8 1.0, 2.8 2.0, 5.4 0.9, 4.4 1.4, 3.5 0.8, 3.1 1.3, 4.6 0.9, 4.6 1.7 3.1 2.0 3.1 4.0 3.65 5.3 5.3 4.4 4.7 3.2 3.8 6.1 5.2 5.7 0.0 −0.5 −0.8
−0.1
V Nb 2.3 3.5 2.5 3.4 3.2 3.5 4.0 5.6 3.4 3.8 5.2 5.9 +0.4
Cr Mo 1.0 2.0 1.2 1.8 4.5 5.4 2.5 3.9 1.8 2.3 3.9 4.5 +0 . 5
0
−0.3
Mn Tc 1.4 2– 2– 2– 2– 2– 2– 3.5 2 –2
Fe Ru 1.6 1.2 1.6 1.3 5.3 6.2 2.6 1.95 2.9 3.5 1.95 −0.6
Co Rh 0.5 0.4 0.5 0.5 5.5 5.8 1.15 1.2 1.4 1.1 −0.25
Ni Pd 0.3 0.2 0.3 0.1 5.0 4.8 0.4 0.4 0.4 0.4 0.0
–2
0.0
0.1
0.0
the empty part of the band from absorption spectra are also useful from the point of view of comparison with band calculations. The BIS data for 3d and 4dmetals were obtained and compared with band calculations in the paper [102] (see Table 2.4). The total resolution was about 0.7eV, and the lifetime broadening at E F about 0.25eV. On the whole, the band shapes obtained are close to those for canonical bands. The agreement with calculated N(E) turns out to be better than for XPS spectra which are strongly distorted in the beginning of periods [103]. Besides that, BIS spectra do not exhibit satellites which correspond to the d n+1 configuration. The dbandwidth increases up to the middle of periods by about 25%. The s–d hybridization is important near the band bottom and is most strong for hcp metals. Peaks near E F, which correspond to the empty dband, are followed by a structureless plateau and at 7−10 eV by a step, which is interpreted as the van Hove singularity. The peaks (dband tails) at E F are observed even in Cu and Ag. Two peaks are observed for Sc, Ti, V and Zr, and one peak in other metals, which is in agreement with band calculations. Strong asymmetry of the peak is observed in molybdenum in agreement with theoretical predictions. The position of 1.6eV peak in Fe corresponds to DOS in ferromagnetic rather than paramagnetic state (Figs.2.22, 2.23). The relative dband BIS intensity in the 3dseries was derived and demonstrate to have a maximum in the middle of the series. Calculated spinresolved densities of states of ferromagnetic transition metals Fe and Ni [24] are shown in Figs.2.24, 2.25. Of great interest 60
Band theory
eV
eV
eV
eV
eV
eV
eV
eV
eV
Fig. 2.22. Comparison of BIS and density of states curves for 3dmetals and Cu. The dashed curves correspond to the nonbroadened DOS, the solid lines to the DOS broadened with Gaussian and Lorentz broadening to simulate instrumental and lifetime broadening respectively. The upper dotted curve is the measured BIS spectrum [102].
for the theory of both the electron structure and magnetism is the investigation of spin splitting ∆. In principle, such investigations may be carried out within the standard PES and IPES methods. However, these methods provide only a rough estimations of averaged values of ∆. According to band calculations, ∆ depends considerably on E and k, so that angle resolved methods are required for obtaining detailed 61
Chapter 2
eV
eV
eV
Fig. 2.23. The same data for 4dmetals and Ag [102].
information. Data on spin and angle resolved photoemission were obtained for Fe [103–107], Ni [103, 107–109] and Co [103]. According to the review [40], there exist in Fe both collapsing and noncollapsing spin subbands which demonstrate different types of behaviour at crossing the Curie point. Fig.2.26 shows spinpolarized angleresolved spectra of Fe in the (100) direction near the Γpoint at hν = 60 eV. These data demonstrate the energy and temperature dependence of ∆. The ultraviolet photoemission spectrum of Fe was investigated by Pessa et al [110]. The observed peaks at 0.58 and 2.4 eV below the Fermi energy may be interpreted within the calculated density of states of ferromagnetic iron provided that one shifts the latter by 0.5eV to higher energies. The value of N(E F ) for Fe obtained in [110] coincides approximately with the results of band calculations 62
Band theory
Integral density of states
Density of states, eV –1
Spin up
Spin down
Fig. 2.24. Calculated spin up and down densities of states of ferromagnetic iron [24].
[194], but is considerably smaller than that determined from electronic specific heat [266] and paramagnetic susceptibility (see the detailed discussion in the corresponding chapters). It should be noted that an error of order 0.1eV in the energy measurement may influence strongly the N(E F ) value. Comparison of results [110] with the spinpolarized spectra [111] confirms that the 0.58 eV peak belongs to the majority spin subband. The energy dependence of spin polarization is not explained by the theoretical density of states. The experimental estimation of spin splitting yields the value not more than 1.9 eV which is considerably smaller than theoretical one (2.35 eV). No shift of the spectrum at the Curie point is observed which may indicate retaining of strong shortrange order above T C . The dbandwidth of Ni from the ARP data [108] makes up 3.4 eV at the point L, the theoretical value being about 4.5 eV. The measured value of the exchange splitting is 0.31 eV at 293 K (the 63
Chapter 2
Density of states, eV –1
Integral density of states
Spin up
Spin down
Fig. 2.25. Calculated spin up and down densities of states of ferromagnetic nickel [24].
theoretical value is 0.7 eV) and about 0.2 eV above the Curie point (Fig.2.27). Evidence of the existence of spontaneous spin splitting above T C in Ni was obtained by the positron annihilation technique [112]. Spinresolved photoemission data on the shortrange magnetic order above T C in Co were obtained in [113]. The problem of spontaneous spin splitting in iron group metals may also be investigated in optical experiments [114]. 64
Band theory
Fe(100)
Intensity with spin resolution
hν =6060eVeV
Energy below E F, eV Fig. 2.26. Spin and angleresolved distribution curves form Fe (100) at 60 eV photon energy for two different temperatures (T/T C = 0.3 and 0.85) [105]. The arrows refer to the spontaneous magnetization direction.
Recently, the Magnetic XRay Dichroism (MXD) method was applied to determine the conduction electron spin polarization [40]. The L 23 absorption edge (2p → 3d transitions) was investigated for Ni, and the asymmetry in photon absorption with different polarization permitted to find both spin and orbital momenta which turned out to be s = 0.52 µ B and l = 0.05 µ B . These values are close to theoretical ones, which are obtained with for manyelectron effects [115]. According to the latter paper, the ground state of the Ni ion is a superposition of the 3d 10 , 3d 9 and 3d 8 states with the weights of 15−20%, 60− 70% and 15−20% respectively. Consider the question about the origin of lowenergy satellites in spectra of some dmetals. Such satellites are observed in Xray 65
Chapter 2
experiment trial ∆ ex = 0.17 eV
∆ ex = 0.28 eV
background
background
Initial energy, eV Fig. 2.27. Angleresolved energy distribution curve showing temperaturedependent exchange splitting δEex = 1.09∆ex in Ni [108]. According to the experimental conditions, only the uppermost dband is observed.
emission spectra of Ni (at 6 eV below E F , see, e.g., [116]) and Zr [57]. There exist mechanisms of satellite formation which are connected with vacancies at excited atoms, Auger processes, shake up potential changes etc. (see [57]). We discuss more interesting manyelectron mechanisms which are specific for transition metals. Liebsh [117] treated the Coulomb interaction between two dholes in Ni. Introducing atomic Slater integrals F(p) (p = 0, 2, 4), he obtained in the low density approximation additional peaks in the spectrum and compared them with experimental data. Besides the 6 eV satellite, the theory yields the second satellite which lies lower by 2 eV. The occurrence of satellites resulted in narrowing of the dband since the total number of states is constant. The exchange splitting obtained turned out to be different for e g and t 2g states (0.37 and 0.21 eV), the average value 0.3 eV being in satisfactory agreement with experiment. Penn [118] performed calculations within the degenerate Hubbard model. The fitted value of the Hubbard parameter was U = 2 eV. The authors of the paper [119] treated this problem exactly at restricting to four point in the Brillouin zone, which is equivalent to consideration of a fouratom cluster. An agreement with experimental data was obtained for U = 4.3 eV and the ratio of the Hund and Coulomb parameters J/U = 1/7. A more consistent consideration of the satellite formation problem 66
Band theory should include manyelectron terms (the satellite corresponds to the multiplet structure of the configuration d 8). The corresponding data of the Auger spectroscopy which contain more information on manyelectron effects are discussed in Sect.1.2. The ARP investigations of γcerium [120] yielded two dispersionless density of states peaks near E F which did not obey the oneelectron selection rule. They were attributed to atomiclike 4fstates. To describe highenergy spectroscopy data for cerium and its compounds, Gunnarsson and Schoenhammer [121] proposed a model, based on the oneimpurity Anderson Hamiltonian and including effects of d–f hybridization. Further this model was applied to consider spectra of actinides and Ti (see [40]).
2.6 BAND CALCULATIONS OF RARE EARTHS AND ACTINIDES Oneelectron band calculations of rare earths are performed by the same methods as for 5dmetals, the role of relativistic effects becoming here still more important because of strong spinorbital interaction. Since the 4fshell lies well below the conduction band, one may assume that the picture of this band is similar for all the 4felements (especially for heavy rare earths). This is confirmed by data of photoemission spectroscopy from the 6s–5d band [122]. However, attempts of description in the oneelectron approach of highlycorrelated felectron themselves meet with serious problems. Results of band structure calculations of various RE metals by nonrelativistic and relativistic augmented plane wave method (APW and RAPW) are presented in the review [19] (see also the discussion of electronic structure for heavy rare earths [15]). For most RE metals (except for Ce, Sm, Eu, Tm and Yb) the conclusions are as follows. The 4fband lies by about 5−10 eV below the conduction (5s,6sp) band and has the width about 0.05eV. The 5dband moves up relative to the conduction band with increase of the atomic number from La to Lu, the delectron density of states at E F increasing from 1.9 to 2.5 eV −1 ⋅atom −1 . For elements with unstable valence Ce, Eu and Yb, especial attention was paid to investigation of 4flevel position ε f . A strong sensitivity to x was found in APW calculations of Ce in 4f 2−x 5d x 6s 2 (x = 0.5−2.0) configurations [123]. The 4flevel is considerably lower than 5d–6s band for x = 0, but rapidly becomes higher and broader with increasing x. The calculated in [124] distance E F − ε f equals to 0.36 and 0.24 Ry, and 4fbandwidth to 0.01 and 0.02 Ry for
67
Chapter 2
γ  and α cerium, respectively. The full calculation of band structure of Ce in the linear RAPW method with account of correction to MTapproximation was performed by Pickett et al [125]. The width of 4fband is about 1 eV and increases by about 60% at the γ – α transition. The occupation numbers of felectron (about 1.1) changes weakly under presure. This leads to the conclusion that the γ–α transition is accompanied by delocalization of 4felectrons rather than by promotion into sdband. Relativistic APW calculations for Yb in 4f 14 6s 2 configuration [126] yielded unexpectedly the 4flevel position which is 0.1 Ry higher than the 6s conduction band (but still lower than E F by 0.2−0.3 Ry). A small gap near E F was obtained in contradiction with experimental situation. In the selfconsistent calculations by Koelling (see [127]), E F ε f and the gap in the spectrum vanishes. APW calculation of 4fband in thulium [128] with the account of 5s6d–4fhybridization yielded ε 5d −ε 4f = 0.69 Ry, ε 6s − ε 4f = 1.27 Ry and the fbandwidth of the order of 10 −2 eV. According to the first calculation of ferromagnetic gadolinium with the account of 4fstates within the selfconsistent RAPW method by Harmon [127], the flevel for spin down states (with the width about 0.03 Ry) lies slightly above E F because of large spin splitting. This should lead to giant values of N(EF), and, consequently, of electronic specific heat, which drastically contradicts the experimental data. Similar conclusions were obtained in [129–131] for Tb, Dy and Gd. These results demonstrate the inadequacy of usual band calculations within localspindensity approximation for 4fstates. This problem is discussed in recent papers [132] with application with gadolinium. In a number of works, attempts to take into account correlation effects were made. Authors of papers [133–134] obtained a picture of 4f and conductionelectron states with account of correlation, screening and relaxation. The flevel energies for the ground and excited configurations f n and f n+1 were determined by (2.90) ∆ − = E ( f n ) − E ( f n −1 ), ∆ + = E ( f n +1 ) − E ( f n ), Calculations were performed within nonrelativistic [133] and relativistic [134] approximations. The crystal potential in [133] was constructed from renormalized Hartree–Fock functions for the configurations 4f n 5d m−1 6s 1 and 4f n±1 5d m−1⫿1 6s 1 (m = 2,3). The renormalization (transfer of atomic wavefunction tails inside the Wigner–Seitz cell) resulted in a strong change of density for 5d, 6s electrons and, because of screening effects, in a considerable (by about 0.05 Ry) increase of oneelectron fenergies. The values of ∆ + were corrected by introducing 68
Band theory correlation effects from comparison with spectral data (the correlation energy was assumed to be the same in the cases of free atom and crystal). Although the correlation energy in each state may be large, their difference
ξ + = Ecorr ( f n d 2 s) − Ecorr ( f n +1ds)
(2.91) makes up about 0.1 Ry only. The results of calculation of the quantity ξ + are shown in Fig.2.28. The edges of 5d and 6sbands were determined from the zero of the wavefunction and its derivative at the Wigner–Seitz cell boundary. The results turned out to be somewhat different from those of standard calculations. The 4fbandwidth made up 0.03 Ry for γ Ce, 0.01 Ry for Pr and Nd and smaller than 0.005 Ry for other rare earths. One of important drawbacks of the calculation [133] was using of flevel energies ε f which are averaged over many electron terms. At the same time, spectral data, which were used, corresponded to transitions between ground states with definite S and L. Since the difference in energies of terms reaches 5eV, the error in the correlation energy may be large. A detailed calculation of the term structure for the f n−1 configuration was performed in [135]. The corresponding line spectrum should be observed in experiments with high resolution. As follows from equation (2.48), the averaged energy ε 4 f may differ considerably from the ionization energy with the final state corresponding to the Hund term. The difference may be presented in the form
Fig. 2.28. Differences of correlation energies ξ for transitions 4f n+15d6s → 4f n 5d6s in free rare earth atoms and for transitions 3d n+1 → 3d n between ground state multiplets of iron group atoms [133]. 69
Chapter 2
b (2) ∆b = b( f n SL) − b( f n S ' L' ), (2.92) −2 + ∆b F , n where the coefficient b(f nSL) determines the contribution of the Slater integral F (2) to the SLterm energy, 2bF (2) /n is the Coulomb energy per electron in the Hartree–Fock approximation, which is averaged over terms. In the rare earth series the value of ∆b changes from 0 (f 0configuration) to 113 (f 7configuration), and ∆b(f n+7) = ∆b(f n). Since the values of F (2) 0.05eV are not too small, this contribution to the felectron energy should be important. In the relativistic calculations [134], an account of term structure was also performed. Final results for the effective oneelectron energies differ weakly from those obtained in [133] (Table 2.5), but the changes in correlation corrections are appreciable. In particular, the correlation energy difference ξ +, which is negative for most rare earths according to [133], becomes positive. One can interpret these data as increase of f–f correlation with increasing number of felectrons. Although the absolute calculated values of ε 4f and E F are not quite reliable because of numerous approximations, general regularities in the rareearth series seem to be qualitatively correct. This is confirmed by data on photoelectron spectra for the fshell [136, 137]. A correct calculation should take into account also the change of wavefunctions in the final configuration f n–1. The total relaxation in the final state (f n d m → f n–1 d m+1 transition, the hole in the 4fshell is completely screened by additional electron in the 5dstate) was assumed in [133–134]. Such an assumption explains the decrease of 4felectron binding energy in comparison with the Hartree–Fock approximation. An attempt of the calculation in absence of relaxation (f n d m → f n–1 d m transitions) [134] agrees worse with experimental data. Table 2.5. Values of ∆_ = E F – ε (4f n ) and ∆ + = ε (4f
n+1
) – E F for rareearth metals.
D6∆ + (eV) (eV)
γ Ce
Pr
Nd
Pm
Sm
Eu
Gd
Tb
Dy
Ho
Er
Tm
Yb
Lu
La
D∆ 2 –
2.1
4.1
5.1

5.6
1.5
8.7
4.6
5.6
6.0
6.0
6.2
0.7


D∆ 2 –
1.9
3.8
5.1

5.5
1.9
8.3
3.3
4.7
5.5
5.4
5.4
1.1
7.5

D∆ 2 –
1.9
3.3 4.5
4.5
4.5

7.0
1.9
3.4
4.8
4.8
5.2

8.5

D∆ 1 +
3.3
2.6
2.1

0.5

3.3
2.1
1.8
1.5
1.5
1.3



D∆ 1 +
3.1
2.0
1.3

0.2

3.2
2.1
1.4
1.6
1.6
1.0


4.7
70
Band theory Now we discuss briefly the results of band calculations for 5felements [138, 139, 57]. Band structure of actinides is to some extent similar to that of rare earths, but the strong spinorbital coupling is accompanied with considerable delocalization of fstates. Thus the spectrum is appreciably disturbed owing to overlap and hybridization between s,p, 5dstates with 5fbands. Concrete forms of the bandstructure and flevel positions in the selfconsistent calculations depend strongly on the selection of the exchangecorrelation potential. In the RAPW calculation of thorium by Keeton and Loucks [140] with the Slater potential ( α = 1) the position of the 5fband (in the middle of the valence band) contradicted the de Haas–van Alphen data. However, the calculation [141] with the Gaspar–Kohn–Sham potential ( α = 2/3) yielded the correct 5fband position (well above the Fermi level). Thus the band structure of Th is similar to that of dmetals. Despite the absence of felectrons, the shape of the dband is appreciably influenced by d–f hybridization. According to [138], the 5fbandwidth decreases with increasing atomic number from uranium (0.4 Ry) to plutonium (0.3 Ry). The electron spectrum of U near E F contains a s–d conduction band which is strongly hybridized with a rather wide 5fband. The 5fbands in Pu are considerably more flat for α = 1 than for α = 2/3. This indicates that Pu lies on the boundary of the felectron localization. In the selfconsistent calculation [142], the fband turns out to be narrower than in [138]. The density of states of Pu contains sharp peaks with the height about 150 Ry − 1 . The total value of N(E F ) is 123.6 states/Ry (the fcontribution is about 50 states/Ry), which corresponds to the linear term in electronic specific heat with γ = 21 mJ/mol ⋅ K 2 . The experimental value makes up about 50 mJ/mol ⋅ K 2 , so that the calculation seems to be qualitatively satisfactory, but correlation enhancement should be taken into account. Relativistic calculations of the band structure in heavy actinides (Am, Cm, Bc) were also performed by Freeman and Koelling [138]. As compared to light actinides, the width of the 7sband increases, 5fbands become rather narrow and flat, the sd–5f hybridization being suppressed. Thus a strong localization of 5felectrons takes place. As well as for rare earths, usual band description cannot be used in such a situation. An important role of correlations is confirmed by the high sensitivity of the spectrum to the number of felectrons. The calculation for Am in the configuration 5f 7 7s 2 (instead of the correct one, 5f 6 6d 1 7s 2 ) yields a shift of 5fstates by 0.5 Ry. The delocalization of 5felectrons in heavy actinides under pressure was investigated in the band calculations [143]. 71
Chapter 2
2.7 FERMI SURFACE One of most powerful tools to verify the results of band calculations is investigation of the Fermi surface (FS). The structure of FS determines a number of the electronic properties of metals, in particular their anisotropy. The shape of FS depends on the geometry of Brillouin zones, crystal potential and interelectron correlations. The volume under FS is fixed by the Luttinger theorem: it has the same value as for the noninteracting electron system. It should be noted that this theorem is valid only provided that the Fermiliquid picture (Landau theory) holds, and may be violated in system where strong Hubbard correlations result in splitting of oneelectron bands (e.g., in systems which exhibit correlationdriven metal–insulator transitions [25]), so that the statistics of oneparticle excitations changes. In band calculations, FS is obtained as the constant energy surface which separates occupied and empty states at T = 0. If FS lies far from the boundaries of the Brillouin zones (e.g., at small band filling), it differs weakly from that of free electrons and has nearly spherical shape. At approaching the zone boundaries, the influence of crystal potential becomes stronger and anisotropy of FS increases. Especial strong singularities of FS occur at crossing a boundary. Since a Brillouin zone contains two electron states per atom (with account of the spin quantum number), in most cases one has to use several zones to place all the conduction electrons. Due to the anisotropy of the lattice and, consequently, of the electrons spectrum, zones with higher numbers start to be filled up when the lower zones are only partially filled, so that FS crosses several zones. In transition dmetals, the valence electrons include delectrons. An important feature of dstates is that they are highly anisotropic and poorly described by the free electron approximation even far from the Brillouin zone boundaries. Therefore the shape of the Fermi surface is very complicated and one has to use a large number of zones to describe it. Usually one considers Fermi surfaces of transition metals in the reduced zone picture. 2.7.1 Methods of Fermi surface investigation and de Haasvan Alphen effect Experimental information on FS may be obtained from investigation of anisotropic electron characteristics of a metal. Most widely used methods of constructing FS which are based on magnetic field effects in electron spectrum. To first place, here belong socalled oscillation effects – de Haas–van Alphen (dHvA) effect (oscillations of magnetic susceptibility) and Shubnikov–de Haas effect (oscillations of conductivity), 72
Band theory and also a number of magnetoacoustical and resonance effects [10]. Microscopical basis for the oscillations effects is the Landau quantization in a magnetic field. It is well known that at inclusion of the field Hz the orbital motion of a free electron becomes a quantum in the xyplane. The quantization condition is written in terms of the area of the circumference with the radius (k 2x + k 2y ) 1/2 :
2π eH 1 (2.93) ν + , 2 c where ν = 0, 1, ... are the numbers of Landau levels. The corresponding condition for energy reads Sν = π (k x2 + k y2 ) =
1 Eν ≡ E (k x , k y , k z ) − E (k z ) = ωc ν + , 2
(2.94)
with 2 k z2 eH , ωc = . (2.95) 2m mc being the kinetic energy of an electron moving in the zdirection and the classical cyclotron frequency which describes rotation of an electron in the xyplane. Therefore the quantization in the magnetic field results in the occurrence of an oscillatory contribution to the electron energy. Comparing (2.93) and (2.94) we may write down E (k z ) =
Sν =
2π mc Eν , 2
(2.96)
mc =
2 ∂ Sν . 2π ∂ Eν
(2.97)
where
the expression (2.97) being valid for an arbitrary dispersion law of conduction electrons [10–12]. Thus, at considering the electron motion in magnetic field the freeelectron mass m is replaced by the cyclotron mass m c . Unlike the band effective mass, which is defined at a point of the kspace, m c is defined for a closed curve coresponding to an electron trajectory on the Fermi surface in the magnetic field. The difference of energies for two neighbour Landau levels reads 2π eH c
−1
∂S (2.98) . ∂E Since the numbers ν are large and the energy differences are small in comparison with energies themselves, we may put Eν +1 − Eν = ω c =
73
Chapter 2
S ( Eν +1 ) − S ( Eν ) ∂ . S ( Eν ) = ∂E Eν +1 − Eν
(2.99)
As follows from (2.98), (2.99), the areas of orbits in the kspace differ by the constant value
∆S = ω c
2π eH c
(2.100)
or (2.101) S ( Eν , k z ) = (ν + λ ) ∆S , where λ does not depend on ν (typically, λ = 1/2). Quantization of electron motion in xyplane leads to the situation in which the quasicontinuous distribution of electron states is influenced by a discrete dependence on Landau level numbers. Therefore the resulting electron density of states N(E) in the external magnetic field will exhibit an oscillating behaviour. To demonstrate the occurrence of oscillations, we suppose that the ν th Landau level crosses E F at some H for a given k z , i.e. (2.102) E ( k z ) + ω c (ν + λ ) = EF . At slightly decreasing H, ω c increases and N(E) decreases. However, with further decreasing field the Fermi level is crossed by the ( ν +1)th Landau level and N(E) takes again the maximum value at H = H'. Subtracting the equalities (2.93) for two adjacent Landau levels one can see that the oscillating behaviour of N(E) (and of related physical properties) as a function of the inverse magnetic field has the period
1 2π e 1 1 [ Sν ( EF )]−1 . ∆ = − ' = (2.103) H H H c To complete the consideration we have to sum over k z which was up to now fixed. Since the energy E depends on k z , for most k z the condition (2.102) will be satisfied at different values of H and the summary oscillating contribution will be absent. However, this condition will approximately hold for a finite segment of k z values provided that the energy varies very weakly in the k z direction, i.e.
∂Ek = 0, ∂k z
(2.104)
∂Sν (k z ) = 0. ∂k z
(2.105)
or, which is equivalent,
74
Band theory Thus the Landau quantization results in an oscillating behaviour of the electron density of states N(E), this quantity having a singularity if E equals to the energy of a stationary (extremal) orbit determined by (2.105). The value of N(E F) which determines the most electron properties of a metal should be singular at
2π eH . (2.106) c This permits to determine the extremal cross section areas by measuring the oscillation period. At T = 0, near each energy E 0 which satisfies the quantization condition, N(E) ~ E − E0−1/2 (as well as in the case of onedimensional Van Hove singularity). In real situations, the oscillation effects are smeared due to thermal excitations at the Fermi surface over the energy interval of order T or due to impurity scattering. The oscillations are observable at Sextr ( EF ) = (ν + λ )
e H = 2µ B H . (2.107) mc Usually one has to use the magnetic fields of order 10 kG at temperatures of a few K. To obtain the oscillating contributions to physical quantities one has to perform the integration over kz. In the case of free electrons the result for the magnetization at T = 0 reads [144] kBT < ω c ∼
π pEF π eEF (−1) p 1/2 − . m µ H ( ) sin ∑ B 2 3/2 p 4π c p µB H 4 The oscillation amplitude may be represented in the form M=
(2.108)
1/2
1 µB H µB (2.109) 2π 3 EF and, for small H, is large in comparison with the smooth part of the magnetization (of the order of H). The diamagnetic susceptibility χ = dM/dH may be of order of unity, so that its oscillations are very strong. The corresponding results for an arbitrary dispersion law are analyzed in detail in the monograph [10]. The oscillation period is obtained by the replacement M∼
π
EF
µB
→
c Sextr ( EF ) e
in (2.108). Thus, investigations of magnetic susceptibility oscillations 75
Chapter 2 (de Haas–van Alphen effect) allow one to determine the areas of extremal cross sections of the Fermi surface. The temperature dependence of the magnetization oscillation amplitude enables one to determine the cyclotron mass: (2.110) M ∼ T exp(−2π 2 mc kBT/eH ). In ferromagnetic metals, oscillation effects take place on the background of large spontaneous magnetization M s. In particular, cross sections of the Fermi surface, which correspond to both spin projections, should be observed. For iron, the oscillation amplitude is by approximately nine orders smaller than M s [145], but is still several orders larger than that which can be measured by the most sensitive modern technique. 2.7.2 Experimental and theoretical results on the Fermi surfaces Investigation of the Fermi surface in TM is a considerably more difficult problem in comparison with simple metals. The reasons for this are as follows. High orbital degeneracy of delectrons (unlike s,pelectrons) results in a large number of sheets of FS. Some of these sheets correspond to large cyclotron masses, which requires using strong magnetic fields in de Haas–van Alphen measurements. For magnetically ordered metals (Fe, Co, Ni, Mn, Cr) the picture is complicated by the presence of spin splitting of conduction band states. Besides that, there exist technical problems at preparing the samples which possess sufficient purity to observe oscillations. As a result, the situation in the fermiology of TM is far from total clearness – there are uncertainties in experimental results for a number of elements and ambiguities in theoretical models. Several dmetals (Sc, Hf, Mn, Tc, Ru) and many rareearths and actinides have not been investigated. Data on cross sections with large m c are often absent. From the theoretical point of view, there exist problems connected with the applicability of oneelectron picture in systems where electron correlations play an important role. Even within one electron band calculations the results are rather sensitive to the choose of the crystal potential, so that the shape of FS may exhibit essential (in particular, topological) changes. This leads to difficulties in the interpretation of experimental data (e.g., in identification of different FS sheets and their details). The accuracy of band calculations does not as a rule exceed 0.5 eV. In a number of case, one has to fit theoretical results to experimental data by modifying some parameters, e.g., by shifting the Fermi level position or changing values of the gaps between different branches of electron spectrum. 76
Band theory However, some important results are now well established. First of all, existence of FS sheets with heavy electron effective masses, which are characteristic for TM and their compounds, should be mentioned. (Especially large values were found for the socalled heavyfermion rareearth and actinide systems which are discussed in detail in Chapter 6.) Thus FS investigations yield direct proof of delocalization of delectrons. In particular, these data demonstrate the itinerant character of strong magnetism in iron group metals. General information about the Fermi surfaces of TM (and, for comparison, of Li, Na and Ca) may be found in the Table 2.6 which contains data on classifications of sheets, stationary cross sections S and corresponding effective masses m c . Since there exist a large number of different data for S and m c/m, the results presented should not be considered as unambiguous. As a rule, we write down later data. In many cases, we restrict ourselves to writing down the interval of corresponding values. Most data on S are taken from the handbook [146], which contains the information up to 1981 and the detailed bibliography. More recent data are included provided that they seem to be important. Unlike [146], we give all the values of S in units of Å −2. The transition from oscillation frequencies in Tesla (or periods in T −1 ) may be made according to the formula
S (Å−2 ) = 9.55 ⋅10−5 F (T). The values of m c /m, which are also included in the Table 2.6, are of especial interest for transition metals. Before discussing the FS characteristics of metals of each group (and, separately, of ferromagnetic TM Fe, Co, and Ni) we make some preliminary notes. As well as in the case of simple metals, correspondence between Fermi surfaces of TM with the same lattice structure may be established. In the rigid band approximation, the modification of FS reduces to a shift of the Fermi energy. This circumstance was used often (especially in the early works) for constructing FS at lack of theoretical calculations [11]. For example, the FS of Rh was obtained by Coleridge from that of Ni. The FS of bcc Fe was used to determine FS of a number of bcc TM (e.g., Cr, Mo, W). The type of FS is fairly good retained within a given column of the periodic system. However, with increasing the atomic number Z, the role of spinorbital interaction increases. The latter may change qualitatively the form and topology of FS: because of the degeneracy lift for some energy bands, additional gaps in the spectrum occur and some open orbits may be transformed into closed ones. Deviations of FS in TM from that for free electrons become
77
Chapter 2 Table 2.6. Characteristics of Fermi surfaces of some simple and transition metals, e N (i) and h N (i) stand for electron and hole orbits at the point N in the Brillouin zone with the number i, jg  jungle gym, mc  multiconnected. S are areas of cross sections; in some cases the corresponding k F values are given in brackets. A 0 , k 0 are the cross section and Fermi quasimomentum for free electrons. Metal
Orbits theor.
SS, , Å2Å2 –2 eexpp. .
(k F, Å1) theor.
mc/m exp.
/m mmc/m theor
Ref.
1. 4 8 1.65 1.82
calc.1472– 149 dHvA 150
1
calc.1472– 149 dHvA 11
Li
eΓ(1) (110) spher. (100) (111)
0.976A 0 0.993A 0 1.011A0
(1.06k 0) (0.98k 0) (0.99k 0)
Na
eΓ(1) spher.
A0
A0
Ca
h(1) eL(2)
calc.151,152 dHvA 153
Sc
hΓ(3,4) eΓk (4) , hMK(4)
calc.154
1
0.032– 2.18
Y
calc.155,156 dHvA 156,157
La
hΓΑ(5), hΓΑ(6) emc(7) eAH(7) , eAH(8)
Ti
hL(3,4),eΓ(5,6) or hΓ(3,4), hA(3), eH(5,6)
0.102– 0.72
0.182– 0.64
Zr
hΓ(3,4) eH(5,6)
0.222– 1.34 2.292– 3.36
2.02– 2.5
V
hΓ(2), hjg(3),
0.242– 0.72
0.322– 0.64
calc.158
0.652– 1.95
1. 6 2 2 . 8 1.6–2.8 0.8, 1.2
calc.1592– 161 dHvA 162 calc.163 dHvA 164,165 calc.1652– 167 dHvA 1682– 171
hN(3), closed Nb
hΓ(2), hjg,N(3) hjg,∆
0.1172– 2.68
0.1382– 1.862
0.572– 1.92
1.122– 1.60
calc.172,173 dHvA 171,174
Ta
hΓ(2), hjg,N(3) hjg,∆
0.2922–– 2.00
0.2792– 2.00
0.842– 1. 6 6
1. 0 9 , 1.35
calc.172,173 dHvA 175
Cr
hH(3), er(4) hrH(5)
(0.1092– 0.226)
(0.172– 0.27)
hH(3) hN(3),eΓ(4), eΓH(5)
0.062– 2.25
– 0.052 2.48
hH(3) hN(3) eΓ(4)
0.0142– 0.43(2π/a)2
12– 1.45 00.06– .062 0.23
Mo
W
78
calc.1762– 181 dHvA 182,183
0.30
0.42– 1.5
0.9 0.252– 1
calc.82,184 dHvA 145, 185,186 calc.177 dHvA 185,187
Band theory Table 2.6. Continued γMn γ– Re
calc 188,189 h(5,6,7) hL(7) eΓA(8) e(9)
0.48 1.18 4.57 6.11 6.6
0 . 4 2  1. 6
hH↑ hN↑ eΓ↓
0.0414.16
0.037 4.16
Co
eΓ↑, eΓ↑ eML↓ eL↓
0.0071. 4 2 0.0254.13
Ni
e(5), e(6) h(3), h(4)
Cu
neck, belly
Ru
eΓ, emc, hΓ, hLM
Os
hLM (7) eΓ (9) eΓ (10) hLM, mc
(0.0570.119)
0.015 0.030 1. 7 1 2 . 19 1.33 1.64 0.73 1.18
Rh
eΓ1 eΓ2 hx1 hx2 hL
1.92 2.5 4.04 5.47 0 . 16  0 . 2 7 0.32 0.46 0.025
2.03 2.46 4.30 0.15 0.25 0.46 0.022
1.43 2.27 3.04 4.35 0.35 0.54 0.91 1.33 0.11
Ir
eΓ1, eΓ2, hx1, hx2 hL
similar to Rh
similar to Rh
1.34 3.02 0.21 1.05
Pd
eΓ(s) hx (d)
2.25 2.58 0 . 10  0 . 7 2
1.34 1.47 0.41 0.7
2.2 0.63 1.91
hmc(d)
0.25, 1.32
2.30 2.59 0.10 0.60 0.05 0.08 0.28 0.24 0.98
1.37, 2.18 9.1, 10.53
2.40 8.1
hL
0.02 0.03
eΓ(s) hopen (d) hclosed (d)
2 . 4 1 3 . 0 0 0.25 1.22 0.004
2.48 3.09 0.25 0.78 0.15
1. 4 2  2 . 0 5 0.91 6.23 0.30
2.06 3.16 1.53 3.62 0.36
calc.215 dHvA 226,227
a axis b axis
0.057 0.63 0 . 0 4 1 0 . 2 1
0.058 0.63 0.044 0.27
1.6 5.3 1.3 4.2
25 90 13 50
dHvA 228
Fe
Pt
UPt3 UPt 3
calc.190 dHvA 191
4 6.7
0.36
0.71
calc.192 194 145 dHvA 195, 196
0.010 . 16
0.1
0.08 0.2
calc.197 200 dHvA 201 203
0.040.75
0.038.03
2.9, 3.7
1 1.9
calc.204 206, dHvA 207 209
0.036A 0 0.98A 0
0.035A 0 0.98A 0
0.41
0.46
calc.210 dHvA 211 calc.11 dHvA 212, 213
0.12 0.2 1.2 1.1 1.5
dHvA 214
calc.215 dHvA 216 219 1.2 0.11 calc.215, 222 dHvA 216 221 calc.215 dHvA 222 225
0 . 8 4 , 1. 2 1
79
Chapter 2 more appreciable with increasing Z in a given period, which agrees with the general statement about increasing the delectron localization. The role of delectrons in the FS formation may be characterized by the value of m c /m. One can see that this quantity increases in each dperiod from left to right. In the beginning of dperiods (up to the Fe column) usually m ctheor /m < 1 (except for Ti where m theor / c m = 1.95), but maximum values of m ctheor /m are considerably larger. The latter fact is apparently connected with effective mass enhancement (electron–phonon, spin fluctuations, etc.) which is not taken into account in band calculations. At the same time, a satisfactory agreement between theory and experiment takes place for cross section areas. Starting from the Co column, large values m ctheor /m = 3.02−10.53 occur, but the experimental values turn out to be smaller (e.g, for Ni, m ctheor /m 8, m exp /m 1.9; the c largest values belong to palladium). This is probably due to the fact that the heaviest electron masses have not as yet been found. Unfortunately, incompleteness of experimental data does not permit to trace a regularity of m c /m values in the periodic table.
Li, Na, Ca To pick out peculiar features of TM, it is instructive to discuss first alkaline metals which are satisfactorily described by the free electron model (FEM). In particular, FEM yields correctly all the FS cross sections and effective masses of sodium (both experimental and theoretical). However, for lithium there exist some deviations, especially in m c values. This is explained by a strong localization of the valence electron in Li near the nucleus, which is due to weakness of nuclear charge screening by the 1s 2 shell (a similar effect takes place for delectrons in TM since their mutual screening is also small). With increasing Z, disagreement with FEM increases and is appreciable for caesium. The band spectrum and Fermi surface of calcium, which stands before dmetals in the periodic system, already differ qualitatively from predictions of FEM. Not all predicted stationary cross sections are experimentally observed. This may be explained by the presence of the abovediscussed DOS peak near the Fermi level. Very strong are the deviations from FEM near the band top. Probably, they are connected with the hybridization with dstates which lie somewhat higher.
80
Band theory
Sc, Y, La Unfortunately, experimental data on delements of first column are poor because of absence of pure samples. Calculated FS of Y and Sc are similar and have multiconnected form with open orbits. They are strongly disturbed in comparison with FEM. Results of various calculations differ considerably, and their verification is difficult because of lack of experimental information.
Ti, Zr, Hf The results of various band calculations demonstrate considerably different results. Thus unambiguous theoretical models of FS are absent for both Ti and Zr. In the work on the dHvA effect in Zr [164], an attempt of interpretation in the nearlyfree electron model was performed. In the papers [159–161], experimental and theoretical cross section and m c /m values for Ti are presented. The calculated FS is very sensitive to small variations of E F position. The maximum value of m exp /m is 2.8. The FS of Hf is not investigated, but theory c predicts its similarity to FS of Zr.
V, Nb, Ta The first attempt to construct the Fermi surfaces of these bcc metals was made in the rigid band model by using the calculation [192] for the bcc Fe. DHvA measurements in Nb and Ta [170, 171] yielded two oscillation periods which were related to holes at the point N. Other periods were attributed to ‘jungle gym’ features. A detailed comparison with theory for Nb and Ta was carried out in [172]. A satisfactory agreement (about 5%) was obtained for the cross sections areas of the types 2 and 3. The holes in the second zone at the point Γ were observed in dHvA experiments [171]. Maximum values of m c /m is 1.8 which agrees with the data on specific heat.
Cr, Mo, W The Fermi surface of chromium is strongly influenced by antiferromagnetism. The spindensity waves are connected with definite pieces of FS [11]. One of recent calculation was performed by Kulikov and Kulatov [181]. Unlike previous papers, appreciable deviations from the sphere were obtained. It was found that the electron masses of the ball orbits exceed considerably those of the ellipsoid orbits. To understand main features of Mo and W, one has to remember that the Fermi level lies at a minimum of the density of states. Thus, 81
Chapter 2 the role of dstates is not so strong as in other TM. Probably, this is the reason for the orbits with large m c /m being absent in both experiment and theory. For all the four FS sheets the values m c /m < 1 are characteristic. The first calculations of FS in Cr, Mo, W used the band calculation for Fe [192]. More recent calculations [176, 177] supported in general the rigid band model. However, because of the strong spinorbital interaction in W, the hole surface h H in the third zone and electron surface e ΓH in the fifth zone vanish or strongly diminish. The LAPW calculation [178] confirms these old results.
Mn, Tc, Re α manganese, which has a complicated cubic structure and is antiferromagnetic at low temperatures, is poorly investigated, as well as radioactive technetium. Band calculations of bcc γ Mn were made in [188, 189]. At the same time, there exist detailed results on rhenium, the theory [190] being in good agreement with experiment. Some uncertainty takes place for open orbits e(8) (cylinder or torus?). Besides m c /m ≅ 2.8, there are very light masses m c /m ≅ 0.07.
Fe, Co, Ni Extensive investigations of FS in Fe and Ni were performed by using dHvA and halvanomagnetic effects. It turned out that the dHvA data may be obtained in a usual way, although the oscillations are periodic in 1/B = 1/(H + 4 π M) rather than in 1/H. However, full picture of the Fermi surface is up to now absent. Experimental data for Fe and Ni are discussed the review [145]. The main conclusion is the corroboration of the itinerant electron ferromagnetism picture: the sum of volumes, corresponding to spin up and down surfaces, agrees with the total number of conduction electrons, and the difference with the magnetization. It should be, however, noted that this conclusion is based not only on experimental results, but uses also some model notions. Besides that, the picture of spinsplit bands is complicated by the spinorbital interaction. The latter results in the degeneracy lift at points of accidental crossing of different spin and orbital subbands. A detailed comparison of the dHvA results for Ni with the theoretical calculations is performed in [145]. The theoretical and experimental pictures demonstrate similarities. The s–d hybridization turns out to be important for understanding the experimental situation. The quasiellipsoidal pocket X 5 has an unusual form which is connected with 82
Band theory the anisotropic interaction with the neighbour X 2 band. The largest experimental mass m c = 1.8m seem to correspond to the X 2↓ pocket. The band calculation yields for the large belly surface in the [001] direction m theor /m ≅ 8 (from the electronic specific heat, m*/m ≅ 10). Unlike Pd and Pt, such large values were not observed in dHvA experiments. The situation with FS of iron is considerably less clear. In particular, no theoretical calculations explain its shape in detail, and there exist several theoretical model to describe this [145]. Calculation of FS of cobalt was performed in [197]. In subsequent papers [198–200] detailed theoretical information on stationary cross sections and effective masses was obtained. Experimentally, a few of dHvA oscillation frequencies were found [201–203]. Two of them, α and β , correspond to cyclotron masses of 0.08m and 0.2m.
Ru, Os DHvA data for ruthenium [212] was interpreted in terms of the rigid band model by using the band structure of rhenium (see also [213]). For osmium, two groups of dHvA frequencies were found which differ by two orders of magnitude [214]. The largest ratio m c/m is 1.5. The dependence mexp /m on the area S turns out to be linear which corresponds c to the quadratic dispersion law E(k).
Rh, Ir, Pd, Pt Despite the difference in the delectron number, it is convenient to combine the d 7 and d 8 metals since they have the same fcc lattice and possess similar properties. Early experiments on the dHvA effect for Rh and Ir [216, 217] and Pd and Pt [223, 224] were interpreted in the rigid band model with the use of results for Cu and Ni. The model of the Fermi surface obtained is shown in Fig.2.29. The calculation in the relativistic APW method was performed in [215]. Comparison of theoretical and dHvA experimental values demonstrates an appreciable enhancement of m c in Pt and Pd for light electron and holes. However, dHvA frequencies corresponding to heavy holes at open sheets (which yield about 80% of N(E F )) with m theor /m = 9.1 and 6.23 were not c observed in early experimental works. Only in the paper [225], the values m c/m = 5.7−8.1 were found for these holes in Pd. These values are still somewhat lower in comparison with the theoretical ones [215] and are by about 15% smaller than those required to explain data on electronic specific heat. At the same time, data on cross section areas [225] agree well with the theoretical predictions. 83
Chapter 2 a
b
Fig. 2.29. The Fermi surface of Pd (a) electron surface at the point Γ (b) of multiconnected hole tubes [11].
RARE EARTHS AND ACTINIDES Fermi surfaces of 4f and 5fmetals were calculated in a number of works (see [11]). On the other hand, direct experimental data are not numerous. DHvA measurements in ytterbium [229] demonstrated the presence of hyperboloid pieces of FS. DHvA investigations of gadolinium [230] yielded the estimation of spin splitting ∆=0.57 eV. Provided that 4fstates (that lie as a rule well below the conduction band) are not taken into account, FS of all the rare earth metals should be similar for the same crystal lattice. A FS model for the hcp structure which describes Gd and Tb is presented in Fig.2.30. The Fermi surface lies within third and fourth zones and is multiconnected. The shape of Fermi surface is in general similar to that of yttrium. At passing to heavy rare earths, changes occur which are connected with the degeneracy lift at some Brillouin zone points owing to the relativistic interactions. According to [231], these interactions result in that the ‘arms’ at the point M vanish, and the ‘arms’ at the point L touch, so that the similarity with FS of yttrium increases. Thus, one may expect that, at increasing atomic number, the Fermi surfaces of heavy hcp rare earths change their shape between those of Gd and Y. A number of attempts were made to use information on FS in rare earths for considering concrete physical effects. This explains the complicated noncollinear magnetic structures (Sect.4.7). 84
Band theory a
b
Fig. 2.30. (a) Theoretical model of the Fermi surface of gadolinium by Freeman, Dimmock and Watson (b) The Fermi surface of Tb in the oneband scheme: hole surface in the third zone and the electron surface in the fourth zone [11].
Actinides (5felements) have been investigated still less than rare earths. Unlike 4felectrons, 5felectrons, at least in light actinides, are delocalized and take part in the electron spectrum near the Fermi level. First FS calculations within the relativistic APW method for Th and Ac were performed in [232]. DHvA data for thorium, obtained in [233], were used to construct an empirical FS model. The latter contains a nearly spherical sheet at the centre of the zone and six closed sheets at the points X along the (100) directions. This model turned out to contradict the band calculation [140]. Some contradictions were eliminated in the subsequent calculation [234].
85
Chapter 3
Chapter 3 THERMODYNAMIC PROPERTIES 3.1 COHESIVE ENERGY AND RELATED PROPERTIES Condensation of atoms from the gaseous states into liquid and solid ones occurs due to various interatomic forces. The main contribution to binding energy comes from valence electrons which have large orbit radii, so that the wavefunctions at different lattice sites overlap appreciably. For metals, the valence electrons become itinerant and propagate freely in a crystal, the energy gain being determined by their interaction with positively charged ions. As discussed in Chapter 1, delectrons (and sometimes felectrons) in transition group metals exhibit the behaviour which is intermediate between the localized and itinerant one. In particular, the collapse of d and forbits in the beginning of periods takes place, which is accompanied by formation of highenergy states in the potential well (Fig.1.2). For delements the energy is close to that of valence spelectrons (although the radius of dshell is much smaller than the radii of sporbits). For 4felectrons the well is much deeper, so that they may contribute appreciably to the binding energy only at the beginning of period, e.g., for cerium. From the thermodynamical point of view, the total cohesive energy may be experimentally determined from the Born–Haber cycle. Thus main physical characteristics of the binding energy are the melting and boiling temperatures, T m and T b , and heats of fusion and sublimation, ∆H f and ∆H s . Besides that, the stability of the crystal is characterized by the density (or atomic volume Va), ionization potentials, work function, Debye temperature, elastic moduli, activation energy for diffusion, specific heat etc. The corresponding values may be found in reviews and standard handbooks, e.g., [235–239]. Some of these quantities for d, 4f and 5fmetals are presented in Tables 3.1–3.3 and shown in Figs.3.1–3.8. As follows from comparison of the values of T m for dmetals with those for preceding and following spelements, delectrons yield an appreciable contribution to the binding
86
Melting point, K
Thermodynamic properties
Group Fig. 3.1. Melting points of the IV, V and VI period elements of the periodic table [235].
energy. At the same time, the entropy change at melting ∆S m in dmetals differs weakly from that in simple metals. In the periodic table, values of ∆S m vary in a wide region (from 0.47 kcal/mol K for white phosphorus to 7.13 kcal/mol⋅K for Si). However, these regions become narrow for element groups with a given lattice: ∆S m (in kcal/mol⋅K) equals to 1.76 ± 0.34 for bcc crystals, 2.28 ± 0.23 for fcc crystals, 2.33 ± 0.23 for hcp crystals and 6.50 ± 0.23 for the diamond structure [235]. The change of the thermodynamic and lattice parameters in the dseries enables one to investigate the dependence of the contribution of delectrons on their number n. The strongest influence of delectrons may be seen in the beginning of dperiods. The atomic volume decreases sharply (almost by two times) at passing from Ca to Sc, which is connected with the collapse of dorbits. With further increasing n, V a continues to decrease, but increases in Cu and Zn 87
Melting point, kcal/gatom
Chapter 3
Group Fig. 3.2. Heat of fusion of the IV, V and VI period elements of the periodic table [235]. Open points are estimated values.
where the dshell is completely filled. The values of the thermodynamic characteristics T m, T b , ∆H f and ∆H s , and elastic moduli of dmetals also exceed corresponding values for simple metals and demonstrate a smooth ndependence. However, unlike Va, these quantities have maxima in the middle of 3dperiod (between V and Mn for different characteristics; a similar situation takes place for 4d and 5dperiods). We shall see in following Chapters that purely electronic characteristics (electronic specific heat coefficient γ and paramagnetic susceptibility χ ) have a quite different (oscillating) ndependence. The simplest explanation of such a behaviour of the thermodynamic properties is the existence of several different factors which influence the total energy. In particular, with increasing number of 88
Thermodynamic properties Table 3.1. Atomic volume V a , Debye temperatureΘ D, melting point T m, boiling point T b , linear coefficient of the thermal expansion α , self, selfdiffusion activation energy Q, heat of fusion ∆H f, cohesive energy ∆H 0, Young's modulus Y, shear modulus µ, Poisson's ratio σ , bulk modulus B, Leibfried, modified Leibfried and Bragg numbers, L, L' and B, for 3d, 4d and 5d transition metals and neighbour elemets. For some metals, estimated values are presented [235, 238] 3d 4d 5d
V a, cm3/mol ΘD, K
TTmm, , K TTbb,, K
α · 106, K K2–11
Ca Sr Ba d0 d0 d0 25.9 33.9 38.1 234 147 110 1112 1045 998 1765 1645 1910 22.4 20 18.8
Sc Y La d1s2 d1s2 d1s2 15.0 19.9 22.5 470 268 142 1812 1775 1193 3537 3670 3 7 13 10 . 0 12 . 0 10 . 4
2.07 2.19 1.83 42.1 39.3 42.8 0.20 0.14 0.13 0.07 0.05 0.05 0.31 0.3 0.28 0.15 0.12 0.10 4.80 4.90 4.44 4.28 4.36 3.96 4.21 4.84 3.84
61.1 40.8 3.70 2.73 1.48 80.1 97.6 10 2 0.81 0.66 0.39 0.32 0.26 0.15 0.27 0.2 0.29 0.58 0.37 0.25 3.20 2.88 2.95 2.85 2.56 2.63 3.08 2.09 1.73
Q · 103, kcal/mol ∆Hf, kcal/mol ∆H0 kcal/mol YY · 1102–66, kg/cm3 3 kg/cm
µµ · 1 02–66,, kg/cm kg/cm2 2 σ BB · 1102–66,, kg/cm2 2 kg/cm L
L'
B
Ti Zr Hf d2s2 d2s2 d2s2 10.6 14 . 0 13 . 4 426 289 256 19 4 1 2 13 3 2495 3586 4650 4575 8.35 5.78 6.01 48.8 52.0 43.7 3.42 3.74 4.39 112 14 6 14 5 1.08 0.94 1. 4 0 0.40 0.35 0.54 0.34 0.3 3.30 1.07 0.85 1.11 3.42 3.69 2.91 3.04 3.29 2.59 2.84 3.06 2.42
V Nb Ta d3s2 d 4s d3s2 8.5 10.8 10.8 326 241 247 2178 2741 3271 3582 4813 5760 8.3 7.07 6.55 9 1. 5 98.0 10 0 3.83 4.82 5.76 12 2 17 4 18 7 1.34 1. 0 7 1.85 0.47 0.38 0.70 0.36 0.35 0.35 1. 6 5 1. 7 4 2.04 4.66 5.62 3.67 4.15 5.00 3.27 3.86 4.66 3.05
Cr Mo W d 5s d 5s d4s2 7.23 9.39 9.55 598 459 388 2148 2888 3653 2918 5785 6000 8.4 4.98 4.59 73.2 96.9 120 3.47 6.66 8.42 94.5 15 7 200 2.48 3.34 4.05 1.19 1.18 1. 5 6 0.21 0.30 0.28 1.94 2.78 3.30 2 . 12 2.21 2.08 1. 8 8 1.97 1.85 1.61 2.40 2.26
89
Mn Tc Re d5s2 d5s2 d5s2 7.39 8.63 8.86 418 351 429 1512 2443 3433 2368 5300 6035 22.6 8.06 6.63
Fe Ru Os d6s2 d 7s d6s2 7.1 8.18 8.44 457 600 500 18 0 8 2553 3300 3 16 0 4325 5300 11.7 9.36 4.7 64.0
Co Rh Ir d7s2 d 8s d7s2 6.6 8.29 8.52 452 480 425 1765 2233 2716 3229 3960 4820 12.4 8.40 6.63 6 1. 9
3.50 5.42 7.86 66.9 152 186 2.02 3.76 4.7 0.78 1. 4 5 1. 8 2 0.24 0.29 0.29 0.61 3.03 3.79 2.24 1. 6 5 1. 8 0 2.00 1.93 2.11 2.44 1.73 1.95
3.67 5.67 7.56 99.4 154 187 2.14 4.20 5.50 0.83 1. 6 3 2.14 0.28 0.29 0.28 1. 7 2 3.27 4.26 2.60 1.62 1. 5 5 2.32 1.90 1.81 2.49 1.70 1.67
3.70 4.96 6.22 102 133 159 2.10 3.70 5.38 0.78 1.50 2.14 0.33 0.27 0.26 1.95 2.76 3.62 2.87 1. 5 2 1.26 3.35 2.78 1.47 2.84 1.59 1. 3 6
Ni Pd Pt d8s2 d10 d 9s 6.59 8.88 9.09 427 283 234 1726 1825 2042 3055 3200 4 10 0 12 . 7 11.5 8.95 67.0 63.5 66.8 4.21 4 . 10 4.70 102 89.9 13 5 1. 9 7 1. 2 6 1.74 0.76 0.52 0.62 0.30 0.37 0.38 1.90 1.84 2.84 2.90 3.34 3.06 3.39 3.90 3.57 3.84 3.54 3.32
Cu Ag Au d10s d10s d10s 7.09 10 . 3 10 . 2 342 228 165 1356 1234 1336 2811 2468 3240 16.7 19.9 14.1 48.9 45.8 39.4 3.12 2.78 2.95 80.8 68.3 87.6 1.26 0.82 0.74 0.46 0.29 0.28 0.34 0.37 0.42 1.33 1.03 1.77 3.51 3.49 3.94 4 . 10 4.07 4.61 3.81 3.70 4.11
Zn Cd Hg d10 d10 d10 9.17 13.0 14 . 1 316 352 75 692 594 234 1175 1038 630 29.7 30.6 61 23.9
1.76 1.48 0.55 3 1. 0 26.8 15 . 4 0.94 0.63 0.28 0.38 0.25 0 . 10 0.29 0.30 0.36 0.61 0.48 0.29 1.69 3.51 1. 9 7 4 . 10 2.03 3.81
Chapter 3 Table 3.2. Atomic volume V a (cm 3 /mol), Debye temperature Θ D (K), melting point T m (K), boiling point T b (K), linear coefficient of thermal expansion α (10 –6 K –1 ), heat of fusion ∆H f (kcal/mol), cohesive energy ∆H 0 (kcal/mol), Young's modulus Y (10 6 kg/cm 2 ), shear modulus µ (10 6 kg/cm 2 ), Poisson's ratio σ , bulk modulus B (10 6 kg/cm 2 ) for rare earth metals [235].
Va ΘD Tm Tb ∆Hf ∆H0
α Y
µ σ B
Va ΘD Tm Tb ∆Hf ∆H0
α Y
µ σ B
La
Ce(γ)
Pr
Nd
Pm
Sm
Eu
f 0d
f 1d
f3
f4
f5
f6
f7
22.54 142 1193 3713 1.48 101.9 10.4 0.387 0.152 0.288 0.248
17.03 146 1070 3972 1.24 97.9 8.5 0.306 0.122 0.248 0.244
20.82 85 1208 3616 1.65 85.8 6.79 0.332 0.138 0.305 0.312
20.59 159 1297 2956 1.71 75.9 9.98 0.387 0.148 0.306 0.333
20.33 158 1308 2730 1.94 64 9.0 0.43 0.17 0.278 0.360
19 . 9 5 116 13 4 5 2 14 0 2.06 50.2 10 . 8 0.348 0 . 12 9 0.352 0.300
28.98 127 10 9 9 1971 2.20 42.9 33.1 0 . 15 5 0.060 0.286 0 . 15 0
Gd
Tb
Dy
Ho
Er
Tm
Yb
f 7d
f 8d
f 10
f 11
f 12
f 13
f 14
19.94 170 1585 3540 2.44 82.7 8.28 0.573 0.227 0.259 0.391
19.26 150 1629 3810 2.46 89.9 10.3 0.586 0.233 0.261 0.407
18.99 172 1680 3011 2.49 66.9 10.0 0.644 0.259 0.243 0.392
18.75 144 1734 3228 3.38 70.5 10.7 0.684 0.272 0.255 0.404
18.46 134 17 7 0 3000 2.62 70.7 12.3 0.748 0.302 0.238 0.419
18.13 127 1818 2266 4.22 58.3 13 . 3 0.77 3.31 0.235 0.405
24.87 118 10 9 7 19 7 0 1. 8 3 40.3 24.96 0 . 18 2 0.071 0.284 0 . 13 5
delectrons, dlevels become lower, so that the participation of dstates in the cohesion decreases. Besides that, the Coulomb repulsion among delectrons also increases with n. In the simple Friedel model the electron energy (2.84) has a minimum at n = 5, i.e. for the halffilled dshell. This result is explained by that the energy of delectrons decreases for the lower half of the dband and increases for the upper one. Such a picture is in agreement with the situation of 3d, 4d and 5d periods except for an appreciable deviation for manganese. Since the dband width W d is inversely proportional to some power 90
Thermodynamic properties Table 3.3. Atomic volume V a (cm 3 /mol), Debye temperature Θ D (K), melting point T m (K), boiling point T b (K), linear coefficient of thermal expansion α (10 –6 K –1 ), heat of fusion ∆H f (kcal/mol), cohesive energy ∆H 0 (kcal/mol), Young's modulus Y (10 6 kg/cm 2 ), shear modulus µ (10 6 kg/cm 2 ), Poisson's ratio σ , bulk modulus B (10 6 kg/cm 2 ) for 5felements [235].
Va ΘD Tm Tb ∆Hf ∆H0
α Y
µ σ B
Ac
Th
Pa
U
Np
Pu
Am
Cm
Bk
Cf
f 0d 1
f 0d 2
f 2d 1
f 3d 1
f 5d 0
f 6d 0
f 7d 0
f 7d 1
f 8d 1
f 10d0
22.56 124 1323 3200 3.03 104 14.9 0.35 0.138 0.269 0.25
19.79 170 2024 4500 3.56 136.7 11.2 0.76 0.284 0.285 0.553
15.03 159 1698 4680 2.99 132 7.3 1.02 0.398 0.282 0.078
13.16 200 1404 3950 2.47 125 12.6 1.90 0.75 0.245 1.007
13.11 121 910 4150 1.60 113 27.5 1.02 0.406 0.255 0.694
12.06 171 913 3727 0.68 91.8 55 0.98 0.446 0.15 0.546
17.78
12.8
1473
913
7.5
of the interatomic distance r 0 , a dependence with a maximum for n = 5 should take place for the compressibility which is determined in terms of dW d /dr 0 . An attempt to explain the anomaly of E coh in Mn with account of the correlation effect were performed by Oles [240]. He started from the earlier paper [241] where the cohesive energy was estimated as the energy difference between the atomic limit and condensed state. We illustrate the idea of this explanation in the simplest case of sband where the estimation gives
n n n2 Ecoh = 1 − W − U , (3.1) 2 2 4 where U is the Hubbard parameter, n < 1. The expression (3.1) has a maximum at band filling
W ¿725)
103
Chapter 3 1.58 n < 1.66. Finally, the hcp ε phase becomes stable at n = 1.75. A geometrical interpretation of this regularity may be obtained by considering the position of the Fermi surface in the reciprocal space with respect to the Brillouin zone boundaries [249]. Appearance of an energy gap in the electron spectrum near the Fermi level, which takes place near these boundaries, is energetically favourable. Indeed, it results in lowering of the electron system total energy since the energy of occupied states becomes lower. In the onedimensional case, this effect results in distortion of a lattice with the formation of an insulating state (Peierls instability). Calculating the volume of the sphere, which is inscribed into the first Brillouin zone, we obtain the electron numbers n = 1.36 for the fcc lattice, 1.48 for the bcc lattice and 1.69 for the ideal hcp lattice in a satisfactory agreement with above experimental data. Thus the HumeRothery rule relates the stability of a crystal structure to the touching of the Fermi surface with the Brillouin zone boundary where electron spectrum is maximally disturbed. Unfortunately, justification of this rule for simple metals within the qualitative band theory in the nearlyfree electron approximation (pseudopotential theory) meets with difficulties: the singularity in the total energy turns out to be very weak in the threedimensional situation (see discussion in [55]). However, one may expect that the influence of Brillouin zone boundary becomes appreciably stronger if density of states peaks are present near the Fermi surface. For transition dmetals, the HumeRothery rule usually does not hold (at the same time, it may be applicable for rare earth alloys [16]). A different concept of correlation between crystal structure and n was put forward by Engel and Brewer (see [250, 251]). According to their theory, the type of lattice is determined by the number of s,p electrons. So, Na, Mg and Al, which possess one, two and three spelectrons respectively, have bcc, hcp and fcc lattices. An attempt was made to generalize this concept to dmetals. In particular, the configuration d 5 s (the same as for isolated atoms) is attributed to metals of the middle of dperiods (Cr, Mo, W) with the bcc structure. Formation of the same structure in V and its analogues is explained by high statistical weight of the d 4 sconfiguration (unlike isolated atoms). The hcp structure in the metals of III and IV groups corresponds to dominating role of configurations dsp and d 2sp respectively. The difference between bcc structure of iron (configuration d 7 s) and hcp metals Ru and Os is related to strong s–d hybridization in the former. At the same time, the applicability of the Brewer–Engel picture is rather restricted, so that it was criticized [251, 252]. Especially 104
Thermodynamic properties unsatisfactory is this theory for fcc metals. In particular, it yields incorrect predictions for alkaline earths Ca and Sr (s 2 configuration) and noble metals Cu, Ag, Au which have one selectron. Generally, the supposition that delectrons take part in chemical bonding but do not influence the lattice symmetry does not seem to be physically reasonable. Of course, the direct calculation of the total energy from the real band electron spectrum is more justified for predicting stable structures, although this requires picking out small energy differences for various structures (of order of 10 −2 −10 −1 eV) on the background of large binding energy (of order of 10 eV). As a rule, such differences are smaller than real accuracy of band calculations. In particular, manyelectron effects should give appreciable contributions and be taken into account in a quantitative theory of crystal structures. The problem of structural transitions at finite temperatures is still more complicated since the density functional approach becomes, generally speaking, inapplicable, and collective excitations of the lattice and electron subsystems should contribute to the entropy term. However, standard band calculations were rather successfully applied in the theory of crystal structures. Stability of the bcc phase in the middle of the dperiods is connected with double peak structure of the density of states for this lattice. Maximal energy gain is achieved at filling of the lower peak. As follows from band calculations [24, 78], this peak is filled in vanadium at n d 4 (which is by unity larger than in free V atom). For fcc and hcp lattices, the density of states has a more complicated manypeak structure, so that they should be stable at the beginning or end of dperiods. From the atomic level point of view, one may consider in cubic lattices the states which have e g and t 2g origin. The e gstates lie lower than t 2g ones in the fcc lattice and higher in the bcc lattice. Since the e g band contains four electrons and the t 2g band six electrons, the fcc structure should be favourable up to n d = 4, and the bcc structure at n d between 4 and 6. This agrees to some extent with the situation in the 3dperiod (the bcc structure between Ti and Fe). However, Sc and Ti (n d < 4) have the hcp (rather than fcc) structure, the stability of which is not described in terms of t 2g  and e gstates. Pettifor [253] calculated the energies of three basic structures (fcc, bcc and hcp) the 3dmetal series within the model pseudopotential approach with two dresonance parameters. The stability of the crystal structures as a function of the number of delectrons n d = n−2 is described by the following sequence 105
Chapter 3
hcp fcc
bcc
dfilling, states/atom Fig. 3.12. Structural energy differences µ S 2 ∆ (∆ = E bcc(hcp)–E fcc , µ is the dband mass, S is the atomic Wigner–Seitz radius), obtained from canonical dbands, as a function of the canonical d occupation [245].
bcc
fcc
dhcp
hcp
dfilling, states/atom Fig. 3.13. Structural energy differences obtained from canonical dbands as functions of the canonical doccupation in the n d range, corresponding to the lanthanide crystalstructure sequence [245].
nd Structure
1 − 1.5
1.5 − 2
2 − 4.5
4.5 − 6.5
fcc
hcp
bcc
hcp
6.5 − 7.9 fcc
These results just correspond to the experimental situation in the 3drow. 106
Thermodynamic properties
fcc
hcp
fcc
dhcp
hcp dhcp
bcc
hcp
bcc Canonical theory (selfconsistent) (conventional)
bcc
hcp
hcp
bcc
bcc
hcp
hcp
fcc
fcc
Experiment
Filling n d . states/atom
dhcp
Fig. 3.14. Diagram of the most stable closepacked crystal structure as a function of the doccupation number. Two estimates of the actual doccupation numbers for the dmetals together with the experimental crystal structures are given below [245].
bcc
fcc
hcp fcc
Fig. 3.15. Structural energy differences for 3d, 4d and 5d rows calculated at the experimentally observed equilibrium volume and plotted as functions of the doccupation numbers [245]. 107
Chapter 3
bcc
fcc
hcp fcc
Fig. 3.16. Calculated bccfcc and hcpfcc structural energy differences (solid and broken lines) for the 4dmetals [245] compared with the enthalpy differences derived from phasediagram studies (open circles).
Skriver [245] evaluated the energy differences for various lattices in the 3d, 4d and 5d series and for rare earths (Figs. 3.12– 3.16), and also for actinides, by using the force theorem approach in the LMTO method. The results by Pettifor were confirmed, and general sequence hcp–bcc–hcp–fcc in other dperiods was also reproduced. Investigations of stability of crystal structures in the lanthanide series yielded the sequence hcp − Smtype − double hcp − fcc − fcc′ The type of the lattice is determined by the number of 5delectrons which is changed from 2 (La) to 1.5 (Lu) (Fig.3.14). The oneelectron band calculations [245] turn out to agree qualitatively with experimental data and give correctly the crystal structure of 35 metals from 42 investigated (in particular, the theory fails for Au, 108
Thermodynamic properties Mn, Fe and Co). As to quantitative agreement (values of the phase diagram parameters, e.g. transition temperatures and pressures), the problem is considerably more difficult, so that satisfactory results are obtained for simple metals only. The calculated energy differences for dmetals [245] turn out to be by 3−5 times greater than enthalpy differences obtained from study of binary phase diagrams (Fig.3.16). Structural and cohesive energies of 5delements were calculated in [254] within the linear augmentedSlatertypeorbital method. Recent calculation of total energies for 3d, 4d and 5d metals [255] was performed by scalar (semirelativistic) RAPW method (unlike the calculations by Skriver [245], the frozen potential approximation was not used). The conclusions agree on the whole with the results for lattice parameters and bulk moduli [24] and crystal structure stability [245], relativistic corrections being not too important. However, the experimental structure for Au was obtained in this calculation. Total energy calculations of crystal structure stability, equilibrium volume and bulk moduli for light actinides Th, Pa and U within the fullpotential approach [256] yielded good agreement with experimental data.
3.3 SPECIFIC HEAT In the previous sections of this Chapter we have treated energy characteristics of a crystal which yield a general description of the electron and ion systems. Here we consider the specific heat, which enables one to obtain a more detailed information about electron and lattice spectrum. 3.3.1 Lattice specific heat Investigation of specific heat played an important role in the development of quantum solid state theory. We remind briefly of principal results. Specific heat at constant volume is defined in terms of the average energy
∂E CV = . (3.19) ∂T V In the classical picture, each degree of freedom of a particle contributes k BT/2 to the thermal energy. Thus the energy of a threedimensional crystal which contains N ions and n electrons is given by
109
Chapter 3
3 E = 3NkBT + nkBT (3.20) 2 (the average energy of ions, which are considered as oscillators, is doubled owing to potential energy). Thus, the lattice specific heat of a monoatomic crystal should be equal to 3R (R = k B N A = 8.3 J/mol ⋅ K is the gas constant, N A is the Avogadro number). This result corresponds to the Dulong–Petit law which was established for a wide number of solids. However, experimentally this law holds as a rule in a not too wide region near the room temperature. With decreasing temperature, C V decreases and tends, in agreement with the general Nernst theorem, to zero at T → 0. On the other hand, C V increases considerably at high T. The quantum theory of lattice contribution to specific heat was developed by Einstein (1906) and Debye (1910). Einstein considered the crystal as a system of independent oscillators with the constant frequency ω E . Then application of the Bose statistics yields 1 E = 3N ω E N B (ω E ) + , 2
(3.21)
with −1
ω − 1 . N B (ω ) = exp kBT
Then 2
2
ω ω ω CV = 3R E exp − E exp − E − 1 . (3.22) kBT kBT kBT Thus specific heat equals to 3R at high temperatures and is exponentially small at low T. Experimental data demonstrate a more slow decreasing of specific heat. This is due to that the Einstein model is well applicable only for optical branches of lattice oscillations (phonons), frequencies of which depend weakly on the wavevector. The calculation of acoustic branch contribution with the model dispersion law
ωq = sq ( q < qD ),
ω D = sqD = kBθ D /
(3.23)
was performed by Debye. The result reads 3
θ /T
T D ez z4 CV = 3R 3 ∫ z dz. (3.24) 2 θ D 0 (e − 1) At high T we come again to the Dulong–Petit law. At low T T m) − C(T 0 for Zn, Cd, Al, Ga, In, Pb despite the absence of structural phase transitions. In the liquid phase, specific heat of dmetals may reach the values of (4−9)R, which are considerably larger than those for simple metals (see, e.g., the discussion in [258]). The increase of C in comparison with 3R, observed above the room temperature in most substances, is usually attributed to anharmonicity effects which result in occurrence of Tlinear terms in the hightemperature lattice specific heat. We illustrate this phenomenon in the simplest onedimensional model with the potential (3.10) (a more detailed discussion is given in [4]). Write down the partition function of an ion as p2 Z (T ) = ∫ exp − + V (u ) kBT dpdu. (3.26) 2M Integrating over momentum p and expanding in the anharmonicity parameters up to b 2 and c we derive
112
Thermodynamic properties
au 2 Z (T ) = (2π kBTM )1/2 ∫ exp − × 2kBT bu 3 1 bu 3 2 cu 4 (3.27) du. × 1 + + + kBT 2 kBT kBT Integration over u yields 1/2 3c 15b 2 M Z (T ) = 2π kBT 1 − 2 − 3 kBT . a a a
(3.28)
Then the specific heat is given by 6 5b 2 c ∂ 2 ∂ ln Z (T ) T = 3 R 1 + 2 − kBT . (3.29) ∂T ∂T a a 2a Since a/b ~ b/c ~ d and the average displacement is given by (3.11), the Tlinear corrections owing to triple and quartic anharmonisms are of the same order of magnitude and may be estimated as – /d)3R. Therefore the anharmonicity may hardly explain the increase (u of specific heat at high temperatures in dmetals, which may be of order 100%, so that this problem needs further investigations. C (T ) = −3 N A
3.3.2 Electronic specific heat Besides the violation the Dulong–Petit law at low temperatures, the second difficulty of the classical theory of specific heat concerned the electronic contribution to specific heat. According to (3.20), this contribution should be equal to 3R/2 for a metal with one electron per atom. However, such large contributions were never found in experiment. Only a small Tlinear electron term in specific heat is observed practically at any temperatures. This contradiction was resolved only in twentieth years of our century after formulation of the Fermi–Dirac statistics for electrons. The corresponding distribution function reads −1
E −ζ f ( E ) = exp + 1 , (3.30) kBT where ζ = ζ (T) is the chemical potential, ζ (0) being equal to the maximum energy of occupied states – the Fermi energy E F. The latter quantity is determined, according to the Pauli principle, by the number of electrons:
113
Chapter 3 ∞
n=
∫ f ( E ) N ( E )dE
(3.31)
−∞
(in this Section the density of states N(E) is determined for both spin projections). In metals, E F /k B is large and makes about 10 4 −10 5 K. This explains the qualitatively small value of electronic specific heat. Indeed, only electrons in a narrow layer with a width about π k BT near the Fermi energy may change their energy and take part in thermal excitations, and most electrons are ‘frozen’. The number of the ‘thermal’ electrons is estimated as
n* /n ∼ kBTN ( EF ) ∼ kBT/EF ,
(3.32)
so that
3 2
δ Ee (T ) ∼ n*kBT ∼ kB2T 2 N ( EF ),
(3.33)
and
Ce ∼ kB2 N ( EF )T . A more accurate calculation (see below (3.40)) yields Ce = γ T ,
γ=
π2
kB2 N ( EF ).
(3.34) 3 Thus electronic specific heat should be linear in a wide temperature interval 0 Ei .
δ N (E ) =
Unlike the expansion (3.40), the relative temperature variation of
γ (T ) =
1 ( I 2 − I12 /I 0 ), 2 T
(3.42)
with ∞
∂f ( E ) N (E) − (3.43) dE. ∂E −∞ may be large. Using the position of the peaks E i and the jumps of N'(E) at these points as parameters, one can restore from the experimental dependence of γ the density of states and compare this with the calculated one. Such an analysis was performed in [264] for the A15 structure superconductors Nb 3 Sn and V 3 Si. Besides the oneelectron mechanism, the dependence γ (T) is determined by the abovediscussed temperature dependences of electronphonon enhancement and correlation mechanisms which are expected to be rather strong for dbands. The relative role of these effects in transition metals is still not investigated in detail. In =
∫ (E − E )
n
F
3.3.3 Specific heat of magnetic metals In magnetically ordered crystals, contributions to entropy and specific heat occur which are due to destruction of magnetic ordering with increasing temperature. Experimental separation of the magnetic entropy may be performed with the use of magnetocaloric effect (change 120
Thermodynamic properties of temperature at adiabatic magnetizing by the external magnetic field) [265]. In the model of localized spins with the value S the total magnetic entropy change is given by ∞
Smag (T → ∞) = ∫ 0
Cmag (T ) T
dT = R ln(2 S + 1).
(3.44)
C p , J/(kg·K)
The magnetic specific heat C mag is especially important at the magnetic phase transition points T M = T C (T N) where it has a singularity. In the simplest meanfield approximation C mag is exponentially small at
C p , J/(kg·K)
Fig. 3.25. Experimental specific heat of iron [239].
Fig. 3.26. Experimental specific heat of nickel according to the data of various authors [239]. 121
Chapter 3 low temperatures, exhibits a jump at crossing T M and vanishes in the paramagnetic region, so that expression (3.44) holds at arbitrary T > T M . In fact, the presence of shortrange order, which is neglected in the meanfield theory, results in that C mag is finite above T M due to interaction with spin fluctuations. Besides that, fluctuations result in a weak powerlaw divergence of C mag at T M . The experimental temperature dependences of specific heat in ferromagnetic transition metals are shown in Figs.3.25, 3.26. At low temperatures (well below TM) there exist contributions owing to spinwave (magnon) excitations (Appendix E). The corresponding average energy is given by
Esw (T ) = ∑ωq Nq , q
(3.45)
with ω q being the magnon frequency. Since in ferromagnets ω q ~ q 2 at q → 0, we have (3.46) Esw (T ) ∼ T 5/2 TC3/2 , Csw ∼ (T TC )3/2 . At the same time, for antiferromagnets the dispersion law is linear and we have (3.47) Esw (T ) ∼ T 4 TN3 , Csw ∼ (T TN )3 . The spinwave contributions are present both in magnetic insulators and metals. In metals the linear electronic specific heat dominates at low temperatures and the spinwave corrections are less important. However, the electronic contribution is appreciably influenced by magnetic ordering. Since an enhancement of the linear γ Tterm takes place due to interaction with spin fluctuations (Sect.4.4), the strict separation of magnetic and electronic contributions is, generally speaking, impossible. Some peculiar terms in specific heat of conducting ferromagnets which are due to incoherent (nonquasiparticle) contributions are discussed in Appendix G. The electron density of states in the ordered phase of ferromagnetic metals (below Curie temperature T C) differs considerably from that in the paramagnetic phase because of spin splitting. As a rule, total N(E F ) = N ↑ (E F ) + N ↓ (E F ) is smaller in the ferromagnetic state since the ordering results in a shift of the peak, which is responsible for the Stoner instability, from the Fermi level. At the same time, in nickel the value of γ (T T C ) = 5.8 mJ/mol ⋅ K 2 [267]. This leads to the conclusion about an important role of correlation effects. Consider the simplest theory of magnetic specific heat. In the meanfield approximation the magnetic (exchange) energy is expressed in terms of magnetization 122
Thermodynamic properties Emag = − IM 2 ,
(3.48)
where I is an exchange parameter. Then the magnetic specific heat reads
dM . (3.49) dT In metals one has to take into account, besides the exchange energy, the kinetic energy of conduction electrons which depends on magnetization through the exchange splitting. The total energy in the Stoner model (see Sect.4.3) may be transformed as Cmag = −2 IM
E = ∑Ek nkσ + In↑ n↓ = ∑Ekσ nkσ − In↑ n↓ = kσ
kσ
n2 (3.50) = ∑ ∫Ef ( E ) Nσ ( E ) dE − I − M 2 , σ 4
where
nσ =
n +σ M, 2
Ekσ = Ek − σ IM ,
1 N ( E + σ IM ). 2 Differentiating with respect to T one obtains Nσ ( E ) =
(3.51)
N ′ (E ) dM , (3.52) − ↓ F T 2I 6 N ↑ ( EF ) N ↓ ( EF ) dT where C σ (T) is the usual electronic specific heat, corresponding to the density of states N σ (E). One can see that the term of the type (3.49) is canceled by the corresponding contribution from the kinetic energy. The magnetic specific heat is determined by the second term in (3.52). Only electrons in the energy layer of order of T near the Fermi level contribute to C mag so that it contains a small factor of order of (k BT/E F) 2 and depends strongly on the DOS shape. The jump of specific heat at the Curie point is given by [26] C (T ) = C↑ (T ) + C↓ (T ) +
∆C =
π 2 N ↑′ ( EF )
2 ∂ζ (π TC ) 2 N ′( EF ) + I 2 MN ′′( EF ) 3 ∂M T =TC
(3.53)
The situation may change somewhat in the presence of DOS peaks. Consideration of specific heat of Ni with account of the realistic DOS structure is performed in [268]. As well as in the Heisenberg magnets, spin fluctuations result in a considerable modifications of C mag behaviour at high temperatures [26, 268]. 123
Chapter 4
Chapter 4 MAGNETIC PROPERTIES Strong magnetism is one of the most important peculiarities of transition d and felements. Iron group metals (Fe, Co and Ni) exhibit ferromagnetic ordering and large spontaneous magnetization, chromium and manganese are antiferromagnetic–magnetic moments are ordered, but the summary magnetization is zero. Ferro and antiferromagnetism are characteristic for most rare earth metals. Many alloys and compounds of transition metals also possess strong magnetic properties and have wide technical applications. The basic magnetic characteristics of strongly magnetic substances are as follows • the value of magnetic moment in the ground state • behaviour of spontaneous magnetization with temperature and magnetic field; values of the ordering temperature T C (TN) and magnetic anisotropy constants; the saturation field H a • the type of temperature dependence of magnetic susceptibility (Pauli or Curie–Weiss) and its anisotropy; presence of local moments above T C; values of the effective moment (Curie constant) and paramagnetic Curie temperature. All these characteristics are described by some microscopical parameters (value of atomic magnetic moment in the localized model of magnetism or the exchange splitting in the itinerant electron model, exchange parameters, spinorbital interaction constant). The main purpose of the theory is comparison of these parameters with observable physical properties. At present, alternative and in some respects contradicting explanations of transition metal magnetic properties exist, and the problem of their strong magnetism is far from the final solution.
124
Magnetic properties
4.1 EXCHANGE INTERACTIONS AND THE HEISENBERG MODEL FOR LOCALIZED SPINS The history of theoretical investigation of ferromagnetism was rather dramatic. First attempts to explain this phenomenon gave rise to development of the theory of exchange interactions within the Dirac–Heisenberg model for localized spins. Although further theoretical developments demonstrated inapplicability of this model to metallic magnets, we discuss this model to first place. Usual relativistic magnetic interactions between localized moments at different lattice sites corresponds to the energy
µB2 a 3 ∼ 10−17 erg cm3 ∼ 10−1 K , so that magnetic ordering should be destroyed by thermal motion at very low temperatures. However, transition metals of iron group and a number of their compounds possess high values of ordering temperature (Curie point T C ) of order of 10 2 –10 3 K. Such large interactions between magnetic moments are not explained by classical electrodynamics and require a quantum mechanical treatment. In the absence of spinorbital interaction the wave function of a twoelectron system has the form of the product of spin and coordinate functions (4.1) Ψ (r1 s1 , r2 s2 ) = Ψ (r1r2 ) χ ( s1 s2 ), and, according to the Pauli principle, should be antisymmetric with respect to permutation of electrons. For symmetric (antisymmetric) spin function, which corresponds to the total spin S = s 1 + s 2 of unity (zero), the trial coordinate wavefunctions may be written in the form 1 [ψ 1 (r1 )ψ 2 (r2 ) ∓ ψ 1 (r2 )ψ 2 (r1 )] (4.2) 2 respectively. Calculating the firstorder perturbation theory correction to the total energy from the electrostatic interaction we obtain Ψ (r1r2 ) =
E = ∫Ψ * (r1r2 )
e2 Ψ (r1r2 ) dr1 dr2 = Q ∓ J ,  r1 − r2 
(4.3)
where we have introduced Coulomb integral
Q = ∫ρ1 (r1 )
1 ρ 2 (r2 ) dr1 dr2 ,  r1 − r2 
ρ (r ) = −eψ * (r )ψ (r )
(4.4)
and the exchange integral, which differs from (4.4) by permutation (exchange) of electrons
125
Chapter 4 J = ∫ψ 1* (r1 )ψ 2* (r2 )
e2 ψ 1 (r2 )ψ 2 (r1 ) dr1 dr2 .  r1 − r2 
(4.5)
Unlike the relativistic magnetic interaction, the exchange interaction has the electrostatic nature and is considerably larger. At the same time, exchange interaction between electrons at different lattice sites is strongly reduced by the squared factor of overlap of the corresponding wavefunctions. We may estimate
J ∼ (10−2 − 10−3 )Q ∼ 10−3 eV ∼ 10 K. The expression (4.3) may be rewritten in the form of the spin Hamiltonian 1 Q − J , S tot = 1, H = Q − J + 2s1s 2 = 2 Q + J , S tot = 0,
(4.6)
where
3 2 2s1s 2 = Stot − 2s 2 = Stot ( Stot + 1) − . (4.7) 2 Besides the ‘potential’ exchange interaction (4.5), there exists another exchange mechanism which is due to kinetic energy of electrons. In the simplest situation of sband, we obtain (Appendix D) 2t 2 1 (4.8) 2S1S 2 − , U 2 with t being the transfer integral and U the intraatomic Coulomb repulsion. This mechanism results in an antiferromagnetic interaction since the gain in the kinetic energy is achieved at antiparallel orientation of electron spins. As demonstrate numerical calculations (see, e.g., [265]), at realistic interatomic distances this contribution as a rule prevails over the ferromagnetic potential exchange. Thus the localized model does not explain ferromagnetism of iron group metals. The derivation of Heisenberg model for orbitally degenerate atomic shells and arbitrary values of spin S is presented in Appendix D. It turns out that in this case the exchange Hamiltonian contains the interaction of not only spin, but also orbital moments. Exchange mechanisms in rare earths owing to indirect interaction via conduction electrons is discussed in Appendix K. In most cases, real exchange mechanisms are complicated, so that we have to consider the Heisenberg Hamiltonian as an effective one. Consider the system of interacting magnetic moments which is described by the Heisenberg Hamiltonian in the magnetic field H H ′=−
126
Magnetic properties
H = − g µB H ∑Siz − ∑J ij Si S j i
(4.9)
ij
with J ij > 0 for nearest neighbours. Direct calculation of the magnetization M = g µ B〈S z 〉 (hereafter we put g µ B = 1) in the model (4.9) is prevented by the nonlinearity of the interspin exchange interaction in spin operators. To simplify the problem, we can linearize the Hamiltonian by introducing the effective mean field H* which is expressed in terms of magnetization z = −( H + H * ) S z , H = − HS S z = ∑Siz , (4.10) i
where H * = λ 〈 S z 〉,
λ = 2∑J ij = 2 J 0 ,
J 0 = J q =0
i
(4.11)
(in the nearestneighbour approximation J 0 = zJ with z being the number of the neighbour spins). In the case of spin S = 1/2 we have
1 〈S z 〉 = (n↑ − n↓ ), 2 Using the Gibbs distribution
n↑ + n↓ = 1.
(4.12)
σ H
H H exp + exp − , (4.13) T T T we obtain the selfconsistent meanfield equation for magnetization nσ = exp
1 H + λ 〈S z 〉 tanh . (4.14) 2 2T The result (4.14) is easily generalized to the case of arbitrary S 〈S z 〉 =
SH 〈 S z 〉 = SBS T
,
(4.15)
where S d 1 1 1 x ln ∑ e− mx/S = 1 + coth . coth 1 + x− dx m = − S 2S 2S 2S 2S is the Brillouin function. In particular cases
BS ( x) =
(4.16)
1 B∞ ( x) = coth x − . (4.17) x The equation (4.15) has nontrivial solutions in the zero magnetic field provided that T < T C , the Curie temperature being given by B1/2 ( x) = tanh x,
127
Chapter 4
TC = S ( S + 1)λ =
2 S ( S + 1) J 0 . 3
(4.18)
Using the expansion 1 x x3 + − +…, x 3 45 we derive near the Curie point coth x =
〈S z 〉 =
5 S ( S + 1) T 1− . 2 3 ( S + S + 1/2) TC
(4.19)
At low T E F which exceed in fact melting points. On the contrary, provided that the ratio T C /E F is small, i.e. 2I χ (0) is close to unity, the susceptibility above T C has the usual Pauli (square) temperature dependence. Thus, the Stoner theory does not explain in fact the Curie–Weiss law. Solving the Stoner equations for the parabolic band (4.39) at T = 0 demonstrates that at
χ (T ) =
(4.45) I > 22/3 EF /n there exist solutions which describe the saturated ferromagnetic state with M 0 = n/2. At
4 EF /n (4.46) 3 we have nonsaturated ferromagnetism with a partially filled spin down subband, and at smaller I magnetic ordering is absent. In the limit of small ground state magnetization we have the relation 22/3 EF /n > I >
2 2 M 0 TC ∼ . 3π n EF
(4.47)
Thus M0 is roughly proportional to the Curie point, in agreement with the Rhodes–Wohlfarth correlation (Fig.4.7). The temperature dependence of magnetization at low T in the saturated state turns out to be exponential M=
E In n 3 π T exp − F − 22/3 . 1 − 2 4 EF T EF
(4.48)
At the same time, corrections, which are proportional to T 2 , occur in the nonsaturated state owing to electronhole spinflip processes (Stoner excitations):
1 T 2 M M 0 1 − . (4.49) 2 TC Near the Curie point the magnetization has the squareroot behaviour, as well as in the meanfield approximation in the Heisenberg model:
2 ( M/M 0 )2 = 3(1 − T/TC ) 1 + (2π )−1/2 ( EF /TC )3/2 . 3 140
(4.50)
Magnetic properties Generally speaking, the results of the solution of the Stoner equations (4.38) turn out to be rather sensitive to the density of states shape. In particular, for the ‘rectangle’ band with constant density of states, considered in [286], only saturated ferromagnetic solutions are possible. Consider the results of the Stoner theory for an arbitrary bandstructure. The criterion of ferromagnetism reads (4.51) IN ( EF ) > 1. Provided that IN(E F) − 1 is small, the saturation magnetization equals [26] 1/2
2[ IN ( EF ) − 1)] M 0 = N ( EF ) . [ N ′( EF )/N ( EF )]2 − 1 N ′′( EF )/N ( EF ) 3
(4.52)
According to (4.41), the value of T C is −1
N ′′( EF ) 6 IN ( EF ) − 1 N ′( EF ) T = 2 . − π IN ( EF ) N ( EF ) N ( EF ) 2
2 C
(4.53)
The susceptibility above T C is presented as
T 2 1 1 1 2I − 1 . − = = (4.54) χ (T ) χ p (T ) χ p (TC ) [ IN ( EF ) − 1]2 TC Of course, the expansion of the Fermi integrals (3.37), used at derivation of (4.52)–(4.54), holds only at T C E0 , where Ñ(E) is a smooth function. Then exact integration in (4.25) gives 1 2
T 2  O + 2 . (4.58) ζ The effect of singularity vanishes at E 0 − ζ  T. According to the band calculations for palladium, there exists the van Hove singularity with E 0 − E F  = 300 K. To describe correctly the experimental behaviour of χ (T ) in Pd (in particular, the position of the maximum), it is necessary to shift the singularity to the Fermi level up to E 0 − E F  = 100 K. Presence of DOS peaks at the Fermi level, which is, as discussed above, typical for both strong and weak itinerant ferromagnets, may influence appreciably the χ (T ) behaviour and the T C value even in the Stoner theory of ferromagnetism. In particular, the triangle peak model was used to describe properties of weak itinerant ferromagnets [280]. Under condition of the linear dependence χ −1 (T ) owing to a DOS singularity the Curie temperature of a ferromagnetic metal is estimated as  E0 − ζ T
χ p (T ) = N (ζ ) + ( A2 − A1 )T ln 1 + exp −
TC ∼ (2 I χ p (0) − 1) EF
and may be considerably smaller than (4.53).
144
(4.59)
Magnetic properties
4.4 SPINFLUCTUATION THEORIES A more radical way to improve the results of the Stoner theory for temperature dependences of magnetic properties is going out beyond the oneelectron meanfield theory. Formally, the Stoner model corresponds to the interaction Hamiltonian of an infinite range,
n2 Hint = In↑ n↓ = I − 〈 S z 〉 2 , nσ = ∑nkσ , (4.60) k 4 so that the meanfield approximation is exact. A more rich physics is described by models which include electron correlations. The simplest among them is the Hubbard model (G.1) with the onsite Coulomb repulsion U. The Stoner approximation for the electron spectrum in this model corresponds to the simplest Hartree–Fock decoupling and may be justified only in the smallU limit which is inconsistent with the ferromagnetism criterion. Therefore correlation (spinfluctuation) effects, generally speaking, turn out to be important. As well as for Heisenberg magnets, lowtemperature thermodynamics of itinerant magnets is determined by spinwave contributions (see, e.g., [295]). Spinwave theory of metallic ferro and antiferromagnets is considered in Appendix G. The simple spinwave treatment enables one also to reproduce some of the results of spinfluctuation theories. Spinfluctuation theories, which describe thermodynamics of itinerant magnets in a wide temperature region, were developed during last twenty years [26, 296–302]. They turned out to be especially successful for weak itinerant ferromagnets which are characterized by extremely small values of saturation magnetic moment M 0 and large ratios p C/p s (Table 4.3, Fig.4.7). These substances correspond to a near vicinity of the Stoner instability and possess strong spin fluctuations. However, unlike systems with local magnetic moments, the fluctuations are localized not in real, but in reciprocal space (near the wavevector q = 0). Presence of the small parameter 2I χ −1 yields a possibility of an analytical treatment of weak itinerant ferromagnetism. The simple RPA expression for magnetic susceptibility (G.12), which follows from the spinwave theory, turns out to be thermodynamically inconsistent. In the theory of Moriya and Kawabata [296] the expression for paramagnetic susceptibility was taken in the form
χ (T ) =
χ p (T ) , 1 − 2 I χ p (T ) + λ (T )
(4.61)
where λ (T) is proportional to the squared amplitude of spin fluc145
Chapter 4 tuations. Calculation of λ in a selfconsistent way by using the expression for the free energy yields in the immediate vicinity of T C
λ (T ) ∼ (T/EF ) 4/3 . Thus λ dominates over 2I χ in the temperature dependence of the inverse susceptibility χ −1 (T ). With increasing T the dependence χ −1 (T) becomes practically linear. It should be noted that the Curie–Weiss behaviour in the spinfluctuation approach has a quite different origin in comparison with the Heisenberg model. The Curie–Weiss law holds approximately not only for weakly ferromagnetic, but also for almost ferromagnetic metals where 0 < 1 − 2 I χ p (0) 1,
e.g., for Pd, HfZr 2. The Curie constant is determined by the electron structure near the Fermi level only and, unlike the Heisenberg magnets, does not depend on the saturation magnetization. At 0 < 2Iχp(0) − 1 T 0 [427, 428, 735], which is due to vanishing of the electronmagnon scattering amplitude at zero magnon wavevector (Appendix G.1). Consider the situation in rareearth metals which are ferromagnetic at low temperatures. Because of strong anisotropy, the dispersion law of spin waves differs from that in dmetals. The magnon spectrum in rare earths contains a gap of order T* ∼ 10 K; in the absence of anisotropy in the basal plane we have the linear law ω q ∼ q.
δσ ( E ) ∼ −V 2 ∫ −
205
ρ ·10 8, Ohm·m
Chapter 5
Fig. 5.11. Temperature dependences of resistivity in the Heusler alloys TMnSb (T = Cu (A), Au (B), Co (D), Ni (E), Pt (F)) and PtMnSn (C) [331].
The gap results in the occurrence of an exponential factor exp (–T*/T) in the magnetic resistivity. For linear dispersion we obtain dependence ρ ∼ T 4 [429] instead of T 2 since each power of q yields at integration a factor of T/T C (instead of (T/T C) 1/2 at ω q ∼ q 2). The latter result was confirmed by the experimental dependence ρ ∼ T 3.7 for gadolinium in the region 4–20 K [430]. Using the formula (5.23) with the Hamiltonian of the s–d model (G.2) in the spinwave region, we obtain for the lowtemperature magnetic resistivity of antiferromagnetic metals
ρ=
π kBT 〈j 〉 2 x
2 I 2 Se 2 ∑(vkx − vkx + q ) 2 nk (1 − nk + q )[ N q (uq + vq )2 ) × kq
×δ ( Ek − Ek + q + ωq ) + N q + Q (uq + Q − vq + Q )2 )δ ( Ek − Ek + q + ωq + Q )].
(5.63)
The resistivity at very low temperatures is determined by contributions of small q in (5.63), i.e. by transitions inside antiferromagnetic subbands (Appendix G.2). Due to the linear dispersion law of magnons, such transitions result, as well as electron–phonon scattering, in a T 5 dependence of resistivity [428]. (The earlier result ρ ∼ T 4 [426] was erroneous since the coefficients of the Bogoliubov transformation (E.10), which have an essential qdependence, were not taken into account.) Because of the singularity in uvtransformation coefficients, the contribution from the region of small q – Q (i.e. of the intersubband contibutions) is, generally speaking, larger. However, as well as for ferromagnets, it is impossible to satisfy the quasimomentum conservation law at q → Q because of antiferromagnetic splitting, so that this 206
Transport properties contribution is in fact exponentially small at (5.64) T < T0 = ω ( q0 ) ∼ ( IS  /EF )TN , with q 0 = 2IS/ υ F being the threshold value of q – Q. (Note that the boundary temperature is not so small as for a ferromagnet, cf. (5.61).) At higher temperatures T > T 0 the intersubband contributions yield the T 2behaviour of resistivity [433]. In the twodimensional situation these contributions become Tlinear which may explain the characteristic dependence ρ (T ) in highT c superconductors. 5.3.4 Resistivity of transition metal alloys Investigations of transport phenomena in alloys as a function of concentration of various components give a possibility to obtain information on their electron structure. In particular, data on concentration dependence of residual resistivity ρ (c) in transition metal alloys yields an important information on change of dstates. In disordered alloys of simple metals with the same valence (metals with different valence do not form usually the continuous solid solution series), the Nordheim rule usually holds
ρ (c) = ρ 0 c(1 − c),
(5.65)
1 d 2 ρ (c) = −2. ρ0 dc 2 c =0,1
1 d ρ (c ) = ±1, ρ0 dc c =0,1
In TM alloys the symmetry of ρ (c) curve is violated (see Fig.5.12). An explanation of this violation can be obtained within the Mott s–d transition model. To demonstrate this we write down the conductivity of the alloy A 1 −c Bc , with A being a transition metal and B a simple metal, in the form
σ = σ s + σ d σ s = ρ s−1 ,
ρ s = ρ ss + ρ sd .
(5.66)
Fig. 5.12. The concentration dependence of resistivity ( µ Ω · cm) in Pd–Au alloys. 207
Chapter 5 Taking into account the relations
ρss = ρ s0 cB (1 − cB ),
ρsd = acB (1 − cB ) Nd ( EF )
(5.67)
and the concentration dependence N d ( EF ) cB (1 − cB ) N A ( EF ),
(5.68)
B (1 − cB ) 2 , ρ ρ s = ρ s0 cB (1 − cB ) + ac
(5.69)
we obtain [434] which yields a deviation from the Nordheim rule. Other factors which lead to violation of this rule may exist. So, for Cu–Ni alloys, delectrons are at localized levels for small nickel concentrations and form band states for c > 40% only [435]. At the critical concentration, an abrupt change of the alloy properties takes place. 5.3.5 Twocurrent model of ferromagnetic metals The twocurrent models considers two types of current carriers in an itinerant ferromagnet which have different spin projections. Unlike the Mott model, where the current of dstates is neglected, contributions of both types of states are comparable. Effects of strong spin polarization are especially important for dbands, but may be appreciable for stype current carriers too. The phenomenological treatment of the model is rather simple [436]. The total current and, consequently, conductivity, are represented as a sum of contributions from majority and minority current carriers:
j = σ E, σ = σ ↑ + σ ↓. Then the resistivity takes the form
(5.70)
−1
ρ =σ
−1
1 ρ↑ ρ ↓ 1 = , + = ρ ↑ + ρ↓ ρ↑ ρ↓
(5.71)
which corresponds to a parallel junction. Further we have to take into account transitions between both the types of carriers. These are due to spinflip scattering processes by spin inhomogeneities, spin waves, magnetic impurities etc. Then we have
ρ↑ = ρ↑0 + ρ↑↓ ,
ρ↓ = ρ↓0 + ρ↓↑
(5.72)
(consecutive junction). On substituting (5.72) into (5.71) we obtain
ρ=
ρ↑0 ρ↓0 + ρ↓0 ρ↑↓ + ρ↑0 ρ↓↑ + ρ↑↓ ρ↓↑ . ρ↑0 + ρ↓0 + ρ↑↓ + ρ↓↑
208
(5.73)
Transport properties Such an approach may be applied to describe transport effects in ferromagnetic transition metals and their alloys. Unfortunately, reliable microscopic calculations of the quantities which enter (5.73) are hardly possible, and it is more convenient to determine them from experimental data. One uses often the data on the deviation from the Matthiessen rule. To illustrate this approach we consider a ternary alloy M 1xyA x B y . We have for the impurity resistivity ( ρ ↑↓ = ρ ↓↑ = 0) where ρ A,B
(5.74) ρ AB = ρ A + ρ B + ∆ρ , are the resistivities of the corresponding binary alloys,
∆ρ = (α A − α B )2 ρ A ρ B [(1 + α A )2 α B ρ A + (1 + α B ) 2 α A ρ B ]−1 ,
(5.75)
with
α A,B = ρA,B↓ ρA,B↑ . Varying the concentrations x and y one can experimentally determine the parameters α A,B . At finite temperatures, additivity of the impurity residual resistivity ρi and Tdependent contributions for a binary alloy is also violated:
ρ↑,↓ (T ) = ρi ↑,↓ + ρl ↑ ,↓ (T ),
(5.76)
2 2 α − µ α −1 + + ρ ( T ) l ρ↑↓ (T ). 1 + α α +1
ρ (T ) = ρi 1 +
with
α = ρ i ↓ /ρ i ↑ ,
µ l = ρ l ↓ /ρ l ↑ ,
ρi↑ ρi↓ ρ ρ ρl = l ↑ l ↓ , , (5.77) ρi ↑ + ρi ↓ ρl ↑ + ρl ↓ where l stands for the index of a concrete temperaturedependent scattering mechanism. Using experimental data on ternary and binary alloys, parameters α A , α B , µ l , ρ i , ρ l (T) and ρ ↑,↓ were determined for the ferromagnetic transition metals [436]. In a number of cases, the parameters α deviate strongly from unity. As an example, data on the alloy NiCo 1–x Rh x are shown in Fig.5.13. Due to strong nonlinearity of the ρ (x) dependence, the parameters ρ↑ and ρ↓ turn out to be considerably different. Note that the deviations from the linear dependence at small x cannot be explained by the Nordheim rule. In a metal with transition metal impurities the scattering of conduction electrons into dresonance impurity states near the Fermi level plays the dominant role. The behavior of the quantity α in the 3dρi =
209
ρ 0 µOhm·cm
Chapter 5
Fig. 5.13. Residual resistivity of NiCo 1–x Rh x alloy. The large deviation from the ‘Matthiessen rule (linear dependence) is accounted for strongly different values of α Coand α Rh ; the solid curve corresponds to their values of 13 and 0.3 respectively [436].
impurity series for Fe and Ni hosts is presented in the Table:
T
Ti α (NiT) α (FeT)
V 1.9 0.38
Cr 0.52 0.12
Mn 0.3 0.22
Fe 10 0.13
Co 15 –
Ni 20 2.1
– 5
Cu 3.4 –
As discussed in [436], qualitatively this behavior may be explained on the basis of the Friedel concept of the virtual bound dstate. The spinup nickel dband is practically filled, and only spin down states may screen the impurity charge perturbation. For early 3dimpurities (Cr, V, Ti) in Ni the spinup impurity dstate is repelled above the spinup dband, so that the impurity density of states g d ↑ (E F ) is rather large, the magnetic moment being opposite to the host one. At the same time, for strongly magnetic Co, Fe and Mn impurities only sstates are present at E F for spin up. The value of g d ↓ (E F) is rather large for all the 3dimpurities in the Ni host. Thus α strongly increases at passing from the first half of 3dseries to the second one. Magnetic moments of 4dimpurities are created mainly by host magnetization, the magnetization perturbation being strongly delocalized. The behavior of α for the first half 4dseries impurities in Ni is similar to that in 3dseries. In pure iron the Fermi level is just below the spinup dband. Therefore in the Fe host the repulsive impurity potential pushes up the spin up dlevel for Mn, Cr, V and Ti impurity series through the Fermi
210
Transport properties energy, the magnetic moment decreasing. At the same time, for Co and Ni impurities g d↓ (E F ) is small. For all the 3dimpurities in iron g d ↓ (E F) is rather small. The qualitative consideration of the problem may be performed also within the Anderson impurity model (see [717]). Quantitatively, the local density of states and other characteristics of the impurity electronic structure are obtained from band calculations. Such calculations were performed for a large number of impurities (including 3d and 4dimpurities) in the Ni and in the Fe host [718–722]. One can see from the results that even for 3dimpurities in Ni the simple Andersonmodel picture is in fact poor: the local impurity DOS g d σ (E) is strongly influenced by the host. Besides that, the Fe host, which has (unlike the Ni host) a large magnetization, determines in a great measure formation of magnetic moment even for later 3dimpurities. The 4dimpurity states are strongly hybridized with the valence host states so that the picture of narrow virtual bound impurity dstate is not applicable. This is especially obvious for Y, Zr and Nb impurities in Ni where g σ (E F) for both σ are quite small and differ by a small exchange spin splitting only [719]. However, for Tc to Pd impurities rather sharp hybridization peaks are present. As compared to Mn, Fe and Co, the spin up peaks for Tc, Ru and Rh are broader and extent somewhat above E F . The most consistent calculation of resistivity may be performed on the basis of the scattering phase shift analysis on the base of band structure calculations. Such calculations were carried out for dimpurities in Cu [723], the role of magnetic moments being neglected, and in Ni [724]. In the latter case the agreement with experiment was not quite satisfactory. A simplified estimation in the case of a ferromagnetic host with appreciable magnetization perturbations was performed in [717] by using the results of band structure calculations and the Friedel sum rule. A general (with neglecting crystalfield effects) expression for resistivity per impurity in terms of the phase shifts η lσ has the form
ρσ = ρ uσ ∑(l + 1)sin 2(ηlσ − ηl +1,σ ), l
(5.78)
where ρ uσ is the resistivity unitary limit for a given spin projection per scattering channel (see Sect.6.1). In the approximation of free conduction electrons we have
ρ uσ = 2m* /(π zσ egσ ). where m*, z σ and g σ are the effective mass, concentration and density of states of conduction electrons at the Fermi level for a given spin
211
Chapter 5 projection, e is the electronic charge. To estimate the phase shifts we use for each spin projection (spinflip processes are neglected) the Friedel sum rule ∆nσ =
1
π
∑(2l + 1)η σ . l
(5.79)
l
The changes of electron numbers are determined by
1 ∆n↑ ,↓ = ( ∆Z ± ∆M ), 2 where ∆Z is excess charge introduced by the impurity ion, i.e. the difference between impurity and host atomic numbers, ∆M is the total magnetization change induced by the impurity (in µ B ). Similar to the standard Friedel approach for nonmagnetic hosts, only dscattering (l = 2) contribution can be taken into account. This is generally speaking, sufficient for rough estimations. However, in a number of cases s,pcontributions play an important role. In particular, for the impurities in the Ni host, which do not destroy strong ferromagnetism (∆Z = −∆M ), the density of spinup dstates near the Fermi level is rather small, and their disturbance by impurity is practically absent [720]. A similar situation takes place for dimpurities from the beginning of dseries where dstates are almost empty and ∆Z + ∆M = 10. The spcontributions are also important for nonmagnetic spimpurities which introduce a strong charge perturbation. The values of ∆M and some data on the partial contributions ∆n l σ = (2l + 1) η l σ / π may be obtained from the band calculations results [720] for the Ni host and in [721] for the Fe host. First we discuss the case of the Ni host. To perform calculations we have to specify the values of ρ u σ . For the Cu host one puts usually ρ u = ρ u σ /2 = 3.8 µ Ω⋅cm/at % [725]. As demonstrate band structure calculations [24], the value of total density of states with spin up for metallic nickel is two times larger, but the scontribution is considerably smaller than for Cu: although the spin up dsubband is practically filled, its tail dominates at E F, so that g d ↑ /g s ↑∼10. Still larger dcontributions occur for spin down where a large density of states peak is present at E F and g d ↓ /g s ↓ ∼ 100. Thus, although delectrons are usually assumed to possess small mobility, the problem of their contribution to conductivity should be investigated. For nonmagnetic impurities Cu, Zn, Ga, Ge in Ni the partial values of ∆n σ may be estimated from results of Ref.720. The calculations according to (5.78) with ρ u ↓ = 15 µ Ω ⋅ cm/at % yield satisfactory 212
Transport properties values of ρ . However, the estimation of ρ ↓ with the same value of ρ u ↓ yields very large values of α . To reduce α up to reasonable values we have to put ρ u ↑ / ρ u ↓ 5. Thus the estimations of Ref.[717] lead to the conclusion that delectrons make an important contribution to conductivity, especially to the spindown current. Indeed, the selectron contribution cannot provide such a large ratio ρ u↑ / ρ u↓ ; besides that, this is expected to yield an opposite tendency since g s ↑ >g s ↓ [24]. Note that in the situation of several conduction electron groups the quantities ρuσ should be considered as phenomenological fitting parameters. Similar statement about the important role of dstates in electronic transport was made by Kondorsky [502,503] on the basis of data on the anomalous Hall effect. Now we consider briefly the case of the Fe host. Unlike nickel, iron is not a strong ferromagnet since dstates with both spin projections are present at E F . Moreover, the Fermi level lies in a pseudogap for the spin down dstates. Therefore one may expect that spin up dstates should make a larger contribution to the transport properties (besides that, band calculations [24] give a strong spin polarization of spelectrons at E F). Indeed, for FeNi and FeCo systems we have ∆M > 0, but α > 1, so that we may estimate ρ u ↑ / ρ u ↓ = 0.2. At present, the twocurrent model was also applied to consider anisotropy of electrical resistivity in magnetic field, temperature dependence of the normal Hall effect, thermoelectric power, magnetoresistivity, transport effects in bulk samples [726] and multilayers (especially, giant ∆ ρ/ρ effect [437]).
5.4 THERMOELECTRIC POWER In the presence of a temperature gradient, the electric and heat currents are given by the linear relations (5.1) and (5.2). For j = 0 we obtain
E=−
λ gradT ≡ α gradT , σ
(5.80)
where α is the absolute differential thermoelectric power. The coefficients in (5.1) and (5.2) are determined by the disturbance of the equilibrium distribution function by external fields. Provided that the kdependent relaxation time τ may be introduced,
1 f1k = −τ kυk eE + (ε k − EF ) gradT . (5.81) T Using the expressions for electric and heat current, we obtain 213
Chapter 5
σ = e2 K0 ,
λ = ν /T = eK1/T ,
where
Kn = −
∂n 1 υk2τ k (ε k − EF )n k . ∑ 3 k ∂ε k
(5.82)
K1 . eTK 0
(5.83)
Then we have
α =−
After expanding (5.83) in T/E F up to the second order we obtain
α =−
π kB2T ∂ ln σ ( E ) , 3 e ∂ E E=E
(5.84)
F
where σ(E) is the conductivity as a function of the Fermi level position (see (5.31),(5.32)). Thus, the thermopower is expressed in terms of conductivity and its energy derivative. The sign of α is determined by the sign of electric charge (or effective mass). In particular, it should be reversed when the Fermi level approaches the Brillouin zone boundaries (a becomes positive). In the simplest approximation we may write down
σ ( E ) = e2 n( E )τ ( E ) / m*,
(5.85) where n(E) is the number of electrons in the kspace under the surface with a given E = E F, so that dn(E)/dE equals to the density of states N(E). Then we have
α =−
π 2 kB
N (E ) 1 ∂τ ( E ) + . kBT 3 e n ( E ) τ ( E ) ∂ E E = EF
(5.86)
The expression (5.86) contains the concentration contribution which is determined by the number of electrons, and the relaxation contribution which depends on the function τ (E). The value of the first contribution is estimated as
α ∼−
π 2 kB kBT 3 ne EF
≈ −0.9 ⋅ 102
kBT µ V , EF K
(5.87)
which agrees roughly with experimental data ( α ~1 µ V/K at k BT/E F~ 10 –2). At the same time, in semiconductors α does not contain the small factor k B T/E F and is considerably larger. The dependences τ (E) are different for various scattering mechanisms. At high temperatures,
τ ( E ) ∼ E 3/2 ,
n( E ) ∼ E 3/2 , 214
σ (E) ∼ E 3.
Transport properties
Fig. 5.14. The typical temperature dependences of thermoelectric power ( µ V/K) in metals (a) noble metals and refractory dmetals in a wide temperature region (b) noble metals at intermediate temperatures (c) alkaline metals at low temperatures [8].
At low temperatures, where impurity scattering dominates and the electron mean free path is constant,
τ ( E ) ∼ E −1/2 ,
σ ( E ) ∼ E.
Then (5.84) yields T > θD , (5.88) eEF 1/3, T θ D . The relation (5.88) gives reasonable results for Na and K which are described by the free electron model, so that α and the Hall coefficient are negative. However, generally speaking, such simple dependences do not reproduce experimental data even for simple metals (see Fig.5.14). One can see that α may become positive and in most cases the dependences α (T) are nonmonotonous. The hightemperature behaviour is usually attributed to the effect of phonon drag [8]. The corresponding contribution in the free electron model may be presented in the form
α =−
π 2 kB2T 1,
Cph
1 = Cph R, (5.89) 3ne 3 where C ph is the lattice specific heat, R is the Hall coefficient. The dependences α (T) in transition metals are still more complicated. Especially large values of α are observed in Pd and Pt. An important fact is a similarity in the α (T) behaviour within each column of the periodic table. The generalized dependences α (T) are shown in Fig. 5.15. A correlation between signs of α and the Hall coefficient is as a rule absent, which demonstrates inapplicability
α ph = −
215
α , µV/deg
Chapter 5
Fig. 5.15. A summary of thermoelectric power data for transition metals, U and Th [438]. Roman numerals indicate the periodic table column.
of simple theories to these quantities in transition metals. In some cases (e.g., for La near the α – β transformation and for Ti near 500K), a simultaneous sign change takes place in R(T) and α (T). In other cases (e.g., for Sc and Hf) the sign inversion temperatures are considerably different. Sometimes the change of α (T) sign is not accompanied with that for R(T) (however, one has to bear in mind that R(T) is measured as a rule in a more narrow temperature interval). As well as other transport properties, thermoelectric power exhibits also anomalies at the magnetic ordering points (Fig.5.16). 216
α, µV/K
Transport properties
Fig. 5.16. The anomaly of thermoelectric power of chromium at the Neel point [438].
To explain complicated α (T) behavior one has apparently to take into account presence of several current carrier groups and scattering mechanisms. One of the possible approaches is using the Mott model of s–d transitions. In this model, main contribution to scattering is connected with transitions of selectrons into the dband. The corresponding relaxation time is proportional to the inverse density of dstates. Assuming that the relaxation contribution in (5.86) dominates we derive
α (T ) = −
∂ ln N d ( E ) . kB2T ∂E 3e E = EF
π2
(5.90)
The expression (5.90) is used frequently to describe the data on the thermopower for metals in the end of periods (e.g., Pd and Pt) and for alloys like Cu–Ni, Pd–Ag. It reproduces satisfactorily the temperature and concentration dependences of α in the cases where a filling of transition metal dband by electrons of second alloy component takes place near its top where the value of dN d (E)/dE is very large. We may conclude that the investigation of the α(T) behavior permits to study the delectron density of states. As discussed above, a sharp dependence N(E) influences considerably a number of physical properties of transition metals. However, the anomalies in thermopower are expected to be especially sensitive to electron structure details due to presence of the factor d τ (E)/dE in (5.86). However, one has to exclude other factors which may influence α (T). In the presence of density of states singularities (e.g., Van Hove ones), the standard scheme of calculating α (T) should be modified. This is due to that the expansion of the integrals which determine thermopower (see (5.83)) in T/E F becomes impossible for peaks with the width of order k B T. Direct integration was performed in paper [439] with application to palladium. A triangle model with a jump
217
Chapter 5 of dN(E)/dE near E F was used. Although an agreement with experimental data was obtained at high temperatures, the maximum at low temperatures remained not explained. This maximum may be due to the phonon drag effect [7] (however, the signs of R 0 and α are opposite in this temperature region). Freezing out of the s–d transitions and occurrence of a manyelectron mechanism at low temperatures may also play a role in the α (T) dependence. Nonmonotonous dependences α (T) are observed also in a number of transition metal compounds, e.g., copperoxide systems which provide a basis for highT c superconductors (see experimental data [440, 441] and theoretical considerations [405, 442]), Kondo lattices and heavyfermion compounds (see discussion in Sect.6.4). In such systems, very narrow density of states peaks near the Fermi level have apparently a correlation (manyelectron) origin and are not obtained in band calculations.
5.5 THE HALL EFFECT Investigation of electric properties of metals in an external magnetic field lead to discovery of a number of interesting physical effects which provided a powerful tool for analyzing their electron structure. This was realized already in the beginning of modern solid state physics development. So, the physical basis of galvanomagnetic effects (the Hall effect and magnetoresistivity) is described correctly in the classical monograph [1]. However, concrete methods of the Fermi surface reconstruction with the use of such effects were developed only after the extensive theoretical work in 50–60s (see [10]). Modern theory explains well most effects in normal metals. At the same time, the situation in transition metals is less satisfactory, which is connected with their complicated electronic structure and the presence of spontaneous magnetization (in ferromagnets). The Hall effect in transition metals includes in fact two effects of different microscopic nature 1. the normal effect connected with the Lorentz force 2. (ii) the anomalous (spontaneous) Hall effect owing to spinorbit coupling. The corresponding Hall constants are defined by E y = R0 j x H z + R1 j x M z ,
R1 = R M ≡ 4π Rs .
(5.91)
Since R sR 0, the anomalous Hall effect dominates in ferromagnetic
218
Transport properties crystals. The Hall effect in magnetically ordered metals will be considered in Sect.5.7.1. Here we note that the spontaneous effect takes place in paramagnets too. Putting in (5.91) M = χH we obtain R0* = R0 + 4πχ Rs .
E y /jx = R0* H z ,
(5.92)
Thus the spontaneous Hall effect may be picked out in the case of a strong dependence χ (T) and is appreciable for large χ, especially near the Curie point. Consider the simple quasiclassical theory of the normal Hall effect. Writing down the phenomenological equations jx = σ xx Ex + σ xy E y ,
j y = σ yx E x + σ yy E y ,
(5.93)
where offdiagonal components are determined by the magnetic field we obtain for cubic crystals ( σ xx = σ yy = ρ 1 )
σ xxσ yy jx = σ xy − E y − ρ 2σ yx jz . E y , σ yx The Hall coefficient is introduced by R=
Ey jx H z
= −ρ 2
σ yx ( H z ) Hz
.
(5.94)
(5.95)
In the presence of the field H x and the Lorentz force
e e Fy = − [ vH] y = vx H z . c c the offdiagonal component σyx is connected with the diagonal one by the dimensionless parameter ω c τ ( ω c is the cyclotron frequency, τ is the relaxation time):
σ yx = ω cτσ xx ,
(5.96)
so that the conductivity tensor in the field H z has the form 1 e 2 nτ /m* σˆ = ω cτ 1 + (ω cτ )2 0
ω cτ 1 0
. 2 1 + (ω cτ ) 0 0
(5.97)
It is interesting that according to (5.96) σ yx ρ –1 . Then we obtain from (5.95)
eτσ xx 1 =− . (5.98) * mc enc Thus, in the simplest approximation the normal Hall effect coefficient is a constant which does not depend on the scattering mechanism. We shall see below that the situation changes drastically for the R = −ρ2
219
Hall coefficient, m3/A·s
Chapter 5
Number of valancy electrons per atom Fig. 5.17. The Hall coefficient as a function of the number of valence electrons for polycrystalline transition metals and alloys according to data of different authors [443].
spontaneous Hall effect. In particular, in the case of the phonon scattering (Appendix M.2) the expansion of σ in the scattering amplitude may start, in contrast with (5.96), from zeroorder terms, so that R s ~ ρ 2. Now we consider the experimental situation. In simple (in particular, alkaline) metals the Hall effect is satisfactorily described by the formula (5.98) which may be used to determine the carrier concentration n. However, in polyvalent metals, where the Fermi surface crosses the boundaries of the first Brillouin zone and several current carrier group exist, there occur considerable deviations and the Tdependence rises [8]. Thus the Hall effect may be used in principle to determine characteristics of the electron structure and the number and mobility of current carriers in various regions of the Brillouin zone. The behaviour of the Hall coefficient in the dseries is shown in Fig.5.17. Unlike ∆ ρ / ρ effect (Sect.5.6), the Hall effect in nonferromagnetic transition metals has essentially peculiar features. The normal Hall 220
R·10 10, m 3 /A·s R·10 10, m 3 /A·s
Transport properties
R·10 10, m 3 /A·s
Fig. 5.18. The temperature dependence of the Hall coefficient in scandium according to data of different authors [239].
R·10 10, m 3 /A·s
Fig. 5.19. The temperature dependence of the Hall coefficient in lanthanum [239].
Fig. 5.20. The temperature dependence of the Hall coefficient in titanium [239].
coefficients of TM exhibit strong temperature dependences which are in some cases nonmonotonous. The forms of the R 0(T) behaviour are as a rule similar in the periodic table columns. These dependences are shown in Figs.5.18–5.28. A weak Tdependence is observed for 221
R·10 10, m 3 /A·s
Chapter 5
R·10 10, m 3 /A·s
Fig. 5.21. The temperature dependence of the Hall coefficient in zirconium [239].
R·10 10, m 3 /A·s
Fig. 5.22. The temperature dependence of the Hall coefficient in hafnium [239].
Fig. 5.23. The temperature dependence of the Hall coefficient in molybdenum [239].
Mo and W only. The local minimum of R 0 (T) dependence in Mn (Fig.5.29) is probably connected with antiferromagnetism of this metal. In principle, the complicated behaviour R 0 (T) may be explained by the presence of several groups of current carriers. Using (5.97) we obtain in the case of two groups R = ( R (1)σ 12 + R (2)σ 22 ) / (σ 1 + σ 2 ) = ρ 2 ( R (1)σ 12 + R (2)σ 22 ) , 2
where R(i) = −
1 , eni c 222
σi =
e 2 niτ i . mi*
(5.99)
R·10 10, m 3 /A·s
Transport properties
R·10 10, m 3 /A·s
Fig. 5.24. The temperature dependence of the Hall coefficient in rhenium [239].
R·10 10, m 3 /A·s
Fig. 5.25. The temperature dependence of the Hall coefficient in ruthenium according to data of different authors [239].
Fig. 5.26. The temperature dependence of the Hall coefficient in rhodium [239].
The result (5.99) may give a strong temperature dependence only provided that the dependences σ1(T) and σ2(T ) are appreciably different. This may take place at low T, e.g., where light carriers (selectrons) are mainly scattered by phonons, and heavy carriers (delectrons with large density of states) due to electron–electron collisions. For example, this mechanism may be responsible for a maximum of R 0(T ) in Cu at low temperatures (Fig.5.30). Similar (but appreciably more pronounced maxima) are present in Pd and Pt. It is known that in all these three metals two groups of carriers with considerably different effective masses exist which correspond to neck and belly Fermi surfaces. Ziman [444] proposed that the increase of R 0(T ) in Cu 223
R·10 10, m 3 /A·s
Chapter 5
R·10 10, m 3 /A·s
Fig. 5.27. The temperature dependence of the Hall coefficient in platinum [239].
Fig. 5.28. The temperature dependences of the Hall coefficient in the field H = 13.5 kOe for Ta (open squares) and V (different measurement series, other symbols) [446].
below 100 K is connected with freezing out Umklapp processes, the lifetime of lightmass belly states becoming lengthened with respect to one on the neck region, τ B/ τ N 1 whereas τ B ~ τ N at room temperatures. These arguments are confirmed by the calculations [445]. The occurrence of the R 0(T ) maximum may be connected with the transition to strong field regime ω c τ 1 and with strong anisotropy of τ . This hypothesis seems to be confirmed by investigations of single crystals (see discussion in [443]). At the same time, the explanation of the maximum in Pd and Pt at T ~ 200K is more difficult. At high T ~ 100–1000K the electron–phonon mechanism dominates for all the carriers in paramagnetic metals. Therefore, the quantitative explanation of the strong R 0(T) change (by several times in Sc, Ti, Zr, Hf, V, Re) is hardly possible on the basis of (5.99). The nonmonotonous dependence R 0 (T) in V and Ta (Fig.5.28) is discussed in [446]. The authors claim that usual Umklapp processes do not explain the R0(T) minimum at T = 20−30 K. Since the temperatures 224
R·10 10, m 3 /A·s
Transport properties
R·10 10, m 3 /A·s
Fig. 5.29. Temperature dependence of the Hall coefficient of polycrystalline α Mn and α Pu [443].
Fig. 5.30. The temperature dependence of the Hall coefficient of polycrystalline Cu [443].
225
Chapter 5 of their freezing in these metals make up about 300 and 200K respectively for closed sheets, and for open sheets the Umkplapp processes do not freeze out up to T = 0. Only Umklapp processes between closed hole sheets h Ν(3) and the open hole surface in the ΓNH plane, which are localized in the region of minimum distance between the sheets, yield reasonable values of the freezing temperature T*. Below T* the anisotropy of scattering decreases which results in R0(T) increase. Adding impurities suppresses the anisotropy too and leads to vanishing of R 0 (T) minima in agreement with experimental data. This interpretation agrees with the theory [415] which considers the anisotropy of nonequilibrium distribution function. Another mechanism of strong dependence R(T ) in paramagnetic metals may be the influence of the anomalous Hall effect. As follows from (5.92), such a dependence may be connected with the dependences χ(T) and R s (T). This possibility was noted in early papers, in particular, in connection with the anomalies at the Curie point. Kondorsky [447] used this idea for explaining the R(T) behaviour in Zr and Re. Of course, reliable independent methods for determining R s in nonferromagnetic metals are absent. The expression (5.92) may give required values provided that R s /R 0 ~10 2 −10 4 , i.e. R s is nearly the same or somewhat larger in comparison with ferromagnetic metals. This assumption seems to be reasonable since the spinorbital coupling has the same order of magnitude for all the transition metals. The expression (5.92) may explain also concrete temperature dependences R(T). As discussed in Sect.4.2, χ increases with T in the periodic table columns with even configurations d n and decreases for odd configurations. At the same time, R s(T) increases in absolute value as ρ 2 (T) due to electron–phonon scattering (Sect.5.7.1). Then we obtain (5.100) R0* = R0 + 4πχ (T )bT 2 , The sign of the temperature correction in (5.100) is determined by the sign of R s. In fact, the value of b is not known exactly and should be used as a fitting parameter. Then we may reproduce various experimental dependences R(T). For example, one has to put R 0 < 0, R s > 0 for Ti, R 0 > 0, R s > 0 for Zr, R 0 > 0, R s < 0 for Re with R s ~ ρ 2 (T) ~ T 2 in all the cases. Unfortunately, it is difficult to separate the normal and anomalous contributions. Apparently, the value of R 0 may be determined from lowtemperature data for highpurity samples where R s → 0.
226
Transport properties
5.6 MAGNETORESISTIVITY The resistivity change in magnetic field (magnetoresistivity, ∆ ρ / ρ effect) corresponds to square terms in H, i.e. is an even effect. One distinguishes the longitudinal (H  E) and transverse (H ⊥ E) effects. As well as the Hall effect, magnetoresistivity occurs due to distortion of electron path owing to external field or magnetization. Naively, one might assume that this distortion should diminish the velocity component v along the electric field and result in a decrease of current, i.e. an increase of resistivity. In fact, the situation is more complicated since one has to take into account the Hall field E y which compensates the influence of magnetic field. The change of resistivity in magnetic field may be described by the Frank law ∆ρ /ρ ≡
ρ ( H ) − ρ (0) BH 2 = . ρ (0) 1 + CH 2
(5.101)
In weak fields (CH 2 1) we have the squarelaw increase, and in strong fields the resistivity is saturated, ∆ρ /ρ = B/C = const. In some situations, the linear dependence ρ (H) (the Kapitza law) is observed in strong fields (see [1,10]). Besides that, for Mo, Re, Pt, Fe and Pd the experimental dependences may be fitted as [448]
∆ρ /ρ ∼ H m , m < 2. According to the Kohler rule,
(5.102)
H ∆ρ / ρ = f , (5.103) ρ with f being an universal function. The Kohler plots for some simple and transition metals are shown in Fig.5.31. The Kohler rule holds in wide intervals of ρ and H almost in all cases. Let us try to estimate the values of the coefficients B and C in (5.101) in the simple theory which considers the motion of an electron in a crystal in external electric and magnetic fields. We use the expansion in T/E F and the relaxation time approximation. Then the longitudinal ∆ ρ / ρ effect turns out to be absent to the secondorder terms, and for the transverse effect one obtains
π 2 el
2
el kBT C = * * 2 3 , 3 (m ) υ mυ – – where l = υ τ is the electron mean free path, the B=
227
2
, (5.104) averages are taken
Chapter 5
kG Fig. 5.31. Reduced Kohler diagram showing the transverse magnetoresistance of some metals in the highfield region [448].
over the Fermi surface. The result (5.104) may be interpreted in terms of competition between the circular motion under the influence of the Lorentz force and the straightforward motion in the electric – field on the path l . The former is characterized by the orbit radius
CH = ( l/rc ) , 2
2
2
BH =
π2 3
( l/r )
2
c
2
kBT * 2 . mυ
(5.105)
– The occurrence of the ratio l /r c ∼ H/ ρ illustrates the Kohler rule. – In weak fields (l r c ) the increase of ρ is determined by that the spiral motion of an electron in the field H z results in decreasing of the path in the xdirection between collisions. At large fields, B π 2 kBT = . C 3 m*υ 2 2
∆ρ / ρ =
228
(5.106)
Transport properties Although the result (5.106) is in agreement with the law (5.101), the value of the coefficient B ∼ (T/E F) 2 is considerably smaller than the experimental one, and the strong temperature dependence is in fact not observed. The difficulties of the above simple theory are eliminated when one includes a dispersion of the relaxation time τ (k). Then the average value
τn = ∑ k
∂nk 2 n vkτ (k ) ∂Ek
∂nk
∑ ∂E k
vk2
(5.107)
k
differs from τ– n , and we obtain the nonzero effect at T = 0: 2
eH ∆ρ / ρ = Q * , m c 2
( ) (τ ) .
2 Q = τ 3τ − τ 2
2
2
(5.108)
Since
( )
2
τ 3τ ≥ τ 2 , ∆ ρ / ρ is positive. The temperature dependence of ∆ ρ / ρ may be calculated provided that the factorization
τ (k ) = ϕ (T ) χ (k )
(5.109)
is possible (this may take place, e.g., at high temperatures). Then we derive
∆ρ /ρ ∼ σ 2 (T ) H 2 ,
(5.110)
with σ (T) being the conductivity. Thus ∆ ρ / ρ is expected to increase with lowering T. The relation (5.110) is in agreement with the Kohler rule. It should be noted that the temperature dependence of (5.110) (a decrease with ρ ) contradicts to expressions (5.101), (5.104) for a single group of current carriers, which yield an increase as ρ 2 with increasing T. Thus the experimental Tdependences of ∆ ρ / ρ effect correspond to essentially anisotropic relaxation time or to existence of several current groups. Consistent calculation of the parameter Q, which is defined in (5.108), is a very complicated problem. More convenient is the simple estimation from experimental data with the use of
Q=
1 ρ (∆ρ /ρ )1/2 , H R0 229
(5.111)
Chapter 5 where R is the Hall coefficient. For most metals, the value of Q varies from 1 to 4. An important exception are semimetals As, Sb, Bi where Q ∼ 10 2 –10 3 . The giant ∆ ρ / ρ effect in these substances is connected with their anomalous electronic structure [10]. Some transition metals also possess large value, e.g., for zirconium Q = 20, which may be connected with strong anisotropy for hcp crystals. Higherorder approximations which take into account the kdependence of electron velocity permit to obtain the longitudinal ∆ ρ/ ρ effect. The corresponding correction to the distribution function is given by [1]
f k(3) = −τ 3
∂ vy ∂ v ∂ v ∂ v e3 2 ∂ nk z x − z + EH υ y ∂ε k ∂ k x ∂ k z ∂ k y ∂ k z 2 c 2 + vy
∂ 2 vz ∂ 2 vz v − x ∂ k x2 ∂ k x∂ k y
+ x ↔ y .
(5.112)
According to experiments by Kapitza (see [1,10]), the longitudinal effect may be comparable with the transverse one. In 50s–60s, investigations of galvanomagnetic effects were widely applied to reconstruction of the Fermi surface shape of metals. In strong magnetic fields where
ωcτ = eHτ (m*c) 1, three types of the ∆ ρ / ρ effect behaviour were found 1. ∆ ρ / ρ is saturated at arbitrary orientation of H in the crystal 2. ∆ ρ / ρ is not saturated at arbitrary orientation of H 3. ∆ ρ / ρ is saturated for some orientations of H and continues to increase in strong fields for other orientations. The type of behaviour depends on that whether a given metal is compensated, i.e. the number of electrons equals to that of holes, n e = n h. Evidently, the compensation situation is impossible for odd number of conduction electrons per atom. Among transition elements, the compensated metals are Ti, Cr, Mo, W, Re, Fe, Os, Ni, Pd, Pt, and Sc, V, Nb, Ta are uncompensated (for other dmetals the data in [10, 443] are absent). As follows from (5.92), at ω e,h τ 1 the offdiagonal conductivities c do not depend on τ and m*, and the Hall fields are given by
230
Transport properties E ye,h = −
1 jx H z , ne,h ec
(5.113)
so that
σ yx = σ yxe + σ yxh = (nh − ne )
ec . H
(5.114)
At n e = n h the quantity σ yx vanishes and
τe τh 1 , + e h me mh ω c ω c τ eτ h
σ xx ne2
(5.115)
so that ρ xx ∼ H 2 . Thus, in the case of a compensated metal ∆ ρ / ρ does not exhibit saturation. In a similar way one may explain the existence of peculiar field directions in a crystal where saturation is absent [10, 144]. To this end we have to consider orbits which are open in some direction (these correspond to an open orbit in the kspace). Then the field H will not influence such electron states and we obtain again ρ xx ∼ H 2 . The linear Kapitza law in strong fields may be connected with the anisotropy of ∆ ρ / ρ effect in single crystals. Such a behaviour is obtained after averaging over orientations with account of open orbits [144]. The above classification may be changed by magnetic ordering because of lifting spin degeneracy. In particular, the compensation may become violated for partial occupation numbers with a given spin projection.
5.7 ANOMALOUS TRANSPORT EFFECTS IN FERROMAGNETIC METALS 5.7.1 The extraordinary Hall effect According to (5.91), the Hall resistivity in ferromagnetic crystals is given by
ρ H = E y /jx = R0 H + R1 M = R0 B + 4π Rs M ,
(5.116)
where B = H + 4 π M is the ‘true’ macroscopic field in the substance, (5.117) R1 = 4π ( R0 + Rs ), Rs = R1 /4π − R0 . The presence of the peculiar Hall coefficient R s in ferromagnets was established in first experimental investigations of the Hall effects (see [265, 384]). Already in 1881 (the ‘normal’ effect was discovered in 1879) Hall found the influence of magnetization on the transverse electric field, which occurred in an external magnetic field. When 231
Chapter 5
Fig. 5.32. The schematic behaviour of Hall resistivity as a function of the field H in ferromagnetic metals. The dependence ρ H (B), which demonstrates explicitly the separation of the normal and spontaneous Hall effect, has the same form.
measuring the electric field as a function of magnetic induction B in nickel, he noted that the slope of the linear increase changed after magnetic saturation. A typical field dependence ρ H (H) in a ferromagnet is shown in Fig.5.32. At 0 < H < H c (H c is the field where magnetic domains become fully oriented) the magnetization increases rapidly from 0 to M s , so that ρ H (H c ) = 4 π (R s + R 0 ) M s and the slope of the curve is determined by the quantity 4 π (R 0 + R s ). At H > H c the slope is determined by the usual coefficient R s and weak highfield susceptibility (‘paraprocess’). The coefficient R s determined in such a way turns out to exceed R 0 by several orders of magnitude, which may be seen explicitly from the break of the plot ρ H (B). This demonstrates wittingly the existence of the extraordinary Hall effect. Besides that, attempts to define the Hall coefficient in ferromagnets in the standard form ρ H = RB resulted in quite strange temperature dependences of the Hall coefficient (in particular, in a jump at the Curie point). Therefore Pugh [449] proposed to express the Hall field in terms of the magnetization. Kikoin [450] investigated the temperature dependence of the Hall field of nickel in a wide region below and above T C. The results yielded convincing evidences for existence of the spontaneous Hall effect. Its temperature dependence was described by the expression (5.118) R1 (T ) = a[ M 2 (0) − M 2 (T )]. It was also found that the relation with the resistivity R( ρ ) ∼ ρ n takes place in iron group metals for varying temperature and impurity con232
R s·10 12 ,
V ⋅ cm A·G
Transport properties
Fig. 5.33. The temperature dependences of the spontaneous Hall coefficient in iron group metals [451].
centration where n = 1.2–2 (see [394,457]). Experimental data on the temperature dependence of Rs in iron group metals are shown in Fig.5.33. The extraordinary contribution to the Hall effect in ferromagnets occurs even in the paramagnetic phase where the magnetization is given by M = χH and (5.119) R = R0 + χ R1 . –3 Despite the small value of χ ∼ 10 , the addition to R 0, may be noticeable. The extraordinary (anomalous) Hall effect is also observed in antiferromagnets and paramagnets. Its value is especially large in compounds with high values of χ, including Kondo lattices and heavy fermion systems (Chapter 6) [451, 452]. The first theoretical consideration of the anomalous Hall effect (AHE) was carried out by Rudnitskii [453]. He demonstrated that the simplest supposition about the deviation of magnetized conduction electrons in the field induced by electric current may not explain the value of the effect, leading to quantities which are smaller by three orders of magnitude than the experimental ones. Further, he put forward the idea to explain the effect by the spinorbit interaction. The corresponding energy (5.120) Eso = 〈Hso 〉, Hso = λ ls = λ[rp]s z is proportional to the magnetization 〈S 〉 = M and yields the force
233
Chapter 5
∂ Eso ∼ [pM ], ∂r which is similar to the Lorentz force. The estimate Fso =
Eso = µ B H so ∼ 10−13 erg, H so ∼ 107 Oe just yields the effective magnetic field required. Already in the paper [453] the basic question about the averaging of the spinorbit interaction over a crystal with possible zero result was considered. Indeed, the periodic SOI itself does not provide the Hall effect, but one has to introduce inhomogeneities which scatter current carriers and lead to an asymmetry of y and –y directions. Thus the value of R s correlates with the electrical resistivity. The first attempt of quantum calculation of the Hall coefficient in ferromagnets with account of SOI was carried out [454]. However, the authors of this paper did not take into account symmetry properties of SOI matrix elements. In fact, no linear in SOI corrections to the electron distribution function exist, so that the result of the calculation [454] should vanish. The absence of the AHE within the lowest order approximation in the transport equation was demonstrated by Karplus and Luttinger [455]. To obtain a nonzero effect, they considered dynamical corrections to the electron energy in the electric field (i.e. to the field term) owing to interband matrix elements of SOI and of velocity. The corresponding offdiagonal conductivity does not depend on the scattering mechanism. Since Rs ≈
1 1 σ yx ( M ) R1 ≈ − , 4π 4π M σ xx2
(5.121)
we obtain
Rs = αρ xx2 ,
(5.122)
where the constant α does not depend on temperature. The result (5.122) was widely used to fit experimental data. Being important for the development of the theory, the calculations [455] still had incomplete and rather artificial character. Indeed, they did not take into account corrections to the collision term which have lower order in the scattering amplitude and may yield larger contributions. Thus the theory of AHE required a more consistent consideration. A step in this direction was made in papers by Kohn and Luttinger [458] where a new method of obtaining transport equations with the 234
Transport properties use of equations of motion for the density matrix was proposed. In [459] this method was applied for calculation of AHE owing to scattering of magnetically polarized current carriers by impurity centres. Unlike [457], contributions owing to collision terms (‘skew scattering’) occurred in both the lowest and next orders with respect to the scattering amplitude. The final result has the form (5.123) Rsi = αρi + βρi2 , where ρ i is the impurity resistivity of a sample. The ratio of the – first term in (5.123) to the second one equals E F /(3n i φ ) where n i – is the concentration of impurity atoms, φ is the impurity potential. At small n i this ratio is large, so that almost linear dependence R s( ρ i ) should be observed. Detailed derivation of the ρ linear term is considered in Appendix M.1. The expression for the coefficient α in (5.123) reads
α =−
µ B2 kF3 ρeff ϕ , 18π∆ 2 M (0)
(5.124)
where the effective charge density ρeff is defined by (M.52) and includes the spinorbital parameter, ∆ is the splitting of energy levels, which is of order of bandwidth. Some peculiarities of this expression should be discussed. The sign of Rs is determined by signs of not only current – carrier charge and SOI, but also the potential φ . Therefore this sign may be reversed by changing the sign of impurity charge. The influence of impurities on the Hall coefficient is stronger than that on resistivity since R s is proportional to the third power of scattering amplitude. The results (5.123) cannot be easily extended by replacing ρ i to the total resistivity (such a replacement may be made only in the second term). Thus a concrete consideration of various scattering mechanisms was needed. As discussed above, the explanation of AHE is based on the spinorbital interaction which results in occurrence of transverse contribution to current even for isotropic scattering. Since SOI is linear in magnetization, we have to calculate corrections to the distribution function which are linear in SOI. On the other hand, for nondegenerate wavefunctions (i.e. for quenched orbital momenta) the operator H so has only offdiagonal matrix elements, so that linear corrections to the electron energy are absent. Therefore the transport equation in the Born approximation, which depends only on the electron energy and the squared scattering amplitude, does not yield AHE. Thus we have to consider higherorder transport equations for various scattering mechanisms (Appendix M). The phonon mechanism was considered by Irkhin and Shavrov 235
Chapter 5 [460]. The lowestorder transport equation which yields the phonon scattering contribution to AHE is the equation of the second order in the perturbation Hamiltonian H′. According to (M.72), the corresponding expression for the spontaneous Hall coefficient reads 2 e 2 n 1 ρ2 Rsph = − g µ B2 2 ρeff t * , m M (0) 3 ∆
(5.125)
where t is the number of subbands. Introducing the effective spinorbital field
π µ B H so = Eso = − µ B2 ρeff , 3
(5.126)
we derive
E e 2 n ρ ph R = 2t so2 * , ∆ m M (0) 2
ph s
(5.127)
Thus the relation R ph ∼ ρ 2ph takes place. The expression (5.127) may s be rewritten in the form Rsph = ±2t
Eso ρ ph , τ ph ∆ 2 M (0)
(5.128)
so that the sign of R s is determined by the sign of m*: R s < 0 for electrons and R s > 0 for holes. Putting ε so ∼ 10 −14 erg, ∆ ∼ 10 −12 erg, ρ ∼ 10 −5 Ω ⋅ cm, τ ∼ 10 −13 s we estimate R s ∼ 10 −13 Ω ⋅ cm/ G. Further theoretical investigations of the phonon mechanisms were performed in papers [461, 462]. The role of twophonon scattering processes was investigated in [463]. The square dependence R s ( ρ ) was also found in the paper [464] for the scattering by spin inhomogeneities; the principal linear term was not found because of too simple decoupling of spin correlators. Kondo [465] considered the latter problem in the framework of the s–d exchange model with account of the proper SOI among localized electrons. He did not derive the transport equation, but used the equations by Kohn and Luttinger [458] for the impurity scattering. Thus the inelastic part of the scattering was not taken into account. The result by Kondo for dmetals reads Rsmag ∼
λ (m* )5/2
z z 3 2 4 〈( S − 〈 S 〉 ) 〉 G G G G , − 2 0 0 1 ∆ EF1/2 4 e 2 〈S z 〉 3
(5.129)
where G are the s–d exchange ‘Slater’ integrals of the type (K.5),
236
Transport properties ∆ is the energy difference for magnetic delectrons. Main shortcoming of the calculation [465] was using delectron states with unquenched orbital momenta. At the same time, the unquenching of orbital momenta in dmetals is connected with the same SOI which is responsible for AHE. This point was taken into account by Abelskii and Irkhin [466] who considered within the twoband s–d model two types of SOI: ‘proper’ d–d interaction λ and the interaction sspin–dorbit λ ′ (see Appendix L). The magnetized delectrons were supposed to be itinerant and described in the tightbinding approximation with a small bandwidth, so that their orbital momenta were almost quenched. The result of this paper for high temperatures for spin S = 1/2 reads (see (M.99)) 2
Rsmag =
9π 1 ρ λ 1 z 2 − 〈S 〉 , 64 EF M (0) 4
(5.130)
where m* I (1) 2 ≈ lz + λ ′. , λ λ eff ∆E 3 e 2 n Taking into account the expression for the spindisorder resistivity (5.57) this result may be presented in the simple form
ρλ = λeff
Rsmag = ±
3 λeff ρ mag , 16 EF M (0)
(5.131)
where the + and − signs correspond to electron and hole conductivity. Thus we obtain a simple connection between ρ mag and R s . The contribution of the electronelectron scattering to the extraordinary Hall effect was calculated in [467]. The result reads 4
T R ∼λ . (5.132) EF Separation of various contributions to AHE may be carried out by investigating the dependence R s (T) at crossing the Curie point, since in the far paramagnetic region the magnetic scattering mechanism is saturated. Another possible way is considering the dependence of R s on the magnetic field in the ferromagnetic phase [468]. Since the magnetic field suppresses spin disorder, d ρ mag /dH < 0 in the paraprocess region. Therefore the signs of R s and dR s /dH should be opposite provided that magnetic mechanism dominates. According to [468], for nickel the signs of both R s and dR s/dH are negative. This may be explained by the large phonon contribution. However, ee s
237
Chapter 5 this does not quite agree with the dependence R s (T) above T C (the rapid increase of R s is not observed). An attempt to formulate a new picture of AHE was made by Berger [469] who considered the ‘sidejump’ scattering of the electron wave packet under influence of various mechanisms. The universal result R s ∼ ρ 2 is obtained in such an approach. It was demonstrated later [470] that the sidejump scattering is just another formulation of the Luttinger’s skew scattering (corrections to the field term). On the whole, experiments at high temperatures are in agreement with the above theoretical results. However, the measurements at low T do not yield a linear dependence between ln R s and ln ρ . Thus a special consideration of the spinwave region, where the mean field approximation is inapplicable, is required. The calculation by Kagan and Maksimov [471] yielded the result R s ∼ T 4 . In the paper [472] another contribution, which was due to energy dependence of the distribution function, was found. It turns out that, because of cancelation of the lowestorder terms, such contributions to AHE (unlike resistivity) are the most important ones. The final result of [472] reads (see Appendix M.3)
Rs = ±
−2 I 2 dEk 3π k 512 e 2 kF M (0) dk k = kF
3 T 4 T A + B , TC TC
(5.133)
where the constants A = 1.1λ l
I (1) , ∆E
B = 0.8λ ′
(5.134)
are determined by ‘proper ’ and ‘improper’ SOI respectively. One can see that a simple connection between the Hall coefficient and resistivity is violated at low temperatures and the dependence R s (T) may be rather complicated. This is confirmed by experimental data on Fe, Co, Ni (Fig.5.33) and diluted ferromagnetic alloys [473], which demonstrate nonmonotonous temperature dependences of R s whereas ρ behaves monotonously. A number of calculations of the anomalous Hall effect with account of realistic band structure (in particular, the Fermi surface topology and anisotropy) were performed [474, 475]. The results show the strong influence of the Fermi surface details on the anomalous Hall effect at low temperatures. The Hall effect in 4fmetals merits a special consideration. Due to the variety of magnetic structures and complicated phase diagrams in rare earths, the role of various factors in the Hall effect may be 238
ρ Η ·10 8 , Ohm·cm
R s, 10 12, Ohm·cm/G
Transport properties
Fig. 5.34. The extraordinary Hall resistivities of gadolinium, terbium and dysprosium as a function of T/T N . The dashed curve is the theoretical plot obtained from the results by Maranzana. Above T N, the values of R s for heavy rare earths are shown which are temperature independent [15].
investigated here. In particular, the influence of antiferromagnetism and strong magnetic anisotropy becomes important. On the other hand, the situation is somewhat simplified in comparison with d metals because of a distinct separation between current carriers (s, p, d electrons) and magnetic felectrons, which permits to separate proper and improper spinorbital interaction effects. The normal and anomalous Hall effects in 4fmetals were extensively investigated starting from 60s. Detailed investigations were performed for heavy rare earths (a review is given the monograph [15]). The temperature dependences of the Hall coefficient for heavy rareearth metals are shown in Fig.5.34. Main distinctive features of the anomalous Hall effect in comparison with 3dmetals are as follows 1. The dependence R s (T) has a more complicated nonmonotonous character. However, the temperatures of a maximum (minimum) do not coincide with points of transitions between magnetic structures. A change in R s(T) sign takes place for Tb and Dy at T ∼ 0.8–0.9T N. 239
R s, 10 12, Ohm·cm/G
Chapter 5
ρ Η ·10 6 , Ohm·cm Fig. 5.35. The extraordinary Hall coefficient of dysprosium with the magnetic field along the aaxis as a function of spindisorder resistivity [15].
2. A good proportionality between Rs and magnetic resistivity takes place (Fig.5.35). 3. R is highly anisotropic: the values in different crystallographic directions vary by several times. 4. The dependence R s (T) is not influenced by ferroantiferro transitions. It would be instructive to compare the R s behavior in AFM region with data on other antiferromagnets, e.g., Cr and Mn [443]. However, this comparison is hampered by that the latter data are insufficient to separate the normal and anomalous contributions. Theory of AHE in rareearths is based on the abovediscussed general theory but some extra factors should be taken into account. The terms with the vector products [k, k′], which arise from the matrix elements of the conduction electron orbital momenta (l) kk′ , describe the anisotropic electron scattering. Such terms correspond to the coupling of conduction electron current in the external electric field to the momentum J and yield therefore the anomalous Hall effect. The Hall coefficient is proportional to A(g – 2), which corresponds to the interaction of electron orbital momenta with the localized orbital momenta (2–g)J (see (B.20)). This picture is different from that in dmetals where the anomalous Hall effect is due to weak spinorbit coupling. For felectrons, this coupling is strong (of order 240
Transport properties 1 eV), which enables us to consider only one Jmultiplet, so that the spinorbit coupling constant does not enter explicitly the results. It is worthwhile to mention that one of first papers, devoted to derivation of the Hamiltonian of the type (K.4), was the paper by Kondo [465] on the theory of the anomalous Hall effect (which preceeded to the famous papers on the Kondo effect). In the antifferromagnetic region one has to determine the saturation magnetization in terms of highfield susceptibility χ s = dM/dH. Then one obtains the following equations for the Hall resistivity ρ H
ρ H ( H dm ) = 4π ( R0 + Rs ) M s ,
(5.135)
∂ρ H = R0 + 4π [ Rs + R0 (1 − N )]χ s , (5.136) ∂H where H dm = 4 π NM s , N is the demagnetization factor. Thus one can separate the normal and anomalous Hall coefficients by measuring M s , χ s , N and ρ H (H). It should be noted that in the AFM region χ is not saturated up to H ∼ 40 kOe. Although the spindisorder scattering mechanism [465, 466] yields the behaviour R s (T) ∼ ρ mag (T) which is really observed at low temperatures, such simple theory does not explain changes in the R s(T) sign. Attempts to do this were performed by a number of authors [476–478]. The idea by Maranzana [476] was using higherorder terms in the s–f Hamiltonian derived by Kondo (see also Appendix K). Besides the main anisotropicscattering term
iλ1 (2 − g )[k , k ′]Jν ck†α ck ′α = iλ1[k , k ′]Lν ck†α ck ′α , the terms were considered, which had the structure iλ2 〈Jν Jν 〉〈[k , k ′]σ αβ 〉ck†α ck ′β ,
(5.137) (5.138)
the scalar product of tensors being defined by
1 1 ( AC )( BD) + ( AD)( BC ) − ( AB)(CD) . (5.139) 2 3 As a result, higher powers of momentum operators occur, which result after averaging in new functions of magnetization. In particular, there exist the contribution to Rs which is proportional to the second derivative of the Brillouin function, 〈 AB〉〈CD〉 =
T M S = 〈( S z − 〈 S z 〉3 )〉 = − J 3 BJ′′ ( y ) = − J 3 f1 , TN where
241
(5.140)
Chapter 5
y=
3〈 J z 〉 TN g J µ B H + . J +1 T kBT
(5.141)
Therefore this contribution is nonmonotonous near T N. Giovannini [477] introduced a still more complicated function
M 4 = J 4 {BJ′′′ ( y) + 2 BJ′′ ( y ) + 2[ BJ′ ( y)]2 } ≡ J 4 f 2 (T/TN )/BJ ( y ), (5.142) which contains the higherorder derivatives of B J . This led to the dependence of the form (5.143) ρ H = C1 f1 (T/TN ) + C2 f 2 (T/TN ). The constants C 1 ∼ λ 1 and C 1 ∼ λ 2 were used as fitting parameters. For Tb and Dy C 2 /C 1 ∼ 30, and 9 respectively, whereas C 2 = 0 for gadolinium. The value of C 1 for Gd corresponds to the unreasonably large spinorbital constant λ ≅ 0.5 eV. The values of R s in paramagnetic regions, which are obtained from the estimations of C 1 and C 2 , turn out to be not quite satisfactory. It should be also noted that the C 2 term corresponds to a rather higher order in the s–f Hamiltonian and hardly may give a dominating contribution. Therefore, despite a qualitative explanation of the Rs(T) behaviour, the mechanism discussed is debatable. Somewhat later Fert [478] considered the influence of the sidejump scattering which corresponds to corrections to the field term in the transport equation. This mechanism yields some renormalizations of the coefficients at the Brillouin function derivatives. However, the value of AHE in gadolinium remains unexplained. The anomalous Hall effect in heavyfermion systems is discussed in the papers [479]. 5.7.2 Magnetoresistivity in the presence of spontaneous magnetization The ∆ ρ / ρ effect in ferromagnets has important peculiarities. Its value may be of order 10 2 , which is much greater than in usual metals, and have both positive and negative sign (Fig.5.36). The Kohler rule is usually not satisfied. An important circumstance of the situation in a magnetized sample is possibility of the nonzero effect in the absence of the external magnetic field. The spontaneous effects are masked in multidomain samples where the average magnetization is zero. The single magnetic domain forms in the fields above the field of technical saturation H c . In the lowfield region (below H c ) the effect is due to a change in relative volumes of domains with M  j and M ⊥ j:
242
∆ ρ / ρ 0 , 10 3
Transport properties
kOe Fig. 5.36. The field dependence of ∆ ρ/ρ in ferromagnetic nickel for parallel and perpendicular orientations of current and magnetic field [265].
1 (V ρ + V⊥ ρ ⊥ ). V
(5.144)
ρ = ρ + ρ ⊥ ,
1 3
(5.145)
∆ρ ( H c ) ∆ρ ⊥ ( H c ) = −2
(5.146)
ρ (H ) = For H = 0 we have
2 3
so that
(Akulov’s rule for even transport effects [265]). Above the technical saturation H > H c , the field dependence of resistivity is considerably weaker and determined by the paraprocess (the field dependence of magnetization M = Ms + χH ). The dependence ρ (H) is owing to suppression of spin disorder, which results in a decrease of exchange scattering of current carriers. This effect should take place also in the paramagnetic region T > T C , resulting in a negative contribution to ∆ ρ / ρ . Experimental data are often described by the equation 243
Chapter 5
∆ρ ρ = a( M s2 − M 2 ( H )),
(5.147)
so that (5.148) ∆ρ ρ = −a1H − a2 H 2 . Thus we obtain the linear ∆ ρ / ρeffect. It should be noted that similar field dependences of ∆ ρ / ρ may take place also in antiferromagnetic metals. For example, the behaviour ∆ ρ / ρ ∼ H 3/2 was found in Fe 3 Pt [480]. As it is clear from the above consideration, the ∆ ρ / ρ effect in a single domain is determined by the difference of ρ ⊥ and ρ  , i.e. by dependence of resistivity on the angle between vectors j and M. This dependence turns out by onetwo order of magnitude stronger than in the usual ∆ ρ / ρ effect. Therefore the Lorentz force does not explain the effect quantitatively. The most natural relevant microscopical mechanism is, as well as for the extraordinary Hall effect, the spin orbital interaction. The extraordinary ∆ ρ / ρ effect, which is quadratic in M, occurs in the second order of perturbation theory in this interaction. Unlike the Hall effect, the microscopic theory of the ∆ ρ / ρ effect in ferromagnets is not developed in detail, and the whole physical picture is still absent. Some calculations with account of different scattering mechanisms and the spinorbital interaction were performed starting from 50s [265]. Smit [481] and Marsocci [482] investigated the Mott s–d transition mechanism. Kondo [465] treated the scattering by magnetic inhomogeneities (as well as for the Hall effect, the picture of unquenched orbital momenta was used). Vu Dinh Ky [483] considered the transport equation for the impurity scattering. In the second order in SOI, corrections, which are proportional to [kM] 2 , occur both in collision and scattering terms. They yield the resisitivity anisotropy required. The final result is rather cumbersome and may be represented in the form
∆ρ ρ ∼ λ 2 M 2 ,
(5.149)
so that ∆ ρ / ρ decreases with temperature and vanishes above the Curie point. A numerical estimation was made in [483] by using the comparison with the anomalous Hall effect. Since the Hall resistivity ρ H = 4 π R s M occurs in the first order in λ , but contains – an extra power of the impurity potential φ , we have (5.150) ∆ρ ρH ∼ Hso /φ . – Putting for nickel H so ∼ 10 −13 erg and φ ∼ 10 −14 erg one obtains ∆ ρ / ρ ∼ 0.1 in a rough agreement with the experimental data 244
Transport properties ( ρ H / ρ ∼ 0.5%, ∆ ρ / ρ ∼ 3%). The phenomenological consideration of magnetoresistivity in ferromagnetic metals may be performed within the twocurrent model with strongly different currents j ↓ and j ↓ [436]. 5.7.3 Magnetooptical effects Magnetooptical (MO) effects in ferromagnetic transition metals are closely related to galvanomagnetic effects. Experimentally, the Faraday and Kerr polarization plane rotation angles in ferromagnets are by several orders larger than in paramagnetic metals. They are proportional to magnetization rather than to magnetic field and strongly decrease above the Curie point. Microscopic mechanisms of the large MO effects are connected with spinorbital interaction. In particular, the Faraday effect is analogous to the highfrequency extraordinary Hall effect. Although the spontaneous Hall effect is determined in the static limit by the magnetization, separation of magnetic and electric characterisitics at high frequencies becomes impossible, so that the similarity with magnetooptical effects occurs. Proportionality of the Hall field and the Faraday rotation was established already in 1893 by Kundt [484]. From the phenomenological point of view, polarization plane rotation is due to gyrotropy, i.e. presence of antisymmetric contribution, in dielectric and magnetic permeability tensors ε αβ ( ω ) and µ αβ ( ω ). In the optical region the magnetic gyrotropy is connected mainly with anisotropy of gyroelectric properties, the qdependence of ε (q, ω ) playing an important role. First physical explanation of MO effects in ferromagnets was given by Hulme [485] and Kittel [486], and the theory of the frequency dependence was developed by Argyres [487] and Cooper [488]. An account of electron scattering permitted to extend the theory to the lowfrequency region [489,490] and the case of low temperatures [491,381]. Consider a simple theory of the MO Kerr effect. At reflection from the magnetic medium with the complex refraction factor ñ = n + ik and offdiagonal conductivity σxy, the light with the frequency ω changes its polarization by the Kerr angle
θK =
4π
ω
( A Im σ xy + B Re σ xy )/( A2 + B 2 ),
where
A = n3 − 3nk 2 − n,
B = −k 3 + 3n2 k − k .
245
(5.151)
Chapter 5 At small damping k n the value of θ K is determined mainly by Im σxy. In the simplest case of a cubic structure with the magnetization vector which is parallel to the (001) plane, the Argyres formula takes the form [316] Im σ xy =
π [ Fmxy′m↑ (k )nkm′↑ (1 − nkm↑ )δ (ω − ω mm′↑ (k )) − ∑ ω k , m ≠ m′ − Fmxy′m↓ (k )nkm′↓ (1 − nkm↓ )δ (ω − ω mm′↓ (k ))],
(5.152)
where m is the band index,
ω mm′σ (k ) = ε kmσ − ε km′σ is the interband transition frequency, n kmσ is the Fermi distribution function, (l z )* lmz ′′m x y + Fmxy′mσ (k ) = 2i ∑ m′′m pmx ′′m pmm pm′′m′ pmy ′m , ′ ω m′m′′σ m′′ ω m′m′′σ
pαm′m = 〈km′σ  −i
(5.153)
∂  kmσ 〉, ∂xα
lmz ′m = 〈km′σ  ξ lz  kmσ 〉, l z is the orbital momentum operator zprojection,
2 ∂Veff , rc 2 ∂r with Veff being the effective potential for conduction electrons. The formula (5.152) demonstrates a strong dependence of the Kerr angle on electronic structure and magnetic ordering. Thus MO effects are promising from the point of view of comparison with band structure calculations. Comparison of magnetooptical properties with results of band calculations is performed, e.g., for nickel [381], Fe–Co alloys [492] and gadolinium [493]. An almost total compensation of the first and second term in the square brackets of (5.152) takes place provided that the spectrum e depends weakly on σ . At the same time, the effect is large in strongly ferromagnetic case. In particular, for halfmetallic ferromagnets (Sect.4.4) at ω < δ σ ( δ σ is the gap for the spin projection σ ) the corresponding term in (5.152) vanishes, so that one may expect large values of Kerr rotation. Indeed, for the system NiMnSn 1−xSb x the intensity of peaks in the frequency dependence of θ K decreases sharply with increasing x, i.e. as the Fermi level goes out of the gap [494]. According to (5.153), the angle θK is proportional to the spinorbit coupling, i.e. increases for
ξ=
246
Transport properties heavy elements. Therefore one may expect that the HMF which contain platinum should have larger values of θ K. Indeed, giant values θ K ≅ 0.15° (for the red light), which exceed considerably the values for NiMnSb, were observed the compound PtMnSb [307, 308] (the results of the calculation are given in [316]). Note, however, that according to [495] main difference between electronic structures of HMF’s PtMnSb and NiMnSb, which results in smaller value of θK in the latter compounds, is connected not so much with the spinorbit matrix element values, as with a shift of some energy levels owing to ‘scalar’ relativistic effects (velocity dependence of mass and the Darvin correction). In this sense, the simplest assumption about the direct connection between the spinorbit coupling strength and the Kerr rotation is not quite adequate. Record values of θ K might be observed in the ferromagnetic phase of the compound UNiSn, which should also have a halfmetallic structure [315, 316]. However, experimentally this turns out to be antiferromagnetic [496, 497] (see discussion in Sect.6.6). Nevertheless, investigation of isostructural compounds containing actinides (e.g., UCoSn, UPdSn) is of interest from this point of view. The polar, meridional and equatorial Faraday and Kerr effects, as well as the gyrotropic effect (change of reflected light intensity with magnetization) in ferromagnetic metals were studied systematically in [498–500]. In the case where the magnetization is perpendicular to the plane of the ingoing light wave it is posssible to determine simultaneously real and imaginary part of the tensors ε and µ [500]. Both intraband (indirect) and interband transitions turn out to play a role. The latter are important near resonance absorption frequencies, so that the frequency dependence of magnetooptical effects is a 1/ωhyperbola with peaks owing to interband transitions. A simple expression for the intraband contribution to offdiagonal magnetic permeability may be presented in the form [499]
ωp iκ , * 2 ω 2m c 2
µ xy (ω ) = −
(5.154)
where ω p is the plasma frequency, κ is an averaged (over the Fermi surface) dimensionless parameter which determines the correction to electron quasimomentum owing to spinorbital interaction. For ω ~10 14 s –1 one has µ xy ~10 –6 –10 –4 in agreement with experimental data. It is instructive to establish a correlation between temperature dependences of magnetooptical and galvanomagnetic effects and compare quantitatively the corresponding microscopic SOI parameters. In the paper [489], the relation between the extraordinary Hall coefficient 247
Chapter 5 R s and the MO parameters defined by
M j = σ 1 (ω )E + σ 2 (ω ) E , M
σ 2 (ω )/σ 1 (ω ) ≡ iq,
(5.155)
was obtained in the form
4π Rs M = −
σ 2 (0) . σ 12 (ω )
(5.156)
Using the expression for the oneband conductivity
σ 1 (ω ) = σ 1 (0)
γ γ + iω
,
(5.157)
where γ = 1/ τ is the relaxation rate we obtain
Re q = −4π Rs M σ 1 (0)
ω , γ
Im q = 4π Rs M σ 1 (0),
(5.158)
so that the signs of Re q and Im q are opposite and determined by the sign of R s , which agrees with the data [501, 451]. At the same time, in the case of the normal MO effect the signs of Re q and Im q coincide. The formulas (5.159) provide the correct order of magnitude for Im q. Since
Rs ∼ [σ 1 (0)]−2 , γ ∼ [σ 1 (0)]−1 , we obtain from (5.158) the temperature dependences Re q ∼ M (T ),
Im q ∼
M (T ) . σ (T )
(5.159)
(5.160)
Their verification is hampered by that the experimental Tdependences [501] correspond to the resonance region. Therefore investigation of the longwave region would be of interest. MO effects in the Xray region seem also to be promising to investigate the band structure. In particular, the magnetic Xray dichroism (MXD) effect is discussed in Sect.2.5. 5.7.4 Thermomagnetic effects Besides abovediscussed electric, thermoelectric and galvanomagnetic effects, there exist a number of effects owing to combined action of the fields E, H, and grad T [7, 8, 265]. Although not investigated now in detail, the thermomagnetic effects (TME) may be of interest since they provide an additional information about microscopic transport mechanisms in solids. Difficulties in studying TME increase for transition metals, 248
Transport properties especially in the case of magnetic ordering. First paper in this direction have demonstrated that TME are described by the same concepts and are determined by the same microscopic parameters as galvanomagnetic effects. In a number of cases one can perform a separation of ‘normal’ and ‘spontaneous’ TME. Therefore a correlation between TME and galvanomagnetic effects should exist which may be used to verify values of the microscopic parameters and separate different scattering mechanisms. Some attempts of this kind were made (see [475]). At present, most investigated TME are the Nernst–Ettingshausen and Righi–Leduc effects (see also Sect.5.1). The transverse NernstEttingshausen effect is the occurrence of the electric power E y in the presence of the magnetic field H z and temperature gradient in the xdirection. Similar to the Hall effect, we have E yNE = (Q0 Bz + 4π Qs M z )grad xT ,
(5.161)
where Q 0 and Qs are the normal and spontaneous Nernst–Ettingshausen coefficients. The general expression (5.1) under the conditions
j = 0,
∂T ∂T = = 0, ∂y ∂z
(5.162)
yields Ey
λxxσ yx − λyxσ xx ∂T . σ xx2 ∂x
(5.163)
The experimental dependence Q s (T) turn out to be stronger than Q 0 (T). This dependence is described by the empirical equation [502] (5.164) Qs (T ) = −T (α + βρ ), where α is determined by impurities. A derivation of the formula (5.164) with the use of the densitymatrix appoach was performed by Kondorsky [503] by analogy with the Hall effect. The case of alloys was considered in papers [504]. The result (5.164) was confirmed also within the ‘sidejump’ mechanism approach by Berger [204]. The spontaneous Righi–Leduc effect (occurrence of grady T in the presence of grad x T and M z ) and the Ettingshausen effect (occurence of grad y T in the presence of electric current j x and magnetization M z ) were also investigated [475]. The normal Righi–Leduc coefficient is known to be expressed in terms of the Hall coefficient and conductivity,
eτ . (5.165) m*c Search of a similar relation for the spontaneous coefficient is of interest. A0 = σ R0 =
249
Chapter 6
Chapter 6 THE KONDO EFFECT AND PROPERTIES OF ANOMALOUS d AND fCOMPOUNDS In this Chapter we consider physics of some types of 4f and 5fcompounds which exhibit anomalous electronic properties. Here belong socalled heavyfermion, Kondo lattice and intermediate valence systems; in some aspects close is physics of some dsystems, in particular of copperoxide highTc superconductors where strong electron correlation effects in CuO 2 planes take place. We shall demonstrate applications of manyelectron models to the description of unusual physical phenomena in these substances. Of course, we do not claim to cover completely this topic which is very wide and rapidly develops, but consider some selected questions which are determined by the authors’ scientific interests. Most exotic properties are characteristic for heavyfermion compounds. They possess giant values of effective electron mass, which are manifested most brightly in the huge linear specific heat. In a somewhat arbitrary definition of heavyfermion systems, the boundary value of γ = 400 mJ/mol ⋅ K 2 was established. Besides that, large paramagnetic susceptibility at low temperatures and large coefficient at the T 2 term in resistivity are observed. An especial interest in the heavyfermion compounds was stimulated by the discovery of unconventional superconductivity in CeCu 2 Si 2 , UBe 13, UPt3. The superconducting state is characterized by an isotropic (nonzero angular momentum) pairing and is possibly not caused by electronphonon interaction [505, 506]; often superconductivity coexists with antiferromagnetic ordering. The properties of the ‘classical’ heavyfermion systems CeAl 3 , CeCu 6, CeCu 2Si 2, UBe 13, UPt 3, U 2Zn 17 , UCd 11 , NpBe 13 are considered in detail in the review [507]. For recent years, a number of ternary Cebased compounds with huge (of order 1 J/mol ⋅ K 2 and larger) 250
Kondo effect and properties of anomalous d and fcomponds Table 6.1. Electronic specific heat and magnetic characteristics (paramagnetic susceptibility, Neel or Curie (in brackets) point, paramagnetic Curie temperature and the ground state moment) of some anomalous rareearth and actinide compounds (heavyfermion, Kondo lattice and intermediate valence systems).
γ
χ (0)
T TNN)(T(TCC))
−3emu mJ/mol ·K2 10 –310emu/mol
CeAl3 CeAl2 CeCu2Si2 CeCu6 CeCu2 CeCu5 CeCu2Ge2 CeIn3 CeInCu2 CePb3 CeCu4Al CeCu4Ga CeCu3Al2 CeCu3Ga2 CeAl2Ga2 CeInPt4 CePtSi CePtSi2 CePt2Sn2 CePtIn CePdIn CePdSn CePdSb CeRu2Si2 CeZn11 CeRh3B2 UPt3 URu2Si2 UBe13 UZn8.5 UCd11 UAgCu4 UNiAl UNi2Al3 UPd2Al3 UPdIn U2PtSi3 YbCuAl YbAsf YbP YbSb YbSi
16 2 0 135 1100 1450 90 100 10 0 260 1200 1000b 2000( 0 being proportional to Z rather than Z (as in (L.3)). The latter fact results in that the interaction between spin and foreign orbit is more important for light elements. As a rule, for 3delectrons λ ′ is smaller than λ by twothree orders of magnitude, but, as we shall demonstrate below, the corresponding interaction may play an important role because of its singular kdependence. For a single electron, the ‘proper ’ SOI makes favourable the antiparallel interactions of its spin and orbital momenta, but the interaction (L.6) orientates its orbital momentum parallel to spin of other electrons. However, for more than halffilled shell the sign of λ changes and the state with the total momentum J = L + S has the lowest energy. Now we discuss SOI in periodic crystals. In the localized Heisenberg model the treatment is close to that for isolated atoms. On the other hand, for crystals containing 3delements the situation changes drastically. As discussed in Sect.1.3, the local crystal potential may quench orbital momenta in the case of crystals with low symmetry only. At the same time, in real dsystems with cubic or hexagonal local symmetry, which possess degenerate irreducible representations of the point group, the degeneracy is lifted by the periodic potential in the band picture (Sect.4.8). Therefore the case of quenched orbital momenta is of interest. Then only offdiagonal matrix elements of SOI are nonzero and the perturbed wavefunctions read 3
384
4
Spinorbital interaction 〈γ ′  Hso  γ 〉 (0) Ψγ ′ , Eγ − Eγ ′ γ ′≠γ
Ψ γ = Ψ γ(0) + ∑
(L.7)
with γ = {km σ } are the states of magnetic delectrons in the degenerate dband. The wavefunctions (L.7) may be used to calculate corrections to various physical quantities, owing to SOI. In particular, such corrections to matrix elements of electrostatic interaction between conduction and localized electrons will be anisotropic. It is these corrections which cause anomalous transport phenomena in magnetic crystals. The role of the proper SOI and the interaction (L.6) is different for different situations and concrete effects. For galvanomagnetic effects in dmagnets one can consider two cases 1.
2.
The mobility of delectrons is large, so that they determine galvanomagnetic effects directly. Then the proper SOI for itinerant delectrons plays the dominant role. There exist two electron groups – conduction selectrons with small magnetization and “magnetic” delectrons with small mobility. Then, among four possible types of SOI (s–s, d–d, s–d and d–s), the proper d–d interaction and the s–d interaction of selectron orbit with delectron spin are most important. The s–s and d–s interactions yield small contributions because of smallness of magnetization for selectrons.
Finally, we derive the Hamiltonian of the s–d model with account of SOI of d–d and s–d type in the second quantization representation. We consider the case of the strong crystal field which destroys total orbital magnetic momenta of delectrons. We have H = ∑tk ck†σ ckσ + ∑Eγ aγ† aγ + kσ
γ
+
∑ [ I (kσ ,γ , k ′σ ′,γ
kσ k ′σ ′
1
2
) − I (kσ , γ 1 , γ 2 , k ′σ ′) +
γ 1γ 2
+ L(kσ , γ 1 , k ′σ ′, γ 2 ) − L(kσ , γ 1 , γ 2 , k ′σ ′)]aγ†1 aγ 2 ck†σ ck ′σ ′ ,
(L.8)
where the Coulomb and exchange matrix elements
e2 ψ 3 ( x)ψ 4 ( x′) dxdx′ (L.9)  r − r′  (x = {r, s}) are to be calculated for the wavefunctions with account of SOI, and the spinorbital matrix elements are I (1,2,3, 4) = ∫ψ 1* ( x)ψ 2* ( x′)
385
Appendix L
e2 [r − r ′, p]s′ ψ * ( x)ψ 2* ( x′) ψ 3 ( x)ψ 4 ( x′) dxdx′. (L.10) 2 2 ∫ 1 mc  r − r ′ 3 In the representation γ={km σ} the diagonal matrix elements of H so(dd) vanish and the offdiagonal ones are obtained within perturbation theory with the use of (L.7). Substituting (L.7) into the exchange part of (L.9) we derive to linear approximation in H so the correction L(1, 2,3, 4) = −
H(1) sd = −λ ∑
〈k1m1σ 1  ls  k1m1′σ 2 〉 × Ek1m1σ1 − Ek1m1′σ 2 × I (0) (kk1m1′, k 2 m2k ′)ak†1m1σ 1 ak 2 m2σ ck†σ ck ′σ 2 + h. c.
(L.11)
The matrix elements in (L.11) are calculated, similar to Appendix K, with the use of the planewave representation for conduction electrons. It is convenient to use the mrepresentation for delectron functions (the functions, corresponding to irreducible representations of a point group are expressed as their linear combinations). This representation enables one to introduce in a simple way spin operators for localized delectrons: am† σ amσ = (1 + σ 2 s z )ϕ m (l z ),
am† ± am ∓ = s ±ϕ m (l z ),
(L.12)
where 1 4
ϕ 0 = 1 + (l z ) 2 [(l z ) 2 − 5], ϕ ±1 = ϕ ±2 =
1 z z l (l ± 1)[4 − (l z )2 ], 6 1 z z l (l ± 1)[(l z ) 2 − 1], 24
(L.13)
and the offdiagonal products a†mσam′σ are expressed in terms of operators l ±. Then we obtain for a cubic crystal
λ ′ ∑ ∑ Fll′ (lν , sν )ei (k −k )Rν ck†σ ck′σ , (L.14) ∆E ll′ ν kk′σ where we have put for simplicity ∆E γγ′(k) = ∆E = const. The expansion term with l = l′ = 1 reads Hsd(1) =
λ 6 2 ′ π e ∑ G11(1) (k , k ′)[kk ′]sν 〈ϕ (lν )〉 ei ( k −k )Rν ck†′σ ckσ (L.15) ∆E 5 ν kk ′σ (where the radial integral G is given by (K.5)) and describes anisotropic scattering. Hsd(1) (11) = −i
386
Spinorbital interaction Now we calculate matrix elements of the ‘improper’ SOI (L.10). Replacing for simplicity squares of wavefunctions of delectrons by δ functions (which is possible since orbital momenta of delectrons do not enter) we derive L(kk ' ) = iλ ∑e
)
i ( k − k' Rν
ν
[kk ' ] sν , (k − k ' )2
(L.16)
with λ ′ ∼ 10 −16 erg. The expression (L.16) does not yield a dependence on orientation of localized spin in the crystal. However, such a dependence will occur for more complicated dwavefunctions. Combining (L.15) with (L.16) we write down the correction to the Hamiltonian of the s–d model owing to SOI as Hsd′ =
∑e ν σ
)
i ( k − k ′ Rν
kk ′
(sν Λ kk ′ )ck†σ ck ′σ ,
(L.17)
where
z = iλ l Λ kk ′ l =
(1) I kk [kk ′]z ′ [kk ′]z + iλ ′ , ∆E kk ′ (k − k ′) 2
2 z 2 1 (l ) [4 − (l z ) 2 ] (l z )2 [(l z )2 − 1] + 2(l z ) 2 [4 − (l z ) 2 ] , 9 4
(L.18)
(L.19)
I (1) is defined by (L.15). Although  λ ′  λ , the role of the second term in (L.17) may be important provided that small values of k − k′′ yield the dominant contribution, as it takes place for extraordinary transport phenomena at low temperatures.
387
Appendix M
Appendix M THE DENSITY MATRIX TECHNIQUE FOR DERIVATION OF TRANSPORT EQUATIONS AND THE THEORY OF THE ANOMALOUS HALL EFFECT Mathematical description of transport phenomena deals with an balance equation for the distribution function of current carriers in external electric, magnetic and thermal fields (5.14). In simple cases such equations may be obtained from a simple physical consideration of the electron motion in the kspace due to external fields and collisions. However, in more complicated situations, where higher orders in the scattering amplitude become important, such simple arguments are not sufficient. Since often we do meet with this situation for transport phenomena in magnetic crystals, constructing a general method for derivation of transport equations is needed. Most convenient is the approach which uses the density matrix. The equations of motion for the latter quantity have usual quantum mechanics form and may be simply reduced to transport equations. Define the density matrix operator
ρˆ = e− β H Sp e− β H ,
β ≡ 1/T ,
(M.1)
where H is the total Hamiltonian of the system including current carriers, scattering system and external fields. The coefficient in (M.1) is determined by the normalization condition Sp ρˆ = 1.
The operator ρˆ, as well as H, may be written down in any quantum representation. In the solid state theory, it is convenient to use the second quantization representation. Then the symbol Sp means the summation over all the possible occupation numbers of quasiparticles in the system. For example, in the case of electronphonon system
388
Density matrix technique
Sp… =
∑
…,
(M.2)
{nk }{ Nq }
where n k = 0, 1 are the electron occupation numbers and N q are the phonon ones. Average value of a physical quantity A is obtained as (M.3) 〈 A〉 = Sp ( ρˆ A). Calculate for example the average occupation numbers for noninteracting conduction electrons. We find
∑ 〈… n
〈nk 〉 = 〈ck† ck 〉 =
k
{ nk ′ }
∑ 〈… n
k
{ nk ′ }
…  ∏ exp(− βε k ′ ck†′ ck ′ )ck† ck  … nk …〉 k′
…  ∏ exp(− βε k ′ ck†′ ck ′ )  … nk …〉 = k′
= ∑ exp(− βε k )nk nk
∑ exp(− βε
k
) = (exp( βε k ) + 1) −1 ,
nk
i.e. we derive the Fermi distribution function. Provided that the Hamiltonian of the system is written in the form H = H0 + H ′, with H ′ being a perturbation, the equilibrium density matrix ρˆ(H ) may be expanded in the powers of H′, which is required at calculating the field term in the transport equation. To this end one may use the theorem about expansion of exponential operators [706]: 〈n  exp(− β (H0 + H ′))  n′〉 = δ nn′ exp( − β En0 ) − exp(− β En0 ) − exp(− β En0 ) 〈 n  H ′  n′′〉〈 n′′  H ′  n′〉 − 〈n  H ′  n′〉 + ∑ × 0 0 En − En ′ En0′′ − En0′ n′′ exp(− β En0′ ) − exp(− β En0 ) exp(− β En0′′ ) − exp( − β En0 ) (M.4) × − , En0 − En0′ En0 − En0′′ where E n0 are the eigenvalues of H 0 . In the second quantization representation, the numbers n mean the occupation number sets, and summing over them yields an expression of ρˆ(H) in terms of powers of H ′ and ρˆ(H ) = ρˆ 0 . In an representation of the wavefunctions l〉 we have
ρˆ = ρˆ (0) + ρˆ (1) + ρˆ (2) +…, where
ρˆ ll(0)′ = ρlδ ll′ ,
ρˆ ll(1)′ =
389
ρ l − ρl ′ H ′′ , ε l − ε l ′ ll
(M.6a)
Appendix M
ρˆ ll(2)′ = γρl δ ll ′ + ∑ l ′′
Hll'′′ Hl ′′'l ′ ρl − ρl ′ ρl − ρl ′′ − ; ε l − ε l ′ ε l − ε l ′ ε l − ε l ′′
(M.6b)
ρl − ρl′ ∂ρl − . (M.6c) ε l − ε l ′ ∂ε l ll' The equation of motion for the density matrix operator has the usual form
γ =∑
 Hll′′ 2 ε l − ε l′
∂ρˆ = [H , ρˆ ]. (M.7) ∂t In any representation l〉, we may write down the system of equations for diagonal and offdiagonal matrix elements. Under certain conditions this system may be reduced to transport equations of the lowest Born and nextorder approximations. In this way, transport equations were obtained for elastic scattering by impurities [458], and further for scattering by phonons [460] and spin inhomogeneities [466]. The theory in the case of arbitrarily strong scattering amplitude, but small impurity concentration was developed by Luttinger [707]. However, for a complicated H 0, calculations in the matrix form are rather cumbersome even for impurity scatterng in the second Born approximation. Therefore it is very convenient for practical calculations to derive transport equations in an operator form without concretizing the Hamiltonian. Now we consider this technique constructed in [471, 472]. The only requirement to the Hamiltonian is the possibility of the representation i
(M.8) Ht = H0 + HE est + H ′, where H0 has a diagonal form in the nrepresentation, H E is the energy of the system in the adiabatically included (s → 0) electric field E, H′ is an offdiagonal part. The total density matrix operator is represented as
ρˆ t = ρˆ + ( fˆa + fˆb )e st ,
(M.9)
where ρˆ is the equilibrium density matrix in the absence of electric field, fˆa and fˆb are the diagonal and offdiagonal components of the correction. Taking into account the relations [H0 , fˆa ] = [H ′, fˆa ]a = [H0 , fˆb ]a ,
we obtain to linear approximation in E 390
Density matrix technique sfˆa = [H E , ρˆ ]a + [H ′, fˆb ]a ,
(M.10)
fˆb = Lˆ−1{[H E , ρˆ ]b + [H ′, fˆa + fˆb ]b },
(M.11)
where
1 , ∆fˆb = [H0 , fˆb ], (M.12) is − ∆ ∆ is the difference of the eigenvalues of H in the corresponding states. The system (M.10), (M.11) may be solved by the iteration method. Substituting (M.11) into (M.10) we derive (M.13) isfˆ = [H , ρˆ ] + [H ′, Lˆ−1{[H , ρˆ ] + [H ′, fˆ + fˆ ] }] . Lˆ−1 =
b
E
a
E
b
a
b b
a
Repeating the procedure we have after the (n−1)th iteration
isfˆa = [HE , ρˆ ]a + [H ′, Lˆ−1{[HE , ρˆ ]b + [H ′, fˆa ]b + + [H ′, Lˆ−1{[HE , ρˆ ]b + [H ′, fˆa ]b + + [H ′, Lˆ−1{{[H , ρˆ ] + [H ′, fˆ ] + …} + E
b
a b
(M.14)
+ [H ′, Lˆ {…{[HE , ρˆ ]b + [H ′, fˆa + fˆb ]b }…}}}]a , −1
where {…{ stands for n curly brackets. The iteration procedure allows one to obtain the solution to any desired order in H ′ provided that the expansion of fˆa in H ′ starts from a lower degree of H′ than that of fˆb . Then, to accuracy of (H ′) n+1 , we may neglect the term [H ′, fˆb ] in (M.14) and solve for fˆa , and further find fˆb from (M.10). Consider the first iteration. To lowest order in H ′ we have (M.15) [H , ρˆ (0) ] + [H ′, Lˆ−1[H ′, fˆ ] ] = 0. E
b
a b a
Taking into account the identity
1 1 Lˆ−nn1′ + Lˆ−n1′n = − + − iπ [δ (∆ nn′ ) + δ (∆ n′n )], (M.16) ∆ nn′ ∆ n′n multiplying by n λ=a †λa λ and summing over the occupation numbers we obtain from (M.15)
Cλ(0) + Tλ(0) = 0,
(M.17)
Cλ(0) = Sp {[HE , ρˆ (0) ]nλ },
(M.18)
where is the field term,
391
Appendix M Tλ(0) = Sp {[H ′, Lˆ−1[H ′, fˆa ]b ]a nλ } = = 2π i Sp {H ′ fˆa H ′ − H ′ fˆ Ha′}δ (∆ )nλ
(M.19)
is the collision term (the δ functions correspond to underlined operator H ′). One can see that fˆa =fˆ (−2) ∼ (H ′) −2 . Thus we obtain an usual Boltzmanntype transport equation. In the next order approximation with respect to H′ we have to take into account terms with fˆ (−1) ∼ (H ′) −1 . One obtains
Cλ(1) + Cλ′(1) = Tλ(0) ( f ( −1) ) + Tλ(0) ( f ( −2) ) = 0,
(M.20)
where
Cλ(1) = Sp {[HE , ρˆ (1) ]nλ },
(M.21)
Cλ′(1) = 2π i Sp {[H ′, ρˆ (0) H E − H ′H E ρˆ (0) ]nλ δ (∆ )},
(M.22)
and, in the case of purely imaginary product H ′H ′H ′ (e.g., for the spinorbital interaction), Tλ(1) = 6π 2 Sp { fˆa δ (∆)H ′nλ H ′H δ′ (∆)}. (M.23) We see that one of important advantages of the method is a simple formation of δ function terms. To second order in H′
Cλ(2) + Cλ′(2) + Cλ′′(2) + Tλ(0) ( f (0) ) + Tλ(1) ( f ( − ) ) + Tλ(2) ( f ( −2) ) = 0, (M.24) where
Cλ(2) = Sp {[HE , ρˆ (2) ]nλ };
(M.25)
Cλ′(2) = Sp {[H ′, Lˆ−1[H E , ρˆ (1) ]]nλ };
(M.26)
Cλ′′(2) = Sp {[H ′, Lˆ−1[H ′, Lˆ−1[H E , ρˆ (0) ]]]nλ };
(M.27)
Tλ(2) = Sp{[H ′, Lˆ−1[H ′, fˆa ]b [[H ′, nˆλ ]Lˆ−1 , H ′]b Lˆ−1}.
(M.28)
In the matrix form this result was derived by Kohn and Luttinger [478]. Further we consider the transport equations for concrete scattering mechanisms.
M.1 IMPURITY SCATTERING The Hamiltonian of the electron–impurity system is given by H0 = ∑ε l cl†cl , l
H E = eE∑rll′cl† cl′ , ll ′
where l = {nk}, n is the band index
392
H ′ = ∑Vll′cl†cl ′ , ll ′
(M.29)
Density matrix technique ni
Vll ′ = ∑e
i ( k −k ′ ) Ri
ϕ ll ′ ,
(M.30)
i =1
ϕll ′ = ∫ul* (r )ul ′ (r )ϕ (r )ei ( k −k ′) r dr,
(M.31)
ϕ (r) is the oneimpurity potential, n i is the number of impurities, u l are the Bloch factors in (2.1). Averaging over random distribution of the impurities yields (M.32) 〈 Vll ′ 2 〉 = ni  ϕ ll ′ 2 (l ≠ l ′). The diagonal matrix elements of the impurity potential may be included into and are not important at derivation of the transport equation. Consider the lowest order equation (M.17). Substituting H E and H ′ into (M.18), (M.19) we obtain ˆ (0) , r ]l = ieE Cl(0) = eE α ∑ ( ρ ll(0)′ rlα′l − rllα′ ρl(0) ′l ) = eE[ ρ l′
∂nl ∂k
(M.33)
(hereafter we use the notation n l = ρl(0) = f ( ε l) for the equilibrium Fermi distribution function), Tl (0) = 2π i ∑  ϕ ll ′ 2 ( f l ′ − f l )δ (ε l ′ − ε l ), l′
(M.34)
with (M.35) f l = Sp ( fˆa cl†cl ). The expressions (M.33), (M.34) yield the field and collision terms of the transport equation for the elastic scattering by impurities in the Born approximation. The results in the two next approximation were obtained by Luttinger [459]. The second Born approximation transport equation for impurity scattering reads (firstorder corrections to the field term vanish)
Tl (1) ( f ( −2) ) + Tl (0) ( f ( −1) ) = 0,
(M.36)
where Tl (1) = −2π ∑δ (ε l − ε l ′ )[( L( −1) )ll ′′ 〈Vll ′′Vl ′′l ′Vl ′l 〉 + l ′l ′′
+ ( L( −1) )*'' 〈Vll ′Vl ′l ′′Vl ′′l 〉( f l − fl ′ )] ll
(M.37)
and T l(0) is given by (M.34). Consider the case where the spinorbital interaction is present. Picking out in (M.37) the imaginary part, which is linear in SOI, and averaging over impurities we obtain
393
Appendix M Tl (2) ( f ( −2) ) = −(2π )2 ni ∑δ (ε l − ε l ′ )δ (ε l − ε l ′′ ) × l' l''
× ( fl ( −2) − f l ′( −2) ) Im (ϕ ll ′ϕ l ′l ′′ϕ l ′′l ).
(M.38)
Assuming that the effective radius r 0 of the potential ϕ (r) is small (k F r 0 1) we may put
ϕ kk ′ ≈ ∫ϕ (r ) dr = ϕ .
(M.39)
Then, using the effective mass approximation we obtain the solution to the first Born approximation (only intraband transitions should be taken into account due to the delta functions)
f l ( −2) = −τ 0 eE
τ 0−1 =
∂nl vl , ∂ε l
(M.40)
ni 2 (2m* )3/2 1/2 ϕ EF . 2π 4
(M.41)
To calculate corrections owing to SOI we have to expand the matrix elements (M.31) in small k−k′:
∂Jαl ∂J βl i ′ ′′ ′ − Im (ϕll ′ϕl ′l ′′ϕ l ′′l ) = ϕ kk ′ϕ k ′k ′′ϕ k ′′k ( kα − kα )(k β − k β ) ∂k β ∂kα 2
,
(M.42)
where
Jαnn′ (k ) = ∫un*k (r )
Jαl = Jαnn (k ),
∂un′k ( r ) dr ∂kα
(M.43)
is proportional to SOI and purely imaginary. Substituting (M.40), (M.42) into (M.38) we derive l ini ϕ EF2τ 0 (2m* )3 ∂nl α ∂Jαl ∂J β − eE k β ∂k 12π 7 ∂ε l β ∂kα 3
+ 2π ni ϕ
2
∑δ (ε
nk
+
− ε nk ′ )( f n(k−1) − f n(k−′1) ) = 0.
(M.44)
k
This equation has the structure of an usual Born equation with modified field term. Its solution has the form
f l ( −1) = −
l iEF ∂nl α ∂Jαl ∂J β − eE k β ∂k β ∂kα 3niϕ ∂ε l
394
.
(M.45)
Density matrix technique Now we estimate the quantities J. To first order of perturbation theory in SOI we obtain
〈 n′  Hso  n〉 un′k ; n′≠ n ε nk − ε nk ′
unk = un(0)k + ∑
rnnα ′ 〈 n′  Hso  n〉 , ε nk − ε nk ′ n′≠ n
Jαl = −2i ∑
(M.46)
(M.47)
where matrix elements of coordinate are connected with those of quasimomentum rnnα ′ (k ) =
−iPnnα ′ (k ) . m* (ε nk − ε nk ′ )
(M.48)
Putting for simplicity ε nk − ε n′k = ∆ = const and substituting the expression for H so we derive 1 ∑ ((Hso )nn′ Pnα′n − Pnnα ′ (Hso )n′n ) = m*∆ 2 [Hso , pα ]n′n . m*∆ 2 n′≠ n Using the Poisson equation Jαl =
∆V (r ) = −4π e2 ρ (r) ( ρ (r) is the charge density) and (L.1) we obtain Jαl = −i
2π 4 e 2 ρeff [kM ]α , 2 2 * 2 3m c m ∆ M (0)
(M.49)
(M.50)
(M.51)
where M is the magnetization,
ρeff = ∫  unk (r ) 2 ρ (r ) dr.
(M.52)
Substituting (M.51) into (M.45) we find the Hall conductivity
σ yx =
ev y a03 Ex
=
e 3 a0 Ex
∑vly fl ( −1) = t l
e2 n 2π 2 M EF µ B ρeff , * 2 m 3∆ M (0) 3niϕ
(M.53)
where t is the number of bands, n = kF3 /6π2 is the electron concentration. Taking into account the expression for the diagonal component of the conductivity tensor
σ xx =
evx e = 3 3 a0 E x a0 Ex
∑vxl fl ( −2) = −τ 0 e2 ∑(vl )2 l
l
∂nl e2 nτ =t *0 , m ∂ε l
we obtain for the Hall coefficient the result (5.124).
M.2 SCATTERING BY PHONONS In the case of electron–phonon interaction we have 395
(M.54)
Appendix M
H0 = ∑ε l cl† cl + ∑ωq bq†bq ,
(M.55)
H ′ = ∑(Qll ′q cl†cl ′bq + Qll*′q cl†′cl bq† ),
(M.56)
l
q
ll ′q
where
2 Qll ′q = i (2M ωq ) −1/2 qCnn′δ k −k ′,q , 3 ω q is the phonon frequency, b †q and b q are the Bose creation and annihilation operators for phonons, C is the Bloch constant in the conductivity theory [1]. Inclusion of the second term in H 0 takes into account the inelastic character of electronphonon scattering. Consider the lowestorder approximation (M.17). Then the field term is determined by (M.33), and the collision term is calculated from (M.19): Tl (0) = 2π i ∑  Qll ′q 2 {[( fl ′ − f l ) N q − f l (1 − nl ′ ) + fl ′ nl ′ ]δ (ε l ′ − ε l + ω q ) + l ′q
+ [( fl ′ − f l )(1 + N q ) + fl (1 − nl ′ ) + fl ′ nl ′ ]δ (ε l ′ − ε l − ωq )}.
(M.57)
Here we have carried out decouplings of manyparticle density matrices, so that N q and n nk are the equilibrium Bose and Fermi functions. The lowestorder contribution to AHE owing to the phonon scattering is described by the equation of the second order in H . The corresponding corrections to the distribution function, which are linear in SOI, occur both from field and collision terms. To simplify the consideration, we follow to paper [460] and do not take into account all such corrections, but restrict ourselves to the equation (M.58) Cl′(2) + Tl (0) ( f (0) ) = 0 (see (M.24)) and neglect C(2), C′′(2) and T(2). The contributions neglected apparently do not influence qualitative results. To calculate C′l (2) we have to expand equilibrium distribution functions up to the first order in the scattering amplitude. Performing the decoupling of manyparticle averages with the use of the theorem about expansion of exponential operators (M.6) we obtain
∑Q l ′q
ll ′q
2 [δ (ε l ′ − ε l + ω q )ϕll(0)′q − δ (ε l ′ − ε l − ωq )ϕll(0)′q ] + + eE∑  Qll ′q 2 β nl ′ (1 − nl )(rl ′ − rl )[δ (ε l ′ − ε l + ωq ) N q + l ′q
+ δ (ε l ′ − ε l − ωq )(1 + N q )] = 0, (M.59) where 396
Density matrix technique
ϕ ll( i′q) = N q ( nl ′ − nl ) + f l ( i ) (1 − nl ′ ) + f l ′( i ) .
(M.60)
For high temperatures T ω q we have
∂nl , ∂ε l so that the solution, which is linear in SOI, has the form
β nl′ (1 − nl′ ) = −
∂nl , (M.61) ∂ε l where the quantity J (see (M.43)) is determined by the diagonal part of the coordinate, which is due to SOI [459]: f l (0) = ieEα Jαl
rllα′ = iδ ll ′
∂ + iJαnn′ (k )δ kk ′ . ∂kα
(M.62)
The offdiagonal part of f (0) is obtained from the equation (M.11): f l ′(0) l =
1 ∆ l ′l
α (0) α eE [ ρˆ , r ]l ′l − ϕ l(′′−lq2) ϕll( −′′q2) * − ∑ Ql ′l ′′q Qll ′′q + − Ql ′′l ′q Ql ′′lq − − ∆ l ′′lq ∆ l ′′lq l ′′q − Qll ′′q Ql*′′l ′q
ϕl(′l−′′2)q ∆ l+′l ′′q
+ Qll ′′q Ql ′l ′′q
ϕll( −′′q2)
(M.63)
, ∆ l−′l ′′q
where ∆ l ′l = ε l − ε l ′ − is,
∆ l±′lq = ε l − ε l ′ ± ω q − is , s → 0.
Using (M.61) and (M.63) we can calculate average velocity of current carriers to zeroth order in Q: ll ′ v = ∑ f l (0) v l + ∑ f l ′(0) ≡ va + vb , l v l
l ′≠ l
∂ε l , vαll ′ = −(ε l − ε l ′ ) Jαnn′δ kk ′ . ∂k Taking into account (M.62) and the relation vl =
∑( J βnn′ Jαn′n − Jαnn′ J βn′n ) = n′
∂J βl ∂kα
−
∂Jαl , ∂k β
(M.64) (M.65)
(M.66)
we obtain
v a = ieEα ∑ l
397
∂nl l l v Jα , ∂ε l
(M.67)
Appendix M
∂J βl ∂Jαl − vbβ = ieE ∑nl , (M.68) ∂kα ∂k β l where we have neglected interband transitions. Integrating (M.68) by parts and combining with (M.67) we get the final expression for the average velocity α
vα = ieE∑ l
∂nl l l v Jα . ∂ε l
(M.69)
Substituting the expression (M.51) into (M.69) we obtain
σ yxph = −
∂n e4 4 Mz 2π ρeff ∑ l vxl k x . * 2 3 m ( mc∆ ) M (0) l ∂ε l
(M.70)
Integrating over k and averaging over subbands yields, similar to (M.53)
σ yxph =
2π e4 n 4 1 Mz ρ t . eff m* M (0) 3 (mc∆ )2
(M.71)
Then the spontaneous Hall coefficient reads Rsph = −
σ yx ρ2 2 µ B2 e 2 n 1 2 ρ ρ t = − . eff m* M (0) 4π M z 3 ∆2
(M.72)
M.3 SCATTERING BY SPIN INHOMOGENEITIES We describe the interaction of conduction electrons with magnetic moments within the s–d exchange model with inclusion of spinorbital interaction (L.17). In the case of high temperatures we include into the interaction of electrons with the mean field: Hd = −WM ∑Siz ,
WM = 2 J 0 〈 S z 〉.
(M.73)
i
In the lowest Born approximation we derive −eE α
∂nl ± = 2π ∑{ I ll ′ ± Λ llz′ 2 ( fl ′(±−2) − f l (±−2) ) K zzδ (ε l ± − ε l ′ ± ) + ∂kα l′ (−2) +  I ll ′ 2 (Φ l ± ,l ′± K ± ∓ − Φ l(′−±2)l ± K ∓ ± )δ (ε l ± − ε l ′ ± ± WM ) + + Λ l+′l Λ l−′l [(Φ l( ±−2),l ′± K +− − Φ l(′−±2)l ± K −+ )δ (ε l ± − ε l ′± + WM ) + + (Φ l( ±−2),l ′ ± K −+ − Φ l(′−±2l)± K +− )δ (ε l ± − ε l ′± − WM )]},
398
(M.74)
Density matrix technique where
Φ (λi′)λ = f λ( i ) (1 − nλ ′ ) − f λ(′i ) nλ ,
(M.75)
ε l ± = ε l ± I ll 〈S z 〉, and we have introduced the onsite averages
K ± ∓ = 〈S ± S ∓ 〉 = 〈( S ± S z )( S ∓ S z + 1)〉, (M.76)
K zz = 〈( S z ) 2 〉 − 〈S z 〉 2 ,
neglecting intersite spin correlators in spirit of meanfield approximation. The equation (M.74) was first derived in [466] by the matrix method. Omitting spinorbital terms we obtain in the oneband approximation (l = k) for I kk′ = const the result by Kasuya [422] −eE α
∂nk ± = 2π I 2 ∑[( f k ′ ± − f k ± ) K zzδ (ε k ± − ε k ′ ± ) + ∂kα k′ + (Φ k( −±2),k ′ ∓ K ± ∓ − Φ k( −′ ±2),k ± K ∓ ± )δ (ε k ± − ε k ′ ± ± WM )].
(M.77)
The trial solution to the equation (M.77) has the standard form
f k(±−2) = −eEατ 0± (ε k ± )
∂nk ± vx . ∂ε k ±
(M.78)
On substituting (M.78) into (M.77) and performing integration over angles we derive
τ 0± (ε ) =
2π 4 ε W (2m* )−3/2 ϕ ± , M 2 v0 I ε T T
,
(M.79)
where
ϕ ± (ε ,η ) = K zz + K ∓ ±
1 + e−ε . 1 + e −ε ±η
(M.80)
In particular,
ϕ + (0,η ) = ϕ − (0,η ) ≡ ϕ (η ) = [ K zz + 2 K −+ (1 + eη )]−1 ,
(M.81)
since K +− = eWM /T K −+ .
For S = 1/2 one has
1 [ϕ (η )]−1 = 3 − 〈 S z 〉 2 . 4 Now we may introduce the transport relaxation time
399
(M.82)
Appendix M
τ0 = −
1 ∂f (ε ) 2 W (ϕ − + ϕ + ) dε EFϕ M 2 ∫ 2 3π I 3π I ∂ε T
.
(M.83)
Then the magnetic resistivity reads −1
ρ mag
e 2 nτ 3π m* I 2 = *0 = 2 e 2 n EF m
−1
WM ϕ T .
(M.84)
Now we consider the case of low temperatures T T C where one can use the spinwave approximation. Using the HolsteinPrimakoff representation for spin operators we derive H ′ = −(2 S )1/2 I ∑(ck† − q↑ ck ↓ bq† + ck† ↓ ck −q↑ bq ) − kq
− I ∑ σ ( I + σΛ kz ,k + q −p )ck†σ ck + q −pσ bq†bp .
(M.85)
kpqσ
The lowestorder collision term is calculated similar to case of electron–phonon interaction. We have f (±ε k ± ) exp( βω q ) Tk(0)± = 2π I 2 S ∑N q fk +q± − q f (±ε k ± − ωq ) f (±ε k ± − ωq ) fk + q ± δ (ε k + q ∓ − ε k ± ± ω q ). − f (±ε k ± )
(M.86)
The solution to the corresponding transport equation (M.17) which describes scattering by spin waves has the form
f kσ =
1 ∂nkσ χασ (ε kσ )kα , T ∂ε kσ
(M.87)
χασ (ε ) = Cασ + ψ ασ (ε ). The energy dependence of χ(ε) is needed to satisfy the integral equation. However, it turns out that, as well as in the case of phonon scattering [1], this dependence results in temperature corrections to resistivity of higher orders only; however, it is important at considering the anomalous Hall effect. Substituting (M.87) into the transport equation yields for the isotropic electron spectrum
400
Density matrix technique −1
∞
ka ∂ε T ∂nk −eE = 2I 2 S 0 k N B (Tx) f (±ε k ) f (±ε k − Tx) × ∂ε k 4π ∂k TC ∫δ x
× {χ x ± (ε k ∓ Tx)(1 − α x) − χ x ± (ε k )}e
± βε k
dx,
(M.88)
where we have neglected the small spin splitting, 2
I T α= (ka0 )−2 . T0 ∼ TC (kF a0 ) → 0, 2TC EF Integrating (M.88) over ε we evaluate the constant C T δ= , T0
4π ka ∂ε T Cx = −eE 2 0 k C , I Sγ ∂k T 2
2
x
(M.89)
with ∞
γ = ∫ γ ( y ) dy, −∞
∞
γ ( y ) = ∫N B (Tx) f (Ty ) f (T ( x + y ))e y dx. δ
Then the equation for ψ takes the form ∞
∫N
B
(Tx) f (ε ) f (ε − Tx)[ψ x (ε − Tx) − ψ x (ε )]e βε dx =
0
2π eE x ∂ε k TC ∂f (ε ) =− 2 . I Ska0 ∂k T ∂ε 2
(M.90)
One can see that ψ x ~ T C /T, so that the contribution of the function ψ to resistivity is proportional to (T/T C ) 3 and may be neglected. Integrating over k we derive for the conductivity
e2 n a0 ∂ε T σ xx = (kF a0 )3 k k C , 2 * 3πγ I Sm vF ∂k kF T 2
4
(M.91)
which agrees with the result (5.62). The nextorder approximation transport equation is important for consideration of the contribution to the anomalous Hall effect in ferromagnets owing to magnetic scattering. At high temperatures we obtain [466]
401
Appendix M
∑ I l′
ll ′
2 K zz ( fl (±−1) − f l ′ ± )δ (ε l ± − ε l ′ ± ) + + ( K ± ∓ Φ l( −±1),l ′± − K ∓ ± Φ (l ′−±1),l ± )δ (ε l ± − ε l ′± ± WM ) × z ( −2) × 2π i ∑Wl (1) − fl ′(±−2) )δ (ε l ± − ε l ′ ± ) = 0, ± Λ ll ′ ( f l ±
(M.92)
l′
where f (−2) is the solution to the equation (M.74), 2 z z 3 Wl (1) ± = ∑  I ll ′′  {〈( S − 〈 S 〉 ) 〉δ (ε l ± − ε l ′′ ± ) + l ′′
+ [〈( S z − 〈 S z 〉) S ± S ∓ 〉 ± (2 K zz − K ± ∓ )nl ′′∓ ± K ∓ ± nl ± + + 2〈 S z 〉 nl ′′∓ nl ± ]δ (ε l ± − ε l ′′ ± ± WM )}. (M.93)
In the oneband approximation, on substituting into (M.92) the solution to the lowestorder transport equation (M.78) and the matrix elements of SOI (L.18) we obtain
−eE x
a 3 km* 64 I (1) ∂nk ± 1 λ + λ′ + v yW±(1)τ 0± (ε k ± ) 0 3 l 4π 35 ∆E 2 ∂ε k ±
+ I 2 ∑[ K zz ( f k(±−1) − fk(′−±1) )δ (ε k ± − ε k ′ ± ) + k
±∓
+( K Φ k( −±1),k ′ ± − K ∓ ± Φ k( −′ ±1),k ± )δ (ε k ± − ε k ′± )] = 0.
(M.94)
The solution to (M.94) is searched as
f k(σ−1) = −eE xτ σ (ε kσ )
∂nkσ vy . ∂ε kσ
(M.95)
Then we derive
τ σ (ε kσ ) =
m*k 3 a0 λeff Wσ(1) [τ 0σ (ε k )]2 , 2
(M.96)
with 32 I (1) l λ + λ ′. 35 ∆E Now we can calculate the Hall current
λeff =
j y = 2e∑ fk(σ−1) v y . kσ
The result for the Hall coefficient reads
402
(M.97)
Density matrix technique 2
mag s
R
9π I m*λeff S zz z −1 zz = K + (4〈 S 〉) 2 K − 2 32 EF e n M (0)
β WM sinh β WM − β WM 1 − ( K +− + K −+ ) + 〈 S z 〉 coth 2 2 cosh β WM − 1
.
(M.98)
In particular, using the equation for magnetization (4.14) we obtain for S = 1/2 2
β WM sinh β WM − β WM 1 + coth . 2 cosh β WM − 1 (M.99) At neglecting the weak temperature dependence of the function in the square brackets the result (M.99) may be represented in the form (5.130). The transport equation of the next Born approximation with account of linear corrections in the spinorbital interaction, which describes electronmagnon scattering at low temperatures, has the form mag s
R
9π I m*λeff 1/4 − 〈 S z 〉 2 = 64 EF e 2 n M (0)
(M.100) Tλ(0) ( f ( −1) ) + Tλ(1) ( f ( −2) ) = 0, (1) where the field term C is zero (as well as for impurity scattering), T (0) is given by (M.86), the solution to the lowest Born equation is given by (M.87). To calculate T we write down for (M.85) H ′ = H ′′ + H ′′′, where H′′ contains the exchange terms and H′′′ the spinorbital ones. Using (M.23) and the properties Hn′′n = Hn′′n , 1 2
Hn′′′n = −Hn′′′n ,
2 1
1 2
2 1
(M.101)
calculating the commutators and performing the decouplings, which are valid to the order under consideration, we obtain: Tk(1)± = 3π I 2 S ∑N q N p × pq
× Λ kz ,k + q −pδ (ε k −p ∓ − ε k ± ± ωq )δ (ε k −p ∓ − ε k ± ∓ ω q ± ωp ) × f (±ε k ± ) f (±ε k ± + ωq − ωp ) β (ωq +ωp ) e f k −p ∓ − × [ f ( ±ε k ± − ω p )]2 f (±ε k ± ) βω e p f k + q −p ∓ + − f ( ±ε k ± + ω q − ω p ) z ( ) ( ) 403
(M.102)
Appendix M + Λ kz − q ,k −pδ (ε k −p ∓ − ε k ± ± ω p )δ (ε k −q ∓ − ε k ± ± ω p ) × ×
f (±ε k ± − ωq ) f (±ε k ± − ωp )
e
βω p
f k −p ∓ .
An interesting feature of the equation (M.100) should be noted. Substituting f (2) ∼ C x = const into (M.102) yields zero after integration over ε in the lowest order in q/k, and higher orders terms in q result in higher powers of T/T C. Therefore one has to take into account the energy dependence of the function (M.87). Then the solution of (M.100) yields [472] −1
f
( −1) kσ
∂n 3a ∂ε T I (1) T = 0 kσ − 0, 24λ ′ − v(∓ε ) kσ k y , (M.103) 4, 4λ l 16π ∂k TC ∆E TC ∂ε kσ
with v(ε ) = λ l
∞ I (1) βω f (ε + ω ) − λ ′ ln(1 + e βω ) dω . N B (ω )ω e ∫ f (ε ) ∆E δ
Calculating σ yx with the use of (M.103) and using the expression for the diagonal conductivity (M.91) we find the expression for the Hall coefficient 4 3 −3 T I (1) T 3π 2I 2 S d ε k 1,1λ l k R =− + 0,8λ ′ , (M.104) 512 e 2 kF M (0) dk k ∆E TC TC F where the largest T 3 term occurs due to the energy dependence of ψ(ε). mag s
404
Degenerate Anderson model
Appendix N DEGENERATE ANDERSON MODEL The periodic Anderson model describes the situation where highly correlated d( f )electrons do not participate directly in the band motion, but are hybridized with the conduction band states. Such a situation takes place in a number of rareearth and actinide compounds (Chapter 6). The hybridization (manyconfiguration) picture is sometimes useful also for discussing some properties of transition dmetals and other delectron systems. For example, strong p–d hybridization takes place in copperoxide highT c superconductors (Sect.6.7). At neglecting spinorbit coupling, which is appropriate for transition metals and their compounds, we write down the Andersonlattice Hamiltonian in the form H = H0 + ∑tk ck†σ ckσ + kσ
∑σ (V
c aklmσ + h. c.),
† klm kσ
klm
(N.1)
where H0 is the Hamiltonian of intrasite interaction between delectrons. A symmetry analysis of hybridization mixing in various situations is performed in the reviews [708, 565]. To simplify the model consideration, we describe the states of conduction electrons by plane waves. Using the expansion in spherical harmonics (C.28) we obtain for the matrix element of hybridization Vklm = i l Ylm* (kˆ )vl (k ),
(N.2)
vl (k ) = 4π ∫r 2 Rl (r )v(r ) jl (kr ) dr
(N.3)
where
and v(r) is a spherically symmetric potential of a given site. In the limit of jjcoupling (actinide compounds) one has to replace in (N.1) lmσ → j µ with j = l ± 1/2 being the total electron momentum and m its projection. In the case of strong correlations for delectrons it is convenient to pass to the representation of the Hubbard operators which 405
Appendix N reduces H 0 to the diagonal form (H.2). Retaining two lowest terms Γ n = {SL}, Γ n−1 = {S′L′} for the configurations d n and d n−1 and defining new conduction electron operators
dk†lmσ =
∑ C µµ
µµ ′MM ′
S 1 S ′ ′, σ 2
CLLM ′M ′ ,lm X k ( SLµ M , S ′L′µ ′M ′),
(N.4)
ck†lmσ = i l Ylm* (kˆ )ck†σ , we present the Hamiltonian (N.1) in the form
H = H0 + ∑ tk ck†σ ckσ + vl (k )(ck†lmσ dklmσ + h. c.) ,
(N.5)
H0 = ∆ ∑ dk†lmσ d klmσ + const ,
(N.6)
kσ
where klmσ
∆ = ESL − ES ′L ′ − ζ (we have passed to the grand canonical ensemble by introducing the chemical potential ζ ), effective hybridization parameters are given by
vl ( k ) = n1/2GSSnn−L1Ln n−1 vl ( k ).
(N.7)
Now we discuss rareearth systems. Because of strong Coulomb interaction between 4f electrons, formation of the f bands, containing 14 electron states, is nonrealistic. Thus one has to use the model with two configurations f n and s(d)f n−1 , which corresponds to delocalization of only one f electron per atom. In the RusselSaunders scheme we may confine ourselves to two lower multiplets of the 4f ion, Γ n = SLJ and Γ n−1 =S′L′J′. Passing in (N.1), (A.31) to the Jrepresentation with the use of (B.5) and summing the product of Clebsh–Gordan coefficients
∑Cµ µµ ′MM ′
JM J S , LM
Sµ CSJ′′µM′,J′L′M ′CLLM ′M ′, lm C
1 S ′µ ′ , σ 2
=
S L J = ∑ S ′ L′ J ′ ([ j ][ j ′][ L])1/2 C 1j µ C JJM′MJJ′ , j µ , σ ,lm jµ 2 j 1/2 l
(N.8)
we derive the Hamiltonian, which is formally similar to that in the case of jjcoupling, H = ∑ ∆f k†j µ f kj µ + tk ck†j µ ckj µ + v j ( k )(ck†j µ f kj µ + h. c.) . kj µ
where we have introduced new electron operators
406
(N.9)
Degenerate Anderson model f k†j µ =
∑C
JM J J ′M ′ , j µ
X k ( SLJM J , S ′L′J ′M J′ ),
M J M J′
ck†j µ = i l ∑C 1j µ Ylm* (kˆ )ck†σ , mσ
2
(N.10)
σ , lm
and the effective hybridization parameters are expressed in terms of a 9jsymbol S L J v j (k ) = S ′ L′ J ′ ([ j ][ j′][ L])1/2 GSSL′L′vl ( k ). 1/2 l j
(N.11)
Thus hybridization effects in ME systems depend strongly on ME quantum numbers S, L, J and, consequently, on the atomic number [709]. Such a dependence in the rareearth element series is similar to de Gennes correlation for the s–f exchange parameter and paramagnetic Curie temperature. Its experimental investigation, e.g., in spectroscopic data, is of great interest. In the case where ∆ is large in comparison with the width of the d( f ) level we may exclude the hybridization term from the Hamiltonians (N.5), (N.9) by a canonical transformation to obtain, respectively, H =−
1 Sµ LM ′′ S µ ′′ × vl (k )vl (k ′)C LLM ′M ′ ,lm C ∑ 1 C L′M ′′′, lm′ C 1 ′ ′ ′µ ′′′, σ ′ S µ σ S , ∆ 2 2 × [ X k −k ′ ( SLµ ′′M ′′, SLµ M )δ µ ′µ ′′δ M ′M + + X k −k ′ ( S ′L′µ ′M ′, S ′L′µ ′′′M ′′′)δ µµ ′′δ MM ′′ ]ck†lmσ ck ′lm′σ ′ , (N.12a)
H =−
1 v j (k )v j ′ (k ′)C JJM′M ′, j µ C JJM′M ′′′′′, j ′µ ′ × ∑ ∆ × [ X k − k ′ ( JM '' , JM )δ
M ' M ''
+
+ X k − k ′ ( J ′M ′, J ′M ′′′)δ MM ′′ ]ck†j µ ck ′j ′µ ′ .
(N.12b)
For ∆ < 0 (∆ > 0) the filling of the level is n (n –1) and only the first (second) term in the brackets of (N.12) should be retained. The expressions (N.12) describe the exchange interaction of conduction electrons with d( f )electrons. It should be noted that in the case under consideration the interaction is highly anisotropic because of spherical harmonics which enter (N.4), (N.10). This should
407
Appendix N result in a strong anisotropy of indirect RKKYtype f–f interaction which is obtained in the second order in the s–f exchange. Such an anisotropy is observed in a number of rareearth and actinide compounds. Using the identity
∑C M′
LM L ′M ′ ,lm
′′ CLLM ′M ′ ,lm′ = 1/2
= ∑(−1) pq
p−q
p LM ′′ lm [ L] l l [ p] L L′ L′' CLM , pq Clm′, p −q , [l ]
(N.13)
the Hamiltonians (N.12) may be decomposed into sum of terms which correspond to interaction of conduction electrons with different multipole components of orbital and spin (or total momentum) degrees of freedom. As well as in the usual s–f exchange model [552], perturbation theory expansion in the models (N.12) yields logarithmic corrections to various physical quantities which indicates reconstruction of the system state at low temperatures. In particular, such a correction to electron selfenergy and resistivity occurs in the third order in I. Unfortunately, the complicated tensor structure of the Hamiltonians (N.12) prevents the calculation of the unique energy scale for the infrared divergences (the Kondo temperature). However, such a calculation may be performed in the case where the energy of the d( f ) level ∆ does not depend on the manyelectron term and is determined by the number of electrons only (see Sect.6.2). Consider the anticommutator retarded Green’s function of localized delectrons (H.3) in the nonmagnetic phase of the model (N.1). The simplest decoupling yields −1
 V 2 Gklm ( E ) = Φ ( E ) − klm , E − tk
(N.14)
where the function Φ is defined by (H.5). The corresponding energy spectrum contains a system of subbands, separated by hybridization gaps (or pseudogaps, provided that V(k) vanishes for some k) which are surrounded by densityofstates peaks. In the model with strong correlations (N.7), we have
1 1 Ek1,2 = (tk + ∆) ± (tk − ∆)2 +  Vklm 2 , 2 4 with
408
(N.15)
Degenerate Anderson model 1/2
[ S ][ L ] Vklm = i l Ylm* (kˆ )vl (k ) ( N SL + N S ′L′ ) . 2[l ]
(N.16)
One can see that the width of hybridization gap depends appreciably on the manyelectron occupation numbers (in particular, on the position of dlevel). The approximation (N.14) does not take into account spinflip processes, which result in the Kondo effect and can change substantially the structure of electron spectrum near the Fermi level. To take into account the Kondo anomalies, we perform a more accurate calculation of the Green’s function. For brevity we consider the model (N.9); in the model (N.5) [ J ] → [ S ][ L],
v j → vl .
It is convenient to use the operators, which are averaged over angles of the vector k: † f kjm = ∫ fk†jm dkˆ ,
† ckjm = ∫ck†jm dkˆ .
(N.17)
Following to the consideration of the SU(N) Anderson model in Sect.6.4, we write down the equation of motion † † ( E − ∆ )〈〈 f kjm  f kjm 〉〉 E = R j (1 + v j ( k )〈〈ckjm  f kjm 〉〉 E ) +
+
∑µ
v j ′ ( q )C JJ′Mµ ′, jm
j ′m ′ Mq
Jµ ∑C J ′M ′, jm′ X k −q ( J ′M , J ′M ′) + M′
† + ∑C JJ′Mµ ′ , j ′m′ X k −q ( J µ ′, J µ ) cqj ′m′  f kjm µ′
,
(N.18)
E
where we have carried out a decoupling for the term, which describes the processes without changing m, Rj =
1 [J ] [J ] − − 1 ∑〈 X ( JM , JM )〉 . [ j ] [ J ′] [ J ′] M
(N.19)
Further we neglect for simplicity the abovediscussed influence of hybridization gap, which is possible provided that the latter lies far below the Fermi level (note that the corresponding contributions are formally small in the inverse degeneracy of f level, 1/N). Carrying out decouplings in the equations for the Green’s function in the righthand side of (N.18) we obtain
409
Appendix N † ( E − tq )〈〈 X k −q ( J µ ′, J µ )cqj′m′  f kjm 〉〉 E = † = v j′ (q )nq ∑C JJ′Mµ ′′′, j′m′ 〈〈 X k −q ( J ′M , J µ ′′)  f kjm 〉〉 E , M′
† ( E − tq )〈〈 X k − q ( J ′M , J ′M ′)cqj′m′  f kjm 〉〉 E = † = − v j′ ( q ) nq ∑C JJ′Mµ ′′′, j′m′ 〈〈 X k −q ( J ′M , J µ ′′)  f kjm 〉〉 E ,
(N.20)
µ ′′
with n k = 〈c †kjm c kjm 〉 = f(t k ) being the Fermi distribution functions. Substituting (N.20) into (N.19), averaging over angles and using the orthogonality relations for the Clebsh–Gordan coefficients, we find † 〈〈 f kjm  f kjm 〉〉 E = RJ [ E − ∆ − Σ f ( E )]−1 ,
Σ f ( E ) = 2 ρ ∑v 2j (kF ) j
J − J′ W ln . [ J ′] E
(N.21) (N.22)
where we have used the approximation (6.5). At J > J′ the Green’s function (N.21) has the pole −1 [ J ] −1 2  ∆ = TK ≈ W exp − − 1  ∆  ρ ∑v j (kF ) . [ J ′] j *
(N.23)
The usual Kondo effect corresponds to the total compensation of magnetic moment (J′ = 0). At J′ > J the pole (N.23) is absent (the strong coupling regime does not occur) since the model under consideration is mapped by a canonical transformation into a Coqblin–Schrieffer model with a positive exchange parameter. An analogue of the result (N.23) for dimpurities has the form −1 [ S ][ L] ∆ TK = W exp − . − 1 ′ ′ 2 [ S ][ L ] ρ vl (kF )
(N.24)
Note that the formula (N.24) satisfies the condition of the particlehole symmetry (n → n′ = 2[l] +1 − n, ∆ → −∆) owing to the relation for the fractional parentage coefficients 2 n[ S ′][ L′] S ′L′ GSL (n, n − 1)} . { (N.25) n′[ S ][ L] At neglecting the dependence ∆(LS), all the ME terms of configurations dn and dn−1 contribute equally to spinflip processes, and, consequently, to the Kondo temperature. Then the coefficients G which enter (N.7) may be summed up in the equations of motion with the use of orthogonality relations (A.8), (A.9) to obtain for the Kondo temperature
{G
SL S ′L ′
(n′, n′ − 1)} = 2
410
Degenerate Anderson model vl2 (kF ) . (N.26) ∆ Note that the expression (N.26) may be represented in the the form, which is similar to (N.24), TK ≈ W exp −(2[l ] + 1 − 2n)−1 ( I  ρ ) −1 ,
I=
2[l ] + 1 − 2n −1 1 − 1 TK ≈ W exp − , (N.27) n n  I  ρ with the factor (2[l] + 1 − n)/n being again the ratio of statistical weights for the configurations d n and d n−1 : 2[l ] + 1 − n (2[l ])! (2[l ])! = . n!(2[l ] − n)! ( n − 1)!(2[l ] − n + 1)! n The result (N.26) differs from the result of hightemperature perturbation theory (6.22) by an unity in the denominator of the exponential only. Such a difference is typical for the calculation of the Kondo temperature in the degenerate Anderson model [565, 574] and is explained by that this approach is justified, strictly speaking, only in the largeN limit.
411
Appendix O
Appendix O MEANFIELD APPROXIMATION FOR THE GROUND STATE OF MAGNETIC KONDO LATTICES To construct the meanfield approximation describing the ground state of Kondo lattices we use the Abrikosov pseudofermion representation for localized spins S = 1/2 (which coincides with the Dirac representation (B.1)) 1 S i = ∑ f iσ† σ σσ ′ f iσ ′ (O.1) 2 σσ ′ with the subsidiary condition f i↑† fi ↑ + f i ↓† fi ↓ = 1.
Making the saddlepoint approximation for the path integral describing the spinfermion interacting system [711] one can reduce the Hamiltonian of the s–f exchange interaction to the effective hybridization model:
1 1 † − I ∑ci†σ ciσ σ σσ ′S i − δ σσ ′ → fi †Vi ci + ci†Vi † fi − Sp (VV i i ), (O.2) I 2 2 ′ σσ where the vector notations are used f i † = ( fi ↑† , fi ↓† ),
ci† = (ci†↑ , ci†↓ ),
V is the effective hybridization matrix which is determined from a minimum of the free energy. Coleman and Andrei [711] considered the formation of a spinliquid state in the twodimensional situation. Here we treat the more simple case of ferromagnetic ordering following to [608]. The Heisenberg Hamiltonian of the f subsystem H f is considered in the meanfield approximation. For a ferromagnet we have (S¯ = 〈S z 〉) Hf = − J 0 S ∑σ f iσ† f iσ ,Vσσ ′ = Vσ δ σσ ′ iσ
and the Hamiltonian of the s–f model takes the form
412
(O.3)
Meanfield approximation
H − ζ n = ∑ (tk − ζ )ck†σ ckσ + wσ f k†σ fkσ + Vσ (ck†σ f kσ + fk†σ ckσ ) + const , kσ
(O.4) where
wσ = w − σ J 0 S , w being the energy of ‘f level’. The equations for w, the chemical potential ζ and S¯ read nσ† ≡ ∑ 〈 f k†σ f kσ 〉 = k
1 +σ S; 2
n = ∑ 〈ck†σ ckσ 〉.
(O.5) (O.6)
k
One can see that −w plays the role of the chemical potential for pseudofermions (note that the numbers of electrons and pseudofermions are conserved separately). After the minimization one obtains the equation for V σ Vσ = 2 I ∑ 〈 f k†σ ckσ 〉. k
(O.7)
Diagonalizing the Hamiltonian (O.4) by a canonical transformation
ck†σ = ukσ α k†σ − vkσ β k†σ ,
fk†σ = ukσ β k†σ − vkσ α k†σ ,
ukσ = cos(θ kσ /2),
(O.8)
vkσ = sin(θ kσ /2),
with
sin θ kσ =
2Vσ , Ekσ
cosθ kσ =
tk − ζ − wσ , Ekσ
(O.9)
we obtain the energy spectrum of a hybridization form
1 Ekασ, β = (tk − ζ + wσ ± Ekσ ). 2 Then the equations (O.5)–(O.7) take the form
(O.10)
nσf =
1 ∑ (1 − cos Θkσ )nkασ + (1 + cos Θkσ )nkβσ , 2 k
(O.11)
n=
1 ∑ (1 + cos Θkσ )nkασ + (1 − cos Θkσ )nkβσ , 2 kσ
(O.12)
1 = −2 I ∑ ( nkβσ − nkασ )/Ekσ . k
(O.13)
At small V σ , w σ  and T = 0 we have
cos Θkσ ≈ sign (tk − ζ − wσ ), 413
(O.14)
Appendix O so that the equations (O.11) and (O.12) are simplified. The edges of the hybridization gaps in spin subbands are given by (O.15) Ekασ > wσ + Vσ2 /ζ , Ekβσ < wσ − Vσ2 /(W − ζ ). Further we consider different types of ferromagnetic solutions. We confine ourselves to the case where the conduction electron concentration n < 1 (the results for n > 1 are obtained after the particlehole transformation). As follows from (O.15), at not too large S¯ for both σ the condition (O.16) wσ > Vσ2 /(W − ζ ), holds, i.e. the chemical potential lies below the energy gap, as well as in the nonmagnetic case. Define the function ζ (c) by ζ (c )
c=2
∫ ρ ( E )dE ,
(O.17)
0
with ρ (E) (0 < E < W) being the bare density of states. Then the equation (O.12) takes the form ζ (n) = ζ , and (O.11) and (O.13) yield
λσ ≡ Vσ2 /wσ = ζ ( n + 2nσf ) − ζ ( n), 1 = −2 I
ζ + λσ
∫ 0
ρ (E) [( E − ζ − wσ ) 2 + 4Vσ2 ]1/2
dE.
(O.18) (O.19)
Calculating the integral in (O.19) to leading and nextorder terms in 1/ln W/V σ  we obtain ζ ( n + 2 nσ ) ζ ρ ( E + ζ ) C ρ (E) 1 = −4 I ρ ln dE + ∫ dE , − 2I ∫ Vσ E E −ζ C C +ζ f
(O.20)
where C is a cutoff parameter which does not enter final results. In the leading approximation V σ does not depend on σ and we have
 Vσ ∼ (WTK )1/2 ,
TK ≡ W exp
1 . 2I ρ
(O.21)
Retaining the next order terms, we calculate the ratio and obtain the selfconsistent equation for magnetization 1 ζ ( n +1+ 2 S ) ρ ( E ) − ρ J 0 S tanh ∫1−2 S ) E − ζ dE = w , 4ρ ζ ( n +
(O.22)
where (O.23) w ≈ V 2 [ζ (n + 1) − ζ ] ∼ TK . The equation (O.22) has no nontrivial solutions for the bare DOS 414
Meanfield approximation
Fig.O.1. The density of states picture for the ferromagnetic solution with a small spin splitting.
Fig.O.2. The density of states picture for the saturated (halfmetallic) ferromagnetic solution.
ρ (E) = const. However, solutions with S¯ ≠ 0 may occur for some ρ (E) if both the left and righthand side of (O.22) are of order unity, i.e. J 0 ∼ T K (see Fig.O.1). Provided that w↓ > V↓2 /(W − ζ ),
w↑ < −V↑2 /ζ ,
(O.24)
i.e. ζ lies in the energy gap for σ = ↑, we obtain the ‘halfmetallic’ ferromagnetic solution with n↑f = 1 − n/2,
n↓f = n/2,
S = (1 − n)/2
(O.25)
(see Fig.O.2). Such a solution exists under the condition −ϕ /ζ < [ζ (2n) − ζ ]−1 − J 0 (1 − n)/V↓2 < ϕ /(W − ζ ),
ϕ≡
V↑ V↓
2
1 W ρ (E ) = exp dE . ρ ζ (2∫n ) E − ζ 415
(O.26)
(O.27)
Appendix O
Fig.O.3. The density of states picture for the ferromagnetic solution where the spin splitting exceeds the energy gap.
For ρ (E) = const (O.26) takes the form J 0 (1 − n) < TK and the corresponding total energy
(O.28)
2 2 n2 n − TK − J 0 S = Enon − mag − J 0 S (O.29) 4ρ 2 is always lower than that of the nonmagnetic Kondo state. Thus the formation of the state of the halfmetallic Kondo ferromagnet is energetically favourable. In this state each conduction electron compensates one localized spin, and the magnetic ordering is due to exchange interaction between noncompensated moments. Such a picture is reminiscent of the situation in the narrowband ferromagnet in the Hubbard or s–d exchange model with large intrasite interaction (Sect.4.6). In our case the bare interaction is small, but effective interaction is large in the strong coupling regime. The expression (O.29) should be compared with the energy of the usual ferromagnetic state with the Kondo effect suppressed:
E=
n2 − J 0 /4 (Vσ = 0, S = 1/2), (O.30) 4ρ We see that the latter state becomes energetically favourable at E=
n J 0 1 − > TK . (O.31) 2 At the critical point, a firstorder transition takes place. Third type of possible ferromagnetic solutions correspond to the situation of large energy splitting where ζ lies in the lower hybridization subband for σ = ↓ and in the upper one for σ = ↓ (Fig.O.3). However, such solutions (at least for ρ (E) = const) are energetically unfavourable [608]. 416
Schwinger and Dyson–Maleev representations
Appendix P SCHWINGER AND DYSON–MALEEV REPRESENTATIONS IN THE THEORY OF TWODIMENSIONAL HEISENBERG ANTIFERROMAGNETS The Schwinger boson representation for spin operators has the form, which is similar to the Abrikosov representation (O.1), the Fermi operators being replaced by Bose operators b iσ : Si =
1 bi†σ σ σσ ′biσ ′ , ∑ 2 σσ ′
1 Siz = (bi†↑bi ↑ − bi†↓bi ↓ ). (P.1) 2 For the given localized spin S, these operators should satisfy at each site i the subsidiary condition (constraint) Si+ = bi†↑ bi ↓ ,
Si− = bi†↓ bi ↑ ,
b σ b σ = 2S . ∑ σ † i
i
(P.2)
It should be noted that the ‘hyperbolic’ operators (B.14) which change the value of momentum may be easily represented in terms of the Schwinger bosons [656]:
1 K z = (b↑†b↑ + b↓†b↓ + 1). (P.3) 2 The representation (P.1) turns out to be convenient at considering lowdimensional systems which do not possess longrange ordering at finite temperatures, but demonstrate developed spin fluctuations (shortrange order). Consider the ‘mean field’ approximation for the twodimensional Heisenberg model within the selfconsistent spinwave theory [623]. (This differs drastically from the usual mean field approximation of Sect 4.1 since permits to describe the strong shortrange order above the ordering point.) The constraint (P.2) is taken into account in the K + = b↑†b↓† ,
K − = b↓b↑ ,
417
Appendix P average by introducing the Lagrange multiplier λ which does not depend on i. Anomalous averages 〈b i↑ b j↓ 〉 describe singlet pairing of bosons, i.e. the shortrange order parameters. Occurence of longrange ordering with the wavevector Q corresponds to the Bose–Einstein condensation with the quasimomenta k = ±Q/2. It is convenient to introduce the interaction with small external magnetic field H. Then the Bogoliubov transformation
bQ/2+k ↑ = cosh
Θk Θ α k − sinh k β −†k , 2 2
bQ/2−k ↓ = cosh
Θk Θ β −k − sinh k α k† , 2 2
(P.4)
reduces the Heisenberg Hamiltonian to the diagonal form Hd = ∑( Ekα α k†α k + Ekβ β k† β k ), k
(P.5)
where, for the square lattice with the parameter a 0 = 1,
1 Ekα , β = Ek ∓ H − 2  J  〈 S z 〉 , 2 sinh Θ k = γ k /Ek ,
Ek = (λ 2 − γ k2 )1/2 ,
cosh Θ k = λ /Ek ,
(P.6) (P.7)
with
1 2 Equations for λ and γ , which are obtained from (P.7), have the form
γ k = γ (sin k x + sin k y ).
2S + 1 =
1=
1 λ (1 + Nkα + Nkβ ), ∑ N k Ek
1 J (sin k x + sin k y ) 2 (1 + Nkα + Nkβ ). ∑ 2 N k Ek
(P.8)
(P.9)
where N kα ,β =N B (Eαk ,β ), N is the number of lattice sites which should be retained explicitly in the problem under consideration. At T = 0 we have λ = γ, and Nkα (but not Nkβ ) contains the condensate term at Eαk = 0, i.e.
k = ±Q/2,
Ek =
1 H − 2 J 〈S z 〉 ∼ H . 2
Then we obtain
418
(P.10)
Schwinger and Dyson–Maleev representations N ± Q/2 = N 〈 S z 〉 = NEQ/2 nB /λ ,
(P.11)
with 2n B being the density of condensed bosons. Equation (P.8) yields −1/2
1 ∑k 1 − 4 (sin k x + sin k y )2 = S − 0.197, (P.12) so that n B equals the ground state sublattice magnetization of the Neel antiferromagnet S¯ (0) with account of zeropoint spinwave corrections. At finite T the boson spectrum (P.6) contains the gap and the condensate is absent. Then we may put H = 0, N k α , β = N k from the beginning. Consider the spin spectral density nB = S +
1 1 − 2 2N
Kq (ω ) = −
1
π
N B (ω ) Im 〈〈Sq  S −q 〉〉ω
(P.13)
in the Schwinger boson representation. The spin Green’s function are expressed in terms of polarization operators of noninteracting bosons α and β , and we derive K q (ω ) =
Θk − Θ k + q 1 2 × (2 − δ µν )cosh ∑ ∑ 4 k ν , µ =α , β 2 × N kµ (1 + N k + qν )δ (ω + Ekν + q − Ekµ ) + + (1 + δ µν )sinh 2
Θk − Θk + q 2
[ N kµ N k + qν δ (ω − Ekν + q − Ekµ ) +
+ (1 + N kµ )(1 + N k + qν )δ (ω + Ekν + q + Ekµ )] . (P.14)
As follows from (P.11), (P.14), the spectral density contains at T = 0, H → 0 the deltafunction contribution
3 (P.15) 2 The factor of 3/2 in (P.15) should in fact be omitted since it is an artifact of the mean field approximation which yields, because of inaccurate account of the condition (P.2),
δ Kq (ω ) = nB2 N δ qQδ (ω ).
3 S ( S + 1), 2 violating thereby the corresponding sum rule at the site. At finite temperatures we have 〈Si2 〉 =
419
Appendix P
1 Ek2 = λ 2 (k ∓ Q/2) 2 + ξ −2 , k → ±Q/2, 2 where the correlation length is given by
(P.16)
(P.17) ξ ∼ exp(πλ nB /2T ). At q = Q the integral in (P.14) is “almost” divergent at the points k = ±Q/2 with the cutoff scale k ∓ Q/2 ∼ ξ −1 . Using the expansion N k ≅ T/E k we present the corresponding singular contribution in the form 2
3 2T 3 δ K q (ω ) = ln ξ ∆ q ∆ω ≈ nB2 ∆ q ∆ω , 2 πλ 2
(P.18)
where ∆ q and ∆ ω are δ (q − Q) and δ ( ω ) like functions smoothed on the scales ξ −1 and ω ξ ∼ J/ ξ respectively. At T J we have ω ξ T and we may neglect the smoothing which yields a formal description of strong shortrange order. To obtain the temperature dependence of the coefficient in (P.18) (‘sublattice magnetization’) we estimate the intensity of the Ornstein–Cernike peak at q = Q in the static spin correlator 1/2
Seff (T ) = ∑ 〈S − q S q 〉 , q − Q< q 0
(P.19)
where q 0 ξ −1 is a cutoff wavevector. Using the result of the scaling consideration [712], which yields the correct preexponential factor
(
)
ξ = Cξ exp π cS (0)/ 2T ,
(P.20)
where c is the magnon velocity and C ξ ≅ 0.01/(2 π ) 1 is a numerical factor. Substituting (P.20) into (P.19), (P.18) and neglecting ln q in comparison with ln C ξ we obtain the linear dependence [713] 2T  ln Cξ  . (P.21) πc The contributions to spectral density from antiferromagnetic spin waves are determined by the terms, which are linear in n B . Putting E k → 0, N k = T/E k , but retaining E k + q and vice versa, and performing integration over k, we derive Seff (T ) = S (0) −
420
Schwinger and Dyson–Maleev representations
δ1 K q (ω ) =
λ 2 − γ kγ k +q 3 T 1 ∑ E2 × 2 Eq + Q/2 N k k
×[(1 + N q + Q/2 )δ (ω + Eq + Q/2 ) + N q + Q/2δ (ω − Eq + Q/2 )] ≈ 3 1 − ϕq ≈ nB 2 1 + ϕ q
1/2
{[1 + N B (ω q )]δ (ω + ω q ) + N B (ωq )δ (ω − ω q )}, (P.22)
where, for q, q − Q ξ −1 ,
ωq = λ (1 − ϕq2 ) ≈ Eq +Q / 2 , ϕq ≡
1 (P.23) ( cos qx + cos qy ) 2 so that ω q is the renormalized magnon frequency. For comparison, we consider the application of the Dyson–Maleev representation (E.2) to the same problem. In the case of a twosublattice antiferromagnet this has the form 1.2
1 † Sl+ = (2S )1/2 1 − al al al , S 2
Sl− = (2S )1/2 al† ,
Slz = S − al† al , l ∈ A, 1 † Sm+ = (2 S )1/2 bm† 1 − bmbm bm , 2S
Sm− = (2S )1/2 bm† ,
(P.24) Smz = − S + bm† bm , m ∈ B. In the selfconsistent approach [624] one puts on each site the condition 〈S z 〉 = 0, i.e.
〈al† al 〉 = 〈bl†bl 〉 = S . Using the Bogoliubov transformation
ak = cosh
(P.25)
Θk Θ α k − sinh k β −†k , 2 2
Θk † Θ β −k − sinh k α k , 2 2 we diagonalize the Hamiltonian to obtain H = ′ω (α †α + β † β ), b−†k = cosh
∑
k
k
k
k
k
(P.26)
(P.27)
k
with
〈α k†α k 〉 = 〈 β k† β k 〉 = Nk = N B (ωk ),
ωk = (λ 2 − γ 2ϕk2 )1/2 , 421
tanh 2Θk = γϕk /λ.
(P.28)
Appendix P Here Σ′ stands for the sum over the reduced Brillouin zone. The equations for λ and γ read
S+
1 λ = ∑′ (1 + 2 Nk ), 2 k ωk
J 1 = ∑′ (cos k x + cos k y )(1 + 2 N k ). k
ωk
(P.29)
(P.30)
At T = 0 (in more general case, in the presence of the longrange ordering), λ = γ + O(1/N), so that the spectrum is gapless. The 1/Ncorrections describe the Bose condensation:
(1− γ /λ ) 2
2 −1/ 2
= NnB.
(P.31)
As follows from the constraint (P.25) and the structure of the Dyson–Maleev transformation, the transverse spin correlation function − 〈S q+ S–q 〉 vanishes. Thus the corresponding spectral density reads
Kq (ω ) = Kqzz (ω ) = =
Θk − Θk + q 1 ′ N k (1 + N k + q )δ (ω + ωk + q − ωk ) + cosh ∑ N k 2 Θk − Θ k + q 1 + sinh 2 [ Nk Nk + qδ (ω − ω k + q − ωk ) + 2 2 + (1 + N k )(1 + Nk + q )δ (ω + ωk + q + ω k )] .
(P.32)
The deltafunction contribution is
δ K q (ω ) = NnB2δ qQδ (ω ).
(P.33)
Unlike (P.15), the expression (P.33) does not contain the superfluous factor 3/2. On the other hand, in contrast with the ‘isotropic’ Schwinger representation, the Dyson–Maleev representation violates the rotational invariance even in the paramagnetic phase. The versions of selfconsistent spinwave theory (SSWT), based on nonlinear boson representations, yield a gap in the spinwave spectrum in the absence of longrange order. This contradicts, e.g., to exact results for onedimensional lattice with halfinteger spin S where the spectrum is gapless (for integer spin, the spectrum contains socalled Haldane gap [714] which is reproduced qualitatively by SSWT). However, as discussed in [622], such approaches are satisfactory in the cases where the ground state possesses longrange order. 422
Schwinger and Dyson–Maleev representations It should be noted that both approaches under consideration describe the longrange order in terms of deltafunction singularity of the spin correlation function, the sublattice magnetization being always zero. The possibility of such a description in the threedimensional situation for a wide range of physical properties, including local characteristics, is demonstrated in [715]. In particular, in such an antiferromagnetic state without sublattices the Green’s function of a nuclear spin at each site turns out to have both poles ±AS (A is the hyperfine interaction parameter). Applications of the nonlinear boson representations to systems with a weak interlayer coupling and magnetic anisotropy are discussed in [713].
423
Conclusions
CONCLUSIONS In the present book we have attempted to consider the whole variety of physical properties of transition metals. The characteristics of TM are much more complicated and interesting than those of simple metals. Simultaneous consideration of all the properties permits to establish some regularities with filling of d and fshells and their connection with the electronic structure. One might expect similarity of the properties within a given transition series, since, with some exceptions, the total number of external spelectrons does not change. In fact, chemical and most physical properties (crystal structure etc.) of rare earths are very close. At the same time, magnetic characteristics of 4fmetals change appreciably with the number of felectrons. Moreover, as demonstrated in Sect.4.8.2, there exists some periodicity within the 4fseries, so that the latter forms a miniature “periodic table”. This regularity is connected with the manyelectron term structure of the 4fshell. On the other hand, non only magnetic, but also other properties of dmetals depend strongly on the number of delectrons n d , and they play an important role in the formation of a crystal. An appreciable delocalization of dstates is directly observed in the experimental investigations of the Fermi surface. In some anomalous rare earth and actinide systems, felectrons also take part in formation of the Fermi surface, due to both oneelectron mechanisms (hybridization) and manyelectron effects (as in Kondo lattices). This may lead to occurrence of states with rather exotic properties, e.g. to greatly enhanced electronic effective masses (Chapter 6). In metallic cerium, direct f–f overlap plays an important role. The “dual” (localized vs. itinerant) nature of delectrons requires using various approaches for analyzing physical properties of TM and their compounds. One can pick out two main approaches. The first one starts from firstprinciple oneelectron band calculations. According to the HohenbergKohn theorem, these calculations can provide an accurate description of some ground state characteristics. At the same time, standard band calculations, which use the local density approximation, are often insufficient for narrow d, 5fand especially 4fbands. Besides that, the density functional approach 424
Conclusions is, generally speaking, unable to describe the whole excitation spectrum and thermodynamic properties. The band approach can explain anomalies in TM properties, which are connected with singularities of electron density of states. Presence of such singularities leads sometimes to considerable modifications of standard formulas of solid state theory, e.g., for electronic specific heat and paramagnetic susceptibility. It should be also noted that for “flat” regions of spectrum with small values of grad E(k), i.e. for density of states peaks, manyelectron perturbation corrections become large and the role of correlation effects increases. The second approach takes into account electron correlations in a microscopic way starting from the atomic picture. The adequacy of this picture is evident for strongly localized 4fstates. However, atomic features are retained to some extent for dstates too. In particular, this is confirmed by a characteristic “toothed” nddependence of electronic properties in transition metals and by manyelectron term effects in spectral measurements. In this connection, the problem of strong (tenfold) degeneracy of dstates seems to be important. Although the degeneracy is lifted at broadening of the atomic levels into energy bands by the periodic lattice potential, it survives in some points of the Brillouin zone. This degeneracy is important, e.g., for the orbital momenta which determine anisotropy of a number of properties. It should be stressed that such a scheme of degeneracy lift takes place in the oneelectron picture only, and the classification of electron states changes in the manyelectron representation where additional quantum numbers occur. The corresponding new quasiparticles may possess different degree of localization and mobility. This may change essentially the results of the standard band theory. From the point of view of the qualitative microscopic description, investigation of simple theoretical models, which include effects of strong intraatomic electron correlations, turns out to be very useful. Such effects turn out to be especially bright for some d and fcompounds. In the case of narrow bands (large Coulomb interaction) the correlations result in a radical rearrangement of electron spectrum formation of the Hubbard subbands. A convenient tool for describing atomic statistics of excitations in such a situation is the formalism of manyelectron Hubbard operators. On the other hand, even small interaction among localized and itinerant electrons may result in a reconstruction of electron spectrum at low temperatures owing to peculiarities of resonance scattering in manyparticle systems (the Kondo effect). 425
Conclusions Methods which combine band structure calculations and model considerations seem to be promising. As discussed in the book, such approaches were developed, e.g, for transition metal oxides and heavyfermion systems. In a number of cases, correlation effects are reduced to a modification of electron spectrum and density of states (e.g., formation of hybridization gap or AbrikosovSuhl resonance in intermediate valence and Kondo systems), so that electron properties may be further calculated in a phenomenological way with the use of oneelectron theory results. However, the modifications of electron spectrum parameters themselves may not be obtained in the standard band theory. In particular, the parameters are often strongly temperature dependent owing to manyelectron renormalizations. On the other hand, sometimes the excitation spectrum is not described within the usual quasiparticle picture and has an essentially incoherent nature. Simple examples are provided by the electron spectrum of the Hubbard ferromagnet (Appendix J) and twodimensional conducting antiferromagnet (Sect.6.7). The spectrum of highlycorrelated systems is often described in terms of auxiliary (slave) Fermi and Bose operators, which correspond to quasiparticles with exotic properties (neutral fermions, charged bosons etc.). Last time such ideas have been extensively applied in connection with the unusual spectra of highT c superconductors and heavyfermion systems. Investigation of these problems leads to complicated mathematics, which uses the whole variety of modern quantum field theory methods, and very beautiful physics. For example, description of the Fermi liquid state in terms of Bose excitations becomes possible. These concepts change essentially classical notions of the solid state theory.
426
Bibliography
BIBLIOGRAPHY 1 . A.Sommerfeld and H.Bethe, Electronentheorie der Metalle, Handb.Phys, Vol.XXIV, ed. H.Geiger and K.Scheel, Springer, Berlin, 1933. 2 . A.H.Wilson, Theory of Metals, Cambridge, 1953. 3 . F.Seitz, Modern Theory of Solids, McGraw Hill, New York, 1940. 4 . R.E.Peierls, Quantum Theory of Solids, Oxford, Clarendon Press, 1955. 5 . C.G.Kittel, Introduction to Solid State Physics, Wiley, New York, 1953. 6 . J.M.Ziman, Principles of the Theory of Solids, London, 1964. 7 . J.M.Ziman, Electrons and Phonons, Clarendon Press, Oxford, 1960. 8 . F.J.Blatt, Physics of Electronic Conduction in Solids, McGraw Hill, New York, 1968. 9 . W.A.Harrison, Solid State Theory, McGraw Hill, New York, 1970. 1 0 . I.M.Lifshitz, M.Ya.Azbel and M.I.Kaganov, Electron Theory of Metals, New York, Consultants Bureau, 1973. 11. A.P.Cracknell and K.C.Wong, The Fermi Surface, Clarendon Press, Oxford, 1973. 12. N.W.Ashcroft and N.D.Mermin, Solid State Physics, Holt, Rienart and Winston, 1976. 13. W.A.Harrison, Electronic Structure and the Properties of Solids, Freeman, San Francisko, 1980. 14. A.A.Abrikosov, Theory of Metals, Moscow, Nauka, 1987. 15. B.Coqblin, The Electronic Structure of Rare Earth Metals and Alloys, Academic Press, 1977. 16. K.N.R.Taylor and M.I.Darby, Physics of Rare Earth Solids, Chapman and Hall, London, 1972. 17. S.A.Nikitin, Magnetic Properties of Rare Earth Metals and their Alloys, Moscow State University, 1989; K.P.Belov, M.A.Belyanchikova, R.Z.Levitin and S.A.Nikitin, Rare Earth Ferro and Antiferromagnets, Moscow, Nauka, 1965. 18. D.C.Griffin, K.Andrew and R.D.Cowan, Phys.Rev.177, 62 (1969). 19. A.J.Freeman, In: Magnetic Properties of Rare Earth Metals, Ed.R.J.Elliot, Plenum Press, 1972, p.245. 20. I.I.Sobelman, Introduction to the Theory of Atomic Spectra, Pergamon Press, Oxford, 1973. 21. P.Soederlind, O.Eriksson, J.M.Wills and B.Johansson, Phys.Rev.B48, 9212 (1993). 22. U.Benedict, W.A.Grosshans and W.B.Holtzapfel, Physica B144, 14 (1986). 23. U.Benedict, J.R.Peterson, R.G.Haire and C.Dufour, J.Phys.F14, L43 (1984). 24. V.L.Moruzzi, J.F.Janak and A.R.Williams, Calculated Electronic Properties of Metals, Pergamon Press, New York, 1978. 25. N.F.Mott, MetalInsulator Transitions, London, Taylor and Francis, 1974. 26. T.Moriya, Spin Fluctuations in Itinerant Electron Magnetism. Springer, Berlin, 1985. 27. A.Abrikosov, L.Gorkov and I.Dzyaloshinsky, Methods of Quantum Field Theory in Statistical Physics, Prentice Hall, New York, 1963. 28. J.Hubbard, Proc.Roy.Soc. A276, 238 (1963). 29. J.Hubbard, Proc.Roy.Soc. A277, 237 (1963). 30. J.Hubbard, Proc.Roy.Soc. A281, 401 (1964). 31. J.Hubbard, Proc.Roy.Soc. A285, 542 (1965). 32. B.R.Judd, Operator Techniques in Atomic Spectroscopy, Mc Graw Hill, New York, 1963; Second Quantization and Atomic Spectroscopy, John Hopkins University Press, Baltimore, 1967. 33. S.Fraga, K.Saxena and J.Karwowski, Handbook of Atomic Data, Elsevier, Amsterdam, 1976. 427
Bibliography 34. C.E.Moore, Atomic Energy Levels, US National Bureau of Standards Circular No 1463, vol.1–3, 1958. 35. R.Dagis and D.Segzda, Fiz.Tverd.Tela 36, 705 (1994). 36. S.P.Kowalczuk, R.A.Pollak, F.R.McFeely, L.Ley and D.A.Shirley, Phys.Rev.B8, 2387 (1973). 37. P.A.Bennett, J.C.Fuggle and F.U.Hillebrecht, Phys.Rev.B27, 2194 (1983). 38. E.Antonides et al, Phys.Rev.B15, 1669 (1977). 39. Yu.P.Irkhin, Usp.Fiz.Nauk 154, 321 (1988) [Sov.Phys.Usp.31, 163 (1988)]. 40. R.J.H.Kappert, H.R.Borsje and J.C.Fuggle, J.Magn.Magn.Mat.100, 363 (1991). 41. S.A.Altshuler and B.M.Kozyrev, Electron paramagnetic resonance of transition group compounds (in Russian), Moscow, Nauka, 1972. 42. K.I.Kugel and D.I.Khomsky, Usp.Fiz.Nauk 136, 621 (1982). 43. R.S.Knox and A.Gold, Symmetry in the Solid State, Benjamin, New York, 1964. 44. B.H.Brandow, Adv.Phys.26, 651 (1977). 45. S.Huefner, Adv.Phys.43, 183 (1994). 46. B.Koiller and L.M.Falicov, J.Phys.C7, 299 (1974). 47. L.H.Tjeng, C.T.Chen, G.Ghijsen, R.Rudolf and F.Sette, Phys.Rev.Lett.67, 501 (1991). 48. A.Fujimori et al, Phys.Rev.B42, 7580 (1990). 49. J.van Elp, P.H.Potze, H.Eskes, R.Berger and G.A.Sawatzky, Phys.Rev.B44, 1530 (1991). 50. J.van Elp, H.Eskes, P.Kuiper and G.A.Sawatzky, Phys.Rev.B44, 5927 (1991). 51. A.Fujimori, F.Minami and S.Sugano, Phys.Rev.B29, 5225 (1984); A.Fujimori and F.Minami, Phys.Rev.B30, 957 (1984). 52. J.M.Ziman, The Calculation of Bloch Functions, In: Solid State Physics, ed.H.Ehrenreich et al., vol.26, Academic Press, 1971. 53. J.O.Dimmock, In: Solid State Physics, ed.H.Ehrenreich et al., vol.26, Academic Press, 1970, p.103. 54. T.L.Loucks, APWMethod, Benjamin, Menlo Park, California, 1967. 55. W.Heine, M.Cohen and D.Weaire, Solid State Physics, ed.H.Ehrenreich et al., vol.24, Academic Press, 1970. 56. A.R.Mackintosh and O.K.Andersen, The Electronic Structure of Transition Metals, in: Electrons at the Fermi Surface, Ed.M.Springford, Cambridge University Press, 1980, p.149. 57. V.V.Nemoshkalenko and V.N.Antonov, Methods of Calculation Physics in the Solid State Theory. Band Theory of Metals (in Russian), Kiev, Naukova Dumka, 1985. 58. J.C.Slater and G.F.Koster, Phys.Rev.94, 1498 (1954). 59. P.Hohenberg and W.Kohn, Phys.Rev.B136, 864 (1964). 60. J.A.Moriarty, Phys.Rev.B1, 1363 (1970); B5, 2066 (1972). 61. M.D.Girardeau, J.Math.Phys., 12, 165 (1971). 62. Z.A.Gursky and B.A.Gursky, Fiz.Metallov Metalloved.50, 928 (1980). 63. G.B.Bachelet, D.R.Hamann and M.Schluter, Phys.Rev.B26, 4199 (1982). 64. K.M.Ho, S.G.Louie, J.R.Chelikowsky and M.L.Cohen, Phys.Rev.B15, 1755 (1977). 65. B.A.Greenberg, M.I.Katsnelson, V.G.Koreshkov et al., phys.stat.sol.(b) 158, 441 (1990); A.S.Ivanov, M.I.Katsnelson, A.G.Mikhin et al, Phil.Mag.69, 1183 (1994). 66. T.L.Loucks, Phys.Rev.139, A1181 (1965). 67. O.K.Andersen, Phys.Rev.B12, 864 (1975). 68. E.Wimmer, H.Krakauer, M.Weinert and A.J.Freeman, Phys.Rev.B24, 864 (1981).
428
Bibliography 69. J.C.Slater, The SelfConsistent Field for Molecules and Solids, Mc Graw Hill, New York, 1974. 70. W.Kohn and L.J.Sham, Phys.Rev.A140, 1133 (1965); L.J.Sham and W.Kohn, Phys.Rev. 145, 561 (1966). 71. O.Gunnarsson and B.I.Lundqvist, Phys.Rev.B13, 4274 (1976). 72. R.O.Jones and O.Gunnarsson, Rev.Mod.Phys, 61, 689 (1989). 73. L.Hedin and B.I.Lundqvist, J.Phys.C4, 2064 (1971). 74. U.von Barth and L.Hedin, J.Phys.C5, 1629 (1972). 75. T.Ziegler, A.Rauk and E.J.Baerends, Theor.Chim.Acta, 43, 261 (1977). 76. U.von Barth, Phys.Rev.A20, 1963 (1979). 77. A.Svane and O.Gunnarsson, Phys.Rev.B37, 9919 (1988); Phys.Rev.Lett.65, 1148 (1990); Europhys.Lett.7, 171 (1988). 78. D.A.Papaconstantopoulos, Handbook of Bandstructure of Elemental Solids, New York, Plenum Press, 1986. 79. R.J.Jelitto, J.Phys.Chem.Sol., 30, 609 (1969). 80. R.H.Swendsen and H.Callen, Phys.Rev.B6, 2860 (1972). 81. S.V.Vonsovsky, M.I.Katsnelson and A.V.Trefilov, Fiz.Metallov Metalloved.76, N3, 3 (1993). 82. D.Koelling, F.M.Mueller, A.J.Arko and J.B.Ketterson, Phys.Rev.B10, 4889 (1974). 83. J.Friedel, Canad.J.Phys.34, 1190 (1956). 84. W.A.Harrison, Phys.Rev.B28, 550 (1983). 85. N.F.Mott and K.W.H.Stevens, Phil.Mag.2, 1364 (1957). 86. W.M.Lomer and W.M.Marshall, Phil.Mag.3, 185 (1958). 87. E.O.Wollan, Phys.Rev.117, 387 (1960). 88. J.B.Goodenough, Phys.Rev.120, 67 (1960). 89. L.F.Matheiss, Phys.Rev.134, A970 (1964). 90. F.J.Himpsel and D.Eastman, Phys.Rev.B18, 5236 (1978). 91. O.K.Andersen, Phys.Rev.B2, 883 (1970). 92. N.E.Christensen, Phys.Rev.B14, 3446 (1976). 93. F.M.Mueller, A.J.Freeman, J.O.Dimmock and A.M.Furduya, Phys.Rev.B1, 4617 (1970). 94. S.G.Louie, Phys.Rev.Lett.40, 1525 (1978). 95. N.I.Mazin, E.G.Maksimov, S.I.Rashkeev and Yu.A.Uspensky, Proc. P.N.Lebedev Physical Institute of Academy of Sciences, vol.190, Moscow, Nauka, 1988, p.3. 96. K.D.Sevier, Low Energy Electron Spectrometry, New York, Wiley, 1972. 97. R.F.Davis, R.S.Williams, S.D.Kevan, P.S.Wehner and D.A.Shirley, Phys.Rev.B31, 1997 (1985). 98. P.S.Wehner, R.S.Williams, S.D.Kevan, D.Denley and D.A.Shirley, Phys.Rev.B19, 6164 (1979). 99. K.A.Mills, R.F.Davis, S.D.Kevan, G.Thornton and D.A.Shirley, Phys.Rev.B22, 581 (1980). 100. A.Svane, Phys.Rev.Lett., 68, 1900 (1992). 101. J.F.van der Veen, F.J.Himpsel and D.E.Eastman, Phys.Rev.B22, 4226 (1980). 102. W.Speier et al., Phys.Rev.B30, 6921 (1984). 103. H.Hoechst et al, Z.Phys.B42, 99 (1981). 104. D.E.Eastman, F.J.Himpsel and J.A.Knapp, Phys.Rev.Lett.44, 95 (1980). 105. E.Kisker, K.Schroeder, W.Gudat and M.Campagna, Phys.Rev.B31, 329 (1985). 106. R.Clauberg, E.M.Haines and P.Feder, J.Magn.Magn.Mater. 54–57, 622 (1986). 107. E.Kisker, J.Magn.Magn.Mater.45, 23 (1984). 108. D.E.Eastman, F.J.Himpsel and J.A.Knapp, Phys.Rev.Lett.40, 1514 (1978); F.J.Himpsel, J.A.Knapp and D.E.Eastman, Phys.Rev.B19, 2919 (1979).
429
Bibliography 109. 110. 111. 112. 113. 114. 115. 116. 117. 118. 119. 120. 121. 122. 123. 124. 125. 126. 127. 128. 129. 130. 131. 132. 133. 134. 135. 136. 137. 138.
139. 140. 141. 142. 143. 144. 145. 146. 147.
K.Kakizaki, J.Fujii, K.Shimada et al, Phys.Rev.Lett.72, 2781 (1994). M.Pessa, P.Heinmann and H.Neddermeyer, Phys.Rev.B14, 3488 (1976). G.Bush, M.Campagna and H.C.Siegmann, Phys.Rev.B4, 746 (1971). P.Genoval, A.A.Manuel, E.Walker and M.Peter, J.Phys.:Cond.Mat. 3, 4201 (1991). C.M.Schneider, P.Schuster, M.S.Hammond and J.Kirschner, Europhys.Lett.16, 689 (1991). P.Guletsky, Yu.A.Knyazev, M.M.Kirillova and L.M.Sandratsky, Fiz.Metallov Metalloved.67, 279 (1989). T.Jo and G.A.Sawatzky, Phys.Rev.B43, 8771 (1991). H.Martensson and P.O.Wilsson, Phys.Rev.B30, 3047 (1984). A.Liebsh, Phys.Rev.B23, 5203 (1981). D.R.Penn, Phys.Rev.Lett.42, 921 (1979). R.H.Victora and L.M.Falicov, Phys.Rev.Lett.55, 1140 (1985). E.Jensen and D.M.Wieliczka, Phys.Rev.B30, 7340 (1984). O.Gunnarson and K.Schoenhammer, Phys.Rev.B28, 4315 (1983). Yu.P.Irkhin, In: Electron Structure and Physical Propertties of Rare Earths and Actinides, Ural Science Centre, Sverdlovsk, 1981, p.50. J.T.Waber and A.C.Switendick, Proc.Vth Rare Earth Research Conf., Iowa State University, 1965, v.B2, p.75. G.Murhopadhyay and C.K.Majumdar, J.Phys.C2, 924 (1969). W.E.Pickett, A.J.Freeman and D.D.Koelling, Phys.Rev.B23, 1266 (1981). G.Johansen and A.R.Mackintosh, Solid State Comm.8, 121 (1970). B.N.Harmon, J.de Phys.40, 65 (1979). M.M.Islam and D.J.Newman, J.Phys.F5, 939 (1975) Tm. T.A.Matveeva and R.F.Egorov, Fiz.Metallov Metalloved.51, 717, 950 (1981). O.V.Farberovich, G.P.Nizhnikova, S.V.Vlasov and E.P.Domashevskaya, phys.stat.sol(b) 121, 241 (1984). H.J.F.Jansen, A.J.Freeman and R.Monnier, Phys.Rev.B31, 4092 (1985). D.M.Bylander and L.Kleinman, Phys.Rev.B49, 1608 (1994); B50, 1363 (1994). J.F.Herbst, D.N.Lowy and R.E.Watson, Phys.Rev.B6, 1913 (1972). J.F.Herbst, R.E.Watson and J.W.Wilson, Phys.Rev.B13, 1439 (1976); B17, 3089 (1978). E.I.Zabolotsky, Yu.P.Irkhin and L.D.Finkelstein, Fiz.Tverd.Tela, 16, 1142 (1974). P.O.Heden, H.Logfren and S.B.M.Hagstrom, Phys.Rev.Lett.26, 432 (1971). C.Bounele, R.C.Karnatek and C.Jorgensen, Chem.Phys.Lett.14, 145 (1972). A.J.Freeman, D.D.Koelling, In: The Actinides: Electron Structure and Related Properties, ed. A.J.Freeman and J.B.Darby, New York, Academic Press, 1974, p.51. B.V.Karpenko, In: Electron Structure and Physical Propertties of Rare Earths and Actinides, Ural Science Centre, Sverdlovsk, 1981, p.86. S.C.Keeton, T.L.Loucks, Phys.Rev.146, 429 (1966). D.D.Koelling, A.J.Freeman, Solid State Comm.9, 1369 (1971); Phys.Rev.B12, 5622 (1975). P.Weinberger, A.M.Boring and J.L.Smith, Phys.Rev.B31, 1964 (1985). O.Eriksson and J.M.Wills, Phys.Rev.B45, 3198 (1992). J.Kittel, Quantum Theory of Solids, Wiley, New York, 1963. C.G.Lonzarich, Fermi Surface Studies in Ferromagnets, in: Electrons at the Fermi Surface, Ed.M.Springford, Cambridge University Press, 1980, p.225. A.P.Cracknell, Band Structures and Fermi Surfaces of Metallic Elements, LandoltBoernstein New Series, Band 13c, Springer, 1984. F.S.Ham, Phys.Rev.128, 2524 (1962).
430
Bibliography 148. 149. 150. 151. 152. 153. 154. 155. 156. 157. 158. 159. 160. 161. 162. 163. 164. 165. 166. 167. 168. 169. 170. 171. 172. 173. 174. 175. 176. 177. 178. 179. 180. 181. 182. 183. 184. 185. 186. 187. 188. 189. 190. 191. 192. 193. 194. 195. 196. 197.
D.R.Jennison, Phys.Rev.B16, 5147 (1977). C.B.So, K.Takegahara and S.Wang, J.Phys.F7, 105 (1977). M.J.G.Lee, Phys.Rev.178, 953 (1969). S.L.Altmann, A.P.Cracknell, Proc.Phys.Soc. 84, 761 (1964). P.Blaha and J.Callaway, Phys.Rev.B32, 7664 (1985). J.H.Condon, J.A.Marcus, Phys. Rev. 134, A 446 (1964). C.S.Fleming, T.L.Loucks, Phys.Rev. 173, 685 (1968). T.L.Loucks, Phys.Rev. 144, 504 (1966). T.L.Loucks, Phys.Rev.A139, 1181 (1965). R.C.Young, P.C.Yordan, D.W.Jones and V.J.Hems, J.Phys.F4, L84 (1984). G.S.Fleming, S.H.Liu and T.E.Loucks, Phys.Rev.Lett.21, 1524 (1968). O.Jepsen, Phys.Rev.B12, 2988 (1975). K.M.Welch and E.H.Hygh, Phys.Rev.B9, 1993 (1974). S.L.Altmann and C.J.Bradley, Proc. Phys. Soc. 92, 764 (1967). A.J.Hughes and J.Callaway, Phys. Rev. 136, A 1390 (1964). T.L.Loucks, Phys. Rev. 159, 544 (1967). A.C.Thorsen and A.S.Joseph, Phys. Rev.131, 2078 (1963). P.M.Everett, Phys.Rev.B20, 1419 (1979). L.L.Boyer, D.A.Papaconstantopoulos and B.M.Klein, Phys.Rev.B15, 3685 (1977). D.G.Laurent, C.S.Wang and J.Gallaway, Phys.Rev.B17, 455 (1978). R.D.Parker and M.H.Halloran, Phys.Rev.B9, 4130 (1974). R.A.Phillips, Phys.Lett.A36, 361 (1971). A.C.Thorsen, T.G.Berlincourt, Phys. Rev. Lett. 7, 244 (1961). G.B.Scott, M.Springford, J.R.Stockton, Phys.Lett.A27, 655 (1968); G.B.Scott and M.Springford, Proc.Roy.Soc.A320, 115 (1970). L.F.Mattheiss, Phys. Rev. B1, 373 (1970). L.L.Boyer, D.A.Papaconstantopoulos and B.M.Klein, Phys.Rev.B15, 3685 (1977). M.Cardona and L.Ley, Photoemission in Solids (Berlin:Springer) 1978. M.H.Halloran et al, Phys.Rev.B1, 366 (1970). T.L.Loucks, Phys.Rev.139, A1181 (1965). L.F.Mattheiss, Phys. Rev.139, A 1893 (1965). D.G.Laurent, J.Callaway, J.L.Fry and N.E.Brener, Phys.Rev.B23, 4877 (1981). L.F.Mattheiss and D.R.Hamann, Phys.Rev.B33, 823 (1986). S.Asano and J.Yamashita, J.Phys.Soc.Jpn, 23, 714 (1967). N.I.Kulikov and E.I.Kulatov, J.Phys.F12, 2292 (1982). K.Okumara and I.M.Tepleton, Proc.R.Soc.A287, 89 (1965). M.J.G.Lee, Phys.Rev.178, 953 (1969). J.B.Ketterson, D.D.Koelling, J.C.Shaw and Windmiller, Phys.Rev.B11, 1447 (1975). D.M.Sparlin and J.A.Marcus, Phys. Rev. 144, 484 (1966). J.A.Hoekstra and J.L.Stanford, Phys.Rev.B8, 1416 (1973). R.F.Girvan, A.V.Gold and R.A.Phillips, J.Phys.Chem.Sol.29, 1485 (1968). G.S.Fleming, S.H.Liu and T.E.Loucks, Phys.Rev.Lett.21, 1524 (1968). G.C.Fletcher, J. Phys.C2, 1440 (1969). L.F.Mattheiss, Phys.Rev.151, 450 (1966). A.C.Thorsen, A.S.Joseph, L.I.Valby, Phys.Rev.150, 523 (1966). J.H.Wood, Phys. Rev. 126, 517 (1962). R.A.Tawil and J.Callaway, Phys.Rev.B7, 4242 (1973). J.Callaway and C.S.Wang, Phys.Rev.B16, 2095 (1977). A.V.Gold, L.Hodges, P.T.Panousis and D.R.Stone, Int.J.Magn.2, 357 (1971). D.R.Baraff, Phys.Rev.B8, 3439 (1973). S.Wakoh, J.Yamashita, J. Phys Soc. Japan 38, 1151 (1970).
431
Bibliography 198. 199. 200. 201. 202. 203. 204. 205. 206. 207. 208. 209. 210. 211. 212. 213. 214. 215. 216. 217. 218. 219. 220. 221. 222. 223. 224. 225. 226. 227. 228. 229. 230. 231. 232. 233. 234. 235.
236.
237.
C.M.Singal and T.P.Das, Phys.Rev.B16, 5068 (1977). J.R.Anderson and J.F.Shirber, J.Appl.Phys.52, 1630 (1980). N.I.Kulikov and E.I.Kulatov, J.Phys.F12, 2267 (1982). F.Batallan, S.Rosenman and C.Summers, Phys.Rev.B11, 545 (1975). I.Rosenman and F.Batallan, Phys.Rev.B5, 1340 (1972). J.R.Anderson, J.J.Hudak and D.R.Stone, AIR Conf.Proc.5, 477 (1972). J.Callaway and C.S.Wang, Phys.Rev.B7, 1096 (1973); C.S.Wang and J.Callaway, Phys.Rev.B9, 4897 (1974). R.Prasad, S.K.Joshi and S.Auluck, Phys.Rev.B16, 1765 (1977); S.Ahuja, S.Auluck and B.Johansson, Physica Scripta 50, 573 (1994). J.R.Anderson, D.A.Papaconstantopoulos, L.L.Boyer and J.E.Schriber, Phys.Rev.B20, 3172 (1979). E.I.Zornberg, Phys.Rev.B1, 244 (1970). D.S.Tsui, Phys.Rev.164, 669 (1967). G.N.Kamm and J.R.Anderson, Phys.Rev.B2, 2944 (1970). J.F.Cooke, H.L.Davies and R.F.Wood, Phys.Rev.Lett.25, 28 (1970). P.T.Coleridge and I.M.Templeton, J.Phys.F2, 643 (1972). P.T.Coleridge, Phys. Lett. 22, 367 (1966); J.Low Temp.Phys.1, 577 (1969). E.S.Alekseyev, V.A.Ventsel, O.A.Voronov, A.I.Likhter and M.V.Magnitskaya, Zh.Eksp.Teor.Fiz.76, 215 (1979) [Sov.Phys.JETP 49, 110 (1979)]. G.N.Kamm, Phys.Rev.B2, 2944 (1970). O.K.Andersen, A.R.Mackintosh, Solid State Commun. 6, 285 (1968). P.T.Coleridge, Phys. Lett. 15, 223 (1965). P.T.Coleridge, Proc. Roy. Soc. A295, 458 (1966). J.J.Grodski, A.E.Dixson, Solid State Commun.7, 735 (1969). S.Hornfeldt, Solid State Commun. 8, 673 (1970). N.V.Volkenshtein, V.A.Novoselov, V.E.Startsev and Yu.N.Tsiovkin, Zh.Eksp.Teor.Fiz.60, 1733 (1971); Sov.Phys.JETP 33, 959 (1971). G.O.Arbman and S.Hornfeldt, J.Phys.F2, 1033 (1972). G.O.Arbman and S.Hornfeldt, J.Phys.F2, 1033 (1972); M.Cooper and B.Williams, Philos.Mag.26, 1441 (1972). J.J.Vuillemin, Phys. Rev. 144, 396 (1966). J.J.Vuillemin, M.G.Priestley, Phys. Rev. Lett. 15, 307 (1965). D.H.Dye, S.A.Campbell, G.W.Grabtree, J.B.Ketterson, N.B.Sandesara and J.J.Vuillemin, Phys.Rev.B23, 462 (1981). J.B.Ketterson and L.R.Windmiller, Phys.Rev.B1, 4747 (1970); B2, 4813 (1970). D.H.Dye, J.B.Ketterson and G.W.Crabtree, J.Low Temp.Phys.30, 813 (1978). N.F.Christensen et al, J.Magn.Magn.Mat.76–77, 23 (1988). S.Tanuma, W.R.Datars, H.Doi, A.Dunsworth, Solid State Commun.8, 1107 (1970). R.C.Young, R.G.Jordan and D.W.Jones, Phys.Rev.Lett.31, 1473 (1973). S.C.Keeton and T.L.Loucks, Phys. Rev. 168, 672 (1968). S.C.Keeton and T.L.Loucks, Phys. Rev. 146, 428 (1966). A.C.Thorsen and A.S.Joseph, L.E.Valby, Phys. Rev. 162, 574 (1967). R.P.Gupta and T.L.Loucks, Phys. Rev. Lett. 22, 458 (1969). K.A.Gschneidner, Jr., Physical Properties and Interrelationships of Metallic and Semimetallic Elements, In: Solid State Physics, ed.H.Ehrenreich et al., vol.16, Academic Press, 1964, p.275. B.Johansson and M.S.S.Brooks, Theory of Cohesion in Rare Earths and Actinides, In: Handbook Phys.Chem. Rare Earths, ed.K.A.Gschneidner,Jr. et al, vol.17, p.149. Properties of Elements, ed.M.E.Dritz, Moscow, Metallurgiya, 1985.
432
Bibliography 238. Properties of Elements, ed.G.V.Samsonov, Moscow, Metallurgiya, 1976. 239. V.E.Zinov’yev, Thermophysical Properties of Metals at High Temperatures, Moscow, Metallurgiya, 1989. 240. A.M.Oles, Phys.Rev.B23, 271 (1981). 241. J.Friedel and C.M.Sayers, J.de Phys.38, 697 (1977). 242. C.D.Gelatt, H.Ehrenreich and R.E.Watson, Phys.Rev.B15, 1613 (1977). 243. V.L.Moruzzi, J.F.Janak and K.Schwarz, Phys.Rev.B37, 790 (1988). 244. H.L.Skriver and M.M.Rosengaard, Phys.Rev.B45, 9410 (1992). 245. H.L.Skriver, Phys.Rev.B31, 1909 (1985). 246. V.A.Finkel, Structure of Rare Earth Metals (in Russian), Moscow, Metallurgiya, 1978. 247. C.M.Hurd and J.E.A.Alderson, Solid State Comm., 12, 375 (1974). 248. W.HumeRothery, The Metallic State, New York, University Press, 1931. 249. H.Jones, Proc.Phys.Soc., 49, 423 (1937). 250. N.Engel, Trans.Amer.Soc.Metals, 57, 610 (1964). 251. G.V.Samsonov, I.F.Pryadko and L.F.Pryadko, Electron Localization in Solids (in Russian), Moscow, Nauka, 1976. 252. W.HumeRothery, Progr.Mater.Sci., 13, 229 (1968). 253. D.G.Pettifor, J.Phys.C3, 367 (1970). 254. J.W.Davenport, R.E.Watson and M.Weinert, Phys.Rev.B32, 4883 (1985). 255. M.Sigalas, D.Papaconstantopoulos and N.C.Bacalis, Phys.Rev.B45, 5777 (1992). 256. J.M.Wills and O.Eriksson, Phys.Rev.B45, 13879 (1992). 257. G.Gladstone, M.A.Jensen and J.R.Schrieffer, In: Superconductivity, ed.R.D.Parks, New York, 1969. 258. J.A.Moriarty, Phys.Rev.B49, 12431 (1994). 259. M.M.Steiner, R.C.Albers and L.J.Sham, Phys.Rev.B45, 13272 (1992). 260. G.Grimwall, J.Phys.Chem.Sol., 29, 1221 (1968). 261. J.Osuzu, Thesis, Nagoya University, 1968. 262. M.Shimizu, Rep.Progr.Phys., 44, 329 (1981). 263. P.Fulde and M.Loewenhaupt, Adv.Phys., 34, 589 (1985). 264. L.M.Noskova, E.V.Rosenfeld and Yu.P.Irkhin, Fiz.Nizkikh Temperatur, 11, 469 (1985). 265. S.V.Vonsovsky, Magnetism, New York, Wiley, 1974. 266. M.Dixon, F.E.Hoare, T.M.Holden and D.E.Moody, Proc.Roy.Soc.A285, 561 (1965). 267. R.E.Pawell and E.E.Stansbury, J.Phys.Chem.Sol.26, 757 (1965). 268. E.V.Rosenfeld, A.A.Siventsev, Yu.P.Irkhin and L.M.Noskova, Fiz.Tverd.Tela 33, 202 (1991). 269. S.A.Nemnonov, Fiz.Metallov Metalloved.19, 550 (1965). 270. E.V.Galoshina, Usp.Fiz.Nauk 113, 105 (1974). 271. R.Kubo and Y.Obata, J.Phys.Soc.Jpn 11, 547 (1956). 272. M.Yasui, Physica B149, 139 (1988). 273. S.Tikadzumi, Physics of Magnetism, Wiley, New York, 1964. 274. R.Huguenin and D.Baldock, Phys.Rev.Lett.Phys.Rev.Lett.16, 795 (1966); R.Huguenin, G.P.Pells and D.N.Baldock, J.Phys.F1, 281 (1971). 275. R.Peierls, Z.Phys.80, 763 (1933). 276. F.Ducastelle and F.CyrotLackmann, J.de Phys.Colloque 32, C1–534 (1971). 277. M.Matsumoto, J.Staunton and P.Strange, J.Phys.:Cond.Mat.3, 1453 (1991). 278. S.G.Das, Phys.Rev.B13,3978 (1976). 279. A.H.MacDonald, K.L.Liu and S.H.Vosko, Phys.Rev.B16, 777 (1977). 280. P.Rhodes and E.P.Wohlfarth, Proc.Roy.Soc. A273, 247 (1963). 281. H.Ido, J.Magn.Magn.Mat.54–57, 937 (1986); H.Ido, S.Yasuda, J.de Phys.Colloque C8, 49, 141 (1988).
433
Bibliography 282. M.J.Otto, R.A.M. van Woerden, P.J. van der Valk et al. J.Phys.:Cond.Mat.1, 2341 (1989). 283. P.J.Webster, J.Phys.Chem.Sol., 32, 1221 (1971). 284. R.Vijayaraghavan, J.Magn.Magn.Mater.47–48, 561 (1985); M.Kasaya et al, J.Magn.Magn.Mater.76–77, 347 (1988). 285. E.S.Stoner, Proc.Roy.Soc.A165, 372 (1938); A169, 339 (1939). 286. E.P.Wohlfarth, Phil.Mag.42, 374 (1951). 287. D.M.Ceperley and B.J.Adler, Phys.Rev.Lett.45, 566 (1980). 288. V.Yu.Irkhin, M.I.Katsnelson and A.V.Trefilov, J.Magn.Magn.Mat.117, 210 (1992); J.Phys.:Cond.Mat.5, 8763 (1993). 289. G.H.O.Daalderop, M.H.Boon and F.M.Mueller, Phys.Rev.B41, 9803 (1990). 290. T.Jarlborg and A.J.Freeman, Phys.Rev.B22, 2332 (1980); T.Jarlborg, A.J.Freeman and D.D.Koelling, J.Magn.Magn.Mat.23, 291 (1981). 291. Yu.P.Irkhin, E.V.Rosenfeld and A.A.Siventsev, Fiz.Tverd.Tela 33, 1646 (1991). 292. O.Gunnarson, J.Phys.F6, 587 (1976). 293. A.M.Oles and G.Stollhoff, J.Magn.Magn.Mat.54–57, 1045 (1986). 294. E.V.Rosenfeld and Yu.P.Irkhin, Fiz.Metallov Metalloved. 57, 837 (1984); Yu.P.Irkhin and E.V.Rosenfeld, Solid State Comm., 44, 1371 (1982). 295. C.Herring, Magnetism, vol.4, New York, Academic Press, 1966. 296. T.Moriya and A.Kawabata, J.Phys.Soc.Jpn, 34, 639 (1973); 35, 669 (1973). 297. I.E.Dzyaloshinskii and P.S.Kondratenko, Sov.Phys.JETP 43, 1036 (1976). 298. J.A.Hertz and M.A.Klenin, Phys.Rev.B10, 1084 (1974); Physica 91B, 49 (1977). 299. K.K.Murata and S.Doniach, Phys.Rev.Lett.29, 285 (1982). 300. J.Hubbard, Phys.Rev.B19, 2626 (1979); B20, 4584 (1979). 301. H.Hasegawa, J.Phys.Soc.Jpn 49, 178; 963 (1980). 302. E.A.Turov and V.I.Grebennikov, Physica B149, 150 (1988). 303. A.A.Siventsev and Yu.P.Irkhin, Fiz.Tverd.Tela 35, 1965 (1993). 304. P.Mohn and E.P.Wohlfarth, J.Phys.F17, 2421 (1987); E.P.Wohlfarth and P.Mohn, Physica B149, 145 (1988). 305. G.G.Lonzarich and L.Taillefer, J.Phys.C18, 4339 (1985). 306. R.A.de Groot, F.M.Mueller, P.G.Mueller, P.G. van Engen and K.H.J.Bushow, Phys.Rev.Lett.50, 2024 (1983). 307. R.A.de Groot, F.M.Mueller, P.G. van Engen and K.H.J.Bushow, J.Appl.Phys.55(6), 2151 (1984). 308. R.A.de Groot and K.H.J.Buschow, J.Magn.Magn.Mat.54–57, 1377 (1986). 309. J.Kuebler, Physica B+C 127, 257 (1984). 310. R.A.de Groot, A.M.von der Kraan and K.H.J.Buschow, J.Magn.Magn.Mat.61, 330 (1986). 311. J.Kuebler, J.R.Williams and C.B.Sommers, Phys.Rev.B28, 1745 (1983). 312. S.Fujii, S.Sugimura, S.Ishida and S.Asano, J.Phys.:Cond.Mat. 2, 8583 (1990). 313. K.Schwarz, J.Phys.F16, L211 (1986). 314. E.Kulatov and I.Mazin, J.Phys.:Cond.Mat. 2, 343 (1990). 315. R.C.Albers, A.M.Boring, G.H.O.Daalderop and F.M.Mueller, Phys.Rev.B36, 3661 (1987). 316. S.V.Halilov and E.T.Kulatov, J.Phys.: Cond.Mat.3, 6363 (1991); Zh.Eksp.Theor.Fiz.98, 1778 (1989). 317. A.Yanase, K.Siratori, J.Phys.Soc.Jpn 53, 312 (1984) (1988). 318. V.Yu.Irkhin and M.I.Katsnelson, Usp.Fiz.Nauk 164, 705 (1994) [Sov.Phys.Uspekhi 37, 565 (1994)]. 319. K.Schwarz, O.Mohn, P.Blaha, J.Kuebler, J.Phys.F14, 2659 (1984).
434
Bibliography 320. S.S.Jaswal, Phys.Rev.B41, 9697 (1990); S.S.Jaswal, W.B.Yelon, G.C.Hadjipanayis et al., Phys.Rev.Lett. 67, 644 (1991). 321. B.I.Min, J.S.Kang, J.H.Hong et al., Phys.Rev.B48, 6317 (1993). 322. S.K.Malik, P.J.Arlinghaus, W.E.Wallace, Phys.Rev.B25, 6488 (1982). 323. J.Inoue and M.Shimizu, J.Phys.F15, 1511 (1985). 324. S.Matar, P.Mohn, G.Demazeau and B.Siberchicot, J.de Phys.49, 1761. 325. S.Fujii, S.Ishida and S.Asano, J.Phys.:Cond.Mat.4, 1575 (1992). 326. A.Sakuma, J.Phys.Soc.Jpn 60, 2007 (1991). 327. Y.Noda and Y.Ishikawa. J.Phys.Soc.Jpn 40, 690, 699 (1976). 328. K.Tajima and Y.Ishikawa, P.J.Webster et al. J.Phys.Soc.Jpn 43, 483 (1977). 329. M.I.Auslender and V.Yu.Irkhin, J.Phys.C18, 3533 (1985). 330. E.Kisker, G.Baum, A.Mahan, W.Raith and B.Reihl, Phys.Rev.B18, 2256 (1978). 331. M.J.Otto, R.A.M. van Woerden, P.J. van der Valk et al. J.Phys.: Cond.Mat.1, 2351 (1989). 332. J.A.Hertz and D.M.Edwards, J.Phys.F3, 2174 (1973); D.M.Edwards and J.A.Hertz, J.Phys.F3, 2191 (1973). 333. V.Yu.Irkhin and M.I.Katsnelson, Fiz.Tverd.Tela 25, 3383 (1983) [Sov.Phys.Solid State 25, 1947 (1983)]. 334. G.L.Bona, F.Meier, M.Taborelli, E.Bucher and P.H.Schmidt, Solid State Comm.56, 391 (1985). 335. T.Moriya, J.Phys.Soc.Jpn 19, 681 (1964). 336. E.A.Turov and M.P.Petrov, Nuclear Magnetic Resonance in Ferro and Antiferromagnets [in Russian], Moscow, Nauka, 1969. 337. V.Yu.Irkhin and M.I.Katsnelson, Fiz.Metallov Metalloved. 66, 41 (1988). 338. V.Yu.Irkhin and M.I.Katsnelson, J.Phys.:Cond.Mat.2, 7151 (1990). 339. H.Enokiya, J.Phys.Soc.Jpn 31, 1037 (1971). 340. M.M.Matsuura, J.Phys.Soc.Jpn 21, 886 (1966). 341. K.Terakura, T.Oguchi, A.R.Williams and J.Kuebler, Phys.Rev.B30, 4734 (1984). 342. Z.Szotek, W.M.Temmerman and H.Winter, Phys.Rev.B47, 4029 (1993). 343. V.I.Anisimov, A.Zaanen and O.K.Andersen, Phys.Rev.B44, 943 (1991). 344. L.L.Chase, Phys.Rev.B10, 2226 (1974). 345. S.Lauer, A.X.Trautwein and F.E.Harris, Phys.Rev.B29, 6774 (1984). 346. G.L.Zhao, J.Callaway and M.Hayashibara, Phys.Rev.B48, 15781 (1994). 347. H.S.Jarrett, W.H.Cloud, H.J.Bouchard, S.R.Butler, C.G.Frederick and J.L.Gillson, Phys.Rev.Lett.21, 617 (1968). 348. J.Kanamori, Progr.Theor.Phys.30, 275 (1963). 349. Y.Nagaoka, Phys.Rev.147, 392 (1966). 350. D.N.Khomsky, Fiz.Metallov Metalloved.29, 31 (1970). 351. P.B.Vissher, Phys.Rev.B10, 932, 943 (1974). 352. E.L.Nagaev, Physics of Magnetic Semiconductors, Moscow, Mir, 1983. 353. M.I.Auslender, V.Yu.Irkhin and M.I.Katsnelson, J.Phys.C21, 5521 (1988). 354. J.Hubbard and K.P.Jain, J.Phys.C1, 1650 (1968). 355. A.Sakurai, Progr.Teor.Phys.39, 312 (1968). 356. J.J.Field, J.Phys C5, 664 (1972). 357. S.V.Tyablikov, Methods of Quantum Theory of Magnetism [in Russian], Moscow, Nauka, 1975. 358. G.Chrobok, M.Hofmann, G.Regenfus and P.Sizmann, Phys.Rev.B15, 429 (1975). 359. A.Vaterlaus, F.Millani and F.Meier. Phys.Rev.Lett.65, 3041 (1990). 360. S.A.Nikitin, A.S.Andreenko, A.K.Zvezdin and A.F.Popov, Zh.Eksp.Teor.Fiz.76, 2159 (1979). 361. K.Yosida and A.Watabe, Progr.Theor.Phys.28, 361 (1962).
435
Bibliography 362. 363. 364. 365. 366. 367. 368. 369. 370. 371. 372. 373. 374. 375. 376. 377. 378. 379. 380. 381. 382. 383. 384.
385. 386. 387. 388. 389. 390. 391. 392. 393. 394. 395. 396. 397. 398. 399. 400. 401. 402.
W.E.Evenson and S.V.Lin, Phys.Rev.178, 783 (1969). R.J.Elliott and F.A.Wedgwood, Proc.Roy.Soc.81, 846 (1963); 84, 63 (1964). P.G.de Gennes, Journ.Phys.Rad.23, 630 (1932). H.Miwa, Proc.Phys.Soc.85, 1197 (1965). A.J.Fedro and T.Arai, Phys.Rev.B6, 911 (1972). V.Yu.Irkhin and M.I.Katsnelson, Z.Phys.B75, 67 (1989). I.E.Dzyaloshinsky, Zh.Eksp.Teor.Fiz.46, 1420 (1964); 47, 336, 992 (1964). J.Bohr and D.Gibbs, Physica A140, 349 (1986). S.K.Godovikov, Thesis, Moscow State University, 1994. K.G.Gurtovoy and R.Z.Levitin, Usp.Fiz.Nauk, 153, 193 (1987). P.G.Huray, S.E.Nave and R.G.Haire, J.LessCommon Met, 93, 393 (1983). S.E.Nave et al, Physica B130, 225 (1985). I.V.Solovyev, A.I.Liechtenstein, V.A.Gubanov, V.A.Antropov and O.K.Andersen, Phys.Rev.B43, 14414 (1991). I.V.Solovyev, Thesis, Sverdlovsk, 1991. E.A.Turov and A.I.Mitsek, Zh.Eksp.Teor.Fiz.37, 1127 (1959). Ch.Kittel and J.H.Van Vleck, Phys.Rev.118, 1231 (1960). H.B.Callen and E.R.Callen, J.Phys.Chem.Sol.27, 1271 (1966). H.Brooks, Phys.Rev.58, 909 (1940). E.I.Kondorsky and E.Straube, Pis’ma ZhETF 17, 41 (1973). E.I.Kondorsky, Band Theory of Magnetism (in Russian), Moscow University Press, 1976 (pt.1), 1977 (pt.2). R.Gersdorf, Phys.Rev.Lett.40, 344 (1978). G.H.O.Daalderop, P.J.Kelly and M.F.H.Schuurmans, Phys.Rev.B41, 11919 (1990). O.Eriksson, G.W.Fernando, R.C.Albers and A.M.Boring, Solid State Comm. 78, 801 (1991); O.Eriksson, A.M.Boring, R.C.Albers, G.W.Fernando and B.R.Cooper, Phys.Rev.B45, 2868 (1992). H.J.F.Jansen, J.Appl.Phys.67, 4555 (1990). D.C.Johnston and J.H.Cho, Phys.Rev.B42, 8710 (1990). Yu.P.Irkhin, E.V.Rosenfeld and L.D.Finkelstein, Fiz.Tverd.Tela 35, 2769 (1993). G.Di Castro, L.F.Feiner and M.Grilly, Phys.Rev.Lett.66, 3209 (1991). Yu.P.Irkhin, V.V.Druzhinin and A.A.Kazakov, Zh.Eksper.Teor.Fiz. 54, 1183 (1968) [Sov.Phys.JETP 27, 633 (1968)]. S.K.Godovikov, M.G.Kozin, V.V.Turovtsev and V.S.Spinel, phys.stat.sol.(b) 78, 103 (1976). Yu.P.Irkhin and E.V.Rosenfeld, Fiz.Tverd.Tela 16, 485 (1974). A.S.Ermolenko et al, Zh.Eksp.Teor.Fiz.69, 1743 (1975). Yu.P.Irkhin, E.I.Zabolotskii and E.V.Rosenfeld, Fiz.Metallov Metalloved.49, 1216 (1980). Yu.P.Irkhin, Thesis, Sverdlovsk, 1968. V.N.Novogrudsky and I.G.Fakidov, Zh.Eksp.Teor.Fiz.47, 40 (1964). E.A.Turov, V.G.Shavrov and Yu.P.Irkhin, Zh.Eksp.Teor.Fiz.47, 296 (1964). S.S.Levina, V.N.Novogrudsky and I.G.Fakidov, Zh.Eksp.Teor.Fiz.45, 52 (1963). E.A.Turov, Transport, Optical and Acoustical Properties of Antiferromagnets (in Russian), Sverdlovsk, 1990. K.B.Vlasov et al, Fiz.Metallov Metalloved.42, 513 (1976); Fiz.Tverd.Tela 22, 1656 (1980). K.B.Vlasov et al, Fiz.Metallov Metalloved.44, 1005 (1977); 53, 493 (1982); Fiz.Tverd.Tela 24, 1338 (1982). L.A.Boyarsky, Fiz.Nizkhikh Temperatur, 22, 912 (1996). R.Kubo, J.Phys.Soc.Jpn 12, 570 (1957).
436
Bibliography 403. 404. 405. 406. 407. 408. 409. 410. 411. 412. 413. 414. 415. 416. 417. 418. 419. 420. 421. 422. 423. 424. 425. 426. 427. 428. 429. 430. 431. 432. 433. 434. 435. 436. 437. 438. 439. 440. 441. 442. 443.
H.Nakano, Progr.Theor.Phys.17, 145 (1957). H.Mori, Progr.Theor.Phys., 34, 399 (1965). V.Yu.Irkhin, M.I.Katsnelson and A.V.Trefilov, Physica C160, 397 (1989). N.V.Volkenshtein, V.P.Dyakina and V.E.Startsev, phys.stat.sol.(b) 57, 9 (1973). N.V.Volkenshtein et al, Fiz.Metallov Metalloved.67, 734 (1989). G.Baber, Proc.Roy.Soc.A158, 383 (1937). J.Appel, Phil.Mag.90, 1071 (1963). M.J.Rice, Phys.Rev.Lett.20, 1439 (1968). P.A.Schroeder, Physica B+C 109–110, 1901 (1982). N.V.Volkenshtein, V.A.Novoselov and V.E.Startsev, Zh.Eksp.Teor.Fiz.60, 1078 (1971); V.E.Startsev, Thesis, Sverdlovsk, 1985. N.V.Volkenshtein et al, Fiz.Nizkikh Temp.10, 841 (1989). F.J.Blatt and H.G.Satz, Helv.Phys.Acta, 33, 1007 (1960). Yu.Kagan and A.P.Zhernov, Zh.Eksp.Teor.Fiz.50, 1107 (1966). K.Ueda and T.Moriya, J.Phys.Soc.Jpn 39, 605 (1975). A.H.MacDonald, Can.J.Phys.60, 710 (1982). N.F.Mott, Proc.Roy.Soc.A153, 699 (1936); A157, 368 (1936); Adv.Phys.13, 325 (1964). A.H.Wilson, Proc.Roy.Soc.A167, 580 (1938). Yu.P.Irkhin, Fiz.Metallov Metalloved.6, 214, 586 (1958). M.D.Wilding and E.W.Lee, Proc.Phys.Soc.85, 955 (1965). T.Kasuya, Progr.Theor Phys. 16, 58 (1956). Sh.Sh.Abelsky and E.A.Turov, Fiz.Metallov Metalloved.10, 801 (1960). S.V.Vonsovsky and Yu.A.Izyumov, Usp.Fiz.Nauk, 58, 3 (1962). E.A.Turov, Izv. AN SSSR (Ser.Fiz.) 19, 474 (1955). T.Kasuya, Progr.Theor Phys. 22, 227 (1959). M.Roessler, phys.stat.sol. 9, K27 (1965). V.S.Lutovinov, M.Yu.Reizer and M.A.Savchenko, Zh.Eksp.Theor.Fiz.77, 707 (1979). A.R.Mackintosh, Phys.Lett.4, 140 (1963). R.V.Colvin and S.Arais, phys.stat.sol.4, 37 (1964). A.A.Berdyshev and I.N.Vlasov, Fiz.Metallov Metalloved. 10, 628 (1960). M.Roesler, phys.stat.sol. 8, K31 (1965). V.Yu.Irkhin and M.I.Katsnelson, Phys.Rev.B52, 6181 (1995). N.V.Ryzhanova, Sh.Sh.Abelsky and Yu.P.Irkhin, Fiz.Metallov Metalloved.56, 843 (1983). H.Ehrenreich and L.Schwartz, In: Solid State Physics, vol.31, ed.F.Seitz and D.Turnbull, New York, Academic Press, 1976. I.A.Campbell and A.Fert, In: Ferromagnetic Materials, ed.P.Wohlfarth, NorthHolland, vol.3, 1982, p.747; A.Fert and I.A.Campbell, J.Phys.F6, 849 (1976). Proc.First Int.Symp.on Magnetic Multilayers (Kyoto, 1993), J.Magn.Magn. Mat.126 (1993). M.V.Vedernikov, Adv.Phys.18, 337 (1969). L.T.Rayevskaya, E.V.Rosenfeld and Yu.P.Irkhin, Fiz.Metallov Metalloved.66, 73 (1988). K.R.Krylov, A.I.Ponomarev, I.M.Tsidilkovsky et al, Phys.Lett.A131, 203 (1988). R.C.Yu et al, Phys.Rev.B37, 7963 (1988). V.Yu.Irkhin, M.I.Katsnelson and A.V.Trefilov, Europhys.Lett.15, 649 (1991); Zh.Eksp.Theor.Fiz.105, 1733 (1994). C.M.Hurd, The Hall Effect in Metals and Alloys, Plenum, New York, 1972.
437
Bibliography 444. M.J.Ziman, Phys.Rev.121, 1320 (1961). 445. T.Matsuda, J.Phys.Chem.Sol.30, 859 (1969); A.Hasegawa and T.Kasuya, J.Phys.Soc.Jpn 28, 75 (1970). 446. N.V.Volkenshtein et al, Zh.Eksp.Teor.Fiz.89, 172 (1985). 447. E.I.Kondorsky, Sov.Phys.JETP 28, 1256 (1969). 448. E.Fawcett, Adv.Phys.13, 139 (1964). 449. E.M.Pugh, Phys.Rev.36, 1503 (1930). 450. I.K.Kikoin, Sow.Phys.9, 1 (1936). 451. N.V.Volkenshtein and G.V.Fedorov, Zh.Eksp.Teor.Fiz.38, 64 (1960). 452. T.Penney et al, J.Magn.Magn.Mat.54–57, 370 (1986). 453. F.Lapierre et al, J.Magn.Magn.Mat.63–64, 338 (1987). 454. V.Rudnitskii, Zh.Eksp.Teor.Fiz.9, 262 (1939); 10, 744 (1940). 455. R.Hulme, Proc.Roy.Soc.A135, 237 (1932). 456. A.G.Samoilovich and B.L.Kon’kov, Zh.Eksp.Teor.Fiz. 20, 783 (1950). 457. R.Karplus and J.M.Luttinger, Phys.Rev. 95, 1154 (1954). 458. W.Kohn and J.M.Luttinger, Phys.Rev.108, 590 (1957). 459. J.M.Luttinger, Phys.Rev.112, 739 (1958). 460. Yu.P.Irkhin and V.G.Shavrov, Zh.Eksp.Teor.Fiz.42, 1233 (1962) [Sov. Phys.JETP 15, 854 (1962)]. 461. H.R.Leribaux, Phys.Rev.150, 384 (1966). 462. A.B.Granovskii and E.I.Kondorskii, Fiz.Metallov Metalloved. 39, 718 (1975). 463. A.N.Voloshinsky and L.F.Savitskaya, Zh.Eksp.Theor.Fiz.61, 2018 (1971). 464. Yu.P.Irkhin and Sh.Sh.Abelskii, Fiz.Metallov Metalloved.14, 641 (1962). 465. J.Kondo, Progr.Theor.Phys.27, 772 (1962); 28,846 (1962). 466. Yu.P.Irkhin and Sh.Sh.Abelskii, Fiz.Tverd.Tela 6, 1635 (1964) [Sov. Phys. – Solid State 5, 1283 (1964)]. 467. L.F.Savitskaya and A.N.Voloshinsky, Fiz.Metallov Metalloved.33, 849 (1972). 468. E.I.Kondorskii, Zh.Eksp.Teor.Fiz.48, 506 (1965). 469. L.Berger, Phys.Rev.B2, 4559 (1970); B5, 1862 (1972); B8, 2351 (1973); P.Nozieres and C.Lewiner, J.Phys.(Paris) 34, 901 (1973). 470. S.K.Lyo and T.Holstein, Phys.Rev.Lett.29, 423 (1972). 471. Yu.Kagan and L.A.Maksimov, Fiz.Tverd.Tela 7, 530 (1965) [Sov.Phys. – Solid State 7, 422 (1965)]. 472. Yu.P.Irkhin, A.N.Voloshinskii and Sh.Sh.Abelskii, phys.stat.sol. 22, 309 (1967). 473. R.Huguenin and D.Rivier, Helv.Phys.Acta 38, 900 (1965). 474. E.I.Kondorskii, Zh.Eksp.Teor.Fiz.55, 558 (1968) [Sov.Phys. JETP 28, 291 (1968)]; Zh.Eksp.Teor.Fiz.55, 2367 (1968) [Sov.Phys. JETP 28, 1256 (1968)]. 475. A.A.Abdurakhmanov, Transport effects in ferromagnetic metals (in Russian), Rostov University Press, 1978. 476. F.E.Maranzana, Phys.Rev.160, 421 (1967). 477. B.Giovannini, Proc.Conf. sur l’effet Hall extraordinaire, ed.G.Cohen et al, University of Geneva, 1973, p.82. 478. A.Fert, J.Phys.Lett.35, L107 (1974). 479. A.Fert and P.M.Levy, Phys.Rev.B36, 1907 (1987); P.M.Levy, Phys.Rev.B38, 6779 (1988). 480. N.O.Kourov, Yu.N.Tsiovkin and N.V.Volkenshtein, Fiz.Tverd.Tela 24, 1059 (1981). 481. J.Smit, Physica 17, 612 (1951); 21, 817 (1955); 24, 39 (1958). 482. V.Marsocci, Phys.Rev.137, A1842 (1965). 483. Vu Dinh Ky, phys.stat.sol.15, 739 (1966). 484. A.Kundt, Wied.Ann. 49, 257 (1893).
438
Bibliography 485. 486. 487. 488. 489. 490. 491. 492. 493. 494. 495. 496. 497. 498. 499. 500. 501. 502. 503. 504. 505. 506. 507. 508. 509. 510. 511. 512. 513.
514. 515. 516. 517. 518. 519. 520. 521.
H.R.Hulme, Proc.Roy.Soc.A135, 237 (1952). C.Kittel, Phys.Rev.53, A208 (1951). P.N.Argyres, Phys.Rev.97, 334 (1965). B.R.Cooper, Phys.Rev.139, A1504 (1965). A.N.Voloshinsky and G.A.Bolotin, Fiz.Metallov Metalloved.17, 481 (1964). L.E.Gurevich and I.N.Yassievich, Fiz.Tverd.Tela 6, 3341 (1964). E.I.Kondorsky and A.V.Vedyaev, J.Appl.Phys.39, 559 (1968). D.Weller et al, J.de Phys.Colloque C8, 49, 41 (1988). A.V.Druzhinin, Yu.V.Knyazev and G.A.Bolotin, Fiz.Metallov Metalloved. 52, 1194 (1981). R.A. de Groot, P.G. van Engen, P.P.J. van Engelen, K.H.J.Buschow, J.Magn.Magn.Mat.86, 326 (1990). J.H.Wijngaard, C.Haas, R.A.de Groot, Phys.Rev.B40, 9318 (1989). H.Fuiji, H.Kawanaka, T.Takabatake et al, J.Phys.Soc.Jpn 58, 3481 (1989). M.Yethirai, R.A.Robinson, J.J.Rhyne, J.A.Gotaas and K.H.J.Bushow, J.Magn.Magn.Mat.79, 355 (1993). G.S.Krinchik and M.V.Chetkin, Zh.Eksp.Teor.Fiz.36, 1924 (1959). V.N.Mayevsky and G.A.Bolotin, Fiz.Metallov Metalloved. 40, 258 (1975). A.V.Druzhinin, Thesis, Sverdlovsk, 1986. G.S.Krinchik and R.D.Nuralieva, Fiz.Metallov Metalloved.7, 697 (1959). E.I.Kondorsky and R.P.Vasilyeva, Zh.Eksp.Teor.Fiz.45, 401 (1963). E.I.Kondorsky, Zh.Eksp.Teor.Fiz.45, 511 (1963); 46, 2080 (1964). A.N.Voloshinsky and N.V.Ryzhanova, Fiz.Metallov Metalloved. 40, 7 (1975); 41, 903 (1976). P.A.Lee, T.M.Rice, J.W.Serene, L.J.Sham and J.W.Wilkins, Comm.Cond. Mat.Phys.12, 99 (1986). A.de Visser and J.J.M.Franse, J.Magn.Magn.Mat.100, 204 (1991). G.R.Stewart, Rev.Mod.Phys. 56, 755 (1984). S.Barth et al, Phys.Rev.B39, 11695 (1989). H.Nakamura, Y.Kitaoka, K.Asayama and J.Floquet, J.Phys.Soc.Jpn 57, 2644 (1988). D.Jaccard, J.Sierro, J.P.Brison and J.Floquet, J.de Phys. Coll.C8, 49, 741 (1988). W.H.Wong and W.G.Clark, J.Magn.Magn.Mater.108, 175 (1992); O.Avenel, J.S.Xia, B.Andraka et al., Phys.Rev.B45, 5695 (1992). J.M.Lawrence, P.S.Riseborough and R.D.Parks, Rep.Progr.Phys.44, 1 (1981). H.Nakamura, Y.Kitaoka, H.Yamada and K.Asayama, J.Magn.Magn.Mater. 76–77, 517 (1988); H.Nakamura, Y.Kitaoka, T.Iwai and K.Asayama, J.Phys.Cond.Mat.4, 473 (1992). Y.J.Uemura et al, Phys.Rev.B39, 4726 (1989); C.Tieng, Phys.Rev.B43, 83 (1991). C.Jin et al, Bull.Am.Phys.Soc.36, 717 (1991). E.Gratz, E.Bauer, B.Barbara et al, J.Phys.F15, 1975 (1985). E.Bauer, E.Gratz and C.Schmitzer, J.Magn.Magn.Mater.63–64, 37 (1987). F.R. de Boer et al, J.Magn.Magn.Mater.63–64, 91 (1987). S.Takagi, T.Kimura, N.Sato, T.Satoh and T.Kasuya, J.Phys.Soc.Jpn, 57, 1562 (1988). D.T.Adroya and S.K.Malik, J.Magn.Magn.Mat.100, 126 (1991) (see also corresponding references therein). D.Gignoux et al, J.Magn.Magn.Mat.74, 1 (1988).
439
Bibliography 522. D.T.Adroya, S.K.Malik, B.T.Padalia and R.Vijayaraghavan, Sol.St.Comm.66, 1201 (1988). 523. Y.Nakazawa et al, Techn.Rep.ISSP A2663 (1993). 524. G.Aeppli, F.Bucher, C.Broholm, J.K.Kjems, J.Baumann and J.Hufnagl, Phys.Rev.Lett. 60, 615 (1988). 525. T.T.M.Palstra et al., Phys.Rev.Lett.55, 2727 (1985). 526. J.K.Kjems and C.Broholm, J.Magn.Magn.Mat.76–77, 371 (1988). 527. R.N.Kleiman, D.J.Bishop, R.H.Ott, Z.Fisk and J.L.Smith, Phys.Rev.Lett. 64,1975 (1990). 528. A.de Visser et al, Phys.Rev.B45, 2962 (1992). 529. L.Degiorgi, H.R.Ott, M.Dressel, G.Gruener and Z.Fisk, Europhys.Lett.26, 221 (1994). 530. J.D.Thompson, Z.Fisk and H.R.Ott, J.Magn.Magn.Mat.54–57, 393 (1986). 531. E.Brueck et al Phys.Rev.B49, 8562 (1994). 532. C.Geibel et al, Z.Phys.B83, 305 (1991); A.Schroeder et al, Phys.Rev.Lett.72, 136 (1994). 533. C.Geibel et al, Z.Phys.B84, 1 (1991). 534. E.Brueck, F.R. de Boer, V.Sechovsky and L.Havela, Europhys.Lett. 7, 177 (1988). 535. E.Sugiura et al, J.Magn.Magn.Mater.90–91, 65 (1990); H.Fujii et al, J.Magn.Magn.Mater.90–91, 507 (1990). 536. N.Sato et al, J.Phys.Soc.Jpn 60, 757 (1991). 537. P.Bonville et al. J.Magn.Magn.Mater.76–77, 473 (1988). 538. T.Sakon, N.Sato, A.Oyamada et al. J.Phys.Soc.Jpn 62, 2209 (1992). 539. P.Bonville et al, J.Phys.:Cond.Mat.1, 8567 (1989). 540. M.Kasaya, T.Tani, K.Kawata et al, J.Phys.Soc.Jpn 60, 3145 (1991). 541. S.K.Dhar et al, Phys.Rev.B49, 641 (1994). 542. A.Ochiai, T.Suzuki and T.Kasuya, J.Magn.Magn.Mater.52, 13 (1985). 543. E.V. Sampathkumaran et al, Solid St.Comm.78, 971 (1991). 544. V.A.Stolyarov, L.S.Danelyan and L.Yu.Prokofyeva, Fiz.Tverdogo Tela 28, 2474 (1986). 545. N.B.Brandt and V.V.Moshchalkov, Adv.Phys.33, 373 (1984); V.V.Moshchalkov and N.B.Brandt, Usp.Fiz.Nauk, 149, 585 (1986). 546. F.Steglich, J.Magn.Magn.Mat.100, 186 (1991). 547. E.Bauer, Adv.Phys.40, 417 (1991). 548. K.Miyake, T.Matsuura and C.M.Varma, Solid State Comm.71, 1149 (1989). 549. M.Springford and P.H.P.Reinders, J.Magn.Magn.Mat.76–77, 11 (1988). 550. G.Zwicknagl, Adv.Phys.41, 203 (1992). 551. P.Fulde, J.Keller and G.Zwicknagl, Solid State Physics, vol.41, ed.F.Seitz et al., New York, Academic Press, 1988, p.1. 552. J.Kondo, Solid State Physics, vol.23, ed.F.Seitz and D.Turnbull, New York, Academic Press, 1969, p.183. 553. P.Nozieres, J.Low Temp.Phys.17, 31 (1974). 554. P.W.Anderson, J.Phys.C3, 2346 (1970). 555. P.Nozieres and A.Blandin, J.Phys.(Paris) 41, 193 (1980). 556. K.G.Wilson, Rev.Mod.Phys.47, 773 (1975). 557. N.Andrei, K.Furuya and J.H.Loewenstein, Rev.Mod.Phys.55, 331 (1983). 558. A.M.Tsvelick and P.B.Wiegmann, Adv.Phys.32, 745 (1983). 559. M.D.Daybell and W.A.Steyert, Rev.Mod.Phys.40, 380 (1968); J.Appl.Phys.40, 1056 (1969). 560. A.J.Heeger, Solid State Physics, vol.23, ed.F.Seitz and D.Turnbull, New York, Academic Press, 1969, p.283.
440
Bibliography 561. J.R.Schrieffer, J.Appl.Phys. 38, 1143 (1967). 562. L.L.Hirst, Z.Phys.244, 230 (1971); Int.J.Magn. 2, 213 (1972); Adv.Phys.21, 295 (1972). 563. V.Yu.Irkhin and Yu.P.Irkhin, Zh.Eksp.Theor.Fiz., 107, 616 (1995). 564. J.S.Griffith, The Theory of TransitionMetal Ions, Cambridge, University Press, 1961; The Irreducible Tensor Method for Molecular Symmetry Groups, New Jersey, PrenticeHall, Englewood Cliffs, 1962. 565. D.M.Newns and N.Read, Adv.Phys.36, 799 (1987). 566. F.G.Aliev et al, J.Magn.Magn.Mat.76–77, 295 (1988); Phys.Rev.B47, 729 (1993). 567. M.Kyogaku et al, J.Phys.Soc.Jpn 59, 1728 (1990). 568. T.Takabatake et al, J.Magn.Magn.Mat.76–77, 87 (1988). 569. S.K.Malik and D.T.Adroya, Phys.Rev.B43, 6277 (1991). 570. B.Andraka, Phys.Rev.B49, 348 (1994). 571. P.C.Canfield et al, J.Appl.Phys.70, 5800 (1991). 572. M.F.Hundley et al, Phys.Rev.B42, 6842 (1990); A.Severing, J.D.Thompson, P.C.Canfield and Z.Fisk, Phys.Rev.B44, 6832 (1991). 573. W.F.Brinkman and S.Engelsberg, Phys.Rev.169, 417 (1968). 574. V.Yu.Irkhin and M.I.Katsnelson, Z.Phys.B70, 371 (1988). 575. M.E.Fisher, J.S.Langer, Phys.Rev.Lett.20, 665 (1968). 576. J.Sakurai, J.Matsuura and Y.Komura, J.Phys.Colloque C8, 49, 783 (1988). 577. Y.Onuki et al, J.Phys.Colloque C8, 49, 481 (1988). 578. T.Ohyama, J.Sakurai and Y.Komura, Sol.St.Comm.60, 975 (1986). 579. G.Sparn et al, J.Magn.Magn.Mat.47–48, 521 (1985). 580. U.Gottwick et al, J.Magn.Magn.Mat.63–64, 341 (1987). 581. P.Coleman, Phys.Rev.B29, 3035 (1984). 582. Y.Ono, T.Matsuura and Y.Kuroda, Physica C159, 878 (1989). 583. F.Marabelly and P.Wachter, J.Magn.Magn.Mat.70, 364 (1989). 584. D.I.Khomsky, Usp.Fiz.Nauk, 129, 443 (1979). 585. B.Johansson, Phil.Mag.34, 469 (1974). 586. D.Wielizka, I.H.Wesver, D.W.Lynch and C.G.Olson, Phys.Rev.B26, 7056 (1983). 587. R.Podloucky and D.Gloetzel, Phys.Rev.B27, 3390 (1983). 588. L.D.Finkelstein, Fiz.Metallov Metalloved., 57, 402 (1984). 589. B.Johansson, J.Magn.Magn.Mat.47–48, 231 (1985). 590. V.Yu.Irkhin and M.I.Katsnelson, Zh.Eksp.Teor.Fiz.90, 1080 (1986) [Sov.Phys.JETP 63, 631 (1986)]; Solid State Comm. 58, 881 (1986). 591. G.Travaglini and P.Wachter, Phys.Rev.B30, 893, 5877 (1984); P.Wachter and G.Travaglini, J.Magn.Magn.Mat.47–48, 423 (1985). 592. A.Amato and J.Sierro, J.Magn.Magn.Mat.47–48, 475 (1985). 593. P.Strange, J.Phys.C17, 4273 (1984); F.LopezAguilar and J.CostaQuintana, J.Phys.C19, 2185 (1986). 594. B.Bucher, P.Steiner and P.Wachter, Phys.Rev.Lett.67, 2717 (1991). 595. S.S.Bader, N.E.Phillips and D.B.McWhan, Phys.Rev.B7, 4686 (1973). 596. T.S.Altshuler, V.N.Mironov, G.G.Khaliullin and D.I.Khomsky, Pis’ma ZhETF 40, 28 (1984) [JETP Lett. 40, 754 (1984)]. 597. V.Yu.Irkhin and M.I.Katsnelson, Fiz.Tverd.Tela 29, 1461 (1987). 598. Yu.P.Irkhin, Pis’ma ZhETF 32, 205 (1980). 599. K.Sugiyama et al, J.Magn.Magn.Mat.52, 283 (1985). 600. M.Kasaya, F.Ida, N.Takigawa and T.Kasuya, J.Magn.Magn.Mat.47–48, 429 (1985). 601. V.Yu.Irkhin and M.I.Katsnelson, Fiz.Metallov Metalloved.N1, 16 (1991).
441
Bibliography 602. P.Frings, B.Renker and C.Vettier, J.Magn.Magn.Mater. 63–64, 202 (1987). 603. Y.Onuki et al, J.Magn.Magn.Mater.76–77, 119 (1989); B.Luthi, P.Thalmeier, G.Bruls and D.Weber, J.Magn.Magn.Mater.90–91, 37 (1990). 604. M.A.Continentino, Phys.Rev.B47, 11587 (1993). 605. C.Lacroix, J.Magn.Magn.Mater.100, 90 (1991). 606. S.M.M.Evans, J.Phys.:Cond.Mat.3, 8441 (1991). 607. S.V.Vonsovsky, V.Yu.Irkhin and M.I.Katsnelson, Physica B163, 321 (1990). 608. V.Yu.Irkhin and M.I.Katsnelson, Z.Phys.B82, 77 (1991). 609. S.V.Vonsovsky, V.Yu.Irkhin and M.I.Katsnelson, Physica B171, 135 (1991). 610. P.Coleman, Physica B171, 3 (1991). 611. P.Fazekas and E.MuellerHartmann, Z.Phys.B85, 285 (1991). 612. V.Yu.Irkhin and M.I.Katsnelson, J.Phys.:Cond.Mat.4, 9661 (1992); Phys.Rev.B56, 8109 (1997). 613. H.Yashima, N.Sato, H.Mori and T.Satoh, Solid State Comm.43, 595 (1982); S.K.Dhar, K.A.Gschneidner (Jr.), W.H.Lee, P.Klavins and R.N.Shelton, Phys.Rev.B36, 341 (1987). 614. S.V.Vonsovsky, Yu.P.Irkhin, V.Yu.Irkhin and M.I.Katsnelson, J.Phys.Colloque C8, 49, 253 (1988). 615. M.Kyogaku, Y.Kitaoka, K.Asayama, T.Takabatake and K.Fujii, J.Phys.Soc.Jpn 61, 43 (1992); A.Kratzner et al, Europhys.Lett.19, 649 (1992). 616. R.Kuentzler, R.Claud, G.Schmerber and Y.Dossmann, J.Magn.Magn.Mat. 104–107, 1976 (1992). 617. J.G.Bednorz and K.A.Mueller, Z.Phys.B64, 189 (1986). 618. M.K.Wu et al, Phys.Rev.Lett.58, 908 (1987). 619. F.C.Zhang, T.M.Rice, Phys.Rev.B37, 3759 (1988). 620. V.Yu.Irkhin and M.I.Katsnelson, J.Phys.:Cond.Mat.3, 6439 (1991). 621. R.J.Birgeneau, H.J.Guggenheim and G.Shirane, Phys.Rev.B1, 2211 (1970); R.J.Birgeneau, D.R.Gabbe, H.P.Jenssen et al, Phys.Rev.B38, 6614 (1988). 622. P.Arovas and A.Auerbach, Phys. Rev.B38, 316 (1988). 623. D.Yoshioka, J.Phys.Soc.Jpn 58, 3393 (1989). 624. M.Takahashi, Phys.Rev.B40, 2494 (1989). 625. C.L.Kane, P.A.Lee and N.Read, Phys.Rev.B39, 6880 (1989). 626. K.J. von Szczepanski, P.Horsch, W.Stephan and M.Ziegler, Phys.Rev.B41, 2017 (1990). 627. A.Kebede, C.S.See, J.Schwegler et al, Phys.Rev.B40, 4453 (1989). 628. J.L.Peng, R.N.Shelton and H.B. Radonsky, Phys.Rev.B41, 187 (1989). 629. T.Brugger, T.Schreiner, G.Roth, P.Adelman and G.Czjzek, Phys.Rev.Lett. 71, 2481 (1991). 630. C.C.Yu and P.W.Anderson, Phys.Rev.B29, 6165 (1984). 631. P.W.Anderson, in Frontiers and Borderlines in Many Particle Physics, ed.J.Schrieffer and R.Broglia, NorthHolland, 1988, p.1. 632. S.Kivelson, Phys.Rev.B36, 7237 (1987). 633. P.W.Anderson, Int.J.Mod.Phys.4, 181 (1990); Yu.A.Izymov, M.I.Katsnelson and Yu.N.Skryabin, Itinerant Electron Magnetism [in Russian], Moscow, Nauka, 1994. 634. V.Yu.Irkhin, A.A.Katanin and M.I.Katsnelson, J.Phys.:Cond.Mat. 4, 5227 (1992). 635. V.Yu.Irkhin and M.I.Katsnelson, Pis’ma ZhETF 49, 500 (1989); Phys.Lett.A150, 47 (1990). 636. J.Deportes, B.Ouladdiaf and K.R.A.Ziebeck, J.Magn.Magn.Mat.70, 14 (1987). 637. H.Wada et al, J.Magn.Magn.Mat.70, 17 (1987); M.Shiga, J.Magn.Magn.Mat.129, 17 (1994).
442
Bibliography 638. G.Krill et al, J.Phys.C9, 761 (1976); S.Sudo, J.Magn.Magn.Mat.114, 57 (1992). 639. T.Furuno, K.Ando, S.Kunii et al, J.Magn.Magn.Mat.76–77, 117 (1988); K.Fraas, U.Ahlheim, P.H.P.Reinders et al, J.Magn.Magn.Mater.108, 220 (1992). 640. O.Nakamura, A.Oyamada, A.Ochiai, S.Kunii, T.Takeda, T.Suzuki and T.Kasuya, J.Magn.Magn.Mater.76–77, 293 (1988). 641. Z.Fisk et al, Phys.Rev.Lett.67, 3310 (1991). 642. J.RossatMignod et al, Phys.Rev.B16, 440 (1977); P.Fisher et al, J.Phys.C11, 345 (1978). 643. M.Sera, T.Fujita, T.Suzuki and T.Kasuya, In: Valence Instabilities, NorthHolland, 1982, p.435. 644. P.W.Anderson, Phys.Rev.Lett., 64, 239 (1990); 65, 2306 (1990); 66, 3226 (1991); 71, 1220 (1993). 645. C.M.Varma, P.B.Littlewood, A.SchmittRink, E.Abrahams and A.E.Ruckenstein, Phys.Rev.Lett.63, 1996 (1989); P.B.Littlewood and C.M.Varma, Phys.Rev.B46, 405 (1992). 646. M.B.Maple et al, J.Low Temp.Phys.95, 225 (1994); G.R.Stewart, Rev.Mod.Phys. 73, 797 (2001); 78, 743 (2006). 647. A.A.Romanyukha, Yu.N.Shvachko, V.Yu.Irkhin, M.I.Katsnelson, A.A.Koshta and V.V.Ustinov, Physica C171, 276 (1990). 648. J.M.Luttinger, J.Math.Phys.15, 609 (1963); G.Mahan, ManyParticle Physics, New York, Plenum Press (1981). 649. F.D.M.Haldane, J.Phys.C12, 4791 (1979). 650. A.H.Castro Neto and E.Fradkin, Phys.Rev.B49, 10877 (1994) A.Houghton, H.J.Kwon and J.B.Marston, Phys.Rev.B50, 1351 (1994). 651. N.N.Bogoliubov, Lectures in Quantum Statistics. In: Collected works, vol.2, Kiev, Naukova Dumka, 1970 (in Russian). 652. Yu.P.Irkhin, Zh.Eksper.Teor.Fiz.50, 379 (1966) [Sov.Phys.JETP 23, 253 (1966)]. 653. V.Yu.Irkhin and Yu.P.Irkhin, Fiz.Metallov Metalloved. 76, N4, 49 (1993). 654. V.Yu.Irkhin and Yu.P.Irkhin, phys.stat.sol.(b) 183, 9 (1994). 655. Yu.P.Irkhin, Zh.Eksper.Teor.Fiz.66, 1005 (1974). 656. D.C.Mattic, The Theory of Magnetism, New York, Harper and Row, 1965. 657. V.A.Popov and A.A.Loginov, phys.stat.sol.(b) 84, 83 (1977). 658. C.W.Nielson and G.F.Koster, Spectroscopic coefficients for the p, d, fconfigurations, Cambridge, 1963. 659. B.G.Wybourne, Symmetry Principles and Atomic Spectroscopy, Wiley, New York, 1970. 660. V.Yu.Irkhin and Yu.P.Irkhin, Zh.Eksper.Teor.Fiz.104, 3868 (1993) [Sov.Phys.JETP 77, 858 (1993)]. 661. P.W.Anderson, Solid State Physics, vol.14, ed.F.Seitz and D.Turnbull, New York, Academic Press, 1963, p.99. 662. S.P.Shubin and S.V.Vonsovsky, Proc. Roy.Soc.A145, 159 (1934). 663. S.V.Vonsovsky and M.I.Katsnelson, J.Phys.C12, 2043 (1979). 664. H.Bethe, Intermediate Quantum Mechanics, Benjamin, New York, 1964. 665. A.B.Bolotin and V.K.Shugurov, Zh.Vych.Mat.Mat.Fiziki, 3, 560 (1963); H.J.Silverstone, J.Chem.Phys. 47, 537 (1967). 666. P.M.Levy, Phys.Rev. 177, 509 (1969). 667. V.V.Druzhinin and A.S.Moskvin, Fiz.Metallov Metalloved. 26, 415 (1968). 668. E.L.Nagaev, Usp.Fiz.Nauk, 136, 61 (1989). 669. T.Moriya, Phys.Rev.120, 91 (1960). 670. R.J.Elliott and M.F.Torpe, J.Appl.Phys. 39, 802 (1968).
443
Bibliography 671. D.N.Zubarev, Usp.Fiz.Nauk 71, 71 (1960). 672. V.G.Bar ’yakhtar, V.N.Krivoruchko and D.A.Yablonsky, Solid St.Comm.46, 613 (1983); Zh.Eksp.Teor.Fiz.85, 602 (1983). 673. R.O.Zaitsev, Zh.Eksp.Teor.Fiz.68, 207 (1975). 674. V.V.Valkov and S.G.Ovchinnikov, Teor.Mat.Fiz. 50, 466 (1982). 675. V.V.Valkov and T.A.Valkova, Teor.Mat.Fiz. 59, 453 (1984). 676. V.V.Valkov, T.A.Valkova and S.G.Ovchinnikov, Zh.Eksp.Teor.Fiz. 88, 550 (1985); phys.stat.sol.(b) 142, 255 (1987). 677. F.P.Onufrieva, Zh.Eksp.Teor.Fiz.80, 2372 (1981); 86, 1691 (1984); 89, 2270 (1985); 94, 232 (1988). 678. I.Affleck, J.Phys.:Cond.Mat. 1, 3047 (1989). 679. E.V.Rosenfeld, Pis’ma ZhETF, 24, 60 (1976). 680. M.I.Kaganov and A.V.Chubukov, Usp.Fiz.Nauk, 153, 537 (1987). 681. K. von Klitzing, G.Dorda and M.Pepper, Phys.Rev.Lett.45, 494 (1980). 682. V.P.Silin and A.Z.Solontsov, Fiz.Metallov Metalloved.58, 1080 (1984). 683. M.I.Auslender, V.Yu.Irkhin, Z.Phys.B56, 301 (1984); B61, 129 (1985). 684. H.Wada, M.Nishigori and M.Shiga, J.Phys.:Cond.Mat.3, 2083 (1991). 685. G.M.Carneiro and C.J.Pethick, Phys.Rev.B11, 1106 (1975). 686. F.Rys, J.C.Helman, W.Baltensperger, Phys.Kond.Mat.6, 105 (1967). 687. V.Yu.Irkhin, Fiz.Tverd.Tela 28, 3066 (1986). 688. S.Jin et al, Science 264, 413 (1994). 689. V.Yu.Irkhin and M.I.Katsnelson, Fiz.Metallov Metalloved.65, 446 (1988). 690. N.A.Cade and W.Young, Adv.Phys.26, 393 (1977). 691. M.C.K.Wiltshire, M.M.Elcombe and C.J.Howard, J.Phys.F15, 1595 (1985). 692. M.I.Katsnelson and V.Yu.Irkhin, J.Phys.C17, 4291 (1984). 693. V.Yu.Irkhin and A.M.Entelis, J.Phys.:Cond.Mat.1, 4111 (1989); V.Yu.Irkhin and M.I.Katsnelson, Phys.Rev.B62,5647 (2000). 694. A.O.Anokhin and V.Yu.Irkhin, phys.stat.sol.(b) 165, 129 (1991). 695. A.O.Anokhin, V.Yu.Irkhin and M.I.Katsnelson, J.Phys.: Cond.Mat.3, 1475 (1991). 696. L.A.Maksimov and K.A.Kikoin, Fiz.Metallov Metalloved.28, 43 (1969). 697. R.O.Zaitsev, Zh.Eksp.Teor.Fiz. 75, 2362 (1978). 698. M.Sh.Erukhimov and S.G.Ovchinnikov, phys.stat.sol.(b) 123, 105 (1984). 699. V.Yu.Irkhin and M.I.Katsnelson, Zh.Eksp.Teor.Fiz.88, 522 (1985). 700. V.Yu.Irkhin and M.I.Katsnelson, J.Phys.C18, 4173 (1985). 701. P.B.Wiegmann, Phys.Rev.Lett.60, 821 (1988); Y.Chen, D.Foerster and P.Larkin, Phys.Rev.B46, 5370 (1992). 702. K.Kubo and N.Ohata, J.Phys.Soc.Jpn, 33, 21 (1972). 703. O.Narikiyo, K.Kuboki and H.Fukuyama, J.Phys.Soc.Jpn 59, 2443 (1990). 704. V.V.Druzhinin and Yu.P.Irkhin, Zh.Eksp.Teor.Fiz.51, 1856 (1966) [Sov.Phys.JETP 24, 1250 (1967)]. 705. A.Georges and G.Kotliar, Phys.Rev.B45, 6479 (1993); X.Y.Zhang and C.M.Zhang, Phys.Rev.B49, 7929 (1994); M.J.Rozenberg, G.Kotliar and X.Y.Zhang, Phys.Rev.B49, 10181 (1994); F.J.Ohkawa, J.Phys.Soc.Jpn 61, 1615 (1992); A. Georges et al., Rev. Mod. Phys. 68, 13 (1996). 706. R.Karplus and J.Schwinger, Phys.Rev.73, 1020 (1948). 707. J.M.Luttinger and W.Kohn, Phys.Rev.109, 1892 (1958). 708. L.L.Hirst, Adv.Phys. 27, 231 (1978). 709. Yu.P.Irkhin, Fiz.Tverd.Tela 30, 1202 (1988). 710. K.A.Kikoin and L.A.Maksimov, Zh.Eksp.Teor.Fiz. 58, 2184 (1970). 711. P.Coleman and N.Andrei, J.Phys.:Cond.Mat.1, 4057 (1989).
444
Bibliography 712. S.Chakravarty, B.I.Halperin and D.R.Nelson, Phys.Rev.B39, 2344 (1989). 713. V.Yu.Irkhin, A.A.Katanin and M.I.Katsnelson, Fiz.Metallov Metalloved., 79, N1, 65 (1995); Phys.Lett.A157, 295 (1991). 714. F.D.M.Haldane, Phys.Rev.Lett.50, 1153 (1983). 715. V.Yu.Irkhin and M.I.Katsnelson, Z.Phys.B62, 201 (1986). 716. V.Yu.Irkhin and M.I.Katsnelson, Phys.Rev.B53, 14008 (1996). 717. V.Yu.Irkhin and Yu.P.Irkhin, J.Magn.Magn.Mater.164, 119 (1996). 718. M.Akai, H.Akai and J.Kanamori, J.Phys.Soc.Jpn 54, 4246,4257 (1985). 719. R.Zeller, J.Phys.F17, 2123 (1987). 720. N.Stefanou, A.Oswald, R.Zeller and P.H.Dederichs, Phys.Rev.B35, 6911 (1987). 721. B.Drittler, N.Stefanou, S.Bluegel, R.Zeller and P.H.Dederichs, Phys.Rev.B40, 8203 (1989). 722. P.H.Dederichs, R.Zeller, H.Akai, H.Ebert, J.Magn.Magn.Mater.100, 241 (1991). 723. I.Mertig, E.Mrosan and R.Schoepke, J.Phys.F12, 1689 (1982); I.Mertig, E.Mrosan, R.Zeller and P.H.Dederichs, phys.stat.sol.(b) 117, 619 (1983). 724. I.Mertig, E.Mrosan, R.Zeller and P.H.Dederichs, Proc.Int.Conf. on the Physics of Transition Metals (Darmstadt, July 1992), World Scientific, 1992, p.778. 725. M.D.Daybell, In: Magnetism, vol.5, ed.H.Suhl, New York, Academic Press, 1973. 726. A.R.Miedema, J.F.Dorleijn, J.Phys.F5, 487,1543 (1975); O.Jaoul, I.A.Campbell and A.Fert, J.Magn.Magn.Mater.5, 23 (1977); T.Farrell and D.Greig, J.Phys.C3, 138 (1970); F.Mauri, A.Lucasson, P.Lucasson, P.Moser, F.Faudot, J.Phys.:Cond.Mat.2, 3269 (1990). 727. V.Yu.Irkhin, Phys.Rev.B57, 13375 (1998). 728. V.Yu.Irkhin, A.A.Katanin, Phys.Rev.B55, 12318 (1997); Phys.Rev.B57, 379 (1998); V.Yu.Irkhin, A.A.Katanin, M.I. Katsnelson, Phys.Rev.B60, 1082 (1999). 729. V.Yu.Irkhin, A.V.Zarubin, Phys.Rev.B70, 035116 (2004); J.Magn.Magn.Mat. 300, 246 (2006). 730. V.Yu.Irkhin, A.V.Zarubin, Eur.Phys.Journal B38, 563 (2004). 731. V.Yu.Irkhin and M.I.Katsnelson, Eur.Phys.Journal B19, 401 (2001). 732. V.Yu.Irkhin and M.I.Katsnelson, JETP Lett. 80, 312 (2004). 733. V.Yu.Irkhin and M.I.Katsnelson, Phys.Rev.B61, 14640 (2000). 734. V.Yu.Irkhin and M.I.Katsnelson, Eur.Phys.Journal B43, 479 (2005). 735. V.Yu.Irkhin and M.I.Katsnelson, Eur.Phys.Journal B30, 481 (2002). 736. V.Yu.Irkhin and M.I.Katsnelson, Phys.Rev.B73, 104429 (2006).
445
Bibliography
446
Index
Index A
Born–Haber cycle 86 Bose condensation 291 Bose creation operator 396 Bose statistics 97, 110 Bose–Einstein condensation 418 Bragg number 98 Brewer–Engel picture 104 Brillouin function 127 Brillouin zone 22, 42, 66 Brillouin–Wigner perturbation theory 22 bunching 171
Abrikosov pseudofermion representation 412, 417 Abrikosov–Suhl resonance 258 actinide metals 102 Akulov–Zener law 175 amplitude of the fluctuating moment 149 Anderson Hamiltonian 67, 272 Anderson impurity model 211 Anderson model 405 Anderson–Falicov model 273 Andersonlattice model 156 Anderson’s kinetic exchange interaction 163 Anderson’s spinons 377 anisotropy energy 174 anomalous Hall effect 401 APW method 28 Argyres formula 246 atomic sphere approximation 172 augmented plane wave 27
C CF splitting 18 characteristic spinfluctuation frequency 263 Clebsh–Gordan coefficients 302, 309, 316, 321 coherence temperature 267 cohesive energy 91 Coqblin–Schrieffer model 267 Coulomb interaction 16 Coulomb potential 1 Coulomb repulsion 6, 145 Curie constant 128 Curie point 62 Curie–Weiss contribution of LMM 166 Curie–Weiss law 128, 139, 140
B band index 246 band theory 20 BCS theory of superconductivity 143 Bessel and Neumann function 29 Bloch function 24 Bloch law 190, 330 Bloch modulation function 196 Bloch states 183 Bloch theorem 20 Bogoliubov transformation 206, 273, 418 Bogoliubov–Tyablikov transformation 331 Bohr radius 34 Born approximation 189
D d–f hybridization 67 Darvin correction 247 de Gennes formula 311 de Haas–van Alphen (dHvA) effect 72 de Haas–van Alphen effect 54, 76 Debye model 96 Debye T3law 111 Debye temperature 96, 99 447
Index density functional 35 diamagnetic susceptibility 136 Dirac–Heisenberg model 125 dispersion law 59 DOS peak 120 Dulong–Petit law 110, 113 Dyson equation 157, 268, 332 Dyson–Maleev ideal magnons 291 Dyson–Maleev representation 329, 334, 422 DzyaloshinskyMoriyatype exchange interaction 326
G Gaspar–Kohn–Sham exchange potential 34, 72 giant magnetoresistivity 155 ‘giant’ Van Hove singularities 167 Gibbs distribution 127 Ginzburg–Landau expansion 148 Green’s function method 28 Green’s functions 332 Grueneisen constant 99 gyromagnetic (magnetomechanical) ratio 135
E
H
effective nuclear charge 3 effective smeared density of states 147 effective temperature 148 Einstein–de Haas effect 135 Einstein model 110 electron–phonon enhancement coefficient 117 electron–phonon interaction constant 293 Emery model 289 enhanced susceptibility 148 equilibrium Fermi distribution 188 equilibrium magnetic moment 148 exchange enhancement factor 159 exchange parameter 123 extraordinary Hall effect 372
Haldane gap 422 halfmetallic ferromagnets 151 halfmetallic’ state formation 152 Hall coefficient 183, 230 Hall current 402 Hall effect 242 Hall field 227, 232 Hartree equations 31 Hartree–Fock approximation 23, 70 Hartree–Fock charge density 5 Hartree–Fock decoupling 145 Hartree–Fock equations 31 Hartree–Fock method 7 heavy actinides 102 Hedin–Lundqvist potential 37 Heisenberg exchange 284 Heisenberg Hamiltonian 126 Heisenberg magnets 145 Heisenberg model 126, 136, 336 Heitler–London model 304 Hellman–Feynman theorem 362 HellmanFeynman theorem 352 Heusler alloys 137, 155 Hill criterion 172 Hohenberg–Kohn theorem 23, 38 Holstein–Primakoff representation 204, 329 Hubbard correlation 161 Hubbard ferromagnet 158, 374 Hubbard intrasite repulsion 162 Hubbard model 9, 145, 341, 363
F Fermi commutation relations 296 Fermi creation operator 311 Fermi distribution function 255 Fermi energy 6, 113, 255 Fermi surface 72, 75, 104 Fermi–Dirac statistics 113 Fermiliquid picture 72 ferromagnetic Curie temperature 334 Fisher–Langer transport properties 266 Frank law 227 Friedel concept 210 Friedel model 90 Friedel sum rule 212
448
Index Hubbard operator 307, 336 Hubbard parameter 66, 91, 161, 318 Hubbard splitting 147, 161 HubbardI approximation 365 HubbardI approximation energies 164 HubbardI decoupling 363, 373 HubbardI spectrum 365 HubbardIII approximation 378 Hubbard’s subband 161 HumeRothery rule 104, 171 Hund atomic terms 8 Hund rules 8, 15, 178 hyperfine interaction constant 159
Korringa law 160 Kubo formula 189
L
interband transition frequency 246 interelectron repulsion 5 intrashell repulsion 5 inverse screening radius 196 irreducible Green’s function 343 isotropic Schwinger representation 422 itinerant electrons 139
Landau level 73, 74 Landau quantization 73, 75 Lande factor 311 lattice Green’s function 28 lattice specific heat 215 LCMTO method 30 Leibfried number 98 Lindemann formula 97 linear Kapitza law 231 local magnetic moments 162 local spin density 37 longitudinal susceptibility 160 Lorentz broadening 32 Lorentz force 244 Lorentz smearing 147 Luttinger Hamiltonian 299 Luttinger model 299 Luttinger theorem 72
J
M
Jahn–Teller effect 179 Jahn–Teller ions 179 jjcoupling 406 jungle gym’ features 81
magnetic anisotropy 173 magnetic entropy 257 Magnetic XRay Dichroism 65 magnetoresistivity 227 magnon damping 344 magnon frequency 122 magnon spectrum 165 magnon velocity 357 manyelectron (ME) wave function 301 manyelectron approach 166 marginal Fermiliquid’ theory 299 Matthiessen rule 188, 209 MNR frequency 159 Moriya formula 159 Morse potential parametrization 99 Mott insulator 18, 297 Mott s–d scattering 191 Mott s–d transition model 207 Mott–Hubbard gap 7 Mott–Hubbard transition 271 MTorbitals 30
I
K kdependent relaxation time 213 kspace 176 Kapitza law 227 Kerr angle 245 Kerr effect 153 Kerr rotation 247 KKR method 28, 40 Knight shift 134 Kohler rule 227 Kohn–Sham quasiparticles 36 Kondo effect 138, 254 Kondo lattice 250, 412 Kondo temperature 257 Koopmans theorem 32 Korringa contribution 159
449
Index MTsphere 30 muffintin (MT) form 27
Rhodes–Wohlfarth correlation 140 Rhodes–Wohlfarth curve 136 Rhodes–Wohlfarth ratio 156 Righi–Leduc effect 186, 249 rotational motion energy 3 Ruderman–Kittel–Kasuya–Yosida indirect interaction 170 Russel–Saunders coupling 14, 172 Rydberg constant 383
N Nagaoka decoupling 260 Nagaoka theorem 163 Neel antiferromagnet 419 Neel point 203 Neel temperature 128 Nernst theorem 110 Nernst–Ettingshausen coefficient 186 Nernst–Ettingshausen effect 249 nonmagnetic Kondo state 416 Nordheim rule 207, 208 nuclear gyromagnetic ratio 159
S s–d hybridization 1, 22, 46, 82, 99 scattering probability 188 Schottky anomaly 277 Schrieffer model 258 Schrödinger equation 24 Schwinger boson representation 417 Schwinger bosons 291, 417 selfconsistent meanfield equation 127 selfconsistent spinwave theory 422 selfenergy 147 Shubnikov–de Haas effect 72 skew scattering 235 Slater integral 8, 10, 12 Slater–Coster parametrization 39 Sommerfeld integral 118 spin diffusion constant 265 spin Green’s function 343 spin Hamiltonian 126 spin sleep’ phenomena 171 spin stiffness constant 158 spin susceptibility 134 spinflip scattering processes 208 spinfluctuation theories 145 spinorbit coupling 13 spinwave contribution 122 spinwave correction 122 spinwave stiffness constant 330 spinwave temperature region 164 spinless Falicov–Kimball model 272 spiral angle 171 Stevens operator 15 Stevens parameter 180 Stoner continuum 204 Stoner criterion 139 Stoner excitations 140
O onsite Hubbard repulsion 147 Onsager symmetry principle 185 orbital magnetic momenta 13 Ornstein–Cernike peak 420 orthogonalized plane wave method 23
P p–d hybridization 152 paramagnetic Curie temperature 128, 334 paramagnetic susceptibility 145, 166 Pauli behaviour 258 Pauli paramagnetism 129 Pauli principle 113, 125 Peierls instability 104 phonon occupation number 190 potential 3 centrifugal 3 HartreeFock 4 pseudopotential operator 24
R Racah formalism 8 Racah’s seniority quantum number 313 radial atomic potential 3 RAPW method 68 relative sublattice magnetization 203 renormalized magnon frequency 421
450
Index Stoner instability 122 Stoner meanfield theory 7 Stoner model 123 Stoner parameter 141, 342 Stoner square law 150 Stoner theory 142 superzone boundary 171
singularities 141 van Hove singularities 44, 144 van Hove theorem 44 van Vleck contribution 132 van Vleck paramagnetism 172 vibration amplitude 97 von Barth–Hedin potential 38
T
W
thermoelectric power 213 transfer integral 21 transverse relaxation rate 159 twomagnon processes 160 Tyablikov’s decoupling 337
weak itinerant ferromagnet 151 weak itinerant ferromagnetism 145 Wigner–Eckart theorem 312 Wigner–Seitz cell 68
X
U Umklapp process 196, 224, 226
Xray spectroscopy 55 xapotential 35
V
Z
Van Hove electron spectrum
Zeeman energy 177
451